Materials: Engineering, Science, Processing and Designis the essential materials engineering text and resource for stude
1,064 254 18MB
English Pages xvi, 631, 26, 69, 19, 12, 5, 19 pages illustrations 24 cm  Year 2019
Ceramic Materials: Science and Engineering is an up-to-date treatment of ceramic science, engineering, and applications
1,199 145 20MB Read more
Sustainable Nanoscale Engineering: From Materials Design to Chemical Processing presents the latest on the design of nan
312 23 64MB Read more
Electrospinning, an electro-hydrodynamic process, is a versatile and promising platform technology for the production of
927 86 51MB Read more
339 113 17MB Read more
This updated and enlarged third edition of a widely used text offers an integrated and completely up-to-date coverage of
275 33 16MB Read more
Ceramic Materials: Science and Engineering is an up-to-date treatment of ceramic science, engineering, and applications
487 106 40MB Read more
The third edition of Krishan Chawla's widely used textbook, Composite Materials, offers integrated and completely u
536 107 14MB Read more
Table of contents :
Front Cover......Page 1
Materials: engineering, science, processing and design......Page 5
Science-led or Design-led? Two approaches to materials teaching......Page 15
What is different about this book?......Page 16
What's new in the fourth edition......Page 17
This book and the CES EduPack materials and process information software......Page 18
Complementary resources available through Granta Design Ltd, www.grantadesign.com:......Page 21
1 - Introduction: materials – history and character......Page 23
1.1 Materials, processes and choice......Page 24
1.2 Material properties......Page 25
1.3 Design-limiting properties......Page 34
1.6 Exercises......Page 35
2 - Family trees: organising materials and processes......Page 37
2.2 Organising materials: the materials tree......Page 38
2.3 Organising processes: the process tree......Page 41
2.4 Process–property interaction......Page 44
2.5 Material property charts......Page 45
2.6 Computer-aided information sources for materials and processes......Page 47
2.8 Further reading......Page 48
2.9 Exercises......Page 49
3 - Strategic thinking: matching material to design......Page 53
3.2 The design process......Page 54
3.3 Material and process information for design......Page 57
3.4 The strategy: translation, screening, ranking and documentation......Page 59
3.5 Examples of translation......Page 62
3.6 Summary and conclusions......Page 65
3.8 Exercises......Page 66
4 - Elastic stiffness, and weight: atomic bonding and packing......Page 69
4.2 Density, stress, strain and elastic moduli......Page 70
4.3 The big picture: material property charts......Page 81
4.4 Manipulating the modulus and density......Page 82
4.5 The science: microstructure and properties......Page 86
4.6 Atomic structure and interatomic bonding......Page 87
4.7 Atomic and molecular packing in solids: the origin of density......Page 98
4.8 Interatomic bonding and properties: the origin of elastic modulus......Page 105
4.9 Summary and conclusions......Page 112
4.11 Exercises......Page 113
5 - Stiffness-limited design......Page 119
5.2 Standard solutions to elastic problems......Page 120
5.3 Material indices for elastic design......Page 130
5.4 Plotting limits and indices on charts......Page 138
5.5 Case studies......Page 140
5.6 Summary and conclusions......Page 147
5.8 Exercises......Page 148
6 - Beyond elasticity: plasticity, yielding and ductility......Page 155
6.2 Strength, ductility, plastic work and hardness: definition and measurement......Page 156
6.3 The big picture: charts for yield strength......Page 162
6.4 Drilling down: the origins of strength and ductility......Page 165
6.5 Manipulating strength......Page 175
6.6 Summary and conclusions......Page 184
6.8 Exercises......Page 185
7.1 Introduction and synopsis......Page 191
7.2 Standard solutions to plastic problems......Page 192
7.3 Material indices for yield-limited design......Page 201
7.4 Case studies......Page 206
7.6 Further reading......Page 212
7.7 Exercises......Page 213
8 - Fracture and fracture toughness......Page 225
8.2 Strength and toughness......Page 226
8.3 The mechanics of fracture......Page 228
8.4 Material property charts for toughness......Page 235
8.5 Drilling down: the origins of toughness......Page 237
8.6 Compressive and tensile failure of ceramics......Page 241
8.7 Manipulating properties: the strength–toughness trade-off......Page 245
8.8 Summary and conclusions......Page 248
8.10 Exercises......Page 249
9 - Cyclic loading and fatigue failure......Page 253
9.2 Vibration: the damping coefficient......Page 254
9.3 Fatigue......Page 255
9.4 Charts for endurance limit......Page 263
9.5 Drilling down: the origins of damping and fatigue......Page 265
9.6 Manipulating resistance to fatigue......Page 266
9.8 Further reading......Page 268
9.9 Exercises......Page 269
10 - Fracture- and fatigue-limited design......Page 277
10.2 Standard solutions to fracture problems......Page 278
10.3 Material indices for fracture-safe design......Page 281
10.4 Case studies......Page 283
10.6 Further reading......Page 296
10.7 Exercises......Page 297
11 - Friction and wear......Page 303
11.2 Tribological properties......Page 304
11.3 Charting friction and wear......Page 307
11.4 The physics of friction and wear3......Page 310
11.5 Friction in design......Page 314
11.6 Friction in material processing......Page 318
11.8 Further reading......Page 321
11.9 Exercises......Page 322
12 - Materials and heat......Page 325
12.2 Thermal properties: definition and measurement......Page 326
12.3 The big picture: thermal property charts......Page 330
12.4 Drilling down: the physics of thermal properties......Page 334
12.5 Manipulating thermal properties......Page 339
12.6 Design and manufacture: using thermal properties......Page 340
12.7 Summary and conclusions......Page 350
12.8 Further reading......Page 351
12.9 Exercises......Page 352
13 - Diffusion and creep: materials at high temperatures......Page 357
13.2 The temperature dependence of material properties......Page 358
13.3 Charts for creep behaviour......Page 364
13.4 The science: diffusion......Page 366
13.5 The science: creep......Page 374
13.6 Materials to resist creep......Page 380
13.7 Design to cope with creep......Page 383
13.9 Further reading......Page 390
13.10 Exercises......Page 391
14 - Durability: oxidation, corrosion, degradation......Page 401
14.1 Introduction and synopsis......Page 402
14.2 Oxidation, flammability, and photo-degradation......Page 403
14.3 Oxidation mechanisms......Page 404
14.4 Resistance to oxidation......Page 407
14.5 Corrosion: acids, alkalis, water, and organic solvents......Page 408
14.6 Drilling down: mechanisms of corrosion......Page 409
14.7 Fighting corrosion......Page 418
14.8 Summary and conclusions......Page 426
14.9 Further reading and software......Page 427
14.10 Exercises......Page 428
15 - Electrical materials: conductors, insulators, and dielectrics......Page 433
15.1 Introduction and synopsis......Page 434
15.2 Conductors, insulators, and dielectrics......Page 435
15.3 Charts for electrical properties......Page 442
15.4 Drilling down: the origins and manipulation of electrical properties......Page 444
15.5 Design: using the electrical properties of materials......Page 456
15.6 Summary and conclusions......Page 462
15.8 Exercises......Page 463
16.1 Introduction and synopsis......Page 469
16.2 Magnetic properties: definition and measurement......Page 470
16.3 The big picture: charts for magnetic properties......Page 477
16.4 Drilling down: the physics and manipulation of magnetic properties......Page 480
16.5 Materials selection for magnetic design......Page 484
16.7 Further reading......Page 492
16.8 Exercises......Page 493
17 - Materials for optical devices......Page 497
17.2 The interaction of materials and radiation......Page 498
17.4 Drilling down: the physics and manipulation of optical properties......Page 507
17.5 Optical design......Page 514
17.6 Summary and conclusions......Page 516
17.8 Exercises......Page 517
18 - Manufacturing processes and design......Page 521
18.1 Introduction and synopsis......Page 522
18.2 Process selection in design......Page 523
18.3 Shaping processes: attributes for screening......Page 526
18.4 Estimating cost for shaping processes......Page 534
18.5 Case studies: selection of shaping processes......Page 537
18.6 Joining processes: attributes for screening......Page 542
18.7 Surface treatment (finishing) processes: attributes for screening......Page 546
18.8 Technical evaluation......Page 548
18.9 Additive manufacturing......Page 561
18.11 Further reading......Page 566
18.12 Exercises......Page 567
19 - Processing, microstructure and properties......Page 573
19.1 Introduction and synopsis......Page 574
19.2 Processing for properties......Page 575
19.3 Microstructure evolution in processing......Page 577
19.4 Metal shaping processes......Page 591
19.5 Heat treatment and alloying of metals......Page 595
19.6 Joining and surface treatment of metals......Page 605
19.7 Powder processing......Page 607
19.8 Polymer processing......Page 609
19.9 Making hybrid materials......Page 613
19.10 Summary and conclusions......Page 615
19.11 Further reading......Page 616
19.12 Exercises......Page 617
20 - Materials, environment, and sustainability......Page 621
20.2 Material production, material consumption, and growth......Page 622
20.3 Natural Capital and the materials life cycle......Page 626
20.4 Embodied energy and carbon footprint of materials......Page 628
20.5 Materials and eco-design......Page 636
20.6 Materials dependence......Page 639
20.7 Materials and sustainable development......Page 642
20.9 Appendix: some useful quantities......Page 645
20.10 Further reading......Page 646
20.11 Exercises......Page 647
Guided Learning Unit 1: Simple ideas ofcrystallography......Page 655
PART 1: Crystal structures......Page 656
PART 2: Interstitial space......Page 663
PART 3: Describing planes......Page 664
PART 4: Describing directions......Page 666
PART 5: Ceramic crystals......Page 668
PART 6: Polymer crystals......Page 673
Answers to exercises......Page 674
Guided Learning Unit 2: Phase diagrams and phasetransformations......Page 681
Introduction and synopsis......Page 682
Alloys and components......Page 683
Constitution, equilibrium, and thermodynamics......Page 685
PART 2: Simple phase diagrams, and how to read them......Page 686
Answers to exercises, Part 2......Page 698
PART 3: The iron–carbon diagram......Page 702
PART 4: Interpreting more complex phase diagrams......Page 706
Answers to exercises, Part 4......Page 710
PART 5: Phase transformations and microstructural evolution......Page 713
PART 6: Equilibrium solidification......Page 715
Answers to exercises, Part 6......Page 726
PART 7: Equilibrium solid-state phase changes......Page 728
Answers to exercises, Part 7......Page 733
PART 8: Non-equilibrium solid-state phase changes......Page 735
Answers to exercises, Part 8......Page 743
Further exercises......Page 744
A - Data for engineering materials......Page 751
B1 Commonly encountered corrosive environments......Page 772
B3 Preferred materials and coatings for given environments......Page 774
B4 Coatings......Page 780
B5 Corrosion inhibitors......Page 781
C3 Polymers and elastomers......Page 784
Back Cover......Page 810
Physical constants in SI units Physical constant
Value in SI units 273.2 9.807 6.022 1023 2.718 1.381 10 23 9.648 104 8.314 1.257 10 6 8.854 10 12 6.626 10 34 2.998 108 22.41 10 3
Absolute zero temperature Acceleration due to gravity, g Avogadro’s number, NA Base of natural logarithms, e Boltzmann’s constant, k Faraday’s constant, k Gas constant, R Permeability of vacuum, m0 Permittivity of vacuum, ε0 Planck’s constant, h Velocity of light in vacuum, c Volume of perfect gas at STP
C m/s2 J/K C/mol J/mol/K H/m F/m J/s m/s m3/mol
Conversion of units, general Quantity
Diffusion coefﬁcient, D
See inside back cover
1 kgf 1 lbf 1 dyne
9.807 N 4.448 N 1.0 10
1 ft 1 inch 1Å
304.8 mm 25.40 mm 0.1 nm
1 ton 1 short ton 1 long ton 1 lb mass
1000 kg 908 kg 1107 kg 0.454 kg
See inside back cover
See inside back cover
Speciﬁc heat, Cp
1 cal/g. C 1 Btu/lb. F
4.184 kJ/kg.K 4.187 kJ/kg.K
Stress intensity, K1
1 ksi Oin
1.10 MN/m3/2 (*)
Surface energy, g
1 mJ/m2 0.556 K
Thermal conductivity, l
1 cal/s.cm. C 1 Btu/h.ft. F
418.8 W/m.K 1.731 W/m.K
1 imp gal 1 US gal
4.546 10 3.785 10
1P 1 lb ft.s
0.1 N.s/m2 0.1517 N.s/m2
(*) Stress intensity is more commonly expressed in the numerically identical MPa.m1/2.
This page intentionally left blank
Materials: engineering, science, processing and design Fourth edition
Mike Ashby, Hugh Shercliff, and David Cebon Department of Engineering, University of Cambridge, UK
Butterworth-Heinemann is an imprint of Elsevier The Boulevard, Langford Lane, Kidlington, Oxford OX5 1GB, United Kingdom 50 Hampshire Street, 5th Floor, Cambridge, MA 02139, United States First published 2007 Second edition 2010 Third edition 2014 Fourth edition 2019 Copyright Ó 2019 Elsevier Ltd. All rights reserved. No part of this publication may be reproduced or transmitted in any form or by any means, electronic or mechanical, including photocopying, recording, or any information storage and retrieval system, without permission in writing from the publisher. Details on how to seek permission, further information about the Publisher’s permissions policies and our arrangements with organizations such as the Copyright Clearance Center and the Copyright Licensing Agency, can be found at our website: www.elsevier.com/permissions. This book and the individual contributions contained in it are protected under copyright by the Publisher (other than as may be noted herein). Notices Knowledge and best practice in this ﬁeld are constantly changing. As new research and experience broaden our understanding, changes in research methods, professional practices, or medical treatment may become necessary. Practitioners and researchers must always rely on their own experience and knowledge in evaluating and using any information, methods, compounds, or experiments described herein. In using such information or methods they should be mindful of their own safety and the safety of others, including parties for whom they have a professional responsibility. To the fullest extent of the law, neither the Publisher nor the authors, contributors, or editors, assume any liability for any injury and/or damage to persons or property as a matter of products liability, negligence or otherwise, or from any use or operation of any methods, products, instructions, or ideas contained in the material herein. Library of Congress Cataloging-in-Publication Data A catalog record for this book is available from the Library of Congress British Library Cataloguing-in-Publication Data A catalogue record for this book is available from the British Library ISBN: 978-0-08-102376-1 For information on all Butterworth-Heinemann publications visit our website at https://www.elsevier.com/books-and-journals
Publisher: Katey Birtcher Acquisition Editor: Steve Merken Editorial Project Manager: Nate McFadden Production Project Manager: Sreejith Viswanathan Cover Designer: Christian Bilbow Typeset by TNQ Technologies
Preface Acknowledgments Resources that accompany this book
xiii xvii xix
Chapter 1 Introduction: materials e history and character 1.1 Materials, processes and choice 1.2 Material properties 1.3 Design-limiting properties 1.4 Summary and conclusions 1.5 Further reading 1.6 Exercises
1 2 3 12 13 13 13
Chapter 2 Family trees: organising materials and processes 2.1 Introduction and synopsis 2.2 Organising materials: the materials tree 2.3 Organising processes: the process tree 2.4 Processeproperty interaction 2.5 Material property charts 2.6 Computer-aided information sources for materials and processes 2.7 Summary and conclusions 2.8 Further reading 2.9 Exercises
15 16 16 19 22 23 25 26 26 27
Chapter 3 Strategic thinking: matching material to design 3.1 Introduction and synopsis 3.2 The design process 3.3 Material and process information for design 3.4 The strategy: translation, screening, ranking and documentation 3.5 Examples of translation 3.6 Summary and conclusions 3.7 Further reading 3.8 Exercises
31 32 32 35 37 40 43 44 44
vi Contents Chapter 4 Elastic stiffness, and weight: atomic bonding and packing 4.1 Introduction and synopsis 4.2 Density, stress, strain and elastic moduli 4.3 The big picture: material property charts 4.4 Manipulating the modulus and density 4.5 The science: microstructure and properties 4.6 Atomic structure and interatomic bonding 4.7 Atomic and molecular packing in solids: the origin of density 4.8 Interatomic bonding and properties: the origin of elastic modulus 4.9 Summary and conclusions 4.10 Further reading 4.11 Exercises
47 48 48 59 60 64 65 76 83 90 91 91
Chapter 5 Stiffness-limited design 5.1 Introduction and synopsis 5.2 Standard solutions to elastic problems 5.3 Material indices for elastic design 5.4 Plotting limits and indices on charts 5.5 Case studies 5.6 Summary and conclusions 5.7 Further reading 5.8 Exercises
97 98 98 108 116 118 125 126 126
Chapter 6 Beyond elasticity: plasticity, yielding and ductility 6.1 Introduction and synopsis 6.2 Strength, ductility, plastic work and hardness: deﬁnition and measurement 6.3 The big picture: charts for yield strength 6.4 Drilling down: the origins of strength and ductility 6.5 Manipulating strength 6.6 Summary and conclusions 6.7 Further reading 6.8 Exercises
133 134 134 140 143 153 162 163 163
Chapter 7 Strength-limited design 7.1 Introduction and synopsis 7.2 Standard solutions to plastic problems 7.3 Material indices for yield-limited design 7.4 Case studies 7.5 Summary and conclusions 7.6 Further reading 7.7 Exercises
169 169 170 179 184 190 190 191
Chapter 8 Fracture and fracture toughness 8.1 Introduction and synopsis 8.2 Strength and toughness 8.3 The mechanics of fracture 8.4 Material property charts for toughness 8.5 Drilling down: the origins of toughness 8.6 Compressive and tensile failure of ceramics 8.7 Manipulating properties: the strengthetoughness trade-off 8.8 Summary and conclusions 8.9 Further reading 8.10 Exercises
203 204 204 206 213 215 219 223 226 227 227
Chapter 9 Cyclic loading and fatigue failure 9.1 Introduction and synopsis 9.2 Vibration: the damping coefﬁcient 9.3 Fatigue 9.4 Charts for endurance limit 9.5 Drilling down: the origins of damping and fatigue 9.6 Manipulating resistance to fatigue 9.7 Summary and conclusions 9.8 Further reading 9.9 Exercises
231 232 232 233 241 243 244 246 246 247
Chapter 10 Fracture- and fatigue-limited design 10.1 Introduction and synopsis 10.2 Standard solutions to fracture problems 10.3 Material indices for fracture-safe design 10.4 Case studies 10.5 Summary and conclusions 10.6 Further reading 10.7 Exercises
255 256 256 259 261 274 274 275
Chapter 11 Friction and wear 11.1 Introduction and synopsis 11.2 Tribological properties 11.3 Charting friction and wear 11.4 The physics of friction and wear 11.5 Friction in design 11.6 Friction in material processing 11.7 Summary and conclusions 11.8 Further reading 11.9 Exercises
281 282 282 285 288 292 296 299 299 300
viii Contents Chapter 12 Materials and heat 12.1 Introduction and synopsis 12.2 Thermal properties: deﬁnition and measurement 12.3 The big picture: thermal property charts 12.4 Drilling down: the physics of thermal properties 12.5 Manipulating thermal properties 12.6 Design and manufacture: using thermal properties 12.7 Summary and conclusions 12.8 Further reading 12.9 Exercises
303 304 304 308 312 317 318 328 329 330
Chapter 13 Diffusion and creep: materials at high temperatures 13.1 Introduction and synopsis 13.2 The temperature dependence of material properties 13.3 Charts for creep behaviour 13.4 The science: diffusion 13.5 The science: creep 13.6 Materials to resist creep 13.7 Design to cope with creep 13.8 Summary and conclusions 13.9 Further reading 13.10 Exercises
335 336 336 342 344 352 358 361 368 368 369
Chapter 14 Durability: oxidation, corrosion, degradation 14.1 Introduction and synopsis 14.2 Oxidation, ﬂammability, and photo-degradation 14.3 Oxidation mechanisms 14.4 Resistance to oxidation 14.5 Corrosion: acids, alkalis, water, and organic solvents 14.6 Drilling down: mechanisms of corrosion 14.7 Fighting corrosion 14.8 Summary and conclusions 14.9 Further reading and software 14.10 Exercises
379 380 381 382 385 386 387 396 404 405 406
Chapter 15 Electrical materials: conductors, insulators, and dielectrics 15.1 Introduction and synopsis 15.2 Conductors, insulators, and dielectrics 15.3 Charts for electrical properties 15.4 Drilling down: the origins and manipulation of electrical properties 15.5 Design: using the electrical properties of materials 15.6 Summary and conclusions
411 412 413 420 422 434 440
Contents 15.7 15.8
Further reading Exercises
ix 441 441
Chapter 16 Magnetic materials 16.1 Introduction and synopsis 16.2 Magnetic properties: deﬁnition and measurement 16.3 The big picture: charts for magnetic properties 16.4 Drilling down: the physics and manipulation of magnetic properties 16.5 Materials selection for magnetic design 16.6 Summary and conclusions 16.7 Further reading 16.8 Exercises
447 447 448 455 458 462 470 470 471
Chapter 17 Materials for optical devices 17.1 Introduction and synopsis 17.2 The interaction of materials and radiation 17.3 Charts for optical properties 17.4 Drilling down: the physics and manipulation of optical properties 17.5 Optical design 17.6 Summary and conclusions 17.7 Further reading 17.8 Exercises
475 476 476 485 485 492 494 495 495
Chapter 18 Manufacturing processes and design 18.1 Introduction and synopsis 18.2 Process selection in design 18.3 Shaping processes: attributes for screening 18.4 Estimating cost for shaping processes 18.5 Case studies: selection of shaping processes 18.6 Joining processes: attributes for screening 18.7 Surface treatment (ﬁnishing) processes: attributes for screening 18.8 Technical evaluation 18.9 Additive manufacturing 18.10 Summary and conclusions 18.11 Further reading 18.12 Exercises
499 500 501 504 512 515 520 524 526 539 544 544 545
Chapter 19 Processing, microstructure and properties 19.1 Introduction and synopsis 19.2 Processing for properties 19.3 Microstructure evolution in processing
551 552 553 555
x Contents 19.4 19.5 19.6 19.7 19.8 19.9 19.10 19.11 19.12
Metal shaping processes Heat treatment and alloying of metals Joining and surface treatment of metals Powder processing Polymer processing Making hybrid materials Summary and conclusions Further reading Exercises
569 573 583 585 587 591 593 594 595
Chapter 20 Materials, environment, and sustainability 20.1 Introduction and synopsis 20.2 Material production, material consumption, and growth 20.3 Natural Capital and the materials life cycle 20.4 Embodied energy and carbon footprint of materials 20.5 Materials and eco-design 20.6 Materials dependence 20.7 Materials and sustainable development 20.8 Summary and conclusions 20.9 Appendix: some useful quantities 20.10 Further reading 20.11 Exercises
599 600 600 604 606 614 617 620 623 623 624 625
Guided Learning Unit 1: Simple ideas of crystallography Introduction and synopsis PART 1 Crystal structures PART 2 Interstitial space PART 3 Describing planes PART 4 Describing directions PART 5 Ceramic crystals PART 6 Polymer crystals Answers to exercises
GL1-1 GL1-2 GL1-2 GL1-9 GL1-10 GL1-12 GL1-14 GL1-19 GL1-20
Guided Learning Unit 2: Phase diagrams and phase transformations Introduction and synopsis PART 1 Key terminology PART 2 Simple phase diagrams, and how to read them PART 3 The ironecarbon diagram PART 4 Interpreting more complex phase diagrams PART 5 Phase transformations and microstructural evolution
GL2-1 GL2-2 GL2-3 GL2-6 GL2-22 GL2-26 GL2-33
Contents PART 6 Equilibrium solidiﬁcation PART 7 Equilibrium solid-state phase changes PART 8 Non-equilibrium solid-state phase changes Further reading Further exercises Appendix A: Data for engineering materials Appendix B: Corrosion tables Appendix C: Material properties and length scales Index
GL2-35 GL2-48 GL2-55 GL2-64 GL2-64 Ae1 Be1 Ce1 Ie1
This page intentionally left blank
Science-led or Design-led? Two approaches to materials teaching The traditional approach to materials teaching starts with fundamentals: the electron, the atom, atomic bonding, and packing, crystallography, and crystal defects. Onto this is built alloy theory, the kinetics of phase transformations and the development of the microstructure on scales made visible by electron and optical microscopes. This sets the stage for the understanding and control of properties at the millimetre or centimetre scale at which they are usually measured. This science-led approach is grounded in a deep physical understanding of the origins of material properties but gives less emphasis to the behavior of structures and components in service, or methods for material selection and design (the schematic below, reading from left to right). Design-led approach
Science-led and Design-led approaches to materials teaching, and the length scales involved.
The alternative approach is design-led (the schematic, reading from right to left). The starting point comprises the requirements that materials must meet if they are to perform well in a given design. To match material to design requires a perspective on the range of properties they offer, how these properties combine to limit performance, the inﬂuences of manufacturing processes on properties, and the environmental impact over the product life-cycledall coupled to the need to access data and expertise to evaluate them. Once the importance of each property is established, there is a clear platform and motivation from which to “drill down,” so to speak, to examine the science that lies beneath itdvaluable because an understanding of the fundamentals itself informs material choice, processing, and usage. Each approach has its place. The best choice depends on the nature of the course and the aspirations of the student. If the intent is to educate future scientiﬁc researchers, the ﬁrst is the logical way
xiv Preface to go. If it is any branch of engineering, design, or applied industrial research, the second makes better sense. This book follows the second, design-led, approach, while providing a balanced treatment of the fundamentals.
What is different about this book? There are many books about the science of engineering materials; many more about design. What is different about this one? First, its design-led approach, speciﬁcally developed to guide material selection and understanding for a wide spectrum of engineering courses. The approach is systematic, leading from design requirements to a prescription for optimized material choice, illustrated by numerous case studies. Practice in the approach is provided by worked Examples in the text and Exercises at the end of each Chapter. Second, its emphasis on visual communication through a unique graphical presentation of material properties as material property charts and numerous schematics. These are a central feature of the approach, helpful in utilizing visual memory as a learning tool, understanding the origins of properties, their manipulation, and their fundamental limits, and providing a tool for selection and for understanding the ways in which materials are used. Third, its inclusivity and breadth. Equal weight is given to all classes of material: metals, polymers, ceramics, and what we call “hybrids”dcomposites, foams, and most natural materials. The aim here is to present the properties of materials, their origins, and the way they enter engineering and design. A glance at the Contents pages will show sections dealing with:
·· · ·· ·
physical, mechanical and thermal properties, and selection methods to deal with them friction, wear, durability and corrosion electrical, magnetic and optical materials, as well as design with the “functional” properties they offer manufacturing processes, and associated selection methods in design materials processing, and the way it inﬂuences properties eco-design and the broader issues of sustainable technology
Throughout we aim for a simple, straightforward presentation, developing the materials science as far as is helpful in guiding engineering and design, avoiding detail where it does not contribute to this end. The fourth feature is that of guided self-learning. Certain topics lend themselves to self-instruction with embedded exercises to build systematic understanding. It works particularly well for topics that involve a contained set of concepts and tools. Crystallography, as an example, involves ideas of three-dimensional geometry that are most easily grasped by drawing and problem-solving. And understanding phase diagrams and phase transformations relies on interpreting graphical displays of compositional and thermodynamic information. Their use to understand and predict microstructure follows procedures that are best learned by application. Both topics have been packaged into self-contained Guided Learning Units, with each new concept presented and immediately practiced using exercises, thereby building conﬁdence. Students who have worked through a package can feel
that they have mastered the topic and know how to apply the ideas it contains. Both topics appear brieﬂy in the main text to give a preliminary overview. The full Guided Learning Units follow later in the book, providing for those courses that require a deeper understanding. The design-led approach is developed to a higher level in ﬁve further textbooks, the ﬁrst relating to Mechanical Design,1 the second and third to Design for the Environment,2,3 the fourth to Industrial Design,4 and the ﬁfth to Manufacturing and Design.5
What’s new in the fourth edition Several main features are new to the fourth edition of this book:
· · 1
The text and ﬁgures have been revised and updated throughout, with particular additions in the following topic areas: the distinction between bonding-sensitive and microstructure-sensitive properties, leading to a discussion of the nature of atomic and molecular bonding; strengthening mechanisms, expanded to include grain-size strengthening; functional properties, including dielectric, ferro, piezo, thermo- and pyro-electric behaviour, ferro- and ferri-magnetic, magneto-strictive and magneto-caloric responses, and optical attributes, with examples of their selection and use in design; selection of manufacturing process, introducing a structured approach to managing the knowledge-base of expertise that links materials, processes, and design; additive manufacture, a review of emerging methods, set within the same framework used to assess established processes; materials and the environment, the coverage of which has been fully updated, with a section on sustainability and sustainable technology offering a new perspective. The number of worked examples in the text has been increased to provide broader illustration of key concepts and equations. The end-of-chapter exercises have been edited and their number expanded to more than 460, with a fully updated solution manual available to instructors.
· ·· · · ·
Ashby, M. F. (2017), Materials selection in mechanical design, 5th edition, Butterworth Heinemann, Oxford, UK. ISBN 9780081005996. (An advanced text developing material selection methods in detail.) Ashby, M.F. (2012), Materials and the Environment e eco-informed material choice, 2nd edition, Butterworth Heinemann, Oxford, UK. ISBN 978-0-12-385971-6. (A teaching text introducing students to the concepts and underlying facts about concerns for the environment and the ways in which materials and products based on them can both help and harm it.) Ashby, M.F., Ferrer-Balas, D., and Segalas Coral, J. (2016), Materials and Sustainable Development, Butterworth-Heinemann, Oxford, UK. ISBN 978-0-08-100176-9. (A text presenting a methodology for assessing whether a material, product or even a whole technology can be regarded as sustainable.) Ashby, M.F., and Johnson, K. (2013), Materials and design, the art and science of material selection in product design, 3rd edition, Butterworth Heinemann, Oxford, UK. ISBN 978-0-08-098205-2. (A text that complements those above, dealing with the aesthetics, perceptions, and associations of materials and their importance in product design.) Tempelman, E., Shercliff, H.R., and Ninaber van Eyben, B. (2014), Manufacturing and design e understanding the principles of how things are made, Butterworth Heinemann, Oxford, UK. ISBN 978-0-08-099922-7. (The source of the manufacturing triangle and the structured approach to process-material-design interactions.)
This book and the CES EduPack materials and process information software Engineering design today takes place in a computer-based environment. Stress analysis (ﬁnite element method, or FEM, codes for instance), computer-aided design (CAD), design for manufacture (DFM), and product data management tools are part of an engineering education. The CES materials and process information software6 for education (the CES EduPack) provides a computer-based environment for optimized materials selection and design, eco-auditing, and introducing processing, including the underlying materials science. This book is self-contained and does not depend on the CES EduPack for its use. But at the same time, it is designed to interface with the CES software, which implements the methods developed in it, should the instructor and student wish to do so. This enables realistic design problems and selection studies to be addressed, properly managing the multiple constraints on material and processes attributes, particularly in project work. The methodology also provides the user with novel ways to explore how properties are manipulated. And with sustainability now a core topic in most materialsrelated teaching in engineering and design, the book and the software introduce students to the ideas of life-cycle assessment. Using the CES EduPack enhances the learning experience and provides a solid grounding in many of the domains of expertise speciﬁed by the various professional engineering accreditation bodies (analysis of components, problem-solving, design and manufacture, economic, societal, and environmental impact, and so on). In addition, the CES Elements database documents the fundamental physical, crystallographic, mechanical, thermal, electrical, magnetic, and optical properties of all 112 stable elements of the periodic table, allowing the origins and inter-relationships among properties to be explored. In a change from previous editions of this book, an extensive set of CES-based exercises for each chapter are now accessible online, again with a fully worked solution manual available for instructors (further details in the section: Resources that accompany this book).
The CES EduPack, Granta Design Ltd., Rustat House, 62 Clifton Court, Cambridge CB1 7EG, UK. www.granta design.com/education.
No book of this sort is possible without advice, constructive criticism, and ideas from others. Numerous colleagues have been generous with their time and thoughts. We would particularly like to recognize the suggestions made by Professors Mick Brown, Archie Campbell, David Cardwell, Ken Wallace, and Ken Johnson, all of Cambridge University, Professor John Abelson of the University of Illinois, and Professor Erik Tempelman of TU Delft. Equally valuable has been the contribution of the team at Granta Design, Cambridge, responsible for the development of the CES software that has been used to make the material property charts that are a feature of this book. We gratefully acknowledge the following Materials, Fourth Edition reviewers, whose valuable insight helped to shape this text.
Reviewers Anton den Boer, Avans University of Applied Science, Netherlands Benjamin Liaw, City College of New York David A. Schiraldi, Case Western Reserve University Atin Sinha, Georgia Southwestern State University
This page intentionally left blank
Resources that accompany this book
Resources available to adopting instructors who register on the Elsevier textbook website, http://textbooks.elsevier.com: Instructor’s manual of exercises and solutions The book includes a comprehensive set of exercises that can be completed using information, diagrams, equations, and data contained in the book itself (with a small number involving Web searches or independent student observation). Fully worked-out solutions to the exercises are freely available online to tutors and lecturers who adopt this book. Image Bank The Image Bank provides adopting tutors and lecturers with electronic versions of the ﬁgures from the book that may be used in lecture slides and class presentations. PowerPoint Lecture Slides Use the available set of lecture slides in your own course as provided, or edit and reorganise them to meet your individual course needs. Interactive online materials science tutorials To enhance students’ learning of materials science, instructors adopting this book may provide their classes with a free link to a set of online interactive tutorials. There are 12 available modules: Bonding, Tensile Testing, Casting and Recrystallization, Fracture and Fatigue, Corrosion, Phase Equilibria, Wear, Ceramics, Composites, Polymers, Light Alloys, and Dislocations. Each module includes a selection of self-test questions. The link is available to instructors who register on the Elsevier textbook website.
Complementary resources available through Granta Design Ltd, www.grantadesign.com: The CES EduPack As explained earlier, the CES EduPack is a software-based package developed by Michael Ashby and Granta Design, that implements many of the methods in this book. Used together, Materials: Engineering, Science, Processing, and Design and CES EduPack provide a complete materials, manufacturing, and design course. CES exercises and solutions Two types of exercises, with fully worked-out solutions and CES project ﬁles, are provided via the Granta Design website: the ﬁrst uses the CES software to apply and reinforce the methods developed in the book, and the second explores the underlying science more deeply using the CES Elements database that is part of the CES system. For further information please visit http://www.grantadesign/education/textbooks/MaterialsESPD.
This page intentionally left blank
Introduction: materials e history and character
Professor James Stuart, the ﬁrst Professor of Engineering at Cambridge, appointed in 1875.
Chapter contents 1.1 1.2 1.3 1.4 1.5 1.6
Materials, processes and choice Material properties Design-limiting properties Summary and conclusions Further reading Exercises
Copyright Ó 2019 Elsevier Ltd. All rights reserved. https://doi.org/10.1016/B978-0-08-102376-1.00001-9
2 3 12 13 13 13
2 Chapter 1 Introduction: materials e history and character
Materials, processes and choice
Engineers make things. They make them out of materials, and they shape, join and ﬁnish them using processes. The materials support loads, they insulate or conduct heat and electricity, and they channel or reject magnetic ﬂux, transmit or reﬂect light, and tolerate hostile surroundings. Ideally, they do all this without damage to the environment or costing too much. To make something, you also need a process, one that is compatible with the material you plan to use. Sometimes it is the process that is the dominant partner, and a material match must be found. Compatibility with viable processing conditions is not always easy to ﬁnd, and material failure can be catastrophic, with issues of liability and compensation. But our aim here is not contention; rather, it is to give a vision of the universe of materials (universe, since even on the remotest planets you will ﬁnd the same elements) and of the universe of processes, and to provide methods for choosing them to ensure a durable, compatible union. But, you may say, engineers have been making things out of materials for centuries, and successfully so e think of Isambard Kingdom Brunel, Thomas Telford, Gustave Eiffel, Henry Ford, Karl Benz and Gottlieb Daimler, the Wright brothers. Why do we need new ways to choose them? A little history helps here. The portrait with which this chapter starts shows James Stuart, the ﬁrst professor of engineering at Cambridge University. In his day, the number of materials available to engineers was small e a few hundred at most. There were no synthetic polymers e there are now over 45,000 of them. There were no light alloys (aluminium was ﬁrst used in engineering only in the 20th century) e now there are thousands. There were no high-performance composites e now there are hundreds to choose from. The history is developed further in Figure 1.1, the time axis of which spans 10,000 years. The timescale is non-linear e almost all the materials we use today were developed in the last 100 years. And this number is enormous: over 160,000 materials are available to today’s engineer, presenting us with a problem that Professor Stuart did not have: that of optimally selecting the best one. Innovative design means the imaginative exploitation of the properties offered by materials. These properties today are largely known and documented in handbooks; one such e the ASM Materials Handbook e runs to 22 fat volumes, and it is one of many. How are we to deal with this vast body of information? Fortunately, another thing has changed since Prof. Stuart’s day: digital information storage and manipulation. Computer-aided design is now a standard part of an engineer’s training, and it is backed up by widely available packages for solid modelling, ﬁnite-element analysis, optimisation and for material and process selection. Software for the last of these e the selection of materials and processes e draws on databases of the attributes of materials and processes, documenting their mutual compatibility, and allows them to be searched and displayed in ways that enable selections that best meet the requirements of a design. If you travel by foot, bicycle or car, you take a map. The materials landscape, like the terrestrial one, can be complex and confusing; maps, here, are also a good idea. This text presents a design-led approach to materials and manufacturing processes that makes use of maps: novel graphics to display the world of materials and processes in easily accessible ways. They present the properties of materials in ways that give a global view, revealing relationships between properties and enabling selection.
1.2 Material properties 3
Before Common Era 10000
Iron Copper Tin Bronze
Wood Fibres Skins
1000 1500 1800
Al-Lithium alloys Zirconium Glassy metals C-steels Aluminum Titanium Microalloyed steels Alloy steels Superalloys Magnesium Metal foams Shape-memory alloys Nano-structures High temperature polymers: PEEK
PC PTFE Acrylics Nylon PS Bakelite Epoxies PE PMMA PP Polyesters
Flint Glass Ceramics & Portland Stone Cement Refractories cement glasses Pottery
High modulus polymers Conducting polymers Diamond-like carbon
Glass fibers Carbon nano-tubes
1000 1500 1800
Figure 1.1 The development of materials over time. The materials of pre-history are those of nature. The development of thermo-chemistry, electro-chemistry and polymer chemistry enabled the production of man-made materials. Three e stone, bronze and iron e were so important that the era of their dominance is named after them.
What are ‘material properties’? Some, like density e mass per unit volume e and price e the cost per unit volume or weight e are familiar enough, but others are not, and getting them straight is essential. Think ﬁrst of those that relate to the safe carrying of loads e the mechanical properties. Mechanical Properties. A steel ruler is easy to bend elastically e ‘elastic’ means that it springs back when released. Its elastic stiffness (here, resistance to bending) is set partly by its shape e thin strips are easier to bend than thick ones e and partly by a property of the steel itself: its elastic modulus, E. Materials with high E, like steel, are intrinsically stiff; those with low E, like polyethylene, are not. Figure 1.2(b) illustrates the consequences of inadequate stiffness.
4 Chapter 1 Introduction: materials e history and character (a)
All as it should be
Not stiff enough (E too low)
Not strong enough (σy too low)
(d) Not tough enough (K1c too low)
Too dense (ρ too high)
Figure 1.2 Mechanical properties.
The steel ruler bends elastically, but if it is a good one, it is hard to give it a permanent bend. Permanent deformation relates to strength, not stiffness. The ease with which a ruler can be permanently bent depends again on its shape and on a different property of the steel e its yield strength, sy. Materials with large sy, like titanium alloys, are hard to deform permanently, even though their stiffness, coming from E, may not be high. Those with low sy, like lead, can be deformed with ease. When metals deform, they generally get stronger (it is called ‘work hardening’), but there is an ultimate limit, called the tensile strength, sts, beyond which the material fails (and the amount it stretches before it breaks is called the ductility). The hardness, H, is related to the strength, sy. High hardness gives scratch resistance and resistance to wear. Figure 1.2(c) gives an idea of the consequences of inadequate strength.
1.2 Material properties 5 So far so good. There is one more property, and it is a tricky one. If the ruler were made not of steel but of glass or of PMMA (Plexiglass, Perspex), as transparent rulers are, it is not possible to bend it permanently at all. The ruler will fracture suddenly before it acquires a permanent bend. We think of materials that break in this way as brittle, and materials that deform and resist fracture as tough. If there is no permanent deformation, then sy is not the right property. The resistance of materials to cracking and fracture is measured instead by the fracture toughness, K1c. Steels are tough e well, most are (steels can be made brittle) e they have a high K1c. Glass epitomises brittleness; it has a very low K1c. Figure 1.2(d) suggests the consequences of inadequate fracture toughness. We started with the material property density, symbol r. Density, in a ruler, is irrelevant. But for almost anything that moves, weight carries a fuel penalty, modest for automobiles, greater for trucks and trains, greater still for aircraft, and enormous in space vehicles. Minimising weight has much to do with clever design e we will get to that later e but equally, to the choice of material. Aluminium has a low density, lead a high one. If our airplane were made of lead, it would never get off the ground at all (Figure 1.2(e)). Example 1.1 Design requirements (1) You are asked to select a material for the teeth of the scoop of a digger truck. To do so, you need to prioritise the material properties that matter. What are they?
Answer. The teeth will be used in a brutal way to cut earth, scoop stones, crunch rock, often in unpleasant environments (ditches, sewers, fresh and salt water and worse), and their maintenance will be neglected. These translate into a need for high hardness, H, to resist wear, and high fracture toughness, K1c, so they don’t snap off. Does the cost of the material matter? Not much e it is worth paying for good teeth to avoid expensive downtime.
6 Chapter 1 Introduction: materials e history and character These are not the only mechanical properties, but they are the most important ones. We will meet them and the others in Chapters 4e11. Thermal Properties. The properties of a material change with temperature, usually for the worse. Its strength falls, it starts to creep e to sag slowly over time e it may oxidise, degrade or decompose (Figure 1.3(a)). This means that there is a limiting temperature called the maximum service temperature Tmax above which its use is impractical. Stainless steel has a high Tmax e it can be used up to 800 C; most polymers have a low Tmax and are seldom used above 150 C.
W High service temperature Tmax
W Low service temperature Tmax
High expansion coefficient α
Low expansion coefficient α
High conductivity λ
Low conductivity λ
High T-diffusivity a
Low T-diffusivity a
Figure 1.3 Thermal properties. Most materials expand when they are heated, but by differing amounts depending on their thermal expansion coefﬁcient, a. The expansion is small, but its consequences can be large. If, for instance, a rod is constrained and then heated, as in Figure 1.3(b), expansion forces the rod against the constraints, causing it to buckle. Railroad track buckles in this way if provision is not made to cope with it. Bridges have expansion joints for the same reason.
1.2 Material properties 7 Metals feel cold; woods feel warm. This feel has to do with two thermal properties: thermal conductivity and heat capacity. The ﬁrst, thermal conductivity, l, measures the rate at which heat ﬂows through the material when one side is hot and the other cold. Materials with high l are what you want if you wish to conduct heat from one place to another, as in cooking pans, radiators and heat exchangers; Figure 1.3(c) suggests consequences of high and low l for a cooking vessel. But low l is useful too e low l materials insulate homes, reduce the energy consumption of refrigerators and freezers, and enable space vehicles to re-enter the Earth’s atmosphere. These applications have to do with long-time, steady heat ﬂow. When time is limited, that other property e heat capacity, Cp e enters the picture. It measures the amount of heat required to make the temperature of a material rise by a given amount. High-heat capacity materials e copper, for instance e require a lot of heat to change their temperature; low-heat capacity materials, like polymer foams, take much less. Steady heat ﬂow has, as we have said, to do with thermal conductivity. There is a subtler property that describes what happens when heat is ﬁrst applied. Think of lighting the gas under a cold slab of material with a scoop of ice cream on top, as in Figure 1.3(d). An instant after ignition, the bottom surface is hot, but the rest is cold. After a time, the middle gets hot; then later still, the top begins to warm up, and only then does the ice cream start to melt. How long does this take? For a given thickness of slab, the time is inversely proportional to the thermal diffusivity, a, of the material of the slab. It differs from the conductivity because materials differ in their heat capacity e in fact, a is proportional to l/Cp. Example 1.2 Design requirements (2) You are asked to select a material for energy-efﬁcient cookware. What thermal property are you looking for? And, apart from the mechanical properties discussed earlier, what other material behaviour will be important?
Answer. To be energy-efﬁcient, the pan must have a high thermal conductivity, l, to transmit and spread the heat well. Also, it mustn’t contaminate the food e that is, it must resist corrosion by anything that might be cooked in it e including hot, salty water, dilute acids (acetic acid e vinegar, for example) and mild alkalis (baking soda).
There are other thermal properties e we’ll meet them in Chapters 12 and 13. Next, we follow up on corrosion and other aspects of the operating environment.
8 Chapter 1 Introduction: materials e history and character Chemical properties. Products often encounter hostile environments and are exposed to corrosive ﬂuids or hot gases or radiation. Damp air is corrosive. So is water; the sweat of your hand is particularly corrosive, and of course, there are far more aggressive environments than these. If the product is to survive for its design life, it must be made of materials e or at least coated with materials e that can tolerate the surroundings in which it operates. Figure 1.4 illustrates some of the commonest of these: fresh and salt water, acids and alkalis, organic solvents, oxidising ﬂames and ultra-violet radiation. We regard the intrinsic resistance of a material to each of these as material properties, measured on a scale of 1 (very poor) to 5 (very good). Chapter 14 deals with material durability.
Acids and alkalis
Figure 1.4 Chemical properties: resistance to water, acids, alkalis, organic solvents, oxidation and
Electrical, magnetic and optical properties. Without electrical conduction, we would lack the easy access to light, heat, power, control and communication that we take for granted. Metals conduct well e copper and aluminium are the best of those that are affordable. But conduction is not always a good thing. Fuse boxes, switch casings, and the suspensions
1.2 Material properties 9 for transmission lines all require insulators that must also carry some load, tolerate some heat, and survive a spark if there is one. Here the property we want is resistivity, re, the inverse of electrical conductivity, ke. Most plastics and glass have high resistivity (Figure 1.5(a)) e they are used as insulators e though, by special treatment, they can be made to conduct a little.
Low resistivity ρe
High resistivity ρe
Low dielectric response
High dielectric response
'Hard' magnetic behiour
Soft magnetic behaviour
Figure 1.5 Electrical, magnetic and optical properties.
Figure 1.5(b) suggests further electrical properties: the ability to allow the passage of microwave radiation, as in the radome, or to reﬂect it, as in the passive reﬂector of the boat. Both have to do with dielectric properties, particularly the dielectric constant εD. Materials with high εD respond to an electric ﬁeld by shifting their electrons about, even re-orienting their molecules; those with low εD are immune to the ﬁeld and do not respond. We explore this and other electrical properties in Chapter 15. Electricity and magnetism are closely linked. Electric currents induce magnetic ﬁelds; a moving magnet induces, in any nearby conductor, an electric current. The response of most
10 Chapter 1 Introduction: materials e history and character materials to magnetic ﬁelds is too small to be of practical value. But a few e ferro-magnets and ferri-magnets e have the capacity to trap a magnetic ﬁeld permanently. These are called ‘hard’ magnetic materials because, once magnetized, they are hard to demagnetize. They are used as permanent magnets in headphones, motors and dynamos. Here the key property is the remanence, a measure of the intensity of the retained magnetism. In contrast, the ‘soft’ magnetic materials are easy to magnetise e they are the materials of transformer cores. They have the capacity to conduct a magnetic ﬁeld, but not retain it permanently (Figure 1.5(c)). For these, a key property is the saturation magnetisation, which measures how large a ﬁeld the material can conduct. These materials and properties we meet again in Chapter 16. Materials respond to light as well as to electricity and magnetism e hardly surprising, since light itself is an electro-magnetic wave. Materials that are opaque reﬂect light; those that are transparent refract it. Some are opaque to all wavelengths (colours); others absorb speciﬁc wavelengths while allowing others to pass freely (Figure 1.5(d)). These are explored in more depth in Chapter 17.
Example 1.3 Design requirements (3) What are the essential and the desirable requirements of materials for eyeglass (spectacle) lenses?
Answer. Essentials: Optical clarity is paramount e a material with optical quality transparency is the ﬁrst requirement. It is essential that it can moulded or ground with precision to the required optical prescription. And it must resist sweat and be sufﬁciently scratch-resistant to cope with normal handling. Desirables: A high refractive index and a low density allow thinner, and thus lighter, lenses. And a material that is cheap allows either a lower cost for the consumer or a greater proﬁt margin for the maker.
Environmental properties. Making, shaping, joining and ﬁnishing materials consumes nearly one-third of global energy demand. The associated emissions are already a cause for international concern, and demand for material extraction and processing is likely to double in the next 40 years. It’s important, therefore, to understand the environmental properties of materials and to seek ways to use them more sustainably than
1.2 Material properties
we do now. Chapter 20 introduces the key ideas of material life-cycle analysis, material efﬁciency and sustainability, all of which are central to the way we will use materials in the future. Three quantities describe the environmental character of a material (Figure 1.6):
· · ·
embodied energy e the energy required to produce 1 kg of the material, including that used to mine and reﬁne the feedstocks, and that required to reﬁne or synthesise these into usable material stock; carbon footprint e the mass of carbon released due to the production of 1 kg of the material (or, strictly, the carbon-equivalent release e a way of including the global warming effect of all the gaseous emissions); water demand e the volume of water that is drawn from usable sources and not returned to them during the production of 1 kg of material.
Embodied energy (MJ/kg)
Carbon footprint (kg/kg)
1 kg Water demand (Litres/kg) MFA ‘17
Figure 1.6 The environmental (eco) properties of materials.
12 Chapter 1 Introduction: materials e history and character Example 1.4 Design requirements (4) What are the essential and the desirable requirements of materials for a single-use (disposable) water bottle that does minimal environmental harm?
Answer. Essentials: Health aspects come ﬁrst: the material of the bottle must be non-toxic and able to be processed in a way that leaves no contaminants. Being disposable, the bottle must be cheap, constraining the choice of material and process to those that are the least expensive. Desirables: The material of the bottle should be recyclable and, if possible, be biodegradable. It makes handling easier if the material is light and it is not brittle, although widely used glass bottles meet neither criterion.
The performance of a component is limited by the properties of the materials of which it is made. To achieve a desired level of performance, the values of the design-limiting properties must meet certain targets e those that fail to do so are not suitable. In the cartoon of Figure 1.2, stiffness, strength, and toughness are design-limiting e if any one of them were too low, the plane wouldn’t ﬂy. In the design of power transmission lines, electrical resistivity is design-limiting; in the design of a camera lens, it is optical qualities that constrain the design. Materials are chosen by identifying the design-limiting properties and applying limits to them and screening out materials that do not meet the limits (Chapter 3). Processes, too, have properties, although we have not met them yet. These, too, can be design-limiting, leading to a parallel scheme for choosing viable processes (Chapters 18 and 19).
Summary and conclusions
Engineering design depends on materials that are shaped, joined, and ﬁnished by processes. Design requirements deﬁne target values for the design-limiting properties. A material is chosen because it has properties that meet these targets and is compatible with the processes that will be used to shape, join, and ﬁnish it. This chapter introduced some of the design-limiting properties: physical properties like density; mechanical properties like modulus and yield strength; functional properties: those describing the thermal, electrical, magnetic and optical behaviour; chemical properties: those determining how the material reacts with its environment; and eco-properties: those that relate to the impact the production of the material has on the world around it. We examine these in more depth in the chapters that follow, but turn next to the materials themselves: the families, the classes and the members.
The history and evolution of materials Delmonte, J. (1985). Origins of Materials and Processes. Pennsylvania, USA: Technomic Publishing Company. ISBN 87762-420-8. (A compendium of information about materials in engineering, documenting the history.) Hummel, R. (2004). Understanding Materials Science: History, Properties, Applications (2nd ed.). New York, USA: Springer Verlag. ISBN 0-387-20939-5. Miodownik, M. (2014). Stuff Matters. London, UK: Penguin. ISBN 978-0-241-95518-5. (An engaging exposition of the diversity of uses of materials, covering modern innovations and their historical evolution.) Singer, C., Holmyard, E. J., Hall, A. R., Williams, T. I., & Hollister-Short, G. (Eds.), (1954e2001). A History of Technology, 21 volumes. Oxford, UK: Oxford University Press. ISSN 0307e5451. (A compilation of essays on aspects of technology, including materials.) Tylecoate, R. F. (1992). A History of Metallurgy (2nd ed.). London, UK: The Institute of Materials. ISBN 0-904357-066. (A total-immersion course in the history of the extraction and use of metals from 6000 BC to 1976, told by an author with forensic talent and a love of detail.)
Use Google to research the history and uses of one of the following materials:
·· ·· ·
Tin Glass Cement Titanium Carbon ﬁbre
Present the result as a short report of about 100e200 words (roughly half a page).
14 Chapter 1 Introduction: materials e history and character
What is meant by the design-limiting properties of a material in an application?
There have been many attempts to manufacture and market plastic bicycles. All have been too ﬂexible. Which design-limiting property is insufﬁciently large?
What, in your judgment, are the design-limiting properties for the material for the blade of a knife that will be used to gut ﬁsh?
What, in your judgment, are the design-limiting properties for the material of an oven glove?
What, in your judgment, are the design-limiting properties for the material of an electric lamp ﬁlament?
A material is needed for a tube to carry fuel from the fuel tank to the carburettor of a motor mower. The design requires that the tube can bend and that the fuel be visible. List what you would think to be the designlimiting properties.
A material is required as the magnet for a magnetic soap holder. Soap is mildly alkaline. List what you would judge to the design-limiting properties.
The cases in which most CDs are sold have an irritating way of cracking and breaking. Which design-limiting property has been neglected in selecting the material of which they are made?
List three applications that, in your judgment, need high stiffness and low weight.
List three applications that, in your judgment, need optical-quality glass.
List three applications that require high thermal conductivity.
List three applications that require low thermal expansion. Think of things that lose accuracy or won’t work if they distort.
Aluminium has a high carbon footprint e its value is 13.1 kg/kg. What does this mean?
Family trees: organising materials and processes
Lego is made of ABS, a thermoplastic polymer.
Chapter contents 2.1 2.2 2.3 2.4 2.5 2.6
Introduction and synopsis Organising materials: the materials tree Organising processes: the process tree Processeproperty interaction Material property charts Computer-aided information sources for materials and processes 2.7 Summary and conclusions 2.8 Further reading 2.9 Exercises
Copyright Ó 2019 Elsevier Ltd. All rights reserved. https://doi.org/10.1016/B978-0-08-102376-1.00002-0
16 16 19 22 23 25 26 26 27
16 Chapter 2 Family trees: organising materials and processes
Introduction and synopsis
A successful product e one that performs well, gives pleasure to the user, and is good value for money e uses the best materials for the job and fully exploits their potential and characteristics. The families of materials e metals, polymers, ceramics and so forth e are introduced in Section 2.2. But it is not, in the end, a material that we seek in design; it is a certain proﬁle of properties e the one that best meets the needs of the design. The members of each family have characteristics in common e a sort of ‘family likeness’ e which is useful when deciding which family offers the best starting point for a given design. Section 2.2 explains how this enables a classiﬁcation scheme for materials, allowing information about them to be organised. Choosing a material is only half the story. The other half is the choice of a process route to shape, join and ﬁnish it. Section 2.3 introduces process families and their attributes. Choice of material and process are tightly coupled: a given material can be processed in some ways but not others, and a given process works with some materials but not with others. On top of that, the act of processing can change, even create, the properties of the material (Section 2.4). Process families, too, exhibit family likenesses e commonality in the materials that members of a family can handle, or the shapes they can make. Section 2.3 introduces a classiﬁcation for processes that parallels that for materials. Family likenesses are most strikingly seen in material property charts, which are a central feature of this book (Section 2.5). These are charts with material properties as axes showing the location of the families and their members. Materials have many properties. They can be thought of as the axes of a ‘materialeproperty’ space e each chart is a two-dimensional slice through this space. Each material family occupies a discrete part of this space, distinct from the other families. The charts give an overview of materials and their properties; they reveal aspects of the science underlying the properties, and they provide a powerful tool for materials selection. Process attributes can be treated in a similar way to create process attribute charts. We leave these for Chapter 18. The classiﬁcation systems of Sections 2.2 and 2.3 provide a structure for computer-based information management, which is introduced in Section 2.6. In common with the rest of the book, the chapter ends with a summary, further reading and exercises.
Organising materials: the materials tree
Classifying materials. It is conventional to classify the materials of engineering into the six broad families shown in Figure 2.1: metals, polymers, elastomers, ceramics, glasses and hybrids e composite materials made by combining two or more of the others. There is sense in this: the members of a family have certain features in common e similar properties, similar processing routes and, often, similar applications. Figure 2.2 illustrates how the families are expanded to show classes, sub-classes and members, each of which is characterised by a set of attributes: its properties. As an example, the Materials Universe contains the family Metals, which in turn contains the class Aluminium alloys, which contains the sub-class the 6000 series, within which we ﬁnd the particular member Alloy 6061. It, and every other member of the Universe, is characterised by a set of attributes that include not only the properties mentioned in Chapter 1, but also its processing characteristics and its typical applications. We call this its property proﬁle.
2.2 Organising materials: the materials tree
Steels Cast irons Al-alloys
Metals Cu-alloys Zn-alloys Ti-alloys
PE, PP, PET, PC, PS, PEEK PA (nylons)
Aluminas Silicon carbides
Silicon nitrides Zirconias
Hybrids Segmented structures, Lattices and foams
Isoprene Neoprene Butyl rubber
Soda glass Borosilicate glass
Glasses Silica glass Glass-ceramics
Polyesters Phenolics Epoxies
Elastomers Natural rubber Silicones EVA MFA ‘17
Figure 2.1 (Left) The menu of engineering materials. The basic families of metals, ceramics, glasses, polymers and elastomers can be combined in various geometries to create hybrids. (Right) Examples of each family.
Attributes Density Al 6061
1000 2000 3000 4000 5000 6000 7000 8000
Mechanical props. Density 6013 6060 6061 6063 6082 6151 6463
Thermal props. Mechanical props. Electrical Thermal props. props. Optical props. Electrical props. Corrosion props. Optical props. Corrosion props. --Documentation specific ----general specific -- general
Figure 2.2 The taxonomy of the universe of materials and their attributes. Computer-based selection software stores data in a hierarchical structure like this.
18 Chapter 2 Family trees: organising materials and processes As already mentioned, the members of one family have certain characteristics in common. Here, brieﬂy, are some of them. Metals have relatively high stiffness, measured by the elastic modulus E. Most, when pure, are soft and easily deformed, meaning that the yield strength sy is low. They can be made stronger by alloying and by mechanical and heat treatment, increasing sy, but they remain ductile, allowing them to be formed by deformation processes like rolling or forging. And, broadly speaking, they are tough, with a usefully high fracture toughness, K1c. They are good electrical and thermal conductors. But metals have weaknesses too: they are reactive, and most corrode rapidly if not protected. Ceramics are non-metallic, inorganic solids, like porcelain or alumina e the material of the insulator casing of the spark plug in a petrol engine. They have many attractive features: they are stiff, hard and abrasion resistant; they retain their strength at high temperatures; and they resist corrosion well. Most are good electrical insulators. They, too, have their weaknesses: unlike metals, they are brittle, with low K1c. giving ceramics a low tolerance for stress concentrations (like holes or cracks) or for high contact stresses (at clamping points, for instance). Glasses are non-crystalline (‘amorphous’) solids, a term explained more fully in Chapter 4. The commonest are the soda-lime and boro-silicate glasses familiar as bottles and Pyrex ovenware, but there are many more. The lack of crystal structure suppresses plasticity, so, like ceramics, glasses are hard and remarkably corrosion resistant. They are excellent electrical insulators, and of course, they are transparent to light. But like ceramics, they are brittle and vulnerable to stress concentrations. Polymers are organic solids based on long-chain molecules of carbon atoms (or, in a few, silicon). Polymers are light e their densities r are less than those of the lightest metals. Compared with other families, they are ﬂoppy, with moduli E that are roughly 50 times less than those of metals. But they can be strong, and because of their low density, their strength per unit weight is comparable to that of metals. Their properties depend on temperature, so a polymer that is tough and ﬂexible at room temperature may be brittle at the 4 C of a household freezer, yet turn rubbery at the 100 C of boiling water. Few have useful strength above 150 C. If these aspects are allowed for in the design, the many advantages of polymers can be exploited. They are easy to shape (which is why they are called ‘plastics’). Complicated parts performing several functions can be moulded from a polymer in a single operation. Their properties are well suited for components that snap together, making assembly fast and cheap. And by accurately sizing the mould and pre-colouring the polymer, no ﬁnishing operations are needed. Good design exploits these properties. Elastomers, the material of rubber bands and running shoes, are polymers with the unique property that their stiffness, measured by E, is extremely low e 500 to 5000 times less than those of metals e and they can be stretched to many times their starting length yet recover their initial shape when released. Despite their low stiffness, they can be strong and tough e think of car tires. Hybrids are combinations of two (or more) materials in an attempt to get the best of both. Glass- and carbon-ﬁbre reinforced polymers (GFRP and CFRP) are hybrids; so, too, are sandwich structures, foams and laminates. And almost all the materials of nature e wood, bone, skin, leaf e are hybrids. Bone, for instance, is a mix of collagen (a polymer) with hydroxyapatite (a mineral). Hybrid components are expensive, and they are relatively difﬁcult to form and join. So despite their attractive properties, the designer will use them only when the added performance justiﬁes the added cost. Today’s growing emphasis on high performance, light weight and fuel efﬁciency provide increasing drivers for their use.
2.3 Organising processes: the process tree
Organising processes: the process tree
A process is a method of shaping, joining or ﬁnishing a material. Casting, injection moulding, fusion welding and electro-polishing are all processes, and there are hundreds of them to choose from (Figures 2.3 and 2.4). It is important to select the right process route at an early stage in the design before the cost penalty of making changes becomes large. The choice for a given component depends on the material of which it is to be made; on its shape, dimensions and precision; and on how many are to be made e in short, on the design requirements.
Material stock Primary shaping Casting methods:
Sand, Die, Investment
Injection, Compression, Blow molding
Rolling, Forging, Drawing,
Sintering, HIPing, Slip casting
Hand lay-up, Filament wind, RTM
Laser deposit, Electro-form, Spray-form
Cut, turn, plane drill, grind
Quench, temper, age-harden
Figure 2.3 The classes of process. The ﬁrst row contains the primary shaping processes; below lie the secondary processes of machining and heat treatment, followed by the families of joining and surface treatment processes. The choice of material limits the choice of process. Polymers can be moulded; other materials cannot. Ductile materials can be forged, rolled and drawn, but those that are brittle must be shaped in other ways. Materials that melt at modest temperatures to low-viscosity liquids can be cast; those that do not have to be processed by other routes. Shape, too, inﬂuences the
20 Chapter 2 Family trees: organising materials and processes Material stock Primary shaping
Friction stir welding
Figure 2.4 Examples of the families and classes of manufacturing processes. The arrangement follows the general pattern of Figure 2.3.
2.3 Organising processes: the process tree
choice of process. Slender shapes can be made easily by rolling or drawing but not by casting. Hollow shapes cannot be made by forging, but they can by casting or moulding. Classifying processes Manufacturing processes are organised under the headings shown in Figure 2.3. Primary processes create shapes. The ﬁrst row lists six primary forming processes: casting, moulding, deformation, powder methods, methods for forming composites, and special methods including additive manufacture. Secondary processes modify shapes or properties; here they are shown as machining, which adds features to an already shaped body, and heat treatment, which enhances bulk properties. Below these come joining, and, ﬁnally, surface treatment. Figure 2.4 illustrates some of these; it is organised in the same way as Figure 2.3. The ﬁgure is a sort of ﬂow chart: a progression through a manufacturing route. It should not be treated too literally; the order of the steps can be varied to suit the needs of the design. Information about processes can be arranged in a hierarchical classiﬁcation like that used for materials, giving each process a place. Figure 2.5 shows part of the hierarchy. The Process Universe has three families: shaping, joining and surface treatment. In this ﬁgure, the shaping family is expanded to show classes: casting, deformation, moulding and so on. One of these, moulding, is again expanded to show its members: rotation moulding, blow moulding, injection moulding and so forth. Each process is characterised by a set of attributes: the materials it can handle, the shapes it can make, their size, precision and an economic batch size (the number of units that it can make most economically).
Attributes Injection molding
Compression Rotation Transfer Injection Foam Extrusion Resin casting Thermoforming Blow molding
Density Material Mechanical props. Shape Thermal props. Size range Electrical props.
Min. batch size
Cost model Documentation -- specific A process record
Figure 2.5 The taxonomy of the universe of processes with part of the shaping family expanded. Each member is characterised by a set of attributes. Processes selection involves matching these to the requirements of the design. The other two families are partly expanded in Figure 2.6. There are three broad classes of joining process: adhesives, welding and fasteners. In this ﬁgure, one of them, welding, is expanded to show its members. As before, each member has attributes. The ﬁrst is the material
22 Chapter 2 Family trees: organising materials and processes or materials that the process can join. After that, the attribute list differs from that for shaping. Here the geometry of the joint and the way it will be loaded are important, as are requirements that the joint can or cannot be disassembled, be watertight or be electrically conducting. Universe
Member Braze Solder Arc Gas e -beam Hot gas Hot bar...
Attributes Gas welding Material Material Joint geometry Joint geometry Size Range Size Range Section thickness Section thickness Relative cost ... Relative cost ... Supporting information Documentation
Anodising Polish Paint Finishing
Coat Print Texture ...
Electroplate Anodise Powder coat Metallise...
Material Material Purpose Purposeof oftreatment treatment Coating Coatingthickness thickness Surface Surfacehardness hardness Relative cost ... Relative cost ... Documentation Supporting information
Figure 2.6 The taxonomy of the process kingdom again, with the families of joining and surface treatment partly expanded. The lower part of the ﬁgure expands the family of surface treatment processes. Some of the classes it contains are shown; one, coating, is expanded to show some of its members. Finishing adds cost; the only justiﬁcation for applying a ﬁnishing process is that it hardens, protects or decorates the surface in ways that add value. We will return to process selection in Chapter 18, exploring how far a database of processes and their attributes can take us in design.
Processing can change properties. If you deform a metal, it gets harder (‘work hardening’); if you then heat it up, it gets softer again (‘annealing’). If polyethylene (PE) e the stuff of plastic bags e is drawn to a ﬁbre, its strength is increased by a factor of ﬁve because the polymer chains are drawn into alignment. Soft, stretchy rubber is made hard and brittle by vulcanising. Glass can be chemically and thermally treated to give it the impact resistance to withstand a projectile (‘bulletproof glass’). And composites like carbon ﬁbre-reinforced epoxy have no useful properties at all until processed e prior to processing, they are just a soup of resin and a sheaf of ﬁbres.
2.5 Material property charts
Joining, too, changes properties. Fusion welding involves the local melting and re-solidifying of the faces of the parts to be joined. As you might expect, the weld zone has properties that differ from those of the material far from the weld e usually worse. Surface treatments, by contrast, are generally chosen to improve properties: electroplating to improve corrosion resistance, or carburising to improve wear. We return to processeproperty interactions in depth in Chapter 19, but many examples of the effect of processing on properties will be encountered on the way.
Material property charts
Data sheets for materials list their properties, but they give no perspective and present no comparisons. The way to achieve these is to plot material property charts. They are of two types: bar charts and bubble charts. A bar chart is simply a plot of one property for all the materials of the Universe, or a subset of them. Figure 2.7 shows an example: it is a bar chart for modulus E. The largest is more than 10 million times greater than the smallest e many other properties have similarly large ranges e so it makes sense to plot them on logarithmic1, not linear scales, as here. The length of each bar shows the range of the property for each material, here segregated by family. The differences between the families now become apparent. Metals and ceramics have high moduli. Those of polymers are smaller, by a factor of about 50, than those of metals, while those of elastomers are some 500 times smaller still.
Low alloy steel
WC BC SiC
High carbon steel Stainless steel
Modulus, E (GPa)
Cu-alloys Zn-alloys Al-alloys Mg-alloys
Glass ceramic Ceramic Acetal, Acetal, POM POM Polyester, rigid PS ABS ABS PC PP
CFRP GFRP Plywood
Silica glass Soda-Limeglass Soda-lime glass
Wood ll to grain Paper, Cardboard
PTFE Ionomer Ionomer EVA Polyurethane Natural Rubber (NR) Neoprene
Metals Metals Metals
Polymers Polymers Polymers
Ceramics Ceramics Ceramics & glass
Hybrids Hybrids Composites
Figure 2.7 A bar chart of modulus E. It reveals the difference in stiffness between the families. 1
Logarithmic means that the scale goes up in constant multiples, usually of 10. We live in a logarithmic world e our senses, for instance, all respond in this way.
24 Chapter 2 Family trees: organising materials and processes Example 2.1 Use of bar charts In a cost-cutting exercise, a designer suggests that certain die-cast zinc parts could be replaced by cheaper moulded polyethylene (PE) parts with the same shape. Another member of the team expresses concern that the PE replacement might be too ﬂexible. By what factor will the stiffness of the part change if the substitution is made? Answer. The stiffness of two parts with the same shape, but made of different materials, will differ by the same factor as the moduli of the materials. The bar chart of Figure 2.7 shows that the modulus of PE is less, by a factor of about 100, than that of zinc alloys. The concern is a real one.
More information is packed into the picture if two properties are plotted to give a bubble chart, as in Figure 2.8, here showing modulus E and density r. As before, the scales are logarithmic. Now the families are more distinctly separated: all metals lie in the reddish zone near the top right; all polymers lie in the dark-blue envelope in the centre, elastomers in the
Modulus - Density
Modulus, E (GPa)
Steels Ni alloys Ti alloys
.1 =0 3 E/ρ g/m ) (k / a GP
PS PP PE
Lead alloys Zinc alloys PEEK Concrete PET Epoxies
Rigid polymer foams
Families occupy discrete fields
WC W alloys
Glass Mg alloys GFRP
Al alloys CFRP
SiC Si3N4 B4C
Foams Silicone elastomers
10-3 Flexible polymer foams
Figure 2.8 A bubble chart of modulus and density. Families occupy discrete areas of the chart.
2.6 Computer-aided information sources for materials and processes
lighter blue envelope below, ceramics in the yellow envelope at the top. Each family occupies a distinct, characteristic ﬁeld. Within these ﬁelds, individual materials appear as smaller ellipses. Example 2.2 Use of bubble charts Steel is stiff (big modulus E) but heavy (big density r). Aluminium alloys are less stiff but also less dense. One criterion for lightweight design is a high value of the ratio E/r, deﬁning materials that have a high stiffness per unit weight. Does aluminium have a signiﬁcantly higher value of E/r than steel? What about carbon ﬁbre-reinforced polymer (CFRP)? Answer. The E/r chart of Figure 2.8 can answer the question in seconds. All three materials appear on it. Materials with equal values of E/r lie along a line of slope 1 e one such line is shown. Materials with high E/r lie towards the top left, those with low values towards the bottom right. If a line with the same slope is drawn through Al alloys on the chart, it passes almost exactly through steels: the two materials have almost the same value of E/r, a surprise when you think that aircraft are made of aluminium, not steel (the reason for this will become clear in Chapter 5). CFRP, by contrast, has a much higher E/r than either aluminium or steel.
Material property charts like these are a core tool used throughout this book:
· · ·
They give an overview of the physical, mechanical and functional properties of materials, presenting the information about them in a compact way. They reveal aspects of the physical origins of properties, a help in understanding the underlying science. They become a tool for optimised selection of materials to meet given design requirements, and they help us understand the use of materials in existing products.
Computer-aided information sources for materials and processes
Computer-based products are now available to manage information about materials and processes, making it easier to ﬁnd data and to manipulate it. They vary greatly in their breadth of coverage and the audience at which they are aimed. We end this chapter with a list of some of these (Table 2.1).
26 Chapter 2 Family trees: organising materials and processes Table 2.1 Computer-based resources for materials information ASM International (http://www.asminternational.org/online-databases-journals) ASM offers an extensive library of micrographs, phase diagrams, crystallographic structures, and failure case studies. CES EduPack (http://www.grantadesign.com/education/). A comprehensive suite of databases for materials and processes with editions for general engineering, aerospace, polymers engineering, materials science, environmental design and industrial design. It includes powerful search, selection and eco-auditing tools. (The property charts in this book were made with this software). DoITPoMS (https://www.doitpoms.ac.uk/) A free teaching resource created by the Materials Science Department of Cambridge University. F*A*C*T (http://www.crct.polymtl.ca/fact/) Thermodynamic data for engineering alloys and compounds. Matbase (www.matbase.com). A database of the technical properties of materials, originally from the Technical University of Denmark. Matdata (www.matdata.com). A well-documented database of the properties of metals. Materia (www.materia.nl). A database aimed at industrial design, with images of some 2000 products. Material Connexion (www.materialconnexion.com). A materials library emphasising industrial design with records for some 7000 materials, each with an image, a description and a supplier. MatWeb (www.matweb.com). A large database of the engineering properties of materials, drawn from suppliers’ data sheets.
Summary and conclusions
Classiﬁcation is the ﬁrst step in creating an information management system for materials and processes. In it the records for the members of each Universe are indexed, so to speak, by their position in the tree-like hierarchies of Figures 2.2, 2.5 and 2.6. Each record has a unique place, making retrieval easy. There are six broad families of materials for mechanical design: metals, ceramics, glasses, polymers, elastomers, and hybrids that combine the properties of two or more of the others. Processes, similarly, can be grouped into families: those that create shape, those that join, and those that modify the surface to enhance its properties or to protect or decorate it. This structure forms the basis of computer-based materials selection systems, now widely available. Property charts are a unique and powerful way of presenting data for materials e two examples appeared in this chapter. They become one of the central features of the chapters that follow.
Askeland, D. R., Phulé, P. P., & Wright, W. J. (2010). The science and engineering of materials (6th ed.). Toronto, Canada: Thomson. ISBN: 9780495296027. (A well-established materials text that deals well with the science of engineering materials.) Bralla, J. G. (1998). Design for manufacturability handbook (2nd ed.). New York, USA: McGraw-Hill. ISBN: 0-0007139X. (Turgid reading, but a rich mine of information about manufacturing processes.)
Budinski, K. G., & Budinski, M. K. (2010). Engineering materials, properties and selection (9th ed.). NY, USA: Prentice Hall. ISBN: 978-0-13-712842-6. (Like Askeland, this is a well-established materials text that deals well with both material properties and processes.) Callister, W. D., & Rethwisch, D. G. (2014). Materials science and engineering: An introduction (9th ed.). New York, USA: John Wiley & Sons. ISBN: 978-1-118-54689-5. (A well-established text taking a science-led approach to the presentation of materials teaching.) Dieter, G. E. (1999). Engineering design, a materials and processing approach (3rd ed.). New York, USA: McGraw-Hill. ISBN: 9-780-073-66136-0. (A well-balanced and respected text focussing on the place of materials and processing in technical design.) Farag, M. M. (2013). Materials and process selection for engineering design (3rd ed.). London, UK: CRC Press, Taylor and Francis. ISBN: 9-781-4665640-9. (A Materials Science approach to the selection of materials.) Lewis, G. (1990). Selection of engineering materials. NJ, USA: Prentice-Hall, Englewood Cliffs. ISBN: 0-13-802190-2. (A text on material selection for technical design, based largely on case studies.) Shackelford, J. F. (2014). Introduction to materials science for engineers (8th ed.). NJ, USA: Prentice Hall. ISBN: 978-0133789713. (A well-established materials text with a design slant.) Thompson, R. (2007). Manufacturing processes for design professionals. London, UK: Thames and Hudson. ISBN: 978-0-500-51375-0. (A beautifully produced and lavishly illustrated introduction to materials and to forming, joining and ﬁnishing processes.)
Material properties from experience. List the six main classes of engineering materials. Use your own experience to rank them approximately: (a) by stiffness (modulus, E). A sheet of a material that has a high modulus is hard to bend when in the form of sheet. A sheet of material with a low modulus is ﬂoppy. (b) by thermal conductivity (l). Materials with high conductivity feel cold when you pick them up on a cold day. Materials with low conductivity may not feel warm, but they don’t freeze your hands as quickly as those with high conductivity.
Classiﬁcation (1). A good classiﬁcation looks simple e think, for instance, of the periodic table of the elements. Creating it in the ﬁrst place, however, is not so simple. This chapter introduced two hierarchical classiﬁcations that work, meaning that every member of the classiﬁcation has a unique place in it, and any new member can be inserted into its proper position without disrupting the whole. This exercise and the three that follow ask you to create hierarchical classiﬁcations following the Universe e Family e Class e Member pattern. Make sure that each level of the hierarchy properly contains all those below it. There may be more than one way to do this, but one is usually better than the others. Test it by thinking how you would use it to ﬁnd the information you want. Classify the different ways in which sheets of paper can be attached to each other, temporarily or permanently. The Universe is ‘Paper attachment’.
28 Chapter 2 Family trees: organising materials and processes Create the Family level by listing the distinctly different mechanisms for attachment. Then add the Class level e the distinct subsets of each family. Exercise E2.3
Classiﬁcation (2). In how many ways can wood be treated to change its surface appearance and feel? The Universe is ‘Wood surface treatment’. Develop the classiﬁcation further using distinct ﬁnishing techniques at the Family level and subsets of these at the Class level based on your own observation of wood products.
Classiﬁcation (3). You run a bike shop that stocks bikes of many types (children’s bikes, street bikes, mountain bikes, racing bikes, folding bikes, etc.), prices and sizes. You need a classiﬁcation system to allow customers to look up your bikes on the internet. The Universe is ‘Bicycles’. Develop the Family and Class levels of the classiﬁcation and note the further levels of hierarchy that would be needed to uniquely classify a given bike.
Classiﬁcation (4). You are asked to organise the inventory of fasteners in your company. Fasteners come in various sizes and materials, and there is more than one type. What would be a logical hierarchical classiﬁcation for the Universe of Fasteners?
Shaping. What is meant by a shaping process? The four products below were shaped using the following processes: A: B: C: D:
Additive manufacturing Casting Forging and milling Turning
By thinking about characteristics of the shape being made, and doing a bit of research, can you match the product to the processes? (We return to this in Chapter 18.)
Joining. The four products below illustrate the four joining methods: A: B: C: D:
Adhesives Arc welding Brazing Threaded fasteners
Can you match the product to the processes, identifying features that conﬁrm your choice? (More on this in Chapters 18 and 19.)
Surface treatment. The four products below illustrate the four surface treatment methods: A: B: C: D:
Anodising Chrome plating Enamelling Powder coating
Can you match the product to the processes from the appearance of the product?
Use of property charts (1). Examine the Modulus chart of Figure 2.7. By what factor, on average, are polymers less stiff than metals? By what factor is neoprene less stiff than polypropylene (PP)?
Use of property charts (2). Wood is a natural polymer, largely made up of cellulose and lignin, and they, like engineering polymers, are almost entirely hydrogen, carbon, oxygen and a little nitrogen. Has nature devised a cocktail of these elements that has a higher modulus than any bulk synthetic polymer? Engineering polymers and woods appear on the charts of Figures 2.7 and 2.8. Use either one to answer the question.
Use of property charts (3). Windows can be made of glass (house windows), polycarbonate (PC) (conservatory roofs) or poly-methyl-methacrylate, PMMA (aircraft cockpit canopies). Would a glass window be more ﬂexible than a replacement of the same thickness made of polycarbonate? Would it be heavier? Use the bubble chart of Figure 2.8 to ﬁnd out.
30 Chapter 2 Family trees: organising materials and processes
Use of property charts (4). Do zinc alloys have a higher speciﬁc stiffness E/r than polypropylene (PP)? Use the bubble chart of Figure 2.8 to ﬁnd out (E is the modulus; r is the density). Contours of E/r are diagonal contours on the axes of this ﬁgure e one is shown at E/r ¼ 0.1 GPa/(kg/m3). Draw a line parallel to this one, passing through zinc alloys. If PP lies above this line, it has higher E/r; if below, it has a lower value.
Strategic thinking: matching material to design
Images embodying the concepts described in the text: pull, geared pull, shear and pressure. Image courtesy of A-Best Fixture Co., 424 West Exchange Street, Akron, Ohio, 44302, USA.
Chapter contents 3.1 3.2 3.3 3.4 3.5 3.6 3.7 3.8
Introduction and synopsis The design process Material and process information for design The strategy: translation, screening, ranking and documentation Examples of translation Summary and conclusions Further reading Exercises
Copyright Ó 2019 Elsevier Ltd. All rights reserved. https://doi.org/10.1016/B978-0-08-102376-1.00003-2
32 32 35 37 40 43 44 44
32 Chapter 3 Strategic thinking: matching material to design
Introduction and synopsis
This chapter develops a strategy for selecting materials and processes that is design-led; that is, it uses the requirements of the design as inputs. To do so, we must ﬁrst look at the design process itself. This chapter introduces some of the vocabulary of design, the stages in its implementation, and the ways in which materials selection links with these. Design starts with a market need. The need is analysed, expressing it as a set of design requirements. Ways to meet these requirements (Concepts) are sought, developed (Embodied) and reﬁned (Detailed) to give a product speciﬁcation. The choice of material and process evolves in parallel with this process. With this background, we can develop the selection strategy. It involves four steps: translation, screening, ranking and documentation. These steps are explained, and the ﬁrst, that of translation, is illustrated with examples.
The design process
Original design starts from a new concept and develops the information necessary to implement it. Evolutionary design (or redesign) starts with an existing product and seeks to change it in ways that increase its performance, reduce its cost, or both. Original design starts from scratch, exploiting new ideas or working principles (the vinyl disk, the audio tape, the compact disc, the MP3 player were all, in their day, completely new). Original design can be stimulated by new materials. High-purity silicon enabled the transistor; high-purity glass, the optical ﬁbre; high coercive-force magnets, the miniature earphone and now the electric car; solid-state lasers, the barcode. Sometimes the new material suggests the new product. More often, new products or enterprises demand the development of a new material: nuclear technology drove the development of new zirconium alloys and stainless steels; space technology stimulated the development of beryllium alloys and lightweight composites; turbine technology today drives development of high-temperature alloys and ceramics; concern for the environment drives the development of bio-polymers. The central column of Figure 3.1 shows the design process. The starting point is a market need or a new idea; the end point is the full product speciﬁcation for a product that ﬁlls the need or embodies the idea. A need must be identiﬁed before it can be met. It is essential to deﬁne the need precisely, that is, to formulate a need statement, often in the form: ‘a device is required to perform task X’, expressed as a set of design requirements. Between the need statement and the product speciﬁcation lie the set of stages shown in Figure 3.1: conceptual design, embodiment design and detailed design. At the conceptual design stage, all options are open: the designer considers alternative concepts and the ways in which these might be separated or combined. The next stage, embodiment, takes the promising concepts and seeks to analyse their operation at an approximate level. This involves sizing the components and a preliminary selection of materials and processes, and examining the implications for performance and cost. The embodiment stage ends with a feasible layout that becomes the input to the detailed design stage. Here, speciﬁcations and dimensions for each component are drawn up. Critical components may be subjected to precise mechanical or thermal analysis. Optimisation methods are applied to components and groups of components to maximise performance, minimise cost and ensure safety. A ﬁnal choice of geometry and material is made, and the methods of production are analysed and costed. The stage ends with a detailed production speciﬁcation.
3.2 The design process
Material data needs Choice of material family (metals, ceramics ..)
Choice of material class (steel, Al alloy, Ni alloy)
Choice of single material (6061 Al; 304 stainless)
Market need: problem definition
Process data needs
Choice of process family
explore working principles
(casting, moulding ..)
Choice of process class
define general layout and scale
(die cast, sand cast..)
Choice of single process
optimise form, manufacture and assembly
(pressure die cast ..)
Product specification MFA ‘17
Figure 3.1 The design ﬂow chart, showing how material and process selection enter. Information
about materials is needed at each stage but at very different levels of breadth and precision. The broken lines suggest the iterative nature of original design and the path followed in redesign.
Redesign Most design is not ‘original’ in the sense of starting from a totally new idea. It starts with an existing product and corrects its shortcomings, enhances its performance or reduces its cost or environmental impact, making it more competitive. Here are some scenarios that call for redesign:
· · · · ·
The ‘product recall’ scenario: if a product, once released to the market, fails to meet safety standards, urgent redesign is required. Often the problem is a material failure; then an alternative must be found that retains the desirable features of the original but overcomes its weaknesses. The ‘poor value for money’ scenario: the product is safe but offers performance that, at its price, is perceived to be mediocre, requiring redesign to enhance performance. The ‘inadequate proﬁt margin’ scenario: the cost of manufacture exceeds the price that the market will bear. Much of the cost of a mass-produced product derives from the materials of which it is made and the processes chosen to make it; the response is to re-examine both with cost-cutting as the objective. The ‘sustainable technology’ scenario: the designer’s reaction to the proﬂigate use of non-renewable materials in products and packaging. The ‘Apple effect’ scenario: in a market environment in which many almost-identical products compete for the consumer’s attention, it is style, image and character that set some products above others. Materials play a large role in this.
34 Chapter 3 Strategic thinking: matching material to design Much of redesign has to do with detail e the last of the three boxes in the central window of Figure 3.1 e but not all. The necessary changes may require a change of conﬁguration and layout (the embodiment phase) or even of the basic concept, replacing one of the ways of performing a function by another. Described in the abstract, these ideas are not easy to grasp; an example will help. Devices to open corked bottles Bottled wine, traditionally, is sealed with a cork. This creates a market need: it is the need to gain access to the wine inside. We might state it thus: ‘a device is required to allow access to wine in a corked bottle’, and we might add, ‘with convenience, at modest cost, and without contaminating the wine’. Three concepts for doing this are shown in Figure 3.2. In order, they are to remove the cork by axial traction (¼ pulling), to remove it by shear tractions, and to push it out from below. In the ﬁrst, a screw is threaded into the cork to which an axial pull is applied; in the second, slender elastic blades inserted down the sides of the cork apply shear tractions when pulled; and in the third, the cork is pierced by a hollow needle through which a gas is pumped to push it out. The opening picture of this chapter has photos of bottle openers based on all three concepts.
Figure 3.2 A market need e that of gaining access to wine in corked bottles e and three concepts for meeting the need. Devices based on all three of these concepts exist and can be bought.
Figure 3.3 shows, left, embodiment sketches for devices based on concept (a), that of axial traction. The ﬁrst is a direct pull; the other three use some sort of mechanical advantage e levered pull, geared pull and spring-assisted pull. The embodiments suggest the layout, the mechanisms and the scale. In the ﬁnal, detailed stage of design, the components are dimensioned so that they carry the working loads safely, their precision and surface ﬁnish are deﬁned, and a ﬁnal choice of material and manufacturing route is made (Figure 3.3, right). Let us examine how this is done.
3.3 Material and process information for design
11.0 4.0 24.0 40.0
Cast phenolic through colored
22.0 2.0 4.0
All dimensions mm
Stainless steel type 302 machined from bar stock
Figure 3.3 Embodiment sketches for the ﬁrst concept: (a) direct pull, (b) levered pull, (c) geared pull and (d) spring-assisted pull. Each system is made up of components that perform a subfunction. Detailed design drawings for the lever of embodiment (b) are shown on the right.
Material and process information for design
Materials selection enters each stage of the design (Figure 3.1, left-hand side). The nature of the data needed in the early stages differs greatly in its level of precision and breadth from that needed later. At the concept stage, the designer requires only approximate property values, but for the widest possible range of materials. All options are open: a polymer may be the best choice for one concept, a metal for another. The problem, at this stage, is not precision and detail; it is breadth and speed of access: how can data for the vast range of available materials be presented to give the designer the greatest freedom in considering alternatives? At the embodiment stage, a concept has been selected, and the materials options narrow. Here we need data for a subset of materials, but at a higher level of precision and detail. These are found in more specialised handbooks and databases that deal with a single class or sub-class of materials e metals, or just aluminium alloys, for instance. The risk now is that of losing sight of the bigger portfolio of materials to which we must return if the details don’t work out; it is easy to get trapped in a single line of thinking when others have potential to offer better solutions. The ﬁnal stage of detailed design requires a still higher level of precision and detail, but for only one or a few materials. A given material (polyethylene, for instance) has a range of properties that derive from differences in the ways different producers make it. At the detailed design stage, suppliers must be identiﬁed and the properties of their materials used in the design calculations. And sometimes even this is not good enough. If the component is a critical one (meaning that its failure could, in some sense or another, be disastrous), then it may be prudent to conduct in-house tests to measure the critical properties, using a sample of the material that will be used to make the product itself. The process is one of narrowing the materials search space by screening out materials that cannot meet the design requirements, ranking those that remain for identifying the most promising choice (Figure 3.4).
36 Chapter 3 Strategic thinking: matching material to design All materials Material search space Translate Screen Rank Increasing constraints
Figure 3.4 The narrowing of material search space as design constraints are applied. The material decisions do not end with the establishment of production. Products fail in service, and failures contain information. It is an imprudent manufacturer who does not collect and analyse data on failures. Often this points to the misuse of a material, one that redesign or reselection can eliminate. The selection of a material cannot be separated from that of process and of shape. To make a shape, a material undergoes a chain of processes that involve shaping, joining and ﬁnishing. Figures 2.3 and 2.4 of Chapter 2 introduced these processes. The selection of process follows a route that runs parallel to that of material (Figure 3.1, right). The starting point is a catalogue of all processes, which is then narrowed by screening out those that fail to make the desired shape or are incompatible with the choice of material. Material, shape and process interact (Figure 3.5). The interactions are two-way: speciﬁcation of shape restricts the choice of
Required property profile
Eco-impact Consequences Cost
Figure 3.5 The interaction between design requirements, material, shape and process.
3.4 The strategy: translation, screening, ranking and documentation
material and process, but equally, the speciﬁcation of process limits the choice of materials and the shape. And it is often processing that is used to develop the properties on which the material has been selected. The more sophisticated the design, the tighter the speciﬁcations and the greater the interactions. Choice of material and process lies at the heart of the selection process. To tackle it, we need a strategy.
The strategy: translation, screening, ranking and documentation
Selection involves seeking the best match between the attribute proﬁles of the materials and processes e bearing in mind that these must be mutually compatible e and those required by the design. The strategy, applied to materials, is sketched in Figure 3.6. The ﬁrst task is that of translation: converting the design requirements into a prescription for selecting a material. This proceeds by identifying the constraints that the material must meet and the objectives that the design must fulﬁl. These become the ﬁlters: materials that meet the constraints and rank highly in their ability to fulﬁl the objectives pass through the ﬁlters; those that do not are ﬁltered out. The second task, then, is that of screening: eliminating the materials that cannot meet the constraints. This is followed by the ranking step: ordering the survivors by their ability to meet a criterion of excellence, such as that of minimising cost. The ﬁnal task is to explore the most promising candidates in depth, examining how they are used at present, case histories of failures, and how best to design and manufacture with them e a step we call Documentation.
Translate requirements: express as function, constraints, objectives and free variables
Screen using constraints: eliminate materials that cannot do the job
Rank using objective: find the screened materials that do the job best
Seek documentation: research the family history of top-ranked candidates
Final material choice
Figure 3.6 The strategy, applied to materials. A similar strategy is later adapted to select processes. There are four steps: translation, screening, ranking and supporting information. All can be implemented in software, allowing large populations of materials to be investigated.
38 Chapter 3 Strategic thinking: matching material to design Process selection follows a parallel route in many respects. In this case, translation means identifying the geometric and other constraints that must be met e material compatibility, shape, dimensions, precision, quality and target properties. Some of these may be used to screen out processes that cannot meet the constraints, while in this context, ranking is almost always a matter of cost. Seeking documentation is replaced by ‘technical evaluation’, requiring expertise to assess the multiple interactions between design, material and process, reﬁning not only design detail and the choice of material, but also identifying optimal processing conditions. We return to process selection in Chapters 18 and 19, but for now we stick to materials and look at the selection steps more closely. Translation Any engineering component has one or more functions: to support a load, to contain a pressure, to transmit heat, and so forth. This must be achieved subject to constraints: that certain dimensions are ﬁxed, that the component must carry the design loads without failure, that it can function at the design temperature and in the design environment, and many more. In designing the component, the designer has one or more objectives: to make it as cheap as possible, perhaps, or as light, or as environmentally benign, or some combination of these. Certain parameters can be adjusted to optimise the objective e the designer is free to vary dimensions that are not constrained by design requirements and, most importantly, free to choose the material for the component and the process to shape it. We refer to these as free variables. Constraints, objectives and free variables (Table 3.1) deﬁne the boundary conditions for selecting a material and e in the case of load-bearing components e a shape for its crosssection.
Table 3.1 Function, constraints, objectives and free variables Function Constraints Objectives Free variables
What does the component do? What non-negotiable conditions must the material meet? What aspects of performance are to be maximised or minimised? What parameters of the problem is the designer free to change?
It is important to be clear about the distinction between constraints and objectives. A constraint is an essential condition that must be met, usually expressed as a limit on a material (or process) attribute: the material must cost less than $4/kg and be an electrical insulator, for example. An objective is a quantity for which an extreme value (a maximum or minimum) is sought, frequently cost, mass or volume, but there are others (Table 3.2). Identifying the constraints and objectives can take a little thought, but it is an essential ﬁrst step. In choosing materials for a super-light sprint bicycle, for example, the objective is to minimise mass, with an upper limit on cost, thus treating cost as a constraint. But in choosing materials for a cheap ‘shopping’ bike, the two are reversed: now the objective is to minimise cost with a (possible) upper limit on mass, treating it as a constraint.
3.4 The strategy: translation, screening, ranking and documentation
Table 3.2 Common constraints and objectives Common constraints*
Meet a target value of Stiffness Strength Fracture toughness Thermal conductivity Electrical resistivity Magnetic remanence Optical transparency Cost Mass
Minimise Cost Mass Volume Impact on the environment Heat loss
·· ·· ·· ·· ·
·· ·· ·
Maximise Energy storage Heat ﬂow
* All these constraints, and products that rely on them, appear in later chapters.
The outcome of the translation step is a list of the design-limiting properties and the constraints they must meet. The ﬁrst step in relating design requirements to material properties is therefore a clear statement of function, constraints, objectives and free variables. Screening Constraints are gates: meet the constraint and you pass through the gate; fail to meet it and you are out. Screening (Figure 3.6) does just that: it eliminates candidates that cannot do the job at all because one or more of their attributes lies outside the limits set by the constraints. As examples, the requirement that ‘the component must function in boiling water’, or that ‘the component must be transparent’, impose obvious limits on the attributes of maximum service temperature and optical transparency that successful candidates must meet. We refer to these as attribute limits. Ranking To rank the materials that survive the screening step, we need a criterion of excellence. They are found in the material indices, developed below and in later chapters, which measure how well a candidate that has passed the screening step can achieve the objective set by the design (Figure 3.6 again). Performance is sometimes limited by a single property, sometimes by a combination of them. Thus, the best materials for buoyancy are those with the lowest density, r; those best for thermal insulation are the ones with the smallest values of the thermal conductivity, l e provided, of course, that they also meet all other constraints imposed by the design. Here, maximising or minimising a single property maximises performance. Often, though, it is not one but a group of properties that are relevant. Thus the best materials for a light, stiff tie rod are those with the greatest value of the speciﬁc stiffness, E/r, where.E is Young’s modulus. The best materials for a spring are those with the greatest value of s2y E, where sy is the yield strength. The property or property group that maximises performance for a given design is called its material index. There are many such indices, each associated with maximising some aspect of performance e subsequent chapters will explain all about them. They provide criteria of excellence that allow ranking of materials by their ability to perform well in the given application. To summarise: screening isolates candidates that do the job; ranking identiﬁes those among them that can do the job best. Documentation The outcome of the steps so far is a ranked shortlist of candidates that meet the constraints and that maximise or minimise the criterion of excellence, whichever is required. You could just choose the top-ranked candidate, but what hidden weaknesses might
40 Chapter 3 Strategic thinking: matching material to design it have? What is its reputation? Has it a good track record? To proceed further, we seek a detailed proﬁle of each: its documentation (Figure 3.6, bottom). What form does documentation take? Typically, it is descriptive, graphical or pictorial: case studies of previous use of the material, details of its corrosion behaviour in particular environments, of its availability and pricing, warnings of its environmental impact or toxicity, or sensitivity in some of its properties to the way it is processed. Such information is found in handbooks, suppliers’ data sheets, failure analyses and case studies. Documentation helps narrow the shortlist to a ﬁnal choice, allowing a deﬁnitive match to be made between design requirements and material attributes. Why are all these steps necessary? Without screening and ranking, the candidate pool is enormous, and the volume of documentation is overwhelming. Dipping into it, hoping to stumble on a good material, gets you nowhere. But once a small number of potential candidates have been identiﬁed by the screeningeranking steps, detailed documentation can be sought for these few alone, and the task becomes viable.
Examples of translation
Here are four examples of the translation step. Example 3.1 A corkscrew lever Figure 3.3 shows the lever for one of the corkscrews in the design case study. In use, it is loaded in bending. It must carry the bending moment without deﬂecting to an awkward degree, which means a high modulus, E. It must not bend permanently (though some cheap corkscrews do), which means a high yield strength, sy. And it must not snap off altogether, which means it must have adequate fracture toughness, K1c. Finally, it must not corrode in wine or water. The length of the lever is speciﬁed, but the cross-section is not e we are free to choose a section that is sufﬁcient to bear the use loads. Given all these, the lever should be as cheap as possible. Formulate the translation. Function Constraints
Objective Free variables
· ·· ·· · · ··
Lever (beam loaded in bending) Stiff enough Strong enough Tough enough Resist corrosion in water and wine Length L speciﬁed
Functional constraints Geometric constraint
Minimize the material cost of the beam Cross-section area of beam, A Choice of material
Answer. Translation for the corkscrew lever. The design-limiting properties are those directly relating to the constraints: modulus E, strength sy, fracture toughness K1c and corrosion resistance.
3.5 Examples of translation
Example 3.2 Redesign of a CD case Music lovers, for many decades, regarded CDs as the ultimate way to store and enjoy their music. But the cases they come in fail to match the quality of their contents. These so-called ‘jewel’ cases are usually made of polystyrene (PS), chosen for its low cost and water-clear transparency, if not exactly jewel quality (see ﬁgure); and they are made by injectionmoulding, and that, too, is cheap if you are making millions. PS can, at least in principle, be recycled. The problem is that PS cases are brittle and crack easily, jam shut, the hinges break, and the broken edges are hard and sharp enough to inﬂict terminal damage on a CD. Decide on the features you think really matter, and formulate constraints, objective and free variables for the redesign of a CD case. Do you think this is a product that is worth redevelopment?
Answer. The way to tackle redesign is to seek a replacement material that retains the good properties of the old one, but without the bad. Thus, we seek a material that is optically transparent to allow the label to be read, is able to be injection-moulded (because it is economic for large numbers) and is recyclable. But it must be tougher (greater Kic) than PS. Of the materials that meet these constraints, we want the cheapest. Translation for the CD case. Function Constraints
Objective Free variables
· ·· ·· · · ·
Contain and protect a CD Optically clear Able to be injection-molded Recyclable Tougher than polystyrene Dimensions identical to current PS case
Functional constraints Geometric constraint
Minimize the material cost Choice of material
Potential design-limiting properties are transparency and fracture toughness. It is unlikely that CD cases will be improved e streaming music to mobile devices has proved to be a ‘disruptive technology’, a step change in meeting consumer demand that causes rapid, and usually terminal, decline in the technology it displaces.
42 Chapter 3 Strategic thinking: matching material to design Example 3.3 Heat sinks for microchips A microchip may only consume milliwatts, but this power is dissipated in a tiny volume, making the power density high. As chips shrink and clock speeds grow, overheating becomes a problem. The chips of today’s PCs require forced cooling to limit temperatures to 85 C. Multiple-chip modules (MCMs) pack hundreds of chips onto a single substrate, and they get even hotter e up to 180 C. Heating is kept under control by attaching the chips to a heat sink (see ﬁgure), taking pains to ensure good thermal contact between chip and sink. The heat sink is a critical component, limiting further miniaturisation of the electronics. How can its performance be maximised? Substrate
Chips Heat sink Cooling fins
To prevent electrical coupling and stray capacitance between chip and heat sink, the heat sink must be a good electrical insulator. If it is to work with one surface at 180 C, it must have a maximum service temperature (the temperature at which it can operate continuously without damage) that is at least as great as 180 C. These deﬁne the constraints. To drain heat away from the chip as fast as possible, it must also have the highest possible thermal conductivity, l, deﬁning the objective. Formulate the translation. Function Constraints
Objective Free variable
· · · · · ·
Heat sink Material must be good electrical insulator Maximum operating temperature >180 C All dimensions are speciﬁed
Functional constraints Geometric constraint
Maximize heat removal rate Choice of material
Answer. Translation for the heat sink. The design-limiting properties, clearly, are maximum service temperature Tmax, electrical resistivity re and thermal conductivity l.
3.6 Summary and conclusions
Example 3.4 Transformer cores An electrical transformer uses electromagnetic induction to convert one AC voltage to another (see ﬁgure). To minimise energy loss, the material must be a soft magnet e one that is easy to magnetise and de-magnetise (Chapter 14). And to avoid eddy current losses at high frequencies, it must also be an electrical insulator. The constraints of ‘soft magnetic material’ and ‘electrical insulator’ are very restrictive e they will screen out all but a small number of candidates. If the transformer is for an everyday product, the objective would be to minimise the cost. Formulate the translation. Core Low-voltage side
Objective Free variable
· ·· · · ·
Transformer core Soft magnetic material Electrical insulator All dimensions are speciﬁed
Functional constraints Geometric constraint
Minimize cost of material Choice of material
Answer. Translation for the transformer core. Design-limiting properties are the magnetic remanence and electrical resistivity.
These translations are the ﬁrst step in selection. In them, we have identiﬁed the constraints; they will be used for screening. We have also identiﬁed the objective; it will be used for ranking. We will return to all four of these examples in later chapters.
Summary and conclusions
The starting point of a design is a market need captured in a set of design requirements. Concepts for a product that meet the need are devised. If initial estimates and exploration of alternatives suggest that the concept is viable, the design proceeds to the embodiment stage: working principles are selected, size and layout are decided, and initial estimates of performance and cost are made. If the outcome is successful, the designer proceeds to the detailed design stage: optimisation of performance, full analysis of critical components, and preparation of detailed production drawings (usually as a computer-aided design, or CAD ﬁle), showing dimensions, specifying precision, and identifying material and manufacturing path. But design is not a linear process, as Figure 3.1 might suggest. Some routes lead to a dead end,
44 Chapter 3 Strategic thinking: matching material to design requiring reiteration of earlier steps. And, frequently, the task is one of redesign, requiring that constraints be re-thought and objectives realigned. The selection of material and process runs parallel to this set of stages. Initially the search space for both is wide, encompassing all possible candidates. As the design requirements are formulated in increasing detail, constraints emerge that both must meet, and one or more objectives is formulated. The constraints narrow the search space, and the objective(s) allow ranking of the candidates that remain. Identifying the constraints, the objectives and the free variables (the process we called ‘translation’) is the ﬁrst step in selection. This chapter ended with examples of translation when the task was that of choosing a material; the exercises suggest more. The other steps in material selection e screening, ranking and documentation e are discussed and illustrated in the chapters that follow. When the task is the choice of process, a similar translation is needed, with a corresponding strategy for screening, ranking and technical evaluation of the options e we return to this in Chapter 18.
Ashby, M. F. (2017). Materials selection in mechanical design (5th ed.). Oxford, UK: Butterworth Heinemann. ISBN: 978-0081-00599-6. (An advanced text developing material selection methods in detail.) Cross, N. (2008). Engineering design methods (4th ed.). Chichester, UK: Wiley. ISBN: 978-0-470-51926-4. (A durable text describing the design process, with emphasis on developing and evaluating alternative solutions.) Pahl, G., Beitz, W., Feldhusen, J., & Grote, K. H. (2007). Engineering design: A systematic approach. Translated by Wallace K, Blessing L. (3rd ed.). London, UK: The Design Council, and Berlin, Germany: Springer Verlag. ISBN: 978-1-84-628318-5. (The Bibledor perhaps more exactly the Old Testamentd of the technical design ﬁeld, developing formal methods in the rigorous German tradition.) Ullman, D. G. (2009). The mechanical design process (4th ed.). New York, USA: McGraw-Hill. ISBN: 978-0072975741. (An American view of design, developing ways in which an initially ill-deﬁned problem is tackled in a series of steps, much in the way suggested by Figure 3.1.) Ulrich, K. T. (2011). Design: Creation of artefacts in society. Philadelphia, USA: University of Pennsylvania Press. ISBN: 978-0-9836487-0-3. (An excellent short introduction to the kind of structured reasoning that lies behind good product design. The text is available on http://www.ulrichbook.org/.) Ulrich, K. T., & Eppinger, S. D. (2008). Product design and development (4th ed.). New York, USA: McGraw Hill. ISBN: 978-007-125947-7. (A readable, comprehensible text on product design, as taught at MIT. Many helpful examples but almost no mention of materials.)
What are the steps in developing an original design?
What is meant by a constraint and what is by an objective in the requirements for a design? How do they differ?
Describe the ‘Translation’ step of the material selection strategy.
Translation (1). The teeth of a scoop for a digger truck, pictured in Chapter 1, must cut earth, scoop stones, crunch rock, often in the presence of fresh or salt water and worse. Translate these requirements into a prescription of Function, Constraints, Objectives and Free variables.
Translation (2). A material for an energy-efﬁcient saucepan, pictured in Chapter 1, must transmit and spread the heat well, it must resist corrosion by foods, and must withstand the mechanical and thermal loads expected in normal use. The product itself must be competitive in a crowded market. Translate these requirements into a prescription of Function, Constraints, Objectives and Free variables.
Translation (3). A material for eyeglass lenses, pictured in Chapter 1, must have optical-quality transparency. The lens may be moulded or ground with precision to the required prescription. It must resist sweat and be sufﬁciently scratch-resistant to cope with normal handling. The mass-market end of the eyeglass business is very competitive, so price is an issue. Translate these requirements into a prescription of Function, Constraints, Objectives and Free variables.
Translation (4). Bikes come in many forms, each aimed at a particular sector of the market:
·· ·· ··
Sprint bikes Touring bikes Mountain bikes Shopping bikes Children’s bikes Folding bikes
Use your judgment to identify the primary objective for each of these. Exercise E3.8
Translation (5). A material is required for the windings of an electric air furnace capable of temperatures up to 1000oC. Think about what attributes a material must have if it is to be made into windings and function properly in a furnace. List the function and the constraints; set the objective to ‘minimise material price’ and the free variables to ‘choice of material’.
Translation (6). A material is required to manufacture ofﬁce scissors. Paper is an abrasive material, and scissors sometimes encounter hard obstacles like staples. List function and constraints; set the objective to ‘minimise material price’ and the free variables to ‘choice of material’.
Translation (7). A material is required for a heat exchanger to extract heat from geothermally heated saline water at 120 C (and thus under pressure). List function and constraints; set the objective to ‘minimise material price’ and the free variables to ‘choice of material’.
46 Chapter 3 Strategic thinking: matching material to design
Translation (8). A material is required for a disposable fork for a fast-food chain. List the objective and the constraints that you would see as important in this application.
Translation (9). Formulate the constraints and objective you would associate with the choice of material to make the forks of a racing bicycle.
Cheap coat hangers used to be made of wood e now it is only expensive ones that use this material. Most coat hangers are now metal or plastic, and both differ in shape from the wooden ones and from each other. Examine wood, metal and plastic coat hangers, comparing the designs, and comment on the ways in which the choice of material has inﬂuenced them.
Cyclists carry water in bottles that slot into bottle cages on their bicycles. Examine metal and plastic bottle holders, comparing the designs, and comment on the ways in which the choice of material has inﬂuenced them.
Elastic stiffness, and weight: atomic bonding and packing Compression member, or column
Tensile member, or tie
Torsion member, or shaft
Tensile member, or tie
Flexural member, or beam
Compression member, or column Flexural member, or beam
Modes of loading. Image of Stansted Airport courtesy of Norman Foster and Partners, London, UK.
Chapter contents 4.1 4.2 4.3 4.4 4.5 4.6 4.7 4.8 4.9 4.10 4.11
Introduction and synopsis Density, stress, strain and elastic moduli The big picture: material property charts Manipulating the modulus and density The science: microstructure and properties Atomic structure and interatomic bonding Atomic and molecular packing in solids: the origin of density Interatomic bonding and properties: the origin of elastic modulus Summary and conclusions Further reading Exercises
Copyright Ó 2019 Elsevier Ltd. All rights reserved. https://doi.org/10.1016/B978-0-08-102376-1.00004-4
48 48 59 60 64 65 76 83 90 91 91
48 Chapter 4 Elastic stiffness, and weight: atomic bonding and packing
Introduction and synopsis
Stress causes strain. If you are human, the ability to cope with stress without undue strain is called resilience. If you are a material, it is called elastic modulus. Stress is something that is applied to a material by loading it. Strain e a change of shape e is its response. The strain depends on the material, on the magnitude of the stress and the way it is applied e the mode of loading. The cover picture illustrates the common modes of loading. Ties carry tension e often, they are cables. Columns carry compression e often they are hollow tubes. Beams carry bending moments, like the wing spar of the plane or the horizontal roof beams of the airport. Shafts carry torsion, as in the drive shaft of cars or the propeller shaft of the plane. Pressure vessels contain a pressure, as in the tires of the plane. Stiffness is the resistance to elastic shape change, ‘elastic’ meaning that the material returns to its original shape when the stress is removed. Strength (Chapter 6) is its resistance to permanent distortion or total failure. Stress and strain are not material properties; they describe a stimulus and a response. Stiffness (measured by the elastic modulus E, deﬁned in a moment) and strength (measured by the elastic limit sy or tensile strength sts) are material properties. Stiffness and strength are central to mechanical design, often in combination with the density, r. This chapter introduces stress and strain and the elastic moduli that relate them. These properties are neatly summarised in a material property chart e the modulusedensity chart e the ﬁrst of many that we shall explore in this book. Density and modulus are microstructure-insensitive properties. They derive directly from the atomic weight and packing, and from the nature of the bonds that bind the atoms of the material together. This distinguishes them (and a number of other such properties) from microstructure-sensitive properties like strength and toughness that depend strongly on the way that the material has been processed. In this chapter, we explore atomic bonding and packing, giving insight into the way modulus and density vary across the rows of the periodic table of the elements and the way they change when elements are combined to form ceramics, glasses, polymers and elastomers. There is not much you can do to change the weight, packing and bonding of atoms, but there are two ways in which modulus and density can be manipulated: by combining two materials together to make a composite, or by dispersing space within them, making foams. Property charts are a good way to show how this works.
Density, stress, strain and elastic moduli
Density Many applications (e.g. aerospace components, automotive bodies, sports equipment) require stiffness and strength at low weight, and this depends in part on the density of the materials of which they are made. Density is mass per unit volume, measured in kg/m3.
4.2 Density, stress, strain and elastic moduli
The density of samples with regular shapes can be determined using a precision mass balance and accurate measurements of the dimensions (to give the volume), but this is not the best way. Better is the ‘double weighing’ method: the sample is ﬁrst weighed in air and then, when fully immersed, in a liquid of known density. When immersed, the sample feels an upward force equal to the weight of liquid it displaces (Archimedes’ principle1). The density is then calculated, as shown in Figure 4.1. Mass m2
Mass m1 Grams
Sample of unknown volume V
Fluid of known density ρfl
m Density ρ = ρfl m -1m 1 2
Figure 4.1 Measuring density. Modes of loading Most engineering components carry loads. Their elastic response depends on the way the loads are applied. As explained earlier, the components in both structures shown on the front page of this chapter are designed to withstand different modes of loading: tension, compression, bending, torsion and internal pressure. Usually one mode dominates, and the component can be idealised as one of the simply loaded cases in Figure 4.2 e tie, column, beam, shaft or shell. Ties carry simple axial tension, shown in (a); columns do the same in simple compression, as in (b). Bending of a beam (c) creates simple axial tension in elements on one side of the neutral axis (the centre-line, for a beam with a symmetric crosssection) and simple compression in those on the other. Shafts carry twisting or torsion (d), which generates shear rather than axial load. Pressure difference applied to a shell, like the cylindrical tube shown in (e), generates bi-axial tension or compression. Stress Consider a force F applied normal to the face of an element of material, as in Figure 4.3 on the left of row (a). The force is transmitted through the element and balanced by an equal but opposite force on the other side, so that it is in equilibrium (it does not move). Every plane normal to F carries the force. If the area of such a plane is A, the tensile stress s in the element (neglecting its own weight) is s¼ 1
Archimedes (287e212 BC), Greek mathematician, engineer, astronomer and philosopher, designer of war machines, the Archimedean screw for lifting water, evaluator of p (as 3 þ 1/7) and conceiver, while taking a bath, of the principle that bears his name.
(a) A tie
(c) A beam
(b) A column
(d) A shaft
(e) A shell
Figure 4.2 Modes of loading and states of stress. Stress
F Tensile stress σ = F/A usual units MPa
σ= E ε
Tensile strain ε = (L - Lo)/Lo
E = Young's modulus
Fs Shear stress τ = Fs/A usual units MPa
Shear strain γ = w/Lo Volume Vo
p Pressure p usual units MPa
τ= G γ
G = Shear modulus
Volume strain (dilatation) Δ= (V - Vo)/Vo
Figure 4.3 The deﬁnitions of stress, strain and elastic moduli.
K = Bulk modulus
4.2 Density, stress, strain and elastic moduli
If the sign of F is reversed, the stress is compressive and given a negative sign. Forces2 are measured in newtons (N), so stress has the dimensions of N/m2. But a stress of 1 N/m2 is tiny e atmospheric pressure is 105 N/m2 e so the usual unit is MN/m2 (106 N/m2), called megapascals, symbol3 MPa. Example 4.1 A brick column is 50 m tall. The bricks have a density of r ¼ 1800 kg/m3. What is the axial compressive stress at its base? Does the shape of the cross-section matter? Answer. Let the cross-section area of the column be A and its height be h. The force exerted by the column at its base is F ¼ rAhg, where g is the acceleration due to gravity, 9.8 m/s2. Using equation (4.1), the axial compressive stress at the base is s ¼ F/A ¼ rgh, where the ‘’ indicates compression (the area A has cancelled out). This is the same formula as for the static pressure at depth h in a ﬂuid of density r. The stress is independent of the shape or size of the cross-section. Hence, s ¼ 1800 9.8 50 ¼ 8.8 105 N/m2 ¼ 0.88 MPa.
If, instead, the force lies parallel to the face of the element, three other forces are needed to maintain equilibrium: an equal and opposite force on the opposing face, for force equilibrium, and a complementary pair of forces on the other two faces, for moment equilibrium (Figure 4.3, row (b)). This creates a state of pure shear in the element. The shaded plane, for instance, carries the shear stress s of s¼
The units, as before, are MPa. One further state of multi-axial stress is useful in deﬁning the elastic response of materials: that produced by applying equal tensile or compressive forces to all six faces of a cubic element, as in Figure 4.3, row (c). Any plane in the cube now carries the same state of stress e it is equal to the force on a cube face divided by its area. The state of stress is one of hydrostatic pressure, symbol p, again with the units of MPa. There is an unfortunate convention here. Pressures are positive when they push e the reverse of the convention for simple tension and compression.
Isaac Newton (1642e1727), scientiﬁc genius and alchemist, formulator of the laws of motion, the inverse-square law of gravity (though there is some controversy about this), laws of optics, the differential calculus and much more. Blaise Pascal (1623e1662), philosopher, mathematician and scientist, who took a certain pleasure in publishing his results without explaining how he reached them. Almost all, however, proved to be correct.
52 Chapter 4 Elastic stiffness, and weight: atomic bonding and packing Engineering components can have complex shapes and can be loaded in different ways, creating complex distributions of stress. But no matter how complex, the stresses in any small element within the component can always be described by a combination of tension, compression and shear. Commonly, the simple cases of Figure 4.3 sufﬁce, using superposition of two cases to capture, for example, bending plus compression. Strain Strain is the response of materials to stress (second column of Figure 4.3). A tensile stress s applied to an element causes the element to stretch. If the element in Figure 4.3(a), originally of side length Lo, stretches by dL ¼ L Lo, the nominal tensile strain is ε¼
A compressive stress shortens the element; the nominal compressive strain (negative) is deﬁned in the same way. Since strain is the ratio of two lengths, it is dimensionless. A shear stress causes a shear strain g (Figure 4.3(b)). If the element shears by a distance w, the shear strain is tanðgÞ ¼
w ¼g Lo
In practice, tan g z g because elastic strains are almost always small. Finally, a hydrostatic pressure p causes an element of volume V to change in volume by dV. The volumetric strain, or dilatation (Figure 4.3(c)), is D¼
Stressestrain curves and moduli Figure 4.4 shows typical tensile stressestrain curves for a ceramic, a metal and a polymer, each taken all the way to failure. The initial part, up to the elastic limit sel, is approximately linear (Hooke’s4 law), and it is elastic, meaning that the strain is recoverable e the material returns to its original shape when the stress is removed. Stresses above the elastic limit cause permanent deformation (ductile behaviour) or brittle fracture. Within the linear elastic regime, strain is proportional to stress (Figure 4.3, third column). The tensile strain is proportional to the tensile stress: s ¼ Eε
and the same is true in compression. The constant of proportionality, E, is Young’s modulus. Similarly, the shear strain g is proportional to the shear stress s: s ¼ Gg 4
Robert Hooke (1635e1703), able but miserable man, inventor of the microscope, and perhaps, too, of the idea of the inverse-square law of gravity. He didn’t get along with Newton. Thomas Young (1773e1829), English scientist, expert on optics and deciphering ancient Egyptian hieroglyphs (among them, the Rosetta stone). It seems a little unfair that the modulus carries his name, not that of Hooke.
4.2 Density, stress, strain and elastic moduli
Stress σ= F/Ao
Stress of order 300 MPa
Elastic limit, σel (fracture)
Ao Strain of order 0.0005
Slope E = σ/ε
Strain ε = δL/L Ductile metals
Tensile strength, σts
Stress σ = F/Ao
Stress of order 500 MPa
Of order 300 MPa
Yield strength, σy
* Strain of order 0.2
Slope E = σ/ε
Strain ε = δL/L
Stress σ = F/Ao
Stress of order 50 MPa
* Strain of order 3.0
Yield stress, σy Slope E = σ/ε
Strain ε = δL/L
Figure 4.4 Tensile stressestrain curves for ceramics, metals and polymers.
54 Chapter 4 Elastic stiffness, and weight: atomic bonding and packing and the dilatation D is proportional to the pressure p: p ¼ KD
where G is the shear modulus and K the bulk modulus, as illustrated in the third column of Figure 4.3. All three of these moduli have the same dimensions as stress, that of force per unit area (N/m2 or Pa). As with stress, it is convenient to use a larger unit, this time an even bigger one, that of 109 N/m2, gigapascals, or GPa. Young’s modulus, the shear modulus and the bulk modulus are related, but to relate them we need one more quantity, Poisson’s6 ratio. When stretched in one direction, the element of Figure 4.3(a) generally contracts in the other two directions, as it is shown doing here. Poisson’s ratio, n, is the negative of the ratio of the lateral or transverse strain, εt, to the axial strain, ε, in tensile loading: εt (4.9) n¼ ε Since the transverse strain itself is negative, n is positive e it is typically about 1/3. Example 4.2 The brick column in Example 4.1 has bricks with Young’s modulus E ¼ 25 GPa and Poisson’s ratio n ¼ 0.2. What are the axial and transverse strains of the bricks at the bottom of the column? Answer. Using the result of Example 4.1 with equation (4.6), the axial strain is ε ¼ s/ E ¼ 8.8 105/25 109 ¼ 3.5 105 (often written as 35 microstrain, mε). From equation (4.9), the transverse strain is εt ¼ nε ¼ 7.0 mε. This time the strain is positive, indicating a small expansion at the base of the column.
In an isotropic material (one for which the moduli do not depend on the direction in which the load is applied), the moduli are related in the following ways: E E ; K¼ (4.10) G¼ 2ð1 þ nÞ 3ð1 2nÞ Commonly, n z 1/3 so that 3 G¼ E 8
Siméon Denis Poisson (1781e1840), French mathematician, known both for his constant and his distribution. He was famously uncoordinated, failed geometry at university because he could not draw, and had to abandon experimentation because of the disasters resulting from his clumsiness.
4.2 Density, stress, strain and elastic moduli
Elastomers are exceptional. For these, n z 1/2 when 1 G¼ E 3
This means that rubber (an elastomer) is easy to stretch in tension (low E), but if constrained from changing shape, or loaded hydrostatically, it is very stiff (large K) e a feature for which designers of shoes must allow. Hooke’s law in three dimensions The simple loading states in Figure 4.2 lead to stresses in one or two perpendicular directions. But, as we have now seen, even under uniaxial load, the strain is inherently three-dimensional, thanks to Poisson’s ratio. So it is helpful to relate stress and strain in a more general way that allows for loading acting in all three perpendicular directions at once. Figure 4.5 shows the cubic element of material, now subjected to three unequal stresses s1, s2 and s3, resulting in strains ε1, ε2 and ε3. To relate stress to strain, we use the principle of superposition e applying each stress in turn, ﬁnding the strains and then summing these to ﬁnd the overall strain when all three stresses act together. First applying a stress s1, the resulting strains (from equations (4.6) and (4.9)) are ε1 ¼
s1 ; E
ε2 ¼ ε3 ¼ nε1 ¼
Figure 4.5 Multi-axial states of stress and strain. Repeating for stresses s2 and s3, and summing the strains gives us Hooke’s law in three dimensions: 1 ðs1 ns2 ns3 Þ E 1 ε2 ¼ ð ns1 þ s2 n3 Þ E 1 ε3 ¼ ð ns1 ns2 þ s3 Þ E
These results are particularly helpful in design problems in which strain is constrained. Figure 4.6 shows a cube of material located in a rigid slot of the same width as the cube. A vertical downwards stress s1 ¼ es is applied to the top face of the cube. At ﬁrst sight, this
56 Chapter 4 Elastic stiffness, and weight: atomic bonding and packing looks like conventional uniaxial compression. But the cube wishes to expand laterally due to Poisson’s ratio. In the 2-direction it can do so, but perpendicular to the slot it is constrained; the strain in the 3-direction is zero. What does Hooke’s law tell us about the stresses and strains? σ
Figure 4.6 Constrained compression. For the 3-direction, we can write (noting that s2 ¼ 0). ε3 ¼ 0 ¼
1 ðþns þ s3 Þ; E
so s3 ¼ ns
The effect of constraint is therefore to induce a compressive stress ns in the constrained direction, perpendicular to the applied stress. But this stress will itself contribute a Poisson strain in the 1-direction, so the strain vertically is ε1 ¼
1 s ðs1 ns3 Þ ¼ 1 n2 E E
Now look at the ratio of stress to strain in the 1-direction: s1 E ¼ ε1 ð1 n2 Þ
The constrained cube behaves like a material with an ‘effective modulus’ which is greater than E (since the factor (1 n2) is less than unity). Example 4.3 By what factor is the modulus effectively increased for the loading geometry of Figure 4.6 for a cube of (a) foam (n z 0); (b) metal (n z 0.33); (c) rubber (n z 0.5)? Answer. From equation (4.14), the factor is 1/(1 n2). Hence (a) for foam, factor ¼ 1 (no Poisson expansion); (b) for metal, 1.12; (c) for rubber, 1.33.
4.2 Density, stress, strain and elastic moduli
The effect is even more marked when there is constraint in both 2- and 3-directions (see Exercises at the end of the chapter), and the effect is most signiﬁcant for values of Poisson’s ratio near 0.5. As noted earlier, the solid material with the lowest modulus e rubber e displays the most signiﬁcant stiffening effect when it is loaded in a geometry that imposes constraint. Elastic energy If you stretch an elastic band, energy is stored in it. The energy can be considerable: catapults can be lethal; the elastic deﬂection of truck springs can cushion the truck and its contents. The super-weapon of the Roman arsenal at one time was a wind-up mechanism that stored enough elastic energy to hurl a 10-kg stone projectile 100 m. How do you calculate this energy? A force F acting through a displacement dL does work FdL. A stress s ¼ F/A acting through a strain increment dε ¼ dL/L does work per unit volume dW ¼
FdL ¼ sdε AL
with units of J/m3. If the stress is acting on an elastic material, this work is stored as elastic energy. The elastic part of all three stressestrain curves of Figure 4.4 e the part of the curve before the elastic limit e is linear; in it, s ¼ Eε. The work done per unit volume as the stress is raised from zero to a ﬁnal value s* is the area under the stressestrain curve: sZ =E
1 ðs Þ2 2 E
This is the energy that is stored, per unit volume, in an elastically strained material. The energy is released when the stress is relaxed. Example 4.4 A steel rod has length Lo ¼ 10 m and a diameter d ¼ 10 mm. The steel has Young’s modulus E ¼ 200 GPa, elastic limit (the highest stress at which it is still elastic and has not yielded) sy ¼ 500 MPa and density r ¼ 7800 kg/m3. Calculate the force in the rod, its extension and the elastic energy per unit volume it stores when it is stretched so that the stress in it just reaches the elastic limit. Compare the elastic energy per unit mass with the chemical energy stored in gasoline, which has a heat of combustion (caloriﬁc value) of 43,000 kJ/kg. Answer. The cross-section area of the rod is A ¼ pd2/4 ¼ 7.85 105 m2. At the elastic limit, from equation (4.1), the force in the rod is: F ¼ syA ¼ 39.2 kN (3.92 tonnes). From equation (4.6), the corresponding strain is: ε ¼ s/E ¼ 500 106/200 109 ¼ 0.0025 (i.e. 0.25%). The extension of the rod, from equation (4.3), is: dL ¼ εLo ¼ 0.0025 10 ¼ 25 mm. The elastic energy per unit volume, from equation (4.16), is: W ¼ s2/2E ¼ (500 106)2/(2 200 109) ¼ 625 kJ/m3, giving an elastic energy per kg of W/r ¼ 80 J/kg. This is less, by a factor of more than 500,000 than that of gasoline.
58 Chapter 4 Elastic stiffness, and weight: atomic bonding and packing Measurement of Young’s modulus You might think that the way to measure the elastic modulus of a material would be to apply a small stress (to be sure to remain in the linear elastic region of the stressestrain curve), measure the strain and divide one by the other. In reality, moduli measured as slopes of stressestrain curves are inaccurate, often by a factor of two or more, because of contributions to the strain from material creep or deﬂection of the test machine. Accurate moduli are measured dynamically: by measuring the frequency of natural vibrations of beam paﬃﬃﬃﬃﬃﬃﬃﬃ ﬃ or wire, or by measuring the velocity of sound waves in the material. Both depend on E=r; so if you know the density r, you can calculate E. Stress-free strain Stress is not the only stimulus that causes strain. Some materials respond to a magnetic ﬁeld by shrinking e an effect known as magnetostriction. Others respond to an electrostatic ﬁeld in the same way e they are known as piezo-electric materials. In each case, a material property relates the magnitude of the strain to the intensity of the stimulus (Figure 4.7). The strains are small, but the stimulus can be controlled with great accuracy, and the material response is extremely fast. Magnetostrictive and piezo-electric strain can be driven at high frequency. This is exploited in precision positioning devices, acoustic generators and sensors e applications we return to in Chapters 15 and 16. Stress field
Stimulus Material property
Response Thermal field
Figure 4.7 Stimuli, material properties and response. A more familiar effect is that of thermal expansion: strain caused by change of temperature. The thermal strain εT is linearly related to the temperature change DT by the expansion coefﬁcient, a: εT ¼ aDT
where the subscript T is a reminder that the strain is caused by temperature change, not by stress. The term ‘stress-free strain’ is a little misleading. It correctly conveys the idea that the strain is not caused by stress but by something else. But these strains can nonetheless give rise to stresses if the body suffering the strain is constrained. Thermal stress, arising from constrained thermal expansion, can be a particular problem, causing mechanisms to jam and railway tracks to buckle. We analyse it in Chapter 12.
4.3 The big picture: material property charts
The big picture: material property charts
If we want materials that are stiff and light, we need an overview of what’s available. That is the role of material property charts (introduced in Chapter 2). The modulusedensity chart The moduli and densities of common engineering materials are plotted in Figure 4.8; material families are enclosed in coloured envelopes. The modulus E spans seven decades7, from 0.0001 to nearly 1000 GPa; the density r spans a factor of 2000, from less than 10 to 20,000 kg/m3. Ceramics (yellow envelope) and metals (red envelope) have high moduli and densities; none has a modulus less than 10 GPa or a density less than 1700 kg/m3. Polymers, by contrast, all have moduli below 10 GPa and densities that are lower than those of any metal or ceramic e most are close to 1000 kg/m3 (the density of water). Elastomers have roughly the same density as other polymers, but their moduli are lower by a further factor of 100 or more. Materials with even lower densities are porous: synthetic foams and natural cellular structures like wood and cork.
Young's modulus - Density
Young's modulus, E (GPa)
Bamboo Wood // grain
Al alloys CFRP
Concrete PEEK PET
Rigid polymer foams
PS TWood grain
WC W alloys
Glass Mg alloys GFRP
Diamond Al O Steels 2 3 Ni alloys SiC Ti alloys Si3N4 B4C
Foams Silicone elastomers
10-3 Flexible polymer foams
Density, ρ (kg/m3)
Figure 4.8 The Young’s modulusedensity chart.
Very-low density foams and gels (which can be thought of as molecular-scale, ﬂuid-ﬁlled foams) can have lower moduli than this. As an example, gelatine (as in Jell-O) has a modulus of about 105 GPa.
60 Chapter 4 Elastic stiffness, and weight: atomic bonding and packing This property chart gives an overview, showing where families and their members lie in Eer space. We will use it in Chapter 5 to select materials for stiffness-limited applications in which weight must be minimised. Anisotropy Glasses have disordered structures with properties that are isotropic, meaning they are the same no matter in which direction they are measured. Crystals, by contrast, are ordered, and because of this, their properties depend on the direction in which they are measured e they are anisotropic. Most real metals and ceramics are polycrystalline, made up of many tiny, randomly oriented crystals. This averages out the directionality in properties, so the aggregate behaves as if it were isotropic. Sometimes, though, anisotropy is important. Single crystals, drawn polymers and natural materials like wood are anisotropic; their properties depend on the direction in the material in which they are measured. Figure 4.8 has separate property bubbles for woods in each of the two loading directions, parallel and perpendicular to the grain. Fibre composites are yet more extreme: the modulus parallel to the ﬁbres can be larger by a factor of 20 than that perpendicular to them e we explore why in the next section. Anisotropy must therefore be considered when wood and composite materials are selected.
Manipulating the modulus and density
The property chart in Figure 4.8 shows that each ceramic (e.g. SiC, Al2O3) or class of metallic alloys (e.g. steels, Ni alloys) occupies a small, well-deﬁned bubble. Polymers show a little more variation, but it is apparent that the modulus and density of solids reﬂect some inherent physical characteristics e in Sections 4.7e4.8, we will see that these properties depend mainly on the atomic bonding and packing. So there’s not much you can do to change these properties in a given solid material, but there are other ways to manipulate modulus and density, to occupy new spaces on the chart. Hybrid materials are mixtures of solid materials (or a solid with air) to give internal structure at a length scale greater than the atomic. Polymers and metals can be reinforced with stiff ceramic particles or ﬁbres to make composites. And almost all materials can be made into porous foams or some other cellular structure. Materials such as woods are in fact natural hybrids of mixed polymers, exploiting both foam and composite characteristics. Synthetic foams and composites either occupy blank spaces on the chart or overlay existing solids, creating new opportunities and competition in design. A bit of simple modelling shows how they work. Composites The development of high-performance composites is one of the great material advances of the last 50 years. Composites are made by embedding ﬁbres or particles in a continuous matrix of a polymer (polymer matrix composites, PMCs), a metal (MMCs) or a ceramic (CMCs), as in Figure 4.9. Composites have high stiffness and strength per unit weight, and e in the case of MMCs and CMCs e improved high-temperature performance.
4.4 Manipulating the modulus and density
Figure 4.9 Composite structures. When a volume fraction f of a reinforcement r (density rr) is mixed with a volume fraction (1 f) of a matrix m (density rm) to form a composite with no residual porosity, the composite density e r is given exactly by the rule of mixtures: e r ¼ f rr þ ð1 f Þrm
The geometry or shape of the reinforcement does not matter except in determining the maximum packing fraction of reinforcement and thus the upper limit for f (typically 50%). The modulus of a composite is bracketed by two bounds e limits between which the e U , is found by assuming that on loading, the two modulus must lie. The upper bound, E components strain by the same amount, like springs in parallel. The stress is then the volume fraction-weighted average of the stresses in the matrix and the stiffer reinforcement, giving, once more, a rule of mixtures: e U ¼ f Er þ ð1 f ÞEm E
where Er is the Young’s modulus of the reinforcement and Em that of the matrix. To calculate eL , we assume that the two components carry the same stress, like springs in the lower bound, E series. The strain is the volume fraction weighted average of the local strains, and the composite modulus is eL ¼ E
Em Er f Em þ ð1 f ÞEr
62 Chapter 4 Elastic stiffness, and weight: atomic bonding and packing Figure 4.10 shows the range of modulus and density that can, in principle, be obtained by mixing two materials together. The boundaries are calculated from equations (4.18), (4.19) and (4.20). There are practical limits of course e the matrix and reinforcement must be chemically compatible and available in the right form, and processing the mixture must be achievable at a sensible cost. The ‘Composites’ bubble in Figure 4.8 shows two successful examples: glass ﬁbre-reinforced plastic (GFRP) and carbon ﬁbre-reinforced plastic (CFRP). Note that the bubble lies between ‘Polymers’ and ‘Ceramics’, as expected. They are as stiff as metals but lighter, a desirable combination.
Ceramics Young's modulus, E (GPa)
Density, ρ (kg/m3)
Figure 4.10 Bounds for the modulus and density of composites.
Example 4.5 A composite material has a matrix of polypropylene and contains 10% glass reinforcement. Estimate the Young’s modulus and density of the composite: (i) if the glass is in the form of long parallel ﬁbres (calculate the properties parallel to the ﬁbres); and (ii) if the glass is in the form of small particles (corresponding to the lower bound). Compare the speciﬁc moduli (E/r) of the constituent materials and the two composites. Use the following property data:
Polypropylene (m) Glass (r)
1.1 103 31.8 103
4.4 Manipulating the modulus and density
Answer. The density of both composites is the same. Using equation (4.18) with f ¼ 0.1 gives e r ¼ 1030 kg/m3 (it would just sink in water). Using the upper bound (equation (4.19)) for Young’s modulus of the ﬁbre-reinforced composite (parallel to the ﬁbres) gives e U r ¼ 7:9 1030 ¼ 7:7 103 GPa.m3/kg. e U ¼ 7.9 GPa with a speciﬁc modulus of E E Using the lower bound (equation (4.20)) for the modulus of the particle-reinforced e L ¼ 1.1 GPa with a speciﬁc modulus E e U r ¼ 1:07 103 GPa.m3/ composite gives E kg. The speciﬁc modulus of the ﬁbre-reinforced composite is seven times that of the matrix. That of the particle-reinforced composite is marginally lower than that of the matrix alone.
Foams Foams are made much as you make bread: by mixing a matrix material (the dough) with a foaming agent (the yeast) and controlling what then happens in such a way as to trap the bubbles. Polymer foams are familiar for insulation and ﬂotation, and as the ﬁller in cushions and packaging. You can, however, make foams from other materials: metals, ceramics and even glass. They are light (they are mostly space), and they have low moduli. This might sound a combination of little use, but that is mistaken: if you want to cushion or to protect a delicate object (such as yourself), what you need is a material with a low, controlled stiffness e foams provide this. Figure 4.11 shows an idealised cell of a low-density foam. It consists of hollow cubic cells edged with solid of thickness t, with the length of the cells being L from the mid-thickness of the edges. Cellular solids are characterised by their relative density, the fraction of the foam occupied by the solid. For the structure shown here (with t L), it is t 2 e r ¼3 L rs
where e r is the density of the foam, and rs is the density of the solid of which it is made.
F Cell edge F
Open cell face
Figure 4.11 Idealised foam cell and its elastic response to load.
64 Chapter 4 Elastic stiffness, and weight: atomic bonding and packing When the foam is loaded, the cell walls bend, as shown on the right of the ﬁgure. This behaviour can be modelled (we will be able to do so by the end of the next chapter), giving the e foam modulus E 2 e e r E ¼ (4.22) rs Es where Es is the modulus of the solid from which the foam is made. This gives us a second way of manipulating the modulus, in this case, decreasing it. At a relative density of 0.1 (meaning that 90% of the material is empty space), the modulus of the foam is only 1% of that of the material in the cell wall, as sketched in Figure 4.12. The range of modulus and density for real polymer foams is illustrated in the chart of Figure 4.8 e as expected, they fall below and to the left of the polymers of which they are made. ρs
Young's modulus, E (GPa)
Es Factor 100
Foam with relative density 0.1 10
E Factor 10
Density, ρ (kg/m3)
Figure 4.12 Estimates for modulus and density of foams.
The science: microstructure and properties
We’re going to start with a distinction that has wide-ranging consequences. It is between properties that depend principally on bonding and atom packing (and are largely insensitive to microstructure) and those that are microstructure dependent and can be manipulated by thermomechanical processing (Figure 4.13). Modulus and density, the subject of this chapter, are examples of microstructure-insensitive properties. To understand them, we must drill down to the structure of the atom and the nature of interatomic bonds. Strength and toughness are examples of microstructure-sensitive properties. We return to these (and others) in later chapters.
4.6 Atomic structure and interatomic bonding
Microstructure-insensiƟve properƟes • • • • • • •
Density Mel ng point Modulus Specific heat Expansion coeﬃcient Heat of fusion, heat of vaporiza on Satura on magnetiza on
Microstructure-sensiƟve properƟes • • • • • • •
Strength Toughness Elonga on Thermal conduc vity Electrical conduc vity Coercive field Energy product
Figure 4.13 Properties that don’t depend strongly on microstructure (left) and those that do (right).
Atomic structure and interatomic bonding
The structure of the atom The core of an atom is its nucleus (Figure 4.14). The nucleus accounts for almost all the atomic mass and almost none of its volume. It is made up of protons (þ charge) and neutrons (no charge), known collectively as nucleons. The nucleus of a given element contains protons equal in number to its atomic number but can exist as isotopes with differing numbers of neutrons and thus atomic weights. Isotopes have identical chemical properties but differ in their nuclear properties, particularly in their nuclear stability. Nucleons: neutrons and protons
Figure 4.14 The atomic core. The most stable nuclei are those with the greatest binding energy per nucleon e they cluster around iron, atomic number 26 (Figure 4.15). Nuclei above iron in atomic number can release energy by ﬁssion; those below iron can do so by fusion. Fission releases, at most, a few hundred keV per event; fusion can release much more.
66 Chapter 4 Elastic stiffness, and weight: atomic bonding and packing 10
Iron Chromium Nickel Titanium Zinc Zirconium Silver Silicon Cadmium Samarium Sodium Thorium Iridium Copper Carbon Lead Cobalt Tin Strontium Uranium Aluminum Molybdenum Barium Gold Oxygen Plutonium Nitrogen
Binding energy per nucleon (MeV)
9 8 7
Most stable: Iron
Fuels for fission reactors
Fuels for fusion reactors
Binding energy per nucleon
Figure 4.15 The binding energy per nucleon, a measure of nuclear stability. One might expect that the most stable elements would also be the most abundant in the Earth’s crust. Figure 4.16 shows that, broadly speaking, this is true. Silicon, aluminium, iron, calcium, sodium, magnesium and oxygen, between them, account for over 80% of content of the crust. The high-atomic number platinum group, by contrast, accounts for only 107% (1 part in 109) of it.
Abundance in the Earth's crust (ppm)
Abundance of the elements
Vanadium Chromium Carbon Zinc Copper Scandium Lithium
Cobalt Gallium Fluorine Arsenic
Niobium Tin Cesium
Samarium Hafnium Tungsten
Rhenium Osmium Iridium
Figure 4.16 The abundance of the elements in the Earth’s crust (ppm by mass).
4.6 Atomic structure and interatomic bonding
Example 4.6 The rare earth elements have unique functionality exploited in advanced batteries, high ﬁeld permanent magnets, displays and advanced sensors. Concern is expressed about their availability (they are, after all, called ‘rare earths’), but are they really all that rare? Use the ‘Abundance’ chart to form an opinion. Answer. The abundance of rare earths in the Earth’s crust, 1e100 parts per million, is comparable with that of lithium, cobalt, copper and lead, about 100 times greater than that of silver and 10,000 times greater than that of the platinum group elements.
Electronic structure of atoms Electrons (e charge) orbit the nucleus in discrete, quantised energy levels (Figure 4.17). Their behaviour requires quantum mechanics for explanation. This involves accepting the idea that electrons behave both as particles and as waves, a more diffuse existence in which the probability of their presence in wave mode (shown in green on this and subsequent ﬁgures) has meaning, although their precise position in particle mode (shown as blue spheres) does not. The wavelengths of electrons round an atomic core, like the vibrational modes of a taut string, have discrete values characterised by a principal quantum number n ¼ 1, 2, 3, 4 or 5. The principal shells split into sub-shells corresponding to a second quantum number, taking the values 0, 1, 2 or 3, designated by the letters s, p, d and f.8 Figure 4.17 suggests the ﬁrst ﬁve energy levels (there are more) and the maximum number of electrons each can contain. The ﬁlling of a given orbit is described by the two quantum numbers with a superscript indicating the number of electrons in it e a number that can’t exceed the values indicated on the ﬁgure. Thus, if the ﬁrst, lowermost, orbit (n ¼ 1, sub-shell s) contains two electrons e the maximum allowed e it is described as 1s2. If the level n ¼ 3, sub-shell d has 6 electrons in it (it can hold 10), it becomes 3d6. Filled principal shells impart maximum stability. The inert gases helium (1s2), neon (1s2 e 2s2 2p6) and argon (1s2 e 2s2 2p6 e 3s2 3p6 e 3d10) are so stable that almost nothing reacts with them. Atoms with unﬁlled shells like sodium, with one 3s electron, can revert to the electron count of neon by giving up an electron. Chlorine, with ﬁve 3p electrons, can acquire the electron count of argon by capturing one. Bringing one sodium atom and one chlorine atom together and transferring one electron from the sodium (making it a positive ion) to the chlorine (making it negative) allows both to acquire ‘inert gas’ electron shells (Figure 4.18).
s, p, d, and f stand for ‘sharp’, ‘principal’, ‘diffuse’, and ‘fundamental’, describing the spectral lines of an atom.
68 Chapter 4 Elastic stiffness, and weight: atomic bonding and packing Energy shell 3d 3p 3s 2p 2s 1s
2 2 6 2 6 10
Number of electrons
Figure 4.17 Electron orbitals and the number of electrons they can contain.
Figure 4.18 Electron transfer from Na to Cl, creating positive and negative ions with more stable electron conﬁgurations (1s shell not shown).
As the atomic number of an atom increases, the electrons ﬁll the energy levels, starting with the lowest, the 1s. The electrons in the outermost shell, known as valence electrons, largely determine the chemical character of an atom. This leads to a periodic pattern of properties as the shells ﬁll, moving from inert gas behaviour when a set of shells is ﬁlled completely, to a reactive, electropositive (electron-donating) character as the ﬁrst electrons enter the next level, up to an electronegative (electron-attracting) response when the shell is nearly full, reverting to inert-gas behaviour when the next level is completely full. The cycle is reﬂected in the periodic table of the elements, shown in Figure 4.19.
4.6 Atomic structure and interatomic bonding
Figure 4.19 The periodic table of the elements. Material properties that depend on electronegativity change in a cyclic way across the rows of the periodic table. Figures 4.20 and 4.21 show examples. The ﬁrst is a plot of atomic volume against atomic number, colour-coded row by row. The volume occupied per atom depends on the packing density of atoms in the crystal (and thus on the crystal structure), but the position in the row has a greater inﬂuence: the atomic volume is a minimum in the middle of a row, rising steeply at the ends. This is because the atom ‘size’ reﬂects the radius of the outermost valence shell of electrons. Explaining this needs the concept of screening, the degree to which the inner ﬁlled electron shells block the outer, valence, electrons from the positive charge of the nucleus. We deﬁne the effective nuclear charge, Zeff, as Zeff ¼ Z S Here S is the number of electrons in the inner ﬁlled shells, equal to the atomic number of the noble gas that ends the row above the element in the periodic table. As an example, the S-value for chlorine is 10, the atomic number of neon. The quantity Z is the total number of electrons, equal to the atomic number of the element itself, 17 for chlorine. The 10 inner electrons (S) of chlorine screen out the positive charge of 10 protons, leaving an effective nuclear charge Zeff of (17 10) ¼ þ7 that pulls the outer electrons closer to the nucleus, reducing the atomic radius. The imperfect screening is a maximum in the middle of the row, leading to the minimum. The effective nuclear charge increases, and the atomic volume decreases from left to right across a row in the periodic table. Moving down a column of the periodic table, the number of ﬁlled electron shells increases. The effective nuclear charge remains the same, but now the orbitals are farther from the nucleus, which exerts less pull on the outer electrons, increasing the atomic radius.
70 Chapter 4 Elastic stiffness, and weight: atomic bonding and packing 2x10-28
Row 6 Cesium
Atomic volume (m3)
Bismuth Thorium Curium
Row 2 2x10-29
Atomic volume - Atomic number
Figure 4.20 The cyclic change of atomic volume across the periodic table.
Modulus - Atomic number Carbon
Young's modulus (GPa)
Molybdenum Chromium Iron
Row 6 Osmium
Ruthenium Tungsten Rhodium
Uranium Platinum Hafnium
Silver Rare earths
Gallium Sodium Phosphorus Potassium Rubidium
Figure 4.21 The cyclic change of elastic modulus across the periodic table.
4.6 Atomic structure and interatomic bonding
Figure 4.20 shows atomic volume, not radius. Screening explains the plunging volume from the start of a row towards the middle (lithium to carbon in row 2, for instance), and the slower increase in volume in moving down a column of the periodic table (the sequence lithium e potassium e rubidium e caesium, for example). Superimposed on this is the effect of atom packing: elements at the start of a row are metallic and mostly close-packed. Elements towards the end of a row are non-metallic and have crystal structures with lower packing density. Example 4.7 What is the effective nuclear charge Zeff of aluminium? Would you expect it to have a larger or smaller atomic radius than calcium? Answer. Referring to the periodic table of Figure 4.19, the atomic number of aluminium is Z ¼ 13, and that of the noble gas one row above it in the table, neon, is S ¼ 10. The effective nuclear charge of aluminium is Zeff ¼ 13 10 ¼ 3. The atomic number of calcium is Z ¼ 20, and that of the noble gas above it in the table, argon, is S ¼ 18. The effective nuclear charge of calcium is Zeff ¼ 20 18 ¼ 2. We expect aluminium to be a smaller atom than calcium for two reasons: it has a greater effective nuclear charge, pulling the valence electrons more strongly towards the core, and it lies in row 3 of the periodic table while calcium is in row 4, so the calcium has an extra ﬁlled inner shell, screening its valence electrons from the charge on the core.
Young’s modulus (Figure 4.21) and many other properties show similar progressions. The modulus peaks at the centre of each row, falling sharply at the end of one row and the start of the next. This is partly explained by the cyclic atomic volume shown in the previous ﬁgure: the smaller the atomic volume, the greater the number of bonds per unit volume and the larger the modulus. Superimposed on this is a change in cohesive energy across a row, associated with the number of free electrons per ion (in a metal) and the number of shared electrons (in a covalently bonded solid). We come to that next. Interatomic bonding Many aspects of interatomic bonding can be understood in terms of electronegativity, the propensity of an atom to attract one or more electrons to become a negative ion. Electronegativity is measured on an arbitrary, dimensionless scale proposed by Pauling9 that ranges from 0.7 (francium, the least electronegative) to 4.0 (ﬂuorine, the most), and it, too, varies in a cyclic way across the rows of the periodic table (Figure 4.22). We will use this plot in a moment as a tool for estimating bond type.
Linus Carl Pauling (1901e1994), American chemist and peace activist, twice Nobel laureate, originator of the exclusion principle and author of How to Live Longer and Feel Better advocating massive doses of vitamin C to ward off colds.
72 Chapter 4 Elastic stiffness, and weight: atomic bonding and packing 4.5
Electronegativity of Elements
tals -me Non tals Me
Ni Co Fe Ti
At Po Bi Tl
Row 2 Row 3 Row 4
Figure 4.22 Electronegativity variation with atomic number. As neutral atoms are brought together from inﬁnity, their electrons begin to interact, tending to form a bond. Some bonds are so weak that at room temperature, thermal energy is enough to disrupt them. Others are so strong that, once formed, they are stable to over 3000 C. As the bond forms and the atoms are drawn together, the energy at ﬁrst falls; but when ﬁlled electron shells start to overlap, the energy rises again because, while unﬁlled shells can share electrons, the Pauling exclusion principle prohibits ﬁlled shells from doing the same. This generates a balancing repulsive force, causing the atoms to sit at an equilibrium spacing. The cohesive energy, Hc, is the energy per mol (a mol is 6.022 1023 atoms) required to separate the atoms of a solid completely, giving neutral atoms at inﬁnity. The greater the cohesive energy, the stronger are the bonds between the atoms. We see later that this energy correlates closely with properties that are governed directly by atomic bonding. There is a number of characteristic types of bonding in solids that depend on how the valence electrons interact. They can do this in several ways, of which we’ll examine four. Metallic bonding About 80% of the elements of the periodic table are metals e the box lists some examples, showing the wide range of cohesive energy. Valence electrons in metallic solids detach themselves from their parent atoms (leaving them as positive ions) and form a negatively charged swarm of almost-freely moving charge carriers (Figure 4.23). The swarm screens the array of positive ions from their mutual repulsion, shutting each off,
4.6 Atomic structure and interatomic bonding
so to speak, from its repulsive neighbours. The coulombic attraction between the swarm and the array of positive ions Metallic bonded materials Hc ¼ 60850 kJ/mol creates the bond. It is not directional, so metallic solids are Copper usually close-packed because this minimises the average disAluminium tance between the positively charged ions and the negatively Lead charged electron swarm. Electronegative atoms attract rather Tungsten than donate electrons, so they are generally non-metallic. Those that are electropositive do the opposite, so that a boundary (blue line) can be sketched onto Figure 4.22, dividing the elements on it, very roughly, into those with metallic character and those with non-metallic.
3s 2p 2s
Figure 4.23 Metallic bonding in magnesium. The two 3s valence electrons detach and move freely through the array of positively charged ions. An electric ﬁeld, applied to a metallic solid, exerts a force on the free, or nearly free, electrons, accelerating them in the direction of the ﬁeld. If they are totally free, they move without resistance, and the material is superconducting. A few materials, when at very low temperatures, are superconducting. In most, the electrons are scattered as they move, giving what we know as ‘resistivity’. More on this in Chapter 15. Ionic bonding If a strongly electro-positive atom approaches one that is strongly electronegative, there is a tendency for Ionically bonded materials Hc ¼ 6001600 kJ/mol electrons to leave the ﬁrst and join the second, giving both ﬁlled Sodium chloride, NaCl outer shells in the way illustrated by Figure 4.18. The ﬁrst atom Potassium chloride, KCl acquires a positive charge, the second a charge that is negative, Calcium chloride, CaCl2 and the two are drawn together by coulombic attraction. The Magnesium oxide, MgO resulting ionic bond is non-directional, attracting equally in all directions. Ionically bonded compounds tend to form when the difference in electronegativity of the atoms (plotted in Figure 4.22) is greater than 1.7. Crystal structures held together by ionic crystals must meet two further conditions: that of overall charge neutrality and that of ensuring that every positive ion has only negative ions as its nearest neighbours and vice versa. The box lists some common ionically bonded materials. The cohesive energy is generally higher than for metallic bonding.
74 Chapter 4 Elastic stiffness, and weight: atomic bonding and packing Covalent or molecular bonding Covalent bonding is so Covalently bonded materials called because it arises from the sharing of valence electrons Hc ¼ 1001200 kJ/mol between atoms in such a way that each acquires an inert-gas Diamond electron structure. It operates in a diverse range of elements Silicon and compounds, including carbon crystals and molecules, Polyethylene, along chain with cohesive energies spanning a wide range overlapping Quartz both metallic and ionic bonding (see box). To understand covalent bonding, however, we start with the water molecule (Figure 4.24). Here the 1s electrons of the two hydrogens are shared with the almost-full 2p shell of the oxygen, giving it the electron structure of neon. It, in turn, shares an electron with each hydrogen, giving them the helium conﬁguration.
Figure 4.24 Covalently bonded water molecule.
Covalent bonds tend to form in molecules when the electronegativity difference between the two atoms is less than 1.7. For water, this difference is 1.4, large enough that the electrons tend to spend more time on the oxygen than on the two hydrogens, giving a polar bond (i.e. the bond is directional, with a permanent dipole moment). When the difference is less than about 0.4, the electrons are more equally shared, and the bond is non-polar. Carbon, particularly, forms strong covalent bonds both with itself and with other atoms. To understand these, we need the idea of orbital mixing or hybridisation. Carbon, 1s2 2s2 2p2, can mix 2s with 2p electrons to create new orbitals that have directionality (Figure 4.25). Mixing one 2s electron with the two 2p electrons gives three sp2 orbits lying in a plane and directed at 120 degrees to each other. Mixing all four 2s with 2p electrons gives four new sp3 orbits directed at the four corners of a tetrahedron. Each hybrid orbit can hold two electrons but has only one until it shares it with another atom, creating a covalent bond.
4.6 Atomic structure and interatomic bonding
Figure 4.25 sp2 and sp3 orbitals of carbon atoms.
These new orbits have fundamental signiﬁcance for the compounds of carbon. Graphite is a hexagonal net of sp2-bonded carbon atoms, each of the three orbits sharing its one electron with another identical atom to form covalently bonded sheets. Diamond is a threedimensional network of sp3-bonded carbon atoms, similarly bonded to other identically hybridised C atoms. Many polymers and many organic molecules are based on sp3-bonded carbon: two of the four orbits are used to make long chain molecules, with other atoms (such as hydrogen) or molecular groups being attached to the other two. The bonding within the polymer chain is covalent, but we also need to consider the bonding between them e that comes next. Dipolar or van der Waals bonding Inert gases become Dipolar-bonded materials liquid or solid at sufﬁciently low temperatures. They Hc ¼ 750 kJ/mol already have full electron shells, so what is binding the Ice atoms together? The bond has its origins in dipoleedipole Dry ice (solid CO2) attraction, illustrated in Figure 4.26. The charge distribuParafﬁn wax tion on an atom ﬂuctuates as the electrons move; at any Polyethylene, between chains instant, the charge is unevenly distributed, giving the atom a temporary dipole moment. The dipole of one atom induces a dipole in an adjacent atom and the pair of dipoles attract, creating a weak bond. Dipolar bonding can arise in another way. As explained above, polar covalent bonds like that of water (Figure 4.24) carry a permanent dipole moment. It is this that binds water molecules together to form ice. The same dipolar bonding glues one polymer chain to its neighbours, such as in polyethylene (PE) and polypropylene. The box shows that the cohesive energy associated with dipolar bonding is much lower than metallic, ionic or covalent.
76 Chapter 4 Elastic stiffness, and weight: atomic bonding and packing 2p 2s
Figure 4.26 Dipolar attraction between neutral atoms. Example 4.8 Boron sulphide is used in high-tech glasses. Would you anticipate that it has metallic, ionic or covalent bonding? Use the electronegativity chart of Figure 4.22 to reach a conclusion. Answer. Both boron and sulphur are non-metals. The difference in their electronegativity is about 0.5 on the Pauling scale, far below the value of 1.7 at which ionic bonding become dominant. We anticipate that the bonding is covalent.
Atomic and molecular packing in solids: the origin of density Introduction to Guided Learning Unit 1: Simple ideas of crystallography
The properties of materials depend on the way the atoms or molecules within them are packed. In glasses, the arrangement is a disordered one with no regularity or alignment. Polymers are largely made up of tangled long-chain molecules. Metals and ceramics, by contrast, are crystalline, with a regularly repeating pattern of atomic packing in structural units. Crystals are described using the language of crystallography, which provides a framework for understanding their three-dimensional geometry. The key ideas of crystallography are introduced brieﬂy in the following pages. Later in the book, you will ﬁnd Guided Learning Unit 1: Simple ideas of crystallography, which develops the ideas in greater depth. The rest of this chapter will be intelligible without reference to the unit, but working through it and its exercises will give more complete understanding and conﬁdence.
Atom packing in metals and the unit cell Atoms often behave as if they were hard, spherical balls. The balls on a pool table, when set, are arranged as a close-packed layer, as shown in Figure 4.27(a). The atoms of many metals form extensive layers packed in this way. There is no way to pack the atoms more closely than this, so this arrangement is called ‘close-packed’. These two-dimensional layers of atoms can then be close-packed in three dimensions. Surprisingly, there are two ways to do this. Where three atoms meet in the ﬁrst layer, layer A, there are natural depressions for atoms of a second close-packed layer B. A third layer can be added
4.7 Atomic and molecular packing in solids: the origin of density
such that its atoms are exactly above those in the ﬁrst layer, so that it, too, is in the A orientation, and the sequence is repeated to give a crystal with ABABAB . stacking, as in Figure 4.27(b); it is called close-packed hexagonal, or CPH (sometimes HCP) for short, for reasons explained in a moment. But there is an alternative stacking sequence. In placing the third layer, there are two choices of position e one aligned with A (as before), and one offset from layer A, giving a third layer, C, that is nested onto B in this alternative position. This stacking becomes (on repeating) ABCABCABC . as shown in Figure 4.27(c); it is called face-centred cubic (FCC for short). Many metals, such as copper, silver, aluminium and nickel, have the FCC structure; many others, such as magnesium, zinc, and titanium, have the CPH structure. The two alternative structures have the same packing fraction, 0.74, meaning that the spheres occupy 74% of the available space. But the small difference in layout inﬂuences properties, particularly those having to do with plastic deformation (Chapter 6).
(a) Close-packed layer A
(b) Layer B on layer A to give ABABAB ... or CPH packing
(c) Layer C on layers A and B to give ABCABC ... or FCC packing
Figure 4.27 Close packing of spheres. Not all structures are close-packed. Figure 4.28 shows one of these, made by stacking square-packed layers. It has a lower packing density than the hexagonal layers of the FCC and CPH structures. An ABABAB . stacking of these layers builds the body-centred cubic structure, BCC for short, with a packing fraction of 0.68. Iron and most steels have this structure. There are many other crystal structures, but for now these three are enough, covering most important metals.
(a) Non close-packed layer A
Figure 4.28 Square packing of spheres.
(b) Layer B on layer A to give ABABAB... or BCC packing
78 Chapter 4 Elastic stiffness, and weight: atomic bonding and packing A regular packing of atoms that repeats itself is called a crystal. It is possible to pack atoms in a non-crystallographic way to give what is called an amorphous structure, sketched in Figure 4.29. This is not such an efﬁcient way to ﬁll space with spheres; the packing fraction is 0.64 at best.
(a) A non-crystallographic layer
(b) An amorphous or non-crystallographic structure
Figure 4.29 Amorphous structures. The characterising unit of a crystal structure is its unit cell. Figure 4.30 shows three; the red lines deﬁne the cell. The atoms have been shrunk to reveal the cell more clearly; in reality, they touch in close-packed directions. In the ﬁrst, shown at (a), the cell is a hexagonal prism. The atoms in the top, bottom and central planes form close-packed layers like that of Figure 4.27(b), with ABAB . stacking e that’s why this structure is called CPH. The second, shown at (b), is also made up of close-packed layers, though this is harder to see; the shaded triangular plane is one of them. If we think of this as an A plane, atoms in the plane above it nest in the B position, and those in the plane below it, in the C position, giving ABCABC . stacking, as in Figure 4.27(c). The unit cell itself is a cube with an atom at each corner and one at the centre of each face e for this reason, it’s called FCC. The ﬁnal cell, shown at (c), is the characterising unit of the square-layer structure of Figure 4.28; it is a cube with an atom at each corner and one in the middle, called, appropriately, BCC.
(a) The CPH unit cell
(b) The FCC unit cell
(c) The BCC unit cell
Figure 4.30 The close-packed hexagonal (CPH), face-centred cubic (FCC), and body-centred cubic (BCC) unit cells. All atoms are the same but are shaded differently to emphasise their positions.
4.7 Atomic and molecular packing in solids: the origin of density
Unit cells pack to ﬁll space as in Figure 4.31. The resulting array is called the crystal lattice; the points at which cell edges meet are called lattice points. The crystal itself is generated by attaching one or a group of atoms to each lattice point so that they form a regular, threedimensional, repeating pattern. The cubic and hexagonal cells are among the simplest; there are many others with edges of differing lengths meeting at differing angles. The one thing they have in common is their ability to stack with identical cells to completely ﬁll space.
Figure 4.31 Unit cells stacked to ﬁll space. (a) The hexagonal cell. (b) The cubic cell. (c) A cell with edges of differing length that do not meet at right angles. Atom packing in ceramics Most ceramics are compounds, made up of two or more atom types, ionically or covalently bonded. They, too, have characteristic unit cells. Figure 4.32 shows those of two materials that appear on the property charts: tungsten carbide (WC) and silicon carbide (SiC). The cell of the ﬁrst is hexagonal; that of the second is cubic, but now a pair of different atoms is associated with each lattice point: a WeC pair in the ﬁrst structure and a SieC pair in the second. More examples are investigated in Guided Learning Unit 1.
(a) The tungsten carbide unit cell
Figure 4.32 Unit cells of compounds.
(b) The silicon carbide unit cell
80 Chapter 4 Elastic stiffness, and weight: atomic bonding and packing Atom packing in glasses The crystalline state is the lowest energy state for elements and compounds. Melting disrupts the crystallinity, scrambling the atoms and destroying the regular order. The atoms in a molten metal look very like the amorphous structure of Figure 4.29. On cooling through the melting point, most metals crystallise easily, though by cooling them exceedingly quickly, it is sometimes possible to trap the molten structure to give an amorphous metallic ‘glass’. With compounds, it is easier to do this, and with one in particular, silica (SiO2), crystallisation is so sluggish that its usual state is the amorphous one. Figure 4.33 shows, on the left, the atom arrangement in crystalline silica: identical hexagonal SieO rings, regularly arranged. On the right is the more usual amorphous state. Now some rings have seven sides, some have six, some ﬁve, and there is no order e the next ring could be any one of these. Amorphous silica is the basis of almost all glasses; it is mixed with Na2O to make soda glass (windows, bottles) and with B2O5 to make borosilicate glasses (Pyrex), but it is the silica that gives the structure. It is for this reason than the structure itself is called ‘glassy’, a term used interchangeably with ‘amorphous’.
Figure 4.33 Two alternative structures for silica, the basis of most glasses. (a) Crystalline silica. (b) Glassy or amorphous silica.
Atom and molecular packing in polymers Polymer structures are quite different. The backbone of a ‘high’ polymer (‘high’ means high molecular weight) is a long chain of sp3-hybridised carbon atoms to which side groups are attached. Figure 4.34 shows a segment of the simplest: polyethylene, PE (eCH2e)n. The chains have ends; the ends of this one are capped with a CH3 group. PE is made by the polymerisation (snapping together) of ethylene molecules, CH2¼CH2, where the ¼ sign is a double bond, broken by polymerisation to give covalent sp3 links to more carbon neighbours to the left and right. Figure 4.35 shows the chain structure of four more of the most widely used linear polymers.
4.7 Atomic and molecular packing in solids: the origin of density
sp3 hybrid Carbon
H H H H H H H H -C-C-C-C-C-C-C-CH H H H H H H H
or - (CH2)n -
Figure 4.34 Polymer chains have a carbonecarbon backbone with hydrogen or other side groups. The ﬁgure shows three alternative representations of the polyethylene molecule.
- (CH2 - CH)n -
Cl Polyvinyl chloride, PVC
F C F
- (CF2)n -
- (CH2 - CH)n -
Cl C H
- (CH2 - CH)n -
F C F
F C F
H H C - C Cl H
F C F
F C F
Cl H C - C H H
F C F
H H C 6 H5 C - C - C H C6H5 H H
F C F
H H C - C Cl H
F C F
H C H
H C6 H5 H C - C - C H
H C6 H5 H
H H H CH3 H H H CH3 C - C - C - C - C - C - C - C H CH3 H H H CH3 H H
Figure 4.35 Four more common polymers, showing the chemical makeup. The strong carbonecarbon bonds are shown in red. Polymer molecules bond together to form solids. The carbonecarbon chains that form the backbone of a linear polymer are covalently bonded and strong. The molecules attract each other, but only weakly (Figure 4.36(a)); the weak dipole ‘hydrogen’ bonds that make them stick are easily broken or rearranged. The resulting structure is sketched in Figure 4.37(a): a dense spaghetti-like tangle of molecules with no order or crystallinity. This is the structure of polymers like those of Figure 4.35; the weak bonds melt easily, allowing the polymer to be moulded when hot e in other words, they are thermoplastic.
82 Chapter 4 Elastic stiffness, and weight: atomic bonding and packing Strong covalent bond
(a) Weak hydrogen bond
Strong covalent bond
(b) Strong covalent cross-link
Figure 4.36 The bonding between polymer chains: dipolar hydrogen bonds and covalent cross-links. Polymer chains
(a) Non-cross-linked Cross links
(c) Slightly cross-linked
(b) Partly crystalline Cross links
(d) Highly cross-linked
Figure 4.37 Polymer structures: (a) amorphous thermoplastic; (b) semi-crystalline thermoplastic; (c) elastomer; (d) thermoset.
4.8 Interatomic bonding and properties: the origin of elastic modulus
The weak bonds of thermoplastics do, however, tend to line segments of the molecules up. Total alignment is not possible, but where segments of molecules manage it, there are small crystalline regions, as in Figure 4.37(b). These crystallites are small e often between 1 and 10 microns across, just the right size to scatter light. So amorphous polymers with no crystallites can be transparent; polycarbonate (PC), polymethyl-methacrylate (PMMA, Plexiglas) and polystyrene (PS) are examples. Those that are semi-crystalline, like PE and nylon (PA), scatter light and are translucent. The real change comes when chains are cross-linked by replacing some of the weak hydrogen bonds by much more muscular covalent CeC bonds, as in Figure 4.36(b), making the whole array into one huge multiply connected network. Elastomers (rubbery polymers) have relatively few cross-links, as in Figure 4.37(c). Thermosets like epoxies and phenolics have many cross-links, as in Figure 4.37(d), making them stiffer and stronger than thermoplastics. The cross-links are not broken by heating, so once the links have formed, elastomers and thermosets cannot be thermally moulded or (for that reason) recycled. Physical origin of density Atoms differ greatly in weight but little in size. Among solids, the heaviest stable atom, uranium (atomic weight 238), is about 35 times heavier than the lightest, lithium (atomic weight 6.9), yet when packed to form solids, their diameters are almost exactly the same (0.32 nm). The largest atom, caesium, is only 2.5 times larger than the smallest, beryllium. So density is mainly determined by the atomic weight and only to a lesser degree by the atom size and the way they are packed. Metals are dense because they are made of heavy atoms, packed densely together (iron, for instance, has an atomic weight of 56). Ceramics, for the most part, have lower densities than metals because they contain light Si, O, N or C atoms. Polymers have low densities because they are largely made of light carbon (atomic weight: 12) and hydrogen (atomic weight: 1) in low-density amorphous or semi-crystalline packings. The lightest atoms, packed in the most open way, give solids with a density of around 1000 kg/m3 e the same as that of water (see Figure 4.8). Materials with lower densities than this are foams (and woods), made up of cells containing a large fraction of pore space. Density of metallic alloys Most metallic alloys are not pure but contain two or more different elements. Often they dissolve in each other, like sugar in tea, but as the material is solid, we call it a solid solution; examples are brass (a solution of Zn in Cu) and stainless steel (a solution of Ni and Cr in Fe). As we shall see in later chapters, some material properties are changed a great deal by making solid solutions; density is not. As a rule, the density e r of a solid solution lies between the densities rA and rB of the materials that make it up, following a rule of mixtures (an arithmetic mean, weighted by volume fraction) known, in this instance, as Vegard’s law: e r ¼ f rA þ ð1 f ÞrB
where f is the fraction of A atoms.
Interatomic bonding and properties: the origin of elastic modulus
Recall from Section 4.6 the cohesive energy, Hc, is the energy per mol required to separate the atoms of a solid completely, giving neutral atoms at inﬁnity (Figure 4.38). The greater the cohesive energy, the stronger are the bonds between the atoms. Materials with strong bonds have high melting points and high elastic moduli. Figure 4.39 shows the correlation between absolute melting temperature, Tm (here multiplied by the gas constant, R), and cohesive energy, Hc. The relationship is linear; the thermal energy RTm at the melting point is about 3% of the cohesive energy.
84 Chapter 4 Elastic stiffness, and weight: atomic bonding and packing
Cohesive energy Hc Atom spacing a
Figure 4.38 Cohesive energy.
Melting point - Cohesive energy Melting temperature *Gas Const. (kJ/mol)
Tantalum Molybdenum Niobium
Strontium Aluminum Antimony Zinc Lead
RTm = 0.03 Hc Tin
Cohesive energy (kJ/mol)
Figure 4.39 Melting temperature and cohesive energy of the elements.
4.8 Interatomic bonding and properties: the origin of elastic modulus
The resistance of an elastic solid to 3D expansion like that sketched in Figure 4.38 is characterised by the bulk modulus K. Consider the work done if the volume occupied by one atom, Vo, is expanded by a volume DV e this is KDV=Vo (per unit volume). Let the critical expansion be DV*¼Vo/C*, at which point the bonds break, absorbing the cohesive energy, Hc; then if the molar volume is Vm: K
DV K Hc ¼ ¼ C Vo Vm
or KVm ¼ C Hc
Figure 4.40 is a plot of KVm against Hc for the elements, showing that this approximate linear relationship holds. The critical expansion constant C* z 3.5, implying that a volume expansion of 1/3.5, or 30% (equivalent to a linear bond stretch of 10%), is enough to break the bond completely. 10000
Modulus - Cohesive energy
Bulk modulus x Molar volume (kJ/mol)
Chromium Manganese Iron
K.Vm = 3.5 Hc
Cohesive energy (kJ/mol)
Figure 4.40 Bulk modulus and cohesive energy of the elements. Bond stiffness and elastic moduli Think of atomic bonds as little springs linking the atom centres. Figure 4.41 shows the springs and the way the energy stored in them changes as the atoms are pulled apart or pushed together e it is an enlargement of the energy minimum in Figure 4.38. When no force is applied, the atoms have equilibrium spacing ao; a force F pulls them apart a little, to ao þ d. A spring that stretches by d under a force F has a stiffness, S, of: S¼
86 Chapter 4 Elastic stiffness, and weight: atomic bonding and packing
Force F Tension
Spring stiffness S
Energy U = Fδ/2 a o+ δ
Equilibrium atom position
Figure 4.41 Bond stretching. A force F applied to an atom of diameter ao corresponds to a stress s ¼ F a2o assuming each atom occupies a cube of side ao. A stretch of d between two atoms separated by a distance ao corresponds to a strain ε ¼ d/ao. Substituting these into equation (4.25) gives s¼
S ε ¼ Eε ao
from which E¼
Table 4.1 lists the stiffness of the different bond types and corresponding ranges for Young’s modulus, E. The covalent bond is particularly stiff; diamond has a very high modulus because the carbon atom is small (giving a high bond density), and its atoms are linked by very stiff springs (S ¼ 200 N/m). For most engineering metals, the metallic bond is somewhat less stiff (S ¼ 8e60 N/m). But metals are close-packed, or nearly so, giving them high moduli e though not as high as that of diamond. Alloys contain a mixture of metallic bonding, between similar and dissimilar atoms, but these are of comparable stiffness. So when two elements are mixed, the modulus generally lies between those of the pure metals. Ionic bonds, found in many ceramics, have stiffnesses comparable with those of metals, giving them high moduli too.
4.8 Interatomic bonding and properties: the origin of elastic modulus
Table 4.1 Bond energies, stiffnesses and moduli Bond type
Cohesive energy Hc (kJ/mol)
Bond stiffness S (N/m)
Young’s modulus E (GPa)
Covalent Metallic Ionic Dipolar
Carbonecarbon bond Engineering metals Sodium chloride Polyethylene
100e1200 60e850 600e1600 7e50
20e200 8e60 4e100 0.5e5
100e1000 20e400 30e400 0.5e5
As noted earlier, the stiffness of a single crystal metal or ceramic will vary with direction relative to the atomic packing e they are anisotropic at the crystal scale. Most solids are polycrystalline, containing very many grains stuck together, each with their own lattice orientation (we return to this in Chapter 6). This averages out the directionality in the crystal stiffness, giving isotropic elastic moduli. Polymers contain both strong covalent bonds along the polymer chain and weak hydrogen or van der Waals bonds (S ¼ 0.5e5 N/m) between the chains; it is the weak bonds that stretch when the polymer is deformed, giving them low moduli. The random molecular structure is automatically isotropic. However, if the polymer is heavily drawn, the molecules align enough for the covalent bonds to be stretched, giving a much higher modulus (see the right-hand end of the polymer stressestrain curve of Figure 4.4). This is exploited in the production of polymer ﬁbres, giving properties that are anisotropic and far superior along the ﬁbre compared to a bulk polymer. This is discussed further in Chapter 19. Table 4.1 allows an estimate to be made of the lower limit for Young’s modulus for a true solid. The largest atoms (ao ¼ 4 1010 m) bonded with the weakest bonds (S ¼ 0.5 N/m) will have a modulus of roughly E¼
0:5 z1 GPa 4 1010
Many polymers do have moduli of about this value. But as the E/r chart (Figure 4.8) shows, materials exist that have moduli that are much lower than this limit. They are either foams or elastomers. As we have seen, foams have low moduli because the cell walls bend easily when the material is loaded (Section 4.4). The origin of the moduli of elastomers takes a little more explaining. The elastic moduli of elastomers An elastomer is a tangle of long-chain molecules with occasional cross-links, as in Figure 4.42(a). The bonds between the molecules, apart from the cross-links, are weak e so weak that, at room temperature, they have melted, meaning that segments are free to slide over each other. Were it not for the cross-links, the material would have no stiffness at all; it would be a viscous liquid.
88 Chapter 4 Elastic stiffness, and weight: atomic bonding and packing
Figure 4.42 Elastomer extension induces order, reducing entropy. Thermal energy tends to restore it. The tangled structure of Figure 4.42(a) has high randomness, or as expressed in the language of thermodynamics, its entropy is high. Stretching it, as in Figure 4.42(b), aligns the molecules: some parts of it now begin to resemble the crystallites of Figure 4.37(b). Crystals are ordered; their entropy is low. Thermal energy displaces atoms, tending to increase entropy again. So here there is a resistance to stretching e a stiffness e that has nothing to do with bond stretching but with thermal pushback to strain-induced molecular ordering. The cross-links give the elastomer a ‘memory’ of the disordered shape it had to start with, allowing large strains that are elastic and fully recoverable. A full theory is complicated e it involves the statistical mechanics of long-chain tangles e so it is not easy to estimate the value of the modulus. The main thing to know is that the modulus of an elastomer is low because it has this strange thermodynamic origin, and (as a side effect) the modulus increases with temperature (unlike that of all other solids) because it is thermal pushback that is providing the stiffness. Temperature dependence of polymer moduli: the glass transition temperature Crystalline solids have well-deﬁned, sharp melting points. Amorphous polymers behave in a different way e bonding is weaker and more diffuse, with the inter-chain bonding spread over a spectrum of atomic spacing because of the tangled molecular structure. The amorphous regions gradually change properties from solid to liquid over a range centred on the glass transition temperature, Tg, as the weak inter-chain bonds progressively melt on heating. In semi-crystalline thermoplastics, however, the crystallites have their own sharp melting temperature, typically about 1.5 Tg, due to the closer, regular packing of the chains. Elastomers and thermosets have a glass transition but do not melt on heating e because of the cross-linking, they degrade and burn instead.
4.8 Interatomic bonding and properties: the origin of elastic modulus
How does the glass transition affect the Young’s modulus? The answer is dependent on the type of polymer, since even if the weak bonding has gone, there can still be elastic behaviour above Tg. Figure 4.43 shows schematics of the variation of modulus with temperature. Below Tg, polymers are referred to as glassy, with the modulus controlled by the hydrogen bonding. Above Tg, amorphous thermoplastics (left-hand ﬁgure), show a tiny residual elasticity that stems from entanglements in the molecular structure, blurring into viscous ﬂow. Semicrystalline thermoplastics also show a drop in modulus across their glass transition, of the order of 10 times if the crystallinity is high, to a broad plateau in modulus where the response is referred to, somewhat misleadingly, as ‘rubbery’. The degree of crystallinity determines how stiff the material remains above Tg, but eventually all thermoplastics melt and ﬂow. Note the position of room temperature (RT) relative to Tg e in amorphous thermoplastics, Tg effectively sets the upper limit of usefulness of the polymer; in semi-crystalline, it sets the lower limit (due to their brittleness in the glassy state). Cross-linked behaviour is shown in Figure 4.43(b). Elastomers display a dramatic drop in modulus through Tg, by a factor of order 1000; the very low modulus of rubbers reﬂects the fact that at room temperature the material is already above Tg. The effect is well illustrated by immersing a rubber tube in liquid nitrogen, when it becomes stiff and brittle! Thermosets have a much higher degree of cross-linking, retaining a higher modulus as temperature falls, with heavily cross-linked thermosets barely showing a glass transition effect at all.
Young’s modulus, E
Young’s modulus, E
Figure 4.43 Schematic temperature dependence of Young’s modulus for: (a) thermoplastics
(amorphous and semi-crystalline); (b) elastomers and thermosets. The glass transition temperature Tg is where the weak inter-chain bonding is lost. RT indicates room temperature.
90 Chapter 4 Elastic stiffness, and weight: atomic bonding and packing Polymer deformation shows other unusual characteristics. Since stretching the material is accompanied by some sliding of the molecules past one another, the stiffness is particularly sensitive to the rate of loading. Rapid loading does not give time for chain sliding; slow loading enables it, giving a quite different response. The glass transition temperature is therefore sensitive to the deformation rate. So at the same temperature, a polymer can switch from being ﬂoppy and resistant to fracture, to being much stiffer and glass-like, by pulling on it rapidly. Design to cope with the effect of temperature on polymers is discussed further in Chapter 13.
Summary and conclusions
When a solid is loaded, it initially deforms elastically. ‘Elastic’ means that when the load is removed, the solid springs back to its original shape. The material property that measures stiffness is the elastic modulus. We need three of them to deal with the different ways in which solids can be loaded:
Young’s modulus, E, measuring resistance to stretching and compressing; shear modulus, G, measuring resistance to twisting; and bulk modulus, K, measuring resistance to hydrostatic compression.
Many applications require stiffness at low weight, particularly ground, air and space vehicles, and that means a high modulus E and a low density r. The E-r property chart helps visualise this information and relate it to material classes. The moduli have their origins in the stiffness of the bonds between atoms in a solid and in the packing of the atoms and thus the number of bonds per unit area. The atomic packing does not vary much from one solid to another, so the moduli mainly reﬂect the stiffness of the bonds. Bonding can take several forms, depending on how the electrons of the atoms interact. Metallic, covalent and ionic bonds are stiff; dipolar bonds are much less so, which is why steel has high moduli and PE has low. Bonding can be understood in terms of the electronegativity of atoms: their propensity to capture one or more electrons to become negative ions. A large difference in electronegativity between two elements favours ionic bonding; a small difference or no difference at all favours covalent bonding. The density of a material is the weight of its atoms divided by the volume they occupy. Atoms do not differ much in size and packing, but they differ a great deal in weight. Thus the density is principally set by the atomic weight; as a general trend, the further down the periodic table we go, the greater the density. There is very little that can be done to change the bond stiffness or atomic weight and packing of a solid, so at ﬁrst sight, we are stuck with the moduli and densities of the materials we already have. But there are two ways to manipulate them: by mixing two materials to make composites, or by mixing a material with space to make foams. Both are powerful ways of creating ‘new’ materials that occupy regions of the Eer map that were previously empty.
Ashby, M. F. (2017). Materials selection in mechanical design (5th ed.). Oxford: Butterworth Heinemann. ISBN 978-0-08-100599-6. (A text that takes the analysis of stiffness and moduli in this chapter to a higher level.) Askeland, D. R., Phulé, P. P., & Wright, W. J. (2010). The science and engineering of materials (6th ed.). Toronto, Canada: Thomson. ISBN 9780495296027. (A well-established materials text that deals well with the science of engineering materials.) Budinski, K. G., & Budinski, M. K. (2010). Engineering materials, properties and selection (9th ed.). NY, USA: Prentice Hall. ISBN 978-0-13-712842-6. (Like Askeland, this is a well-established materials text that deals well with both material properties and processes.) Callister, W. D., & Rethwisch, D. G. (2014). Materials science and engineering: An introduction (9th ed.). New York, USA: John Wiley & Sons. ISBN 978-1-118-54689-5. (A well-established text taking a science-led approach to the presentation of materials teaching.) Shackelford, J. F. (2014). Introduction to materials science for engineers (8th ed.). NJ, USA: Prentice Hall. ISBN 978e0133789713. (A well-established materials text with a materials and a design slant.)
Identify which of the ﬁve modes of loading (Figure 4.2) is dominant in the following components:
·· ·· ·· ··
Fizzy drinks container Overhead electric cable Shoe soles Wind turbine blade Climbing rope Bicycle forks Aircraft fuselage Aircraft wing spar
Can you think of another example for each mode of loading? Exercise E4.2
The cable of a hoist has a cross-section of 80 mm2. The hoist is used to lift a crate weighing 500 kg. What is the stress in the cable? The free length of the cable is 3 m. How much will it extend if it is made of steel (modulus 200 GPa)? How much if it is made of polypropylene, PP (modulus 1.2 GPa)?
Water has a density of 1000 kg/m3. What is the hydrostatic pressure at a depth of 100 m? How many times atmospheric pressure is this (1 atm ¼ 0.1 MPa)?
92 Chapter 4 Elastic stiffness, and weight: atomic bonding and packing
Figure 4.5 shows a cubic element of material with Young’s modulus E and Poisson’s ratio n that is subjected to normal stresses s1, s2 and s3, resulting in strains ε1, ε2 and ε3 (equation (4.13)). (a) Find an expression for the dilatation D (fractional volume change) when a unit cube experiences strains of ε1, ε2 and ε3, assuming the strains are elastic and therefore small (1). (b) Find the dilatation D for an element subjected to a uniaxial tensile stress s1 ¼ s (i.e. s2 ¼ s3 ¼ 0). For what value of Poisson’s ratio is volume conserved? (c) Find the dilatation D for an element subjected to equal pressure p in all directions, i.e. s1 ¼ s2 ¼ s3 ¼ ep. Hence, derive the formula relating the bulk modulus, K, to Young’s modulus, E, and Poisson’s ratio, n (equation (4.10)).
A mounting block made of butyl rubber of modulus ¼ 0.0015 GPa is designed to cushion a sensitive device against shock loading. It consists of a cube of the rubber of side length L ¼ 40 mm located in a slot in a rigid plate, exactly as shown in Figure 4.6. The slot and cube have the same crosssectional dimensions, and the surrounding material is much stiffer, so the strain in one direction is constrained to be zero. A vertical compressive load F is applied, and the downward deﬂection of the top of the block is d. The maximum expected value of F is 50 N. Use equation (4.14) to ﬁnd the stiffness of the cube (F/d) in this constrained condition, assuming n z 0.5. Hence ﬁnd the maximum deﬂection d of the top face of the block. What would this deﬂection be without any constraint?
A cube of linear elastic material is again subjected to a vertical compressive stress s1 in the 1-direction, but is now constrained (ε ¼ 0) in both the 2 and the 3 directions. (a) Find expressions for the induced transverse stresses, s2 and s3 in terms of s1. Hence, derive an expression for the ‘effective modulus’ (s1/ε1) in this case. (b) Sketch the variation of effective modulus with n, and comment on the limiting values when n ¼ 0 (foam) and n z 0.5 (rubber). (c) Explain why the rubber soles of running shoes are designed with some combination of air or gel pockets, partially foamed rubber, and a tread.
A catapult has two rubber arms, each with a square cross-section with a width 4 mm and length 300 mm. In use, its arms are stretched to three times their original length before release. Assume the modulus of rubber is 103 GPa and that it does not change when the rubber is stretched. How much energy is stored in the catapult just before release?
Use the modulusedensity chart of Figure 4.8 to ﬁnd, from among the materials that appear on it: (a) (b) (c) (d)
the material with the highest density the metal with the lowest modulus the polymer with the highest density the approximate ratio of the modulus of woods measured parallel to the grain and perpendicular to the grain (e) the approximate range of modulus of elastomers (f) the range of modulus of CFRP (carbon ﬁbre-reinforced plastic)
Both magnesium alloys and CFRP have excellent stiffness-to-weight characteristics as measured by the ratio E=r, but which is the better of the two? Draw a contour of E=r onto a copy of Figure 4.8 and use it to resolve the question.
The density r of carbon steel is 7500 kg/m3, and its Young’s modulus E is 210 GPa. What is the velocity of longitudinal sound waves in steel? Watch the units! pﬃﬃﬃﬃﬃﬃﬃﬃﬃ The speed of longitudinal waves in a material is proportional to E=r. Plot contours of this quantity onto a copy of a modulusedensity chart allowing you to read off approximate values for any material on the chart. Which metals have the about the same sound velocity as steel? Does sound move faster in titanium or glass?
Derive the upper and lower bounds for the modulus of a composite quoted as equations (4.19) and (4.20) of the text. To derive the ﬁrst, assume that the matrix and reinforcement behave like two springs in parallel (so that each must strain by the same amount), each with a stiffness equal to its modulus E multiplied by its volume fraction f. To derive the second, assume that the matrix and reinforcement behave like two springs in series (so that both are stressed by the same amount), again giving each a stiffness equal to its modulus E multiplied by its volume fraction, f.
A volume fraction f ¼ 0.2 of silicon carbide (SiC) particles is combined with an aluminium matrix to make a metal matrix composite. The modulus and density of the two materials are listed in the table. The modulus of particlereinforced composites lies close to the lower bound, equation (4.20), discussed in the text. Calculate the density and approximate modulus of the composite. Is the speciﬁc modulus, E=r, of the composite greater than that of unreinforced aluminium? How much larger is the speciﬁc modulus if the same volume fraction of SiC is used in the form of parallel continuous ﬁbres instead? For continuous ﬁbres the modulus lies very close to the upper bound, equation (4.19).
94 Chapter 4 Elastic stiffness, and weight: atomic bonding and packing
Aluminium Silicon carbide
Density r (kg/m3)
Young’s modulus E (GPa)
Medical prosthetic implants, such as hip replacements, are, at present, made of metals such as stainless steel or titanium. These metals are much stiffer than the bone, giving poor transfer of load into the bone. New composite materials aim for closer stiffness match. One uses a matrix of high-density polyethylene (HDPE) reinforced with particulate hydroxyapatite (HA), the natural mineral in bone. Data for experimental composites are listed below. Those for bone and for the bulk materials in the composite are: bone, 7 GPa; HDPE, 0.65 GPa; hydroxyapatite, 80 GPa. (a) Plot the upper and lower bounds for the Young’s modulus of HDPEeHA composites against the volume fraction of reinforcement, f (from 0 to 1), together with the experimental data. (b) Which of the bounds is closer to the data for the particulate composite? Use this bound as a guide to extrapolate the experimental data to ﬁnd the volume fraction of hydroxyapatite needed to match the modulus of bone. Is this practical?
Volume fraction of HA
Young’s modulus (GPa)
0 0.1 0.2 0.3 0.4 0.45
0.65 0.98 1.6 2.73 4.29 5.54
(a) Use the material property data in the table below to ﬁnd the composite e U for the following composites: density e r and upper bound modulus E (i) carbon ﬁbre/epoxy resin (f ¼ 0.5), (ii) glass ﬁbre/polyester resin (f ¼ 0.5).
Density r (kg/m3)
Young’s modulus E (GPa)
Carbon ﬁbre Glass ﬁbre Epoxy resin Polyester resin
1900 2550 1150 1150
390 72 3 3
(b) A magnesium company has developed an experimental metalematrix composite (MMC) by casting magnesium containing 20% (by volume) of particulate SiC. Use the lower bound estimate for Young’s modulus e L for this MMC, with the following data for matrix to estimate E and particles: Mg alloys, E ¼ 44.5 GPa, r ¼ 1850 kgm3; SiC, E ¼ 380 GPa, r ¼ 3100 kgm3. e e (c) Find the speciﬁc stiffness E r for the three composites in (a) and (b). Compare the composites with steels, for which E=r z 0.028 GPa.m3/kg. Exercise E4.16
Read the modulus E for polypropylene (PP) from the Er chart of Figure 4.8. Estimate the modulus of a PP foam with a relative density e r=rs of 0.2. 2 r e ¼ Es e Use the relationship E (equation (4.22)) to estimate the ranges of rs modulus and density achievable by foaming the following metals to relative densities e r=rs in the range 0.1e0.3: (a) Ni alloys (E ¼ 205 GPa, r ¼ 8890 kg/m3); (b) Mg alloys (E ¼ 44.5 GPa, r ¼ 1850 kg/m3). Locate approximate ‘property bubbles’ for these new metallic foams on a copy of the modulusedensity chart. With which existing materials would these foams compete in terms of modulus and density? Which other properties of these metal foams will differ signiﬁcantly from the competition?
Solar panels, touchscreens and other displays use indium (atomic number 49) to provide an electrically conducting ﬁlm that is transparent to light. Use the abundance plot of Figure 4.16 to form a judgement about possible future availability of indium.
Figures 4.20 and 4.21 illustrated how the atomic volume and Young’s modulus change in a cyclic way across the rows of the periodic table. Would you expect the following properties to behave in this way? (a) Absolute melting point (b) Latent heat of fusion (c) Yield strength
The electronegativity of germanium is 1.8; that of bromine is 2.8 on the Pauling scale. Will they form an ionic bond?
Assess what sort of bonding you would expect in (a) Strontium, Sr (atomic number 38)? (b) Magnesium iodide, MgI2? (c) Aluminium phosphide, AlP? Use the electronegativity chart of Figure 4.22 as a basis for your reasoning.
96 Chapter 4 Elastic stiffness, and weight: atomic bonding and packing
Rank the following bonds in order from the most covalent to the most ionic: (a) NaeCl; (b) LieH; (c) HeC; (d) HeF; (e) RbeO, given the following electronegativities: Element
What is meant by:
·· ·· ·
a crystalline solid an amorphous solid a thermoplastic a thermoset an elastomer?
The stiffness S of an atomic bond in a material is 50 N/m and its centre-tocentre atom spacing is 0.3 nm. What, approximately, is its elastic modulus?
The table shows the density and Young’s modulus for two brasses (CueZn alloys), and for pure Cu and Zn. The atomic packing and metallic bonding in alloys suggests that mixtures of metallic elements are expected to follow a simple rule of mixtures for these properties. Investigate if this is the case for these brasses.
Atomic % Zn
Density r (kg/m3)
Young’s modulus E (GPa)
Pure Cu Cue10 Zn brass Cue30 Zn brass Pure Zn
0 10 30 100
8960 8710 8450 7130
124 120 112 95
A pole vaulter e the pole stores elastic energy. Image courtesy of Gill Athletics, 2808 Gemini Court, Champaign, IL 61822-9648, USA.
Chapter contents 5.1 5.2 5.3 5.4 5.5 5.6 5.7 5.8
Introduction and synopsis Standard solutions to elastic problems Material indices for elastic design Plotting limits and indices on charts Case studies Summary and conclusions Further reading Exercises
Copyright Ó 2019 Elsevier Ltd. All rights reserved. https://doi.org/10.1016/B978-0-08-102376-1.00005-6
98 98 108 116 118 125 126 126
98 Chapter 5 Stiffness-limited design
Introduction and synopsis
A few years back, with the millennium approaching, countries and cities around the world turned their minds to iconic building projects. In Britain, there were several. One was e and still is e a new pedestrian bridge spanning the river Thames, linking St Paul’s Cathedral to the Museum of Modern Art, facing it across the river. The design was daring: a suspension bridge with suspension cables that barely rise above the level of the deck instead of the usual great upward sweep. The result was visually striking: a sleek, slender span like a ‘shaft of light’ (the architect’s words). Just one problem: it wasn’t stiff enough. The bridge opened, but when people walked on it, it swayed and wobbled sideways, so alarmingly that it was promptly closed. A year and $5,000,000 later, it reopened, much modiﬁed with vibration dampers attached in many places, and now it is ﬁne. The ﬁrst thing you tend to think of with structures, bridges included, is strength: they must not fall down. Stiffness, often, is automatically achieved by a strength-limited analysis and taken for granted. But, as the bridge story relates, that can be a mistake e stiffness is important. Here we explore stiffness-limited design and the choice of materials to achieve it. This involves the modelling of material response in a given application. The models can be simple because the selection criteria that emerge are insensitive to the details of shape and loading. The key steps are those of identifying the constraints that the material must meet, and the objective by which the excellence of choice will be measured. We saw at the beginning of Chapter 4 that there are certain common modes of loading: tension, compression, bending and torsion. The loading on any real component can be decomposed into some combination of these. So it makes sense to have a catalogue of solutions for the standard modes, relating the component response to the loading. In this chapter, the response is elastic deﬂection; in later chapters, it will be yielding or fracture. You need to understand the underlying assumptions behind these solutions and how to use them appropriately, which takes practice. You also need to know where to ﬁnd them e the most useful are provided here; the sources listed under ‘Further reading’ give more. The ﬁrst section of this chapter, then, is about standard solutions to elastic problems. The second is about their use to derive material limits and indices. We then explain how to plot them onto material property charts, and illustrate their use for stiffness-limited material selection problems via case studies. The chapter closes with examples of low stiffness design of foams and elastic mechanisms.
Standard solutions to elastic problems
Modelling is a key part of design. In the early, conceptual stage, approximate models establish whether a concept will work at all and identify the combination of material properties that maximise performance. At the embodiment stage, more accurate modelling brackets values for the design parameters: forces, displacements, velocities, heat ﬂuxes and component dimensions. And in the ﬁnal stage, computational modelling gives precise values for stresses, strains and failure probabilities in key components, allowing optimised material selection and sizing.
5.2 Standard solutions to elastic problems
Engineers have produced analytical models for many standard geometries under idealised loading. A component can often be modelled approximately by appropriate simpliﬁcation of shape and loading details e treating real loads as if they act at a point, for example. Standard solutions for loading in tension, bending, torsion, or buckling are presented here, without full details of their derivation e there is no shortage of books on structural mechanics for this. The important thing in design is to know that the results exist, how they work, and when to use them. Elastic extension or compression Figure 5.1(a) shows a tensile stress s ¼ F/A applied axially to a tie of length Lo, and constant cross-section area A leads to a strain ε ¼ s/E. The strain ε is the extension d as a fraction of the initial length: ε ¼ d/Lo (Figure 5.1(a)). Thus, the relation between the load F and deﬂection d is Lo F AE
F AE ¼ d Lo
d¼ The stiffness S is deﬁned as S¼
Figure 5.1 (a) A tie with a cross-sectional area A, loaded in tension with a force F. Its stiffness S ¼ F/d, and the tensile stress is uniform. (b) A beam of rectangular cross-section loaded in bending with a moment M, giving a radius of curvature R. The stress s varies linearly from tension to compression, changing sign at the neutral axis.
Note that the shape of the cross-section area does not matter because the stress is uniform over the section. If the stress is compressive, we call the component a strut, with stress and strain both negative, but exactly the same stiffness. If the strut is slender, however, it will not carry axial stress for long but will buckle e we come to this later.
100 Chapter 5 Stiffness-limited design Elastic bending of beams When a beam is loaded by a bending moment, M, its initially straight axis is deformed into a curve of radius R (Figure 5.1(b)). Provided the transverse deﬂection of the beam, u(x), is reasonably small compared to its length (as is the case for most materials in the elastic regime), the curvature k (¼1/R) can be written as k¼
d2 u 1 ¼ dx2 R
This curvature generates a linear variation of axial strain ε across the section, with tension on one side and compression on the other e the position of zero strain being the neutral axis. As stress is proportional to strain in uniaxial tension and compression, the bending stress varies linearly with distance y from the neutral axis (Figure 5.1(b)). Material is more effective at resisting bending the farther it is from that axis, so the shape of the cross-section is now important. Elastic beam theory (see Further reading) gives the stress s caused by a moment M in a beam made of material of Young’s modulus E, as s M d2 u ¼ ¼ Ek ¼ E 2 y I dx where I is the second moment of area, deﬁned as Z Z 2 y dA ¼ I¼ section
The distance y to each element dA of the cross-sectional area is measured perpendicular to the neutral axis, and b(y) is the width of the section at y. The second moment I characterises the resistance of the section to bending e it includes the effect of both size and shape. Expressions for the cross-section area A and the second moment of area I are shown for four common sections in Figure 5.2. Area, A (m2)
Second moment of area, I (m4)
b h3 12
bh3 b (1 – 0.58 ) 3 h
π 4 r 4
π 4 r 2
π (ro2– ri2) ≈ 2 π ro t (t Tg 1% strain
Strain ε = δL/L
Figure 6.2 Stressestrain curve for a polymer.
Stress σ = F/Ao
Ceramics Compressive strength σel Compression
Ao Slope E
L Tensile strength σts Tension
Strain ε = δL/L
Figure 6.3 Stressestrain curve for a ceramic.
136 Chapter 6 Beyond elasticity: plasticity, yielding and ductility For polymers, sy is identiﬁed as the stress at which the stressestrain curve becomes markedly non-linear: typically, a strain of 1% (Figure 6.2). The behaviour beyond yield depends on the temperature relative to the glass temperature Tg. Well below Tg, most polymers are brittle. As Tg is approached, plasticity becomes possible until, at about Tg, thermoplastics exhibit cold drawing: large plastic extension at almost constant stress during which the molecules are pulled into alignment with the direction of straining, followed by hardening and fracture when alignment is complete. At still higher temperatures, thermoplastics become viscous and can be moulded; thermosets become rubbery and ﬁnally decompose. The yield strength sy of a polymerematrix composite is also best deﬁned by a set deviation from linear elastic behaviour, typically 0.5%. Composites that contain aligned ﬁbres (and this includes natural composites like wood) are a little weaker (up to 30%) in compression than tension because the ﬁbres buckle on a small scale. Ceramics and glasses are brittle at room temperature (Figure 6.3). They do have yield strengths, but these are so enormously high that, in tension, they are never reached: the materials fracture ﬁrst. Even in compression, ceramics and glasses crush before they yield. To measure their yield strengths, special tests that suppress fracture are needed. We will return to the fracture-controlled strength of ceramics in Chapter 8. For now, it is useful to have a practical measure of the strength of ceramics to allow their comparison with other materials. The measure used here is the compressive crushing strength, and since it is not a yield point but is still the end of the elastic part of the stressestrain curve, we call it the elastic limit and give it the symbol sel. Returning then to ductile materials, the plastic strain, εpl, is the permanent strain resulting from plasticity; thus, it is the total strain εtot minus the recoverable elastic part: s (6.1) E The ductility is a measure of how much plastic strain a material can tolerate. It is measured in standard tensile tests by the elongation εf (the plastic tensile strain at fracture) expressed as a percentage (Figures 6.1 and 6.2). Strictly speaking, εf is not a material property because it depends on the sample dimensions e the values that are listed in handbooks and in the Cambridge Engineering Selector software are for a standard test geometry e but it remains useful as an indicator of the ability of a material to be deformed. In Chapter 4, the area under the elastic part of the stressestrain curve was identiﬁed as the elastic energy stored per unit volume (s2y 2E). Beyond the elastic limit, plastic work is done in deforming a material permanently by yield or crushing. The increment of plastic work done for a small permanent extension or compression dL under a force F, per unit volume V ¼ AoLo, is εpl ¼ εtot
FdL F dL ¼ ¼ sdεpl V Ao Lo
Thus, the plastic work per unit volume at fracture is Z εf Wpl ¼ sdεpl
which is just the area under the whole stressestrain curve (minus the elastic unloading at the end). This is important in energy-absorbing applications, such as the crash boxes in the front of cars or roadside crash barriers.
6.2 Strength, ductility, plastic work and hardness: deﬁnition and measurement
Example 6.1 A steel rod with a yield strength sy ¼ 500 MPa is uniformly stretched to a strain of 0.1 (10%). Approximately how much plastic work is absorbed per unit volume by the rod in this process? Assume that the material is elastic perfectly plastic; that is, it deforms plastically at a constant stress sy. Compare this plastic work with the elastic energy per unit volume calculated in Example 4.4. Answer. Assuming that the material is ‘elastic perfectly plastic’, that is, the stress equals the yield strength up to failure, and neglecting the elastic contribution, the plastic energy per unit volume at failure is approximately: Wpl ¼ sy εf ¼ 500 106 0:1 ¼ 50 MJ m3
This plastic energy is 80 times the elastic strain energy of 625 kJ/m3 in Example 4.4 (but is still only 0.015% of the chemical energy stored in the same mass of gasoline).
Tensile and compression tests are not always convenient: the component or sample is destroyed. The hardness test (Figure 6.4) is a non-destructive test that avoids this problem. A pyramidal diamond or a hardened steel ball is pressed into the surface of the material. This leaves a tiny permanent indent, the width of which is measured with a microscope and can be converted to a projected area A perpendicular to the load. The indent means that plasticity has occurred, and the hardness H measures the resistance to plastic indentation. By the simplest deﬁnition, hardness is deﬁned as: H¼
Vickers H = F/A
Projected area A Load F
Figure 6.4 The hardness test. The Vickers test uses a diamond pyramid; the Rockwell and Brinell tests use a steel sphere, producing the indent shapes shown on the right.
138 Chapter 6 Beyond elasticity: plasticity, yielding and ductility In practice, corrections may also be made to convert the projected area A to the actual area of contact between indenter and material e this is a small correction, as the indentations are shallow compared to their width. The plastic region under the indenter is surrounded by material that has not deformed, and this pushes inwards and constrains the plastic deformation so that H is larger than the (uniaxial) yield strength sy e in practice, it is about 3sy. Strength, as we have seen, is measured in units of MPa, and since H is also a force per unit area, it would be logical to measure it in MPa too, but convention dictates otherwise in this case. A commonly used scale, that of Vickers hardness (symbol Hv), has units of kg/mm2, which is equivalent to H in MPa divided by g (¼9.81 m/s2, the acceleration due to gravity), with the result that Hv z
3 sy sy z g 3
The conversion between hardness scales and the corresponding approximate yield strength are shown in Figure 6.5. The hardness test has the advantage of being non-destructive, so strength can be measured without destroying the component, and it requires only a tiny volume of material. But the information it provides is less accurate and less complete than the tensile test, so it is not used to provide critical design data.
Rockwell C 90
1500 1400 1200 1100
50 40 30 20 10
80 75 70 65 60
700 600 500
3000 6 2500
Approx. yield strength, MPa
Figure 6.5 Common hardness scales compared with the yield strength.
6.2 Strength, ductility, plastic work and hardness: deﬁnition and measurement
True stress and true strain The graphs of Figures 6.1e6.3 strictly show the nominal stressenominal strain responses; that is, the area and length used are the original values at the start of the test. But once materials yield, they can change dimensions signiﬁcantly. The true stress, st, takes account of the current dimensions, so in tension, for example (equation (4.1)) st ¼
To relate this to the nominal stress, which we will refer to as sn, we note that in plastic deformation, the volume of the sample is conserved, for reasons discussed later in this chapter; that is Volume ¼ Ao Lo ¼ AL
where A and L are the current area and length of the test sample, and were initially Ao and Lo. Hence, the nominal stress is F F Lo sn ¼ ¼ (6.7) Ao A L Returning to the deﬁnition of nominal strain, εn (equation (4.3)) dL L Lo L εn ¼ ¼ ¼ 1 Lo Lo Lo
Combining with equations (6.5) and (6.7) gives the true stress as st ¼ sn ð1 þ εn Þ
True strain, εt, is a bit more involved. An incremental change in length, dL, gives an incremental strain relative to the current length L. To ﬁnd the cumulative true strain, we therefore integrate these increments over the full extension from Lo to L, giving Z L dL L ¼ ln εt ¼ (6.10) ¼ lnð1 þ εn Þ L L o Lo To see how different the true and nominal quantities are in practice, let’s do an example. Example 6.2 Find the true strain for the following values of the nominal strain during a tensile test on a metal: (a) the 0.2% offset strain, used to deﬁne the proof stress (Figure 6.1); (b) a strain of 20%, typical for the onset of failure at maximum stress. What is the ratio of true to nominal stress at these points? Answer. The true strains are (a) ln(1 þ 0.002) ¼ 0.002 (to three decimal places); (b) ln(1.2) ¼ 0.182. The ratio of true to nominal stress is (1 þ εn), giving: (a) 1; (b) 1.2.
140 Chapter 6 Beyond elasticity: plasticity, yielding and ductility
The example shows that for the elastic regime and small plastic strains, the difference between nominal and true stresses and strains is negligible. This explains the effectiveness of using nominal values to deﬁne key properties such as the yield stress. By the end of the tensile test in a metal, the discrepancy between the two is typically 20%. What about compressive true stress and strain? Now the cross-sectional area increases with plastic deformation (to conserve volume). Equations (6.5) to (6.10) all hold, so long as care is taken with the sign of the applied force F and the strain increments dL, which are negative. Figure 6.6 shows nominal and true stressestrain curves superimposed, for both compression testing and for the stable part of a tensile test up to the tensile strength. As observed in Example 6.2, in tension, the true stress is higher than nominal, whereas for strain, the reverse is true. In compression, nominal stress exceeds true, and again the reverse for strain. Figure 6.6 shows one beneﬁt of true stressestrain: the curves are identical in shape for tension and compression. The compressive side also extends to larger values of stress and strain, as the instability of necking in tension is avoided. The true stressestrain behaviour is most useful for metal forming, where plastic strains of the order of 50% or more are common. And some forming processes use multiple passes, with several plastic deformations one after another. In the Exercises at the end of the chapter, you can show that the total strain in this case can simply be found by adding up the true strains, but this is not the case for nominal strains.
− σy True Nominal
Figure 6.6 Nominal and true stressestrain curves for a ductile metal, in tension and compression.
The big picture: charts for yield strength
Strength can be displayed on material property charts. Two are particularly useful: the strengthedensity chart and the modulusestrength chart. The strengthedensity chart Figure 6.7 shows the yield strength sy or elastic limit sel plotted against density r. The range of strength for engineering materials, like that of the modulus,
6.3 The big picture: charts for yield strength
spans about 6 decades: from less than 0.01 MPa for foams, used in packaging and energyabsorbing systems, to 104 MPa for diamond, exploited in diamond tooling for machining and as the indenter of the Vickers hardness test. Members of each family again cluster together and can be enclosed in envelopes, each of which occupies a characteristic part of the chart. 10000
Strength, σy or σel (MPa)
Polymers and elastomers
Natural materials 10
Ti alloys Metals Steels Ni alloys Tungsten alloys
GFRP PEEK PET PA PC PMMA
Rigid polymer foams
Metals and polymers: yield strength Ceramics and glasses: MOR Elastomers: tensile tear strength Composites: tensile failure
SiC Al alloys
Zinc alloys Lead alloys
Concrete Butyl rubber
Flexible polymer foams
Figure 6.7 The strengthedensity property chart. Comparison with the modulusedensity chart (Figure 4.7) reveals some marked differences. The modulus of a solid is a well-deﬁned quantity with a narrow range of values. The strength is not. The strength range for a given class of metals, such as stainless steels, can span a factor of 10 or more, while the spread in stiffness is at most 10%. Since density varies very little (Chapter 4), the strength bubbles for metals are long and thin. The wide ranges for metals reﬂect the underlying physics of yielding, and present designers with an opportunity for manipulation of the strength by varying composition and process history. Both are discussed later in this chapter. Polymers cluster together with strengths between 10 and 100 MPa, and the modulus and strength vary by a similar amount for a given polymer. The composites carbon ﬁbre-reinforced polymer (CFRP) and glass ﬁbre-reinforced polymer (GFRP) have strengths that lie between those of polymers and ceramics, as we might expect since they are mixtures of the two. The analysis of the strength of composites is not as straightforward as for modulus in Chapter 4, though the same bounds (with strength replacing modulus) generally give realistic estimates.
142 Chapter 6 Beyond elasticity: plasticity, yielding and ductility Example 6.3 An unidentiﬁed metal from a competitor’s product is measured to have a ‘Rockwell A’ hardness of 50 and a density of approximately 8800 kg/m3. Estimate its Vickers hardness and its yield strength. Locate its position on the strengthedensity chart (Figure 6.7). What material is it likely to be? Answer. From Figure 6.5, the Vickers hardness is approximately 510, and the yield strength is approximately 1600 MPa (which agrees reasonably with equation (6.4)). This is a strong metal. It falls near the top of the nickel alloys on the strengthedensity chart.
The modulusestrength chart Figure 6.8 shows Young’s modulus, E, plotted against yield strength, sy or elastic limit, sel. This chart allows us to examine a useful material characteristic, the yield strain, sy/E, meaning the strain at which the material ceases to be linearly elastic. On log axes, contours of constant yield strain appear as a family of straight parallel lines, as 1000
Cu alloys Silica glass
CFRP Cast irons Zinc alloys
Al alloys Mg alloys
Yield strain σy = 10-4 E
Ni alloys Steels
Young's modulus, E (GPa)
Metals and polymers: yield strength Ceramics and glasses: MOR Elastomers: tensile tear strength Composites: tensile failure
B C SiC 4
Epoxies PMMA PC
Rigid polymer foams
PE PTFE Ionomers
Leather Silicone elastomers EVA Polyurethane
Strength, σy or σel (MPa)
Figure 6.8 The Young’s modulusestrength chart. The contours show the strain at the elastic limit, sy =E.
6.4 Drilling down: the origins of strength and ductility 143 shown in Figure 6.8. Engineering polymers have large yield strains, between 0.01 and 0.1; the values for metals are at least a factor of 10 smaller. Composites and woods lie on the 0.01 contour, as good as the best metals. Elastomers, because of their exceptionally low moduli, have values of sy/E in the range 1e10, much larger than any other class of material. This chart has many other applications, notably, in selecting materials for springs, elastic diaphragms, ﬂexible couplings and snap-ﬁt components. We explore these in Chapter 7.
Drilling down: the origins of strength and ductility
Perfection: the ideal strength The bonds between atoms, like any other spring, have a breaking point. Figure 6.9 shows a stressestrain curve for a single bond. Here an atom is assumed to occupy a cube of side length ao (as in Chapter 4) so that a force F corresponds to a stress F a2o . The force stretches the bond from its initial length ao to a new length a, giving a strain (a ao)/ao. When discussing the modulus in Chapter 4, we focused on the initial, linear part of this curve, with a slope equal to the modulus, E. Stretched farther, the curve passes through a maximum and falls to zero as the atoms lose their interaction altogether. The peak is the bond strength e if you pull harder than this, it will break. The same is true if you shear it rather than pull it.
Stress σ = F/ao2
Equilibrium Fmax/ao2 spacing, ao
Spacing at F failure, a*
Strain a - ao ao
Figure 6.9 The stressestrain curve for a single atomic bond (it is assumed that each atom occupies a cube of side ao).
The distance over which inter-atomic forces act is small e a bond is broken if it is stretched to more than about 10% of its original length. So the force needed to break a bond is roughly: F¼
where S, as before, is the bond stiffness. On this basis, the ideal strength of a solid should therefore be roughly sideal ¼
Fmax S E ¼ ¼ 2 10ao 10 ao
144 Chapter 6 Beyond elasticity: plasticity, yielding and ductility remembering that E ¼ S/ao, equation (4.26). Hence: sideal 1 ¼ 10 E
This doesn’t allow for the curvature of the forceedistance curve; more reﬁned calculations give a ratio of 1/15. Figure 6.10 shows sy/E for metals, polymers and ceramics. None achieves the ideal value of 1/15; most don’t even come close. To understand why, we need to look at the microstructure and imperfections in each material class.
Yield strength, σy / Young's modulus, E
Ideal strength 10-1
Ti alloys LA steels
PE Al alloys Copper
PVC Zirconia Alumina Glass
Brass Mild steel Lead
Figure 6.10 The ideal strength is predicted to be about E=15, where E is Young’s modulus. The ﬁgure shows sy =E with a shaded band at the ideal strength. Strength of polymers Figure 6.2 showed a range of stressestrain responses in polymers. Recall ﬁrst that in Chapter 4, the glass transition temperature Tg was deﬁned, being the temperature at which the inter-molecular hydrogen bonds melt. This is usually associated with a marked drop in the material stiffness, depending on whether the polymer is amorphous, semi-crystalline or cross-linked. Not surprisingly, the strength of a polymer also depends strongly on whether the material is above or below the glass transition, and a number of different failure mechanisms can occur. At low temperatures, meaning below about 0.75 Tg, polymers are elasticebrittle, like ceramics, and fail by propagation of a dominant ﬂaw (see Chapter 8). Above this temperature, they become plastic. When pulled in tension, the chains slide over each other, unravelling, so that they become aligned with the direction of stretch, as in Figure 6.11(a), a process called drawing. It is harder to start drawing than to keep it going, so the zone where it starts draws down completely before propagating farther along the sample, leading to proﬁles like that shown in the ﬁgure. The drawn material is stronger and stiffer than before, by a factor of about 8, giving drawn polymers exceptional properties, but because you can only draw ﬁbres, or sheet (by pulling in two directions at once), the geometries are limited.
6.4 Drilling down: the origins of strength and ductility 145
Initially non-aligned molecules
Drawn segment with aligned molecules
Figure 6.11 (a) Cold drawing e one of the mechanisms of deformation of thermoplastics. (b) Crazing e local drawing across a crack. (c) Shear banding.
Many polymers, among them PE, PP and nylon, draw at room temperature. Others with higher glass temperatures, such as PMMA, do not, although they draw well at higher temperatures. At room temperature, they craze. Small crack-shaped regions within the polymer draw down. Because the crack has a larger volume than the polymer that was there to start with, the drawn material ends up as ligaments of aligned segments of molecules that link the craze surfaces, as in Figure 6.11(b). Crazes scatter light, so their presence causes whitening, easily visible when cheap plastic articles are bent. If stretching is continued, one or more crazes develop into proper cracks, and the sample fractures. While crazing limits ductility in tension, large plastic strains may still be possible in compression by shear banding (Figure 6.11(c)). These bands allow blocks of material to either side of the band to shear with respect to one another, without the material coming apart. Continued compression causes the number of shear bands to increase, giving increased overall strain. The upshot of all this is that polymers do have a strength that is not very far below their ideal value (Figure 6.10). But we shouldn’t get too excited e their moduli are much lower than metals to begin with, but it does mean that polymers are not so far below metals when compared on strength (an observation you can make for yourself on the modulusestrength property chart of Figure 6.8). Crystalline imperfection: defects in metals and ceramics Crystals contain imperfections of several kinds e Figure 6.12. All crystals contain point defects called vacancies, shown in (a): sites at which an atom is missing. They play a key role in diffusion, creep and sintering (Chapter 13), but we don’t need them for the rest of this chapter because they do not inﬂuence strength.
146 Chapter 6 Beyond elasticity: plasticity, yielding and ductility Substitutional solute
Extra half plane
Figure 6.12 Defects in crystals. (a) Vacancies e missing atoms. (b) Foreign (solute) atoms in interstitial and substitutional sites. (c) A dislocation e an extra half-plane of atoms. (d) Grain boundaries. No crystal is made up of a single pure element. Other elements are always present at some concentration e either as impurities inherited from the process by which the material was made, or they are deliberately added, creating alloys: a material in which two or more elements are mixed. If the foreign elements ‘dissolve’ and are spread out atomically in the crystal e like salt in water e then we have a solid solution. Figure 6.12(b) shows both a substitutional solid solution (the dissolved atoms replace those of the host) and an interstitial solid solution (the dissolved atoms squeeze into the spaces or ‘interstices’ between the host atoms). The dissolved atoms or solute rarely have the same size as those of the host material, so they distort the surrounding lattice. The red atoms here are substitutional solute, some bigger and some smaller than those of the host; the cages of host atoms immediately surrounding them, shown green, are distorted. Only the smallest atoms dissolve interstitially, like the black atoms in the ﬁgure, but these too distort the surrounding lattice. So solute causes local distortion; this distortion is one of the reasons that alloys are stronger than pure materials, as we shall see in a moment. Now to the key player, portrayed in Figure 6.12(c): the dislocation. We will see shortly how these are responsible for making metals soft and ductile, well below their ideal strength. ‘Dislocated’ means ‘out of joint’, and this is not a bad description of what is happening here.
6.4 Drilling down: the origins of strength and ductility 147 The upper part of the crystal has one ‘half-plane’ of atoms than the lower part e the region around the bottom of this half-plane is a dislocation. They are actually line defects, extending perpendicular to the view shown in the ﬁgure. Dislocations distort the lattice e here the green atoms are the most distorted e and because of this, they have elastic energy associated with them. If they cost energy, why are they there? To grow a perfect crystal just one cubic centimetre in volume from a liquid or vapour, about 1023 atoms have to ﬁnd their proper sites on the perfect lattice, and the chance of this happening is just too small. Even with the greatest care in assembling them, all crystals contain vacancies and dislocations. Most crystalline solids are polycrystalline, made up of very many tiny crystals, or grains. Figure 6.12(d) shows three perfect, but differently oriented, grains meeting, which leads to interfaces between the grains where the packing is irregular. These planar defects are called grain boundaries. In this sketch, the atoms of the three crystals have been given different colours to distinguish their packing orientations, but they are all the same atoms. In reality, grain boundaries form in pure materials (when all the atoms are the same) and in alloys (when the mixture of atoms in one grain may differ in chemical composition from those of the next). So the outward perfection of the steel of a precision machine tool, or of the polished case of a gold watch, is an illusion: both metals are full of defects of the types shown in Figure 6.12. Between them, they explain diffusion of atoms in solids, and the microstructure-sensitive properties: strength, ductility, electrical resistance, thermal conductivity and much more. At the heart of metal alloying and processing is the direct manipulation of these defects to control properties e in this chapter, we learn how strength depends on microstructure; in Chapter 19 and Guided Learning Unit 2, we add the context of processing. So defects in crystals are inﬂuential. For the rest of this section, we focus on dislocations, as these control the plastic behaviour of metals. First we need to understand them to explain why the strength of metals is below ideal (Figure 6.10), and then in Section 6.5, we address how strength is increased by forcing dislocations to interact with the other defects. Ceramics can also deform plastically e but only if they are very hot (and generally they also need to be in compression). But their tensile strength shown in Figure 6.10 is also well below yield. To explain this, we need fracture mechanics, and a different type of defect: cracks. Chapter 8 is where we will tackle fracture. Dislocations and plastic ﬂow Recall that the strength of a perfect crystal computed from inter-atomic forces gives an ‘ideal strength’ around E/15 (where E is the modulus). In reality, the strengths of engineering alloys are nothing like this big; often they are barely 1% of it. This was a mystery until the 1930s when an Englishman, G. I. Taylor3, and a Hungarian, Egon Orowan4, realized that a ‘dislocated’ crystal could deform at stresses far below the ideal. So what is a dislocation, and how does it enable deformation? 3
Geoffrey (G. I.) Taylor (1886e1975), known for his many fundamental contributions to aerodynamics, hydrodynamics and to the structure and plasticity of metals e it was he, with Egon Orowan, who realised that the ductility of metals implied the presence of dislocations. One of the greatest of contributors to theoretical mechanics and hydrodynamics of the 20th century, he was also a supremely practical man e a sailor himself, he invented (among other things) the anchor used by the Royal Navy. Egon Orowan (1901e1989), Hungarian/US physicist and metallurgist, who, with G. I. Taylor, realised that the plasticity of crystals could be understood as the motion of dislocations. In his later years, he sought to apply these ideas to the movement of fault lines during earthquakes.
148 Chapter 6 Beyond elasticity: plasticity, yielding and ductility Figure 6.13(a) shows how to make a dislocation. Imagine that the crystal is cut along a horizontal atomic plane up to the line shown as t e t, and the top part above the cut is then slipped across the bottom part by one full atom spacing. Then most of the atoms either side of the cut can be reattached across the slip plane, except at the very end of the cut, where there is a misﬁt in the atom conﬁguration, as shown in Figure 6.13(b) for a simple cubic lattice packing. The problem is that there is now effectively an extra half-plane of atoms in the top part of the crystal, with its lower edge along the t e t line. This is the dislocation line e the line separating the part of the plane that has slipped from the part that has not. This particular conﬁguration is called an edge dislocation because it is formed by the edge of the extra halfplane, represented by the symbol t.
Slip vector b
Extra half plane
Slip vector b
Slip plane Slipped area
Extra half plane
Edge dislocation line
Figure 6.13 (a) Making a dislocation by cutting, slipping and rejoining bonds across a slip plane. The slip vector b is perpendicular to the edge dislocation line tet. (b) The atom conﬁguration round an edge dislocation in a simple cubic crystal.
Dislocations control plastic strain, since if a dislocation moves across its slip plane, then it makes the material above the plane slide one atomic spacing relative to that below. Figure 6.14 shows how this happens. At the top is a perfect crystal. In the central row, a shear stress s is acting parallel to the slip planes, and this drives an edge dislocation in from the left; it sweeps through the crystal and exits on the right. Note that no individual atom moves very far as the dislocation moves e the bonds round the dislocation are stretched to and fro to allow the pattern of misﬁtting atoms to move along the slip plane. By the end of the process, the upper part has slipped relative to the lower part by a slip step b, known as the Burger’s vector. The result is the shear strain g shown at the bottom. Note that in this conﬁguration, the shear stress is perpendicular to the edge dislocation, which moves in the direction of the stress, and the resulting slip step b is in the direction of the shear stress.
6.4 Drilling down: the origins of strength and ductility 149
(d) b γ
Figure 6.14 An initially perfect crystal is shown at (a). A shear stress s drives the passage of a
dislocation across the slip plane, shown in the sequence (b), (c), and (d), and shears the upper part of the crystal over the lower part by the slip vector b, leading at (e) to a shear strain g.
There is another way to make a dislocation in a crystal. After making the cut in Figure 6.13(a), the upper part of the crystal can be displaced parallel to the edge of the cut rather than normal to it, as in Figure 6.15(a). That too creates a dislocation, but one with a different conﬁguration of misﬁtting atoms along its line e more like a corkscrew e and for this reason, it is called a screw dislocation. We don’t need to try and visualise the details of its structure; it is enough to know that its properties are similar to those of an edge dislocation, with the following distinction: the driving shear stress is now parallel to the screw dislocation, which sweeps sideways through the crystal, again moving normal to itself, but the slip step b remains in the direction of applied shear stress. In fact, dislocations also form curves as they move over a slip plane, in which case they are called mixed dislocations, meaning that they are made up of little steps of edge and screw. The ‘pure’ edge and screw conﬁgurations are then found at two positions on the dislocation at 90 to one another e as shown in Figure 6.15(b). Once we’ve seen all this, it is easiest to forget about where the atoms are and just to think of dislocations as ﬂexible line defects gliding over the slip planes under the action of an applied shear stress. It doesn’t matter whether the dislocation is edge, screw or mixed: it always moves perpendicular to itself, and every part of it produces the same slip vector b in the direction of the shear stress e the dislocation line is just the boundary on the plane up to which point which a ﬁxed displacement b has occurred.
150 Chapter 6 Beyond elasticity: plasticity, yielding and ductility Slip vector b
Shear stress τ
S Slipped area
S Screw dislocation line
Slip vector b
S Slipped area
Figure 6.15 (a) A screw dislocation, with the slip vector b parallel to the dislocation line SeS; (b) a curved, mixed dislocation, connecting a pure edge to a pure screw dislocation.
The dislocation is key to understanding why metals have a strength that is so far below their ideal strength: it is far easier to move a dislocation through a crystal, stretching and remaking bonds only locally along its line as it moves, than it is to simultaneously break all the bonds in the plane before remaking them. It is like moving a heavy carpet by pushing a fold across it rather than sliding the whole thing at one go. In real crystals, it is easier to make and move dislocations on some planes than on others. The preferred planes are called slip planes, and the preferred directions of slip in these planes are called slip directions. We have seen these previously in the close-packed hexagonal, face-centred cubic (FCC) and body-centred cubic structure unit cells of Figure 4.30 e dislocations prefer planes and directions that are closepacked, or nearly so. Single slip steps are tiny e one dislocation produces a displacement of about 1010 m. But if large numbers of dislocations traverse a crystal, moving on many different planes, the shape of a material changes at the macroscopic length scale. Figure 6.16 shows just two dislocations traversing a sample loaded in tension, and then another two on a different pair of slip planes. The slip steps (here very exaggerated) cause the sample to get a bit thinner and longer. Repeating this millions of times on many planes gives the large plastic extensions observed in practice. Since none of this changes the average atomic spacing, the volume remains unchanged. So this is how materials deform plastically at stresses well below the ideal strength e but note the crucial advantages: the material remains fully intact without any loss of strength as its shape changes signiﬁcantly. This ductility is essential for safe design e we can live with a bit of unintended strain, but not with everything being brittle e and it also enables us to shape components from lumps of metal in the solid state.
6.4 Drilling down: the origins of strength and ductility 151
Figure 6.16 Dislocation motion leads to strain but conserves volume. Why does a shear stress make a dislocation move? A shear stress is needed to move dislocations because crystals resist their motion with a friction-like resistance f per unit length e we will examine its origins in a moment. But for yielding to take place, the shear stress must overcome the resistance f. Imagine that one dislocation moves right across a slip plane, traveling the distance L2, as in Figure 6.17. In doing so, it shifts the upper half of the crystal by a distance b relative to the lower half. The shear stress s acts on an area L1L2, giving a shear force Fs ¼ sL1L2 on the surface of the block. If the displacement parallel to the block is b, the force does work W ¼ sL1 L2 b
Force τb per unit length
Slip vector b
Shear stress τ
Resistance f per unit length
Slipped area of plane
Force τb per unit length
Resistance f L per unit length 1
Dislocation line L2
Figure 6.17 The force on a dislocation. (a) perspective view; (b) plan view of slip plane.
152 Chapter 6 Beyond elasticity: plasticity, yielding and ductility This work is done against the resistance force f per unit length, or f L1 on the length L1, and it does so over a displacement L2 (because the dislocation line moves this far against f), giving a total work against f of fL1L2. Equating this to the work W done by the applied stress s gives sb ¼ f
This result holds for any dislocation e edge, screw or mixed. So, provided the shear stress s exceeds the value f/b, it will make dislocations move and cause the crystal to shear. Line tension The atoms near the ‘core’ of a dislocation are displaced from their proper positions, as shown by green atoms back in Figure 6.12(c), and thus they have higher potential energy. To keep the potential energy of the crystal as low as possible, the dislocation tries to be as short as possible e it behaves as if it had a line tension, T, like an elastic band. The tension can be calculated but it needs advanced elasticity theory to do it (the books listed under ‘Further Reading’ give the analysis). We just need the answer. It is that the line tension T, an energy per unit length (just as a surface tension is an energy per unit area), is 1 T ¼ Gb2 2
where G is the shear modulus (since dislocations are associated with local lattice straining in shear), and b is the magnitude of the Burger’s vector. Recall that for metals, G scales with Young’s modulus E, with G z 3/8 E (Chapter 4). The line tension has an important bearing on the way in which dislocations interact with obstacles, as we shall see in a moment. At ﬁrst, it is perhaps surprising that we explain plastic deformation via dislocation motion, which turns out to depend on an elastic property e the shear modulus, G. But it derives from the fact that dislocations strain the lattice elastically by small (elastic) changes in the atomic spacing. This local elastic distortion enables the dislocations to move large distances, leading to large plastic strains. The lattice resistance Where does the resistance to slip, f, come from? There are several contributions. Consider ﬁrst the lattice resistance, fi: the intrinsic resistance of the crystal structure to plastic shear. Plastic shear, as we have seen, involves the motion of dislocations. Pure metals are soft because the non-localised metallic bond does little to obstruct dislocation motion, whereas ceramics are hard because their more localised covalent and ionic bonds (which must be stretched and reformed when the lattice is sheared) lock the dislocations in place. When the lattice resistance is high, as in ceramics, further hardening is superﬂuous e the problem becomes that of suppressing fracture. On the other hand, when the lattice resistance fi is low, as in metals, the material needs to be strengthened by introducing obstacles to slip. This is done by adding alloying elements to give solid solution hardening (fss), and using precipitates or dispersed particles to give precipitation hardening (fppt), while other dislocations give what is called work hardening (fwh), and polycrystals also have grain boundary hardening (fgb). These techniques for manipulating strength are central to alloy design. We look at them more closely in the next section.
6.5 Manipulating strength
Strengthening metals: dislocation pinning The way to make crystalline materials stronger is to make it harder for dislocations to move. As we have seen, dislocations move in a pure crystal when the force sb per unit length exceeds the lattice resistance fi. There is little we can do to change this e it is an intrinsic property like the modulus E. Other strengthening mechanisms add to it, and here there is scope for manipulation. Figure 6.18 shows views of a slip plane containing obstacles from the perspective of an advancing dislocation; each strengthening mechanism presents a different obstacle course. In the perfect lattice shown in (a), the only resistance is the intrinsic strength of the crystal; solution hardening, shown in (b), introduces atom-size obstacles to motion; precipitation hardening, shown in (c), presents larger obstacles; and in work hardening, shown in (d), the slip plane becomes stepped and threaded with ‘forest’ dislocations.
(a) Perfect lattice, resistance fi Precipitate particle
(c) Precipitate hardening, resistance fppt
(b) Solution hardening, resistance fss Forest dislocation (with slip step)
(d) Work hardening, resistance fwh
Figure 6.18 A ‘dislocation-eye’ view of the slip plane across which it must move. Figure 6.19(a) shows what happens when dislocations encounter obstacles, which act as pinning points. From equation (6.14), the force on the dislocation between two pinning points of spacing L is F ¼ sbL. From the ﬁgure, there is one obstacle for each length L of dislocation, so the force on each obstacle is also F ¼ sbL. To keep the dislocation moving, an increase in the shear stress is needed to bow out the dislocation through the gap. The bowing angle q and applied shear stress s increase until the force F can overcome the pinning force p that the obstacle can apply on the dislocation. Figsure 6.19(b) and (c) show two ways in which dislocations escape from pinning points: ‘weak’ obstacles are passed when the bowing angle q lies between 0 and 90 ; for ‘strong’ obstacles, the bowing angle reaches the limiting value
154 Chapter 6 Beyond elasticity: plasticity, yielding and ductility q ¼ 90 , and the dislocation escapes by other means e the arms of the dislocations link up and the dislocation advances, but leaving a dislocation loop around the obstacle (Figure 6.19(c)). A helpful way to think about dislocation pinning is to recall that dislocations have a ‘line tension’ trying to make the dislocation as short as possible. As the dislocation bows out, the line tension ‘pulls’ against the obstacle, with the maximum pull being exerted when q ¼ 90 .
Region of slip
Region of slip
Region of slip
θ Force τbL
θ = 90o
Figure 6.19 Dislocation pinning: (a) force on dislocation between pinning points; (b, c) dislocation bowing and escape from weak and strong obstacles, respectively.
In both weak and strong cases in Figure 6.19, the dislocation escapes when F ¼ p. Hence, the additional contribution to the shear stress s needed to overcome the pinning points is Ds ¼
Dislocation pinning is an elastic effect, locally distorting the atoms around the dislocation. As a result, the pinning force p, for each type of obstacle in a given material, scales with the energy per unit length (or line tension), of the dislocation, Gb2/2 (equation (6.15)). Combining this with equation (6.16), the shear stress s needed to force the dislocation through a ﬁeld of obstacles therefore has the form s¼a
where a is a dimensionless constant characterizing the obstacle strength. Take a close look at this equation: G and b are material constants, so in order to manipulate the strength, the parameters that we can control are: a (the obstacle strength) and L (the obstacle spacing). Armed with equation (6.17), we can now explain strengthening mechanisms. Solid solution hardening Solid solution hardening is strengthening by alloying with other elements that disperse atomically into the host lattice (Figure 6.20(a)). They are added when the alloy is molten and are then trapped in the solid lattice as it solidiﬁes. Adding zinc to copper makes the alloy brass e copper dissolves up to 30% zinc. The zinc atoms replace copper atoms to form a random substitutional solid solution. The zinc atoms are bigger than those of copper, and, in squeezing into the copper lattice, they distort it. This ‘roughens’ the slip plane, so to
6.5 Manipulating strength
speak, making it harder for dislocations to move e they are pinned by the solute atoms and bow out, thereby adding an additional resistance fss to dislocation motion. The ﬁgure illustrates that the concentration of solute, c, expressed as an atom fraction within a given plane, is on average: c¼
where L is the spacing of obstacles in the slip plane, and b is the atom size. Thus, L¼
Region of slip
Force τb per unit length
b c1=2 Precipitate particle Region of slip
Force tb per unit length
Successive positions of the dislocation line
Force τb per unit length
Forest dislocations, density ρd
Jogged forest dislocations Region of slip in Grain 1
Region of slip
Dislocations in Grain 2
Grain size, D
Slip plane in Grain 2
Figure 6.20 (a) Solid solution hardening. (b) Precipitation or dispersion hardening. (c) Forest hardening (work hardening). (d) Grain boundary hardening.
Plugging this into equation (6.17) relates the concentration of the solid solution to the additional shear stress sss required to move the dislocation: sss ¼ aGc1=2 .
So sss increases as the square root of the solute concentration. Brass, bronze and stainless steels, and many other metallic alloys, derive their strength in this way. They differ only in the
156 Chapter 6 Beyond elasticity: plasticity, yielding and ductility extent to which the solute distorts the crystal, described by the constant a. The bowing angle q for solute is small e much less than 90 e so solute provides weak pinning. Dispersion and precipitate strengthening A more effective way to impede dislocations is to disperse small, strong particles in their path. One way to make such a microstructure is to mix small solid particles of a high melting point compound into a liquid metal and to cast it to shape, trapping the particles in place e it is the way that metalematrix composites such as AleSiC are made. But in practice, these particles are rather far apart, so an alternative route is used to give the best outcomes e this is to form the particles in situ by a precipitation process, controlled by heat treatment. Solute atoms often form solid solutions more easily at high temperature than low. So if a solute is ﬁrst dissolved in a metal at high temperature, and the alloy is cooled, the solute precipitates out as tiny crystals of compounds embedded in the host lattice e much as salt will crystallize from a saturated solution when it is cooled. An alloy of aluminium containing 4% copper, for instance, precipitates very small, closely spaced particles of the hard compound CuAl2. Copper alloyed with a little beryllium, similarly treated, gives precipitates of the compound CuBe. And most steels are strengthened by carbide precipitates obtained in this way. In practical heat treatment, the particle spacing is kept as small as possible by ﬁrst quenching to room temperature and then reheating to form the precipitates e this is discussed in more depth in Guided Learning Unit 2. Figure 6.20(b) shows how particles obstruct dislocation motion. In this case, the particles are ‘strong’ obstacles, and the dislocation bows out to q ¼ 90 , escaping as shown in Figure 6.19(c), leaving a loop of dislocation wrapped round the particle. In this semi-circular conﬁguration, the dislocation of line tension T ¼ 1/2 Gb2 is applying the biggest force it can on each obstacle, equal to 2T, so this is the maximum pinning force p. From equations (6.15) and (6.16), the strength contribution from precipitates is therefore sppt ¼
2T Gb ¼ bL L
Comparison with equation (6.17) shows that the maximum value of the constant a is therefore 1. Precipitation hardening is the most effective way to increase strength: precipitation-hardened aluminium alloys can be 15 times stronger than pure aluminium. Work hardening The rising part of the stressestrain curve of Figure 6.1 is known as work hardening: the plastic deformation causes dislocations to accumulate. The dislocation density, rd, is deﬁned as the length of dislocation line per unit volume (m/m3). Even in an annealed soft metal, the dislocation density is around 1010 m/m3, meaning that a 1-cm cube (the size of a cube of sugar) contains about 10 km of dislocation line. When metals are deformed, dislocations multiply, causing their density to grow to as much as 1017 m/m3 or more e 100 million km per cubic centimetre! The reason that the yield stress rises is because a moving dislocation now ﬁnds that its slip plane is penetrated by a ‘forest’ of intersecting dislocations with a steadily decreasing average spacing L ¼ r1/2 (since rd is a number per unit area). d Figure 6.20(c) shows the idea schematically. As a moving dislocation advances, it bows out between pinning points at dislocation intersections e a relatively weak obstacle (a < 1). As the pinning point gives way, material above the slip plane slips relative to that below and creates a little step called a jog in each forest dislocation. These jogs have potential energy e they are tiny segments of dislocation of length b e and this is the source of the pinning force p, with
6.5 Manipulating strength
the result that p again scales with Gb2/2. Assembling these results into equation (6.17) gives the work-hardening contribution to the shear stress: swh ¼ a
Gb pﬃﬃﬃﬃﬃ ¼ aGb rd L
The greater the density of dislocations, the smaller the spacing between them, and so the greater their contribution to swh. All metals work harden. It can be a nuisance: if you want to roll thin sheet, work hardening quickly raises the yield strength so much that you have to stop and anneal the metal (that is, heat it up to remove the accumulated dislocations) before you can go on e a trick known to blacksmiths for centuries. But it is also useful: it is a potent strengthening method, particularly for alloys that cannot be heat-treated to give precipitation hardening. Grain boundary hardening Grain boundary hardening is a little different to the other mechanisms. Almost all metals are polycrystalline, made up of tiny, randomly oriented grains, meeting at grain boundaries like those of Figure 6.12(d). The grain size, D, is typically 10e100 mm. These boundaries obstruct dislocation motion, as shown in Figure 6.20(d). Dislocations in Grain 1 can’t just slide into the next one (Grain 2) because the slip planes don’t line up. Instead, new dislocations have to nucleate in Grain 2 with combined slip vectors that match the displacement caused by dislocations in Grain 1. The mechanism is as follows: dislocations ‘pile up’ at the boundary, creating the stress needed in the next grain to nucleate the matching dislocations. The number of dislocations in a pile-up scales with the size of the grain, and the bigger the pile-up, the lower the extra shear stress needed to enable slip to continue into the next grain. This gives another contribution to the shear stress, sgb, that is found to scale as D1/2, giving kp sgb ¼ pﬃﬃﬃﬃ D
where kp is called the Hall-Petch constant after the scientists who ﬁrst measured it. For normal grain sizes, sgb is small and not a signiﬁcant source of strength, but for materials that are microcrystalline (D < 1 mm) or nanocrystalline (D approaching 1 nm), it becomes signiﬁcant. Controlling the grain size is routine in conventional processing e in the initial casting of a liquid to make a solid shape, and then by deformation and heat treatments that lead to ‘recrystallisation’ in the solid e more on this in Chapter 19. More exotic processing is needed to produce really ﬁne grain sizes e rapid cooling from the melt, electroplating, vapor deposition, laser surface treatment, or compaction of nanoscale particles. These are difﬁcult to make and not easy to keep ﬁne-grained e the energy per unit area associated with grain boundaries means that, given a little thermal energy, the grains grow. Relationship between dislocation strength and yield strength To a ﬁrst approximation the strengthening mechanisms add up, giving a dislocation shear yield strength, sy, of sy ¼ si þ sss þ sppt þ swh þ sgb
Strong materials either have a high intrinsic strength, si (like diamond), or they rely on the superposition of solid solution strengthening sss, precipitation sppt and work hardening swh
158 Chapter 6 Beyond elasticity: plasticity, yielding and ductility (like high-tensile steels). Nanocrystalline solids exploit, in addition, the contribution of sgb. But before we can use this information, one problem remains: we have calculated the shear yield strength of one crystal, loaded in shear parallel to a slip plane. What we want is the yield strength of a polycrystalline material in tension. To link them, there are two simple steps. First, when a remote shear stress is applied to an aggregate of crystals, some crystals will have their slip planes oriented favourably with respect to the shear stress; others will not. This randomness of orientation means that the shear stress applied to a polycrystal that is needed to make all the crystals yield is higher than sy, by a factor of about 1.5 (called the Taylor factor, after the same G.I. Taylor who postulated the dislocation mechanism, with Orowan). This remote shear stress is referred to as the yield strength in shear, k e it is the shear stress that would cause a tube to yield in pure torsion, for instance. Second, yield strength is measured in uniaxial tension, so how does this axial stress produce the shear stress k that leads to yield of the polycrystal? The answer is that a uniform tensile stress s creates shear stress on all planes that lie at an angle to the tensile axis. Figure 6.21 shows a tensile force F acting on a rod of cross-section A. An inclined plane is shown with the normal to the plane at an angle q to the loading direction. It carries components of force Fsinq and Fcosq, parallel and perpendicular to the plane. The area of this plane is A/cosq, so the shear stress parallel to the plane is s¼
F sinq ¼ s sinq cosq A=cosq
where s ¼ F/A is the tensile stress. The variation of s is plotted against q in the ﬁgure e the maximum shear stress is found on planes at an angle of 45 , when s ¼ s/2. The yield strength in shear k is therefore equal to sy/2, where sy is the tensile yield stress.
Tensile stress σ
Area A F sin θ
Area A cos θ
θ = 90ο
ar She ss τ e r t s
τ = σ sin θ cos θ
F cos θ
θ = 0ο
τ = σ /2
Figure 6.21 The variation of stress with angle of the reference axes. A tensile stress s gives a maximum shear stress s ¼ s=2 on a plane at 45 to the tensile axis.
6.5 Manipulating strength
Combining these two factors, the tensile stress to cause yielding of a polycrystalline sample is approximately three times the shear strength of a single crystal: sy ¼ 2kz3sy As a result, the superposition of strengthening mechanisms in equation (6.22) applies equally to the yield strength, sy. Example 6.4 A polycrystalline aluminium alloy contains a dispersion of hard particles of diameter 108 m and an average centre-to-centre spacing of 6 108 m, measured in the slip planes. The shear modulus of aluminium is G ¼ 26 GPa and b ¼ 0.286 nm. Estimate the contribution of the hard particles to the yield strength of the alloy. Answer. For the alloy, L ¼ (6 1) 108 m ¼ 5 108 m, giving sppt ¼
Gb 27 109 0:286 109 ¼ ¼ 154 MPa L 5 108
Since sy ¼ 3sy for polycrystals, the contribution to the yield stress sy ¼ 462 MPa.
Example 6.5 Two cubes of aluminium of side length 1 cm are produced in annealed (soft) and coldworked (hard) conditions. The dislocation densities in the two samples are 105 mm2 and 109 mm2, respectively. Assuming a square array of parallel dislocations, estimate: (a) the total length of dislocation in each sample; (b) the distance between dislocations in the cold-worked sample; (c) the ratio of the contribution made by dislocation hardening to the strength of the cold-worked sample, to that of the annealed sample. Answer. (a) The dislocation density rd is the length of dislocation per unit volume. For a 1-cm cube, the volume ¼ 1000 mm3. For a dislocation density rd ¼ 105 mm2 (mm/mm3), the total length of dislocation ¼ 105 1000 ¼ 108 mm ¼ 100 km; for rd ¼ 109 mm2 (mm/mm3), the length is 1012 mm ¼ 1 million km!
160 Chapter 6 Beyond elasticity: plasticity, yielding and ductility (b) Assume that the dislocations form a uniform square array of side d. In this case, each dislocation sits at the centre of an area d2. For a unit length of dislocation, the volume of material per dislocation is 1 d2, so the dislocation density is rd ¼ 1/d2; hence, for the cold-worked sample 1 1 d ¼ pﬃﬃﬃﬃﬃ ¼ pﬃﬃﬃﬃﬃﬃﬃﬃ ¼ 32 nm rd 109
pﬃﬃﬃﬃﬃﬃ p10 ﬃﬃﬃﬃﬃﬃ95 10
pﬃﬃﬃﬃﬃ swh f rd ;
Strength and ductility of alloys Of all the properties that materials scientists and engineers have sought to manipulate, the strength of metals and alloys is probably the most explored. It is easy to see why: Table 6.1 gives a small selection of the applications of metals and their alloys e their importance in engineering design is clearly enormous. The hardening mechanisms are often used in combination. This is illustrated graphically for copper alloys in Figure 6.22. Good things, however, have to be paid for. Here the payment for increased strength is, almost always, loss of ductility, so the elongation εf is reduced. The material is stronger, but it cannot be deformed as much without fracture. This general trend is evident in Figure 6.23, which shows the nominal stressestrain curves for a selection of engineering alloys. Chapter 19 and Guided Learning Unit 2 will explore the practicalities of manipulating the strength and ductility of alloys in the context of processing.
Table 6.1 Metal alloys with typical applications, indicating the strengthening mechanisms used Solution hardening
Precipitation Work hardening hardening
Pure Al Pure Cu Cast Al, Mg Bronze (CueSn), Brass (CueZn) Non-heat-treatable wrought Al Heat-treatable wrought Al Low-carbon steels
Kitchen foil Wire Automotive parts Marine components
Ships, cans, structures
Car bodies, structures, ships, cans Automotive parts, tools Pressure vessels Jet engine turbines
U UUU UUU
UUU U UUU
Low-alloy steels Stainless steels Cast Ni alloys
Symbols: UUU, Routinely used; U, Sometimes used.
UUU UUU UU
6.5 Manipulating strength
σy, Yield strength
Brass, work hardened
Pure copper, work hardened
Pure, soft copper 20 1
Elongation εf (%)
Figure 6.22 Strengthening and ductility (elongation to fracture) for copper alloys. The hardening
mechanisms are frequently combined, but in general, the greater the strength, the lower the ductility.
Medium carbon steel
400 Drawn brass
Strain εn (%)
Figure 6.23 Nominal stressestrain curves for a selection of engineering alloys. Stronger alloys tend to have lower ductility.
162 Chapter 6 Beyond elasticity: plasticity, yielding and ductility Strengthening polymers In non-crystalline solids, the dislocation is not a helpful concept. We think instead of some unit step of the ﬂow process: the relative slippage of two segments of a polymer chain, or the shear of a small molecular cluster in a glass network. Their strength has the same origin as that underlying the lattice resistance: if the unit step involves breaking strong bonds (as in an inorganic glass), the materials will be strong and brittle, as ceramics are. If it only involves the rupture of weak bonds (the van der Waals bonds in polymers, for example), it will have low strength. Polymers, too, must therefore be strengthened by impeding the slippage of segments of their molecular chains. This is achieved by blending, by drawing, by crosslinking and by reinforcement with particles, ﬁbres or fabrics e again, we manipulate the microstructure-sensitive property of strength by a combination of composition and processing (see Chapter 19 for more details). A blend is a mixture of two polymers, stirred together in a sort of industrial food mixer. The strength and modulus of a blend are just the average of those of the components, weighted by volume fraction (a rule of mixtures again). If one of these is a low molecular weight hydrocarbon, it acts as a plasticiser, reducing the modulus and giving the blend a leather-like ﬂexibility. Drawing is the deliberate use of the molecule-aligning effect of stretching, like that sketched in Figure 6.11(a), to greatly increase stiffness and strength in the direction of stretch. Fishing line is drawn nylon, mylar ﬁlm is a polyester with molecules aligned in the plane of the ﬁlm, and geotextiles, used to restrain earth banks, are made from drawn polypropylene. Cross-linking, sketched in Figures 4.36 and 4.37, creates strong bonds between molecules that were previously linked by weak van der Waals forces. Vulcanized rubber is rubber that has been cross-linked, and the superior strength of epoxies derives from cross-linking. Reinforcement is possible with particles of cheap ﬁllers e sand, talc or wood dust. Far more effective is reinforcement with ﬁbres e usually glass or carbon e either continuous or chopped, as explained in Chapter 4.
Summary and conclusions
Load-bearing structures require materials with reliable, reproducible strength. There is more than one measure of strength. Elastic design requires that no part of the structure suffers plastic deformation, and this means that the stresses in it must nowhere exceed the yield strength, sy, of ductile materials or the elastic limit of those that are not ductile. Plastic design and deformation processing, by contrast, require some or all parts of the structure to deform plastically, either to absorb energy or to enable the shape to be changed. Then two further properties become relevant: the ductility, εf, and the tensile strength, sts, which are the maximum strain and the maximum stress the material can tolerate before fracture. The tensile strength is generally larger than the yield strength because of work hardening. Charts plotting strength, like those plotting modulus, show that material families occupy different areas of material property space, depending on the strengthening mechanisms on which they rely. Strength for metals is a particularly microstructure-sensitive property. Crystal defects e particularly dislocations e are central to the understanding of alloy hardening. It is the motion of dislocations that gives plastic ﬂow in crystalline solids, giving them unexpectedly low strengths. When strength is needed, it has to be provided by the strengthening mechanisms that impede dislocation motion.
First among these is the lattice resistance e the intrinsic resistance of the crystal to dislocation motion. Others can be deliberately introduced by alloying and heat treatment. Solid solution hardening, dispersion and precipitation hardening, work hardening and grain boundary hardening add to the lattice resistance. The strongest materials utilise more than one mechanism. Non-crystalline solids e particularly polymers e deform in a less organised way by the tangled polymer chains sliding and sometimes aligning with the direction of deformation. This leads to cold drawing with substantial plastic strain and, at lower temperatures, to crazing or shear banding. The stress required to do this is signiﬁcant, giving polymers useful intrinsic strength. This can be enhanced by blending, cross-linking and reinforcement with particles or ﬁbres to give the engineering polymers we use today.
Ashby, M. F., & Jones, D. R. H. (2011/2012). Engineering materials I & II (4th ed.). Oxford, UK: Butterworth-Heinemann. ISBN 978e0080966656 and ISBN 978-0080966687. (An introduction to mechanical properties and processing of materials.) Cottrell, A. H. (1953). Dislocations and plastic ﬂow in crystals. Oxford, UK: Oxford University Press. (Long out of print but worth a search: the book that ﬁrst presented a coherent picture of the mechanisms of plastic ﬂow and hardening.) Friedel, J. (1964). Dislocations. Reading. MA, USA: Addison-Wesley. Library of Congress No. 65e21133. (A book that, with that of Cottrell, ﬁrst established the theory of dislocations.) Hertzberg, R. W. (1989). Deformation and fracture of engineering materials (3rd ed.). New York, USA: Wiley. ISBN 0-471-61722-9. (A readable and detailed coverage of deformation, fracture and fatigue.) Hull, D., & Bacon, D. J. (2001). Introduction to dislocations (4th ed.). Oxford, UK: ButterworthHeinemann. ISBN 0-750-064681-0. (An introduction to dislocation mechanics.) Hull, D., & Clyne, T. W. (1996). An introduction to composite materials (2nd ed.). Cambridge, UK: Cambridge University Press. ISBN 0-521-38855-4. (A concise and readable introduction to composites that takes an approach that minimises the mathematics and maximises the physical understanding.) Young, R. J. (1981). Introduction to polymers. London, UK: Chapman & Hall. ISBN 0-412-22180-2. (A good starting point for more information on the chemistry, structure and properties of polymers.)
Sketch a stressestrain curve for a typical metal. Mark on it the yield strength, sy , the tensile strength sts and the ductility εf . Indicate on it the work done per unit volume in deforming the material up to a strain of ε < εf (pick your own strain ε).
On a sketch of a typical stressestrain curve for a ductile metal, distinguish between the maximum elastic energy stored per unit volume and the total energy dissipated per unit volume in plastic deformation. Give examples of
164 Chapter 6 Beyond elasticity: plasticity, yielding and ductility engineering applications in which a key material characteristic is: (i) maximum stored elastic energy per unit volume; (ii) maximum plastic energy dissipated per unit volume. Exercise E6.3
In Exercise E4.2, the extension of the cable of a hoist was considered when lifting a mass of 250 kg. Find the stress in the cable of cross-sectional area 80 mm2, and evaluate the factor of safety between the applied stress and the yield stress, for steel (yield stress 300 MPa) and polypropylene (yield stress 32 MPa)? What mass would lead to failure in each material?
(a) Write down expressions for the nominal strain and the true strain for the following situations: (i) in a tensile test where the length of the specimen increases from Lo to L. (ii) in a compression test where the height of the specimen decreases from ho to h. (b) In what circumstances can the true strain be approximated by the nominal strain?
In a two-stage elongation of a specimen, the length is ﬁrst increased from lo to l1 and then from l1 to l2 . Write down the true strains ε1 and ε2, respectively, for each of the two elongation processes considered separately. Show that the true strain for the overall elongation lo to l2 is given by the sum of the true strains for each of the two separate processes. Is the same true for the nominal strains?
In a ‘tandem’ rolling process, a wide metal strip passes continuously between four sets of rolls, each of which apply a reduction in thickness. The strip elongates without getting wider, and therefore accelerates. For an incoming thickness hin ¼ 25 mm moving at speed vin ¼ 5 cms1, and an exit thickness hout ¼ 3.2 mm, calculate: (i) the overall true strain applied to the material; (ii) the exit speed vout. State any assumptions made.
Explain brieﬂy why the material property bubbles for metals are very elongated on the Young’s modulusestrength chart (Figure 6.8). Comment on whether the same is true for the polymers. Why is this?
Using the material property tables in Appendix A, compare the densities, the Young’s moduli and the yield strengths of the ferrous alloys (alloys based on iron, usually with carbon, and commonly other alloying elements). Comment on the spread of values for each property, and identify which of the properties is microstructure-sensitive.
Use the yield strengthedensity chart or the yield strengthemodulus chart (Figures 6.7 and 6.8) to ﬁnd:
the metal with the lowest strength the approximate range of strength of the composite GFRP
whether there are any polymers that are stronger than wood measured parallel to the grain how the strength of GFRP compares with that of wood whether elastomers, that have moduli that are far lower than polymers, are also far lower in strength.
CFRP and the ‘light alloys’ (Mg, Al and Ti) have excellent strength-to-weight characteristics as measured by the ratio sy/r, but how closely do they compete? Draw a contour of sy/r onto a copy of Figure 6.7 and use it to resolve the question (using the strongest variants in each case).
(a) Use the property data in Appendix A to tabulate density r, and yield strength sy of Mg, Al and Ti alloys and CFRP. (b) The arithmetic mean of two numbers P1 and P2 is P ¼ ðP1 þ P2 Þ 2. The p ﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ ﬃ b ¼ P1 P2 . Calculate the arithmetic and geometric geometric mean is P means of the strength and density values of the materials in the table, and comment on the size of the difference in the two means for each property. (c) Plot the geometric means for the strength as horizontal lines on Figure 6.7. What do you observe about the position of the lines relative to the bubbles for each material?
What is meant by the ideal strength of a solid? Which material class most closely approaches it?
(a) Explain brieﬂy the four main microstructural mechanisms by which metals are hardened. Identify which mechanisms account for the following increases in yield stress (NB there may be more than one): (i) Pure annealed aluminium: 25 MPa; cold rolled non-heat-treatable AleMneMg alloy: 200 MPa. (ii) Pure annealed copper: 20 MPa; cast 60e40 brass (60% Cu, 40% Zn): 105 MPa. (iii) Pure annealed iron: 140 MPa; quenched and tempered mediumcarbon steel: 600 MPa. (iv) Pure annealed copper: 20 MPa; nanocrystalline pure Cu: 500 MPa. (b) For each of mechanisms (i)e(iii) in part (a), give other examples of important engineering alloys which exploit these mechanisms.
An aluminium alloy used for making cans is cold rolled into a strip of thickness 0.3 mm and width 1m. It is coiled round a drum of diameter 15 cm, and the outer diameter of the coil is 1 m. In the cold-rolled condition, the dislocation density is approximately 1015 m2. Estimate: (i) The mass of aluminium on the coil. (ii) The total length of strip on the coil. (iii) The total length of dislocation in the coiled strip.
166 Chapter 6 Beyond elasticity: plasticity, yielding and ductility
The lattice resistance of copper, like that of most FCC metals, is small. When 10% of nickel is dissolved in copper to make a solid solution, the strength of the alloy is 150 MPa. What would you expect the strength of an alloy with 20% nickel to be (neglecting the lattice resistance)?
(a) Explain brieﬂy how impeding the motion of dislocations with dispersed precipitates in a metal can raise the yield stress. (b) A straight segment of dislocation line of length L is pinned at two particles in a crystal. The application of a shear stress s causes the dislocation to bow outwards as shown in the ﬁgure, decreasing its radius of curvature as it does so. The force per unit length acting on the dislocation is sbL, where b is the Burgers vector. Given that the dislocation line tension T ¼ Gb2 2, show that the stress just large enough to fully bow out the dislocation segment into a semi-circle is given by s ¼ Gb=L:
(c) Estimate the tensile yield stress of aluminium containing an array of equally spaced second phase precipitates, where the volume fraction of the second phase is 5% and the precipitate diameter is 0.1 mm. The Burgers vector for aluminium is 0.29 nm, and the shear modulus G ¼ 27 GPa. (d) If incorrect heat treatment of the aluminium alloy results in a nonuniform distribution of precipitates, explain the effect this would have on the yield stress. Exercise E6.17
A metal matrix composite consists of aluminium containing hard particles of silicon carbide SiC with a mean spacing of 1 mm. The yield strength of the composite is found to be 8 MPa greater than the unreinforced matrix alloy. If a new grade of the composite with a particle spacing of 0.2 mm were developed, what would you expect the strength contribution of the particles to be?
Nano-crystalline materials have grain sizes in a range 0.01e0.1 mm. If the contribution of grain boundary strengthening in an alloy with grains of 0.1 mm is 20 MPa, what would you expect it to be if the grain size were reduced to 0.01 mm?
The yield strength sy of low-carbon steel is moderately dependent on the grain size D, and the relation can be described by the equation: pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ sy ¼ so þ k 1=D where so and k are material constants. The yield strength is 322 MPa for a grain size of 180 mm and 363 MPa for a grain size of 22 mm. (a) Calculate the yield strength of the steel for a grain size of 11 mm. (b) Explain brieﬂy the physical signiﬁcance of the constant so .
From the uniaxial stressestrain responses for various metals in Figure 6.23: (a) Find the yield stress (or if appropriate a 0.2% proof stress), the tensile strength, and the ductility of each alloy. (b) Account for the differences in strength, comparing annealed copper with each of the other alloys in turn. The ﬁgure shows typical data for a selection of Al alloys on a strengtheductility property chart. Compare this with the corresponding data for Cu alloys (Figure 6.22). Do the same overall trends apply with regard to: (i) the trade-off between strength and ductility? (ii) the ranking of the hardening mechanisms in order of increasing effectiveness? Estimate the ratio of the highest strength alloy to that of the pure, annealed base metal for Al and Cu. 1000
Heat-treatable Al alloys
Rolled Al-Mg alloy 200
Rolled pure Al
Rolled Al-Mg-Mn alloy
Annealed Al-Mg alloy
Annealed Al-Mg-Mn alloy Annealed pure Al 20 1
Elongation εf (%)
168 Chapter 6 Beyond elasticity: plasticity, yielding and ductility
From the uniaxial stressestrain responses for various polymers in the ﬁgure: (a) Estimate the tensile strengths and ductility of each material. (b) Account for the main differences between the shapes of the graphs for PMMA, ABS and polypropylene. Polyester + 20% chopped glass fibre
Stress σn (MPa)
Polypropylene, PP (>500% strain)
20 10 0
Strain εn (%)
Polycarbonate, PC (yield strength 70 MPa), is blended with polyester, PET (yield strength 50 MPa), in the ratio 30%:70%. If the strength of blends follows a rule of mixtures, what would you expect the yield strength of this blend to be?
Sketch a Young’s modulusestrength chart using log scales with ranges of E from 1 to 10 GPa, and strength sy from 10 to 100 MPa. Plot the data given in the table below for polypropylene with various additions. Comment on the effect of each type of addition on Young’s modulus and strength.
Material PP (unmodiﬁed) PP þ 10% EP rubber (impact modiﬁer) PP þ 20% CaCO3 PP þ 40% CaCO3 PP þ 20% talc PP þ 40% talc PP þ 20% glass ﬁbre PP þ 40% glass ﬁbre
Young’s modulus E (GPa)
Strength sy (MPa)
1.3 1.7 1.6 3.0 3.0 8.0
21 19 25 24 47 90
Strength-limited design can be elastic e ensuring that the cabin of the car does not deform in a crash e or plastic e absorbing the impact energy in the front of the car (left). Plasticity allows metals to be formed (right) and polymers to be moulded. (Image of crash testing courtesy AutoNews; image of hot rolling courtesy of Tanis Inc., Delaﬁeld, WI).
Chapter contents 7.1 7.2 7.3 7.4 7.5 7.6 7.7
Introduction and synopsis Standard solutions to plastic problems Material indices for yield-limited design Case studies Summary and conclusions Further reading Exercises
169 170 179 184 190 190 191
Introduction and synopsis
Stiffness-limited design, described in Chapter 5, is design to avoid excessive elastic deﬂection. Strength-limited design, our concern here, is design to avoid plastic collapse. That generally means design to avoid yield, arranging that the component remains elastic throughout, when it is called elastic design. Elastic design is not always possible or necessary: local yielding may be permissible provided general yield is avoided. That is half the picture. The other half is design to permit controlled plastic collapse. The safety of modern cars relies on the front of the car absorbing the kinetic energy in a collision by plastic deformation. And the manufacturing processes of metal rolling, forging, extrusion and Copyright Ó 2019 Elsevier Ltd. All rights reserved. https://doi.org/10.1016/B978-0-08-102376-1.00007-X
170 Chapter 7 Strength-limited design drawing use plastic ﬂow. Here, the strains are large, and the focus is on the forces and work necessary to achieve a prescribed change of shape. Plasticity problems are solved in more than one way. When yield is to be avoided, we analyse the elastic state of stress in a component and make sure that this nowhere exceeds the yield strength. Full plasticity, by contrast, requires general yield. Then the mechanism of plastic collapse must be identiﬁed and the collapse load calculated by requiring that yield does occur where it needs to. Chapter 5 introduced elastic solutions for common modes of loading: tension, compression, bending, torsion or internal pressure. Not surprisingly, there are equivalent results for plastic design, and we start with these, using them to develop material indices for strength-limited design and applying them via case studies.
Standard solutions to plastic problems
Yielding of ties and columns A tie is a rod loaded in tension; a column is a rod loaded in compression. The state of stress within them is uniform, as was shown in Figure 5.1(a). If this stress, s, is below the yield strength sy, the component remains elastic; if it exceeds sy, it yields. Yield in compression is only an issue for short, squat columns. Slender columns and panels in compression are more likely to buckle elastically ﬁrst (Chapter 5). Yielding of beams and panels The stress state in bending was introduced in Chapter 5. A bending moment M generates a linear variation of longitudinal stress s across the section (Figure 7.1(a)) deﬁned by s M ¼ ¼ Ek y I
where y is the distance from the neutral axis, k is the beam curvature, and the inﬂuence of the cross-section shape is captured by I, the second moment of area. For elastic deﬂection, we were interested in the last term in the equation e that containing the curvature. For yielding, it is the ﬁrst term. The maximum longitudinal stress smax occurs at the surface (Figure 7.1(a)) at the greatest distance, ym, from the neutral axis smax ¼
Mym M ¼ Ze I
The quantity Ze ¼ I/ym is called the elastic section modulus (not to be confused with the elastic modulus of the material, E). If smax exceeds the yield strength sy of the material of the beam, small zones of plasticity appear at the surface where the stress is highest, as in Figure 7.1(b). The beam is no longer elastic and, in this sense, is damaged even if it has not failed completely. If the moment is increased further, the linear proﬁle is truncated e the stress near the surface remains equal to sy, and plastic zones grow inward from the surface. Although the plastic zone has yielded, it still carries load. As the moment increases further, the plastic zones grow until they penetrate through the section of the beam, linking to form a plastic hinge (Figure 7.1(c)). This is the maximum moment that can be carried by the beam; further increase causes it to collapse by rotating about the plastic hinge.
7.2 Standard solutions to plastic problems 171 y
1/κ (a) Elastic
y Tension σy
(b) Onset of plasticity Plastic zone
y Tension σy
(c) Full plasticity
Figure 7.1 A beam loaded in bending. The stress state is shown on the right for (a) purely elastic loading, (b) the onset of plasticity, and (c) full plasticity.
Example 7.1 Calculate the maximum bending stress in the 300 25 1-mm stainless steel ruler in Examples 5.2 and 5.4, when it is mounted as a cantilever with the X-X axis horizontal with 250 mm protruding and a weight of 10 N is hung from its end, as shown. Compare this bending stress with the range of yield strength of the material from Appendix A, and with the direct stress when a 10 N force is used to pull the ruler axially.
172 Chapter 7 Strength-limited design Answer. The maximum bending moment M in the cantilever (at its base e adjacent to the support) is M ¼ WL ¼ 0.25 10 ¼ 2.5 Nm. Using equation (7.2) with IXX ¼ 2.1 mm4 (from Example 5.2), and ym ¼ 0.5 mm at the extreme ﬁbre of the beam, s¼
Mym 2:5 0:0005 ¼ ¼ 595 MPa Ixx 2:1 1012
From Appendix A, the yield strength of stainless steel lies in the range 170e1000 MPa. So the ruler would have to be made of quite a strong stainless steel to withstand this load without yielding. When loaded by the same force in tension, the stress would be s¼
F 10 ¼ ¼ 0:4 MPa wt 25 1
This stress is far less than the bending stress for the same load, and well below the strength of most engineering materials (see Figure 6.7).
Figure 7.2 shows simply supported beams loaded in bending. In the ﬁrst, the maximum moment M is FL, in the second, it is FL/4 and in the third, FL/8. Plastic hinges form at the positions indicated in red when the maximum moment reaches the moment for collapse. This failure moment, Mf, is found by integrating the moment caused by the constant stress distribution over the section (as in Figure 7.1(c)), compression one side, tension the other Z Mf ¼ bðyÞ jyj sy dy ¼ Zp sy (7.3) section
where Zp is the plastic section modulus. So two new functions of section shape have been deﬁned for failure of beams: one for ﬁrst yielding, Ze, and one for full plasticity, Zp. In both cases, the moment required is simply Zsy. Example expressions for both are shown in Figure 7.3. The ratio Zp:Ze is always greater than one and is a measure of the safety margin between initial yield and collapse. For a solid rectangle, it is 1.5, meaning that the collapse load is 50% higher than the load for initial yield. For efﬁcient shapes, like tubes and I-beams, the ratio is much closer to 1 because yield spreads quickly from the surface to the neutral axis.
Figure 7.2 The plastic bending of beams.
7.2 Standard solutions to plastic problems 173
Area A m2
Elastic section modulus Ze m3
Plastic section modulus Zp m3
b h2 6
b h2 4
t 2 ri
π (r 4– r 4) o i
π (ro2 – ri2)
(t 1 is found by integrating over time: ! 1 1 1 t¼ ðn 1ÞBE sn1 sn1 i Solving for s=si as a function of t gives s 1 ¼ with to ¼ ðn 1ÞBEsn1 i si ðt=to þ 1Þ1=ðn1Þ The stress s=si is plotted as a function of t=to in Figure 13.28, for three values of n. The relaxation is most extensive when n is small. As it rises, the drop in stress becomes less, until it disappears as n approaches inﬁnity (i.e. rate-independent plasticity). Since transient creep is neglected, these curves overestimate the relaxation time for the ﬁrst tightening of the bolt, but improve for longer times.
368 Chapter 13 Diffusion and creep: materials at high temperatures
Summary and conclusions
All material properties depend on temperature. Some, like the density and the modulus, change relatively little and in a predictable way, making compensation easy. Transport properties, meaning thermal conductivity and conductivity for matter ﬂow (which we call diffusion), change in more complex ways. The last of these e diffusion e has a profound effect on mechanical properties when temperatures are high. To understand and use diffusion we need the idea of thermal activation e the ability of atoms to jump from one site to another, using thermal energy as the springboard. In crystals, atoms jump from vacancy to vacancy, but in glasses, with no ﬁxed lattice sites, the jumps occur when enough free volume comes together to make an atom-sized hole. This atom motion allows the intermixing of atoms in a concentration gradient. External stress, too, drives a ﬂux of atoms, causing the material to change shape in a way that allows the stress to do work. Diffusion plays a fundamental role in the processing of materials, the subject of Chapters 18 and 19 and Guided Learning Unit 2. It is also diffusion that causes creep and creep fracture. Their rates increase exponentially with temperature, introducing the ﬁrst challenge for design: that of predicting the rates with useful accuracy. Exponential rates require precise data e small changes in activation energy give large changes in rates e and these data are hard to measure and are sensitive to slight changes of composition. And there is more than one mechanism of creep, compounding the problem. The mechanisms compete, the one giving the fastest rate winning. If you design using data and formulae for one, but another is dominant under service conditions, then you are in trouble. Deformation mechanism maps help here, identifying both the mechanism and the approximate rate of creep. A consequence of all this is that materials selection for high-temperature design, and the design itself, is based largely on empirical data rather than on modelling of the sort used for elastic and plastic design in Chapters 5, 7, and 10. Empirical data are presented as plots, for individual alloys, of the creep strain-rate and life as functions of temperature and stress. For polymers a different approach is used. Because their melting points and glass temperatures are low, they are visco-elastic at room temperature. Then design can be based on plots of the creep modulus e the equivalent of Young’s modulus for a creeping material. The creep modulus at a given temperature and time is read off the plot and used in standard solutions for elastic problems (Chapter 5) to assess stress or deﬂection. The chapter presented examples of the use of some of these methods and case studies in material innovation to manage the extremes of high temperature performance, for example, in aerospace.
Cottrell, A. H. (1964). The mechanical properties of matter. London, UK: Wiley. Library of Congress Number 64e14262. (Now over 50 years old and out of print, but still a superb introduction to the mechanical properties of matter. Worth hunting for.) Finnie, I., & Heller, W. R. (1959). Creep of engineering materials. New York, USA: McGraw-Hill. Library of Congress No. 58e11171. (Old and somewhat dated, but still an excellent introduction to creep in an engineering context.)
Frost, H. J., & Ashby, M. F. (1982). Deformation mechanism maps. Oxford, UK: Pergamon Press. ISBN 0-08-029337-9. (A monograph compiling deformation mechanism maps for a wide range of materials, with explanation of their construction.) Penny, R. K., & Marriott, D. L. (1971). Design for creep. New York, USA: McGraw-Hill. ISBN 07-094157-2. (A monograph bringing together the mechanics and the materials aspects of creep and creep fracture.) Waterman, N. A., & Ashby, M. F. (1991). The Elsevier materials selector. Barking, UK: Elsevier Applied Science. ISBN 1-85166-605-2. (A three-volume compilation of data and charts for material properties, including creep and creep fracture.)
Use the property chart in Figure 13.7 to identify materials with potential for use above 1000 C.
Use the property chart in Figure 13.8 to identify materials that are suitable for carrying a tensile stress of 100 MPa at 950 C, with a creep strain-rate below 106 s1. Use the contours of speciﬁc creep strength at this temperature, s950 C =r , to identify the lightest material.
The diffusion constants Do and Qd for lattice self-diffusion of aluminium are listed in Appendix A, Table A9. Use these to calculate the diffusion coefﬁcient D in aluminium at 400 C.
The element lead (Pb) has a number of isotopes. The most stable and commonest is Pb (207). A thin layer of Pb (204) is plated onto a thick plate of Pb (207) and the couple is held at 200 C for 4 h. What is the approximate depth of penetration of the Pb (204) into the plate? You will ﬁnd data for diffusion coefﬁcients in Appendix A, Table A9.
A steel component is nickel plated to give corrosion protection. To increase the strength of the bond between the steel and the nickel, the component is heated for 4 h at 1000 C. If the diffusion parameters for nickel in iron are Do ¼ 1.9 104 m2/s and Qd ¼ 284 kJ/mol, how far would you expect the nickel to diffuse into the steel in this time?
The diffusion coefﬁcient at the melting point for materials is approximately constant, with the value D ¼ 1012 m2/s. What is the diffusion distance if a material is held for 12 h at just below its melting temperature? This distance gives an idea of the maximum distance over which concentration gradients can be smoothed by diffusion.
In the fabrication of a silicon semiconductor device, boron is diffused into silicon in two stages: a pre-deposition stage lasting 10 min at a temperature of 1000 C, followed by a drive-in stage for 2 h at 1100 C. Compare the characteristic diffusion distances of these two stages. For the diffusion of boron in silicon, Do ¼ 3.7 106 m2/s, and the activation energy Q ¼ 333 kJ/mol.
370 Chapter 13 Diffusion and creep: materials at high temperatures Exercise E13.8
(a) The diffusion constant for carbon diffusion in FCC iron is Do ¼ 2.3 105 m2/s, and the activation energy Q ¼ 148 kJ/mol. Find the diffusion coefﬁcient D for carbon in iron at 1000 C and its approximate distance of diffusion in time t. (b) Compare this with the thermal diffusivity of steel at 1000 C, a ¼ 9 106 m2/s.
Use your knowledge of diffusion and solid solutions to account for the following observations: (a) The rate of diffusion of oxygen from the atmosphere into an oxide ﬁlm is strongly dependent on the temperature and the concentration of oxygen in the atmosphere. (b) Diffusion is more rapid in polycrystalline silver with a small grain size than in coarse-grained silver. (c) Carbon diffuses far more rapidly than chromium through iron.
(a) Explain brieﬂy, with sketches as appropriate, the differences between the following pairs of mechanisms in metal deformation: (i) room temperature yielding and power-law creep; (ii) power-law creep and diffusional ﬂow. (b) Explain the following manufacturing characteristics: (i) superplastic forming requires a ﬁne grain size material; (ii) creep-resistant alloys are often cast as single crystals.
A high-temperature alloy undergoes power-law creep when the applied stress is 70 MPa and the temperature is 1000 C. The stress exponent n is 5. By what factor will the strain-rate increase if the stress is raised to 80 MPa at the same temperature?
The high temperature alloy of Exercise E13.11 undergoes power-law creep when the applied stress is 70 MPa and the temperature is 1000 C. The activation energy for creep Q is 300 kJ/mol. By what factor will the strainrate increase if the temperature is increased to 1100 C?
Pipework with a radius of 20 mm and a wall thickness of 4 mm made of 2¼ CreMo steel contains a hot ﬂuid under pressure. The pressure is 10 MPa at a temperature of 600 C. The table lists the creep constants for this steel. Calculate the creep rate of the pipe wall, assuming steady-state power-law creep.
Reference strain-rate ε_ o (1/s)
Reference stress so (MPa)
Creep exponent n
Activation energy Qc (kJ/mol)
2¼ CreMo steel
There is concern that the pipework described in Exercise E13.13 might rupture in less than the design life of 1 year. If the MonkmaneGrant constant for 2¼ CreMo steel is C ¼ 0.06, how long will it last before it ruptures?
If the creep rate of a component made of 2¼ CreMo steel must not exceed 108/s at 500 C, what is the greatest stress that it can safely carry? Use the data in Exercise E13.13 to ﬁnd out.
The designers of a chemical plant are concerned about creep failure of a critical alloy tie bar. They have carried out creep tests on specimens of the alloy under the nominal service conditions of a stress s of 25 MPa at 620 C, and found a steady-state creep rate ε_ of 3.1 1012/s. In service it is expected that for 30% of the running time the stress and temperature may increase to 30 MPa and 650 C, respectively, while for the remaining time the stress and temperature will be at the nominal service values. Calculate the expected average creep rate in service. It may be assumed that the alloy creeps according to the equation: Qc ε_ ¼ Csn exp RT where C and Q are constants, R is the universal gas constant, and T is the absolute temperature. For this alloy, Q ¼ 160 kJ/mol and n ¼ 5.
(a) The steady-state creep strain-rate at constant temperature ε_ ss depends on the applied stress according to ε_ ss ¼ Bsn where B and n are constants. The ﬁgure shows the steady-state creep response of a 12% Cr steel at 500 C. Determine B at this temperature, and the creep exponent n for this material. (b) A 12% Cr steel turbine blade of length 10 cm runs with an initial clearance of 100 mm between its tip and the housing in a generator operating at 515 C. Determine the lifetime of the blade if it runs continuously, assuming a uniform tensile stress of 60 MPa is applied along its axis. (The creep activation energy Q for 12% Cr steel is 103 kJ/mol.) (c) The axial stress in the blade derives from the centripetal force of the fast rotating turbine. Is the assumption of a uniform stress justiﬁed? If the stress varies along the length of the blade, is it adequate to use an average value?
372 Chapter 13 Diffusion and creep: materials at high temperatures
5 255 MPa
2 205 MPa
Time (x 1000 minutes)
Molten aluminium is cast into a copper mould having a wall thickness of 5 mm. The diffusion coefﬁcient D of aluminium in copper is 2.6 1017 m2/s at 500 C and 1.6 1012 m2/s at 1000 C. (a) Calculate the activation energy Q and the pre-exponential Do for the diffusion of aluminium in copper. By considering the mechanisms of diffusion, list some factors that will affect the value of Q in diffusioncontrolled processes in crystalline solids. (b) Use the diffusion constants derived in part (a) to calculate the coefﬁcient of diffusion of aluminium in copper at 750 C. (c) A useful rule of thumb in diffusion problems pﬃﬃﬃﬃﬃﬃstates that the characteristic diffusion distance in time t is given by Dt, where D is the diffusion coefﬁcient for the temperature concerned. Make an order-of-magnitude estimate of the time taken for an aluminium atom to diffuse through the wall of the copper mould if the mould temperature is 750 C.
A thick steel plate of thickness 2w ¼ 0.2 m is continuously cast into a long sheet. Segregation during solidiﬁcation (discussed in Guided Learning Unit 2) gives a non-uniform concentration of a key substitutional alloying element in the steel. The initial distribution of solute is sinusoidal with the maximum concentration on the centre-line, falling to zero at the surface. A homogenisation treatment is proposed to redistribute the solute more uniformly. Solution of the differential equation for transient diffusion predicts that the concentration proﬁle has the form px Cðx; tÞ ¼ Co þ Co cos expðt=sÞ w where s ¼ w2 p2 D , where D is the diffusion coefﬁcient for the solute element in steel.
(a) Sketch the solute distribution for times t ¼ 0, s, and 10s. (b) An attempt is made to homogenise the casting by holding at a high temperature for 12 h. At the treatment temperature, the relevant diffusion coefﬁcient D ¼ 4 1015 m2/s. Will this treatment make any signiﬁcant difference to the solute distribution? (c) The casting process is modiﬁed to prevent the solute distribution developing across the whole plate. A micro-probe analysis then identiﬁes a sinusoidal variation of amplitude 0.2Co across the grains in the casting, about a mean of Co. If the grain size is 50 mm (i.e. the length scale of the concentration gradient w ¼ 25 mm), what is the maximum % deviation from the average concentration within the grain after the 12 h heat treatment? Exercise E13.20
A carbon steel component containing Co ¼ 0.2 wt% C is to be carburised at a temperature of 1000 C, at which the maximum solubility of carbon is 1.6 wt% e this is the (constant) surface concentration Cs throughout the treatment. The concentration as a function of time t and depth below the surface x is given by
x Cðx; tÞ ¼ Co þ ðCs Co Þ 1 erf pﬃﬃﬃﬃﬃﬃ 2 Dt The diffusion coefﬁcient D for carbon diffusion in iron at 1000 C is 1.94 1011 m2/s, and values for the error function are given in the table.
Sketch the variation of carbon concentration C against distance x below the surface, for treatment times of 15 min and 1 h. By what factor does the diffusion depth increase between these two treatment times? Find the time required for carburisation to a depth of 0.3 mm, if the target concentration at this depth is C ¼ 0.5 wt% carbon. Exercise E13.21
(a) Brieﬂy summarise the important microstructural characteristics of a creep-resistant material, distinguishing between features that inﬂuence diffusional ﬂow and power-law creep. (b) Polycrystalline copper has a steady-state creep rate of 104 s1 at 560 C when subjected to a given tensile stress. The activation energy Q for self-diffusion in copper is 197 kJ/mol. Calculate the steady-state creep rate of copper at 500 C at the same stress.
374 Chapter 13 Diffusion and creep: materials at high temperatures Exercise E13.22
Creep data for a stainless steel at two constant temperatures are shown in the ﬁgure. The steel obeys the steady-state creep equation ε_ ¼ C'sn expð Q=RTÞ where R ¼ 8.314 J/mol K. (a) A specimen of the steel of length 750 mm was subjected to a tensile stress s ¼ 40 MPa at a temperature T ¼ 538 C. Use the data plotted in the ﬁgure to estimate the extension after 5000 h. (b) Use the data plotted in the ﬁgure to evaluate the constants n and Q for the stainless steel. 200
Creep strain-rate (%/1000h)
A solid cylinder of the stainless steel described in Exercise E13.22 was designed for operation as a support for a turbine housing under a uniform tensile load P ¼ 6 kN and a temperature T ¼ 450 C. A routine check after 10,000 h in service revealed that the extension of the cylinder was 50% higher than expected, due to the applied load being higher than the design speciﬁcation. The extension that had occurred was half of the maximum allowable before the component would need to be replaced. (a) Evaluate the load that had actually been applied, given that the operating temperature had been correctly maintained. (b) The loading on the component could not be corrected, but a drop in operating temperature of 20 C was possible. Would this be sufﬁcient to allow a further 40,000 h of operation before replacement?
The ﬁgure shows a deformation mechanism map for a nickel alloy. The contours are lines of equal strain-rate for steady-state creep in units of se1. (a) Estimate by eye the maximum allowable stress at 600 C if the maximum allowable strain rate is 1010 s1. (b) Estimate the creep rate if the stress were increased by a factor of 3 and the temperature raised by 200 C. Nickel alloy
Stress σ, MPa
grain size 0.5mm
Diffusional flow 0.1
Temperature T, oC
The strain-rate contours on the map in Exercise E13.24 for both diffusional ﬂow and power-law creep are based on curve ﬁts to the creep equation: ε_ ¼ C0 sn expð Q=RTÞ Use the strain-rate contours on the map to estimate the value of the stress exponent n, for diffusional ﬂow and for power-law creep.
A stainless steel suspension cable in a furnace is subjected to a stress of 100 MPa at 700 C. Its creep rate is found to be unacceptably high. By what mechanism is it creeping? What action would you suggest to tackle the problem? The ﬁgure shows the deformation mechanism map for the material.
376 Chapter 13 Diffusion and creep: materials at high temperatures
grain size 10 μm
Yielding by dislocation plasticity 10
Stress σ, MPa
800 Temperature oC 600
The wall of a pipe of the same stainless steel as that of Exercise E13.26 carries a stress of 3 MPa at the very high temperature of 1000 C. In this application it, too, creeps at a rate that is unacceptably high. By what mechanism is it creeping? What action would you suggest to tackle the problem?
It is proposed to make a shelf for a hot-air drying system from acrylic sheet. The shelf is simply supported, as in the diagram, and has a width w ¼ 500 mm, a thickness t ¼ 8 mm, and a depth b ¼ 200 mm. It must carry a distributed load of 50 N at 60 C with a design life of 8000 h (about a year) of continuous use. Use the creep modulus plotted in Figure 13.19 and the solution to the appropriate elastic problem (Chapter 5, equation (5.5) and Figure 5.3) to ﬁnd out how much it will sag in that time. F t
In a series of stress relaxation experiments on PMMA conducted at 25 C, a cylindrical bar of polymer is subjected to an instantaneous step-wise compressive strain of 1%, at time t ¼ 0. The stress in the bar decays with time according to the following table.
Stress (MPa) Time (s)
The relaxation of the polymer can be represented by a Maxwell model of a spring of modulus E (for which E ¼ s=ε in series with a dash-pot of viscosity h, for which h ¼ s=_ε, as in Figure 13.18). The relaxation response is given by s ¼ so expðt=sÞ where s ¼ h=E, and so is the initial stress at t ¼ 0. Use the experimental data to estimate the values of E; h, and the relaxation time s ¼ h=E.
This page intentionally left blank
Durability: oxidation, corrosion, degradation
Corrosion Image courtesy of Norbert Wodhnl Ó Norbert Wodhnl.
Chapter contents 14.1 14.2 14.3 14.4 14.5 14.6 14.7 14.8 14.9 14.10
Introduction and synopsis Oxidation, ﬂammability, and photo-degradation Oxidation mechanisms Resistance to oxidation Corrosion: acids, alkalis, water, and organic solvents Drilling down: mechanisms of corrosion Fighting corrosion Summary and conclusions Further reading and software Exercises
Copyright Ó 2019 Elsevier Ltd. All rights reserved. https://doi.org/10.1016/B978-0-08-102376-1.00014-7
380 381 382 385 386 387 396 404 405 406
380 Chapter 14 Durability: oxidation, corrosion, degradation
Introduction and synopsis
The Gospel according to St Matthew reminds us that we live in a world in which ‘moth and rust doth corrupt’ e a world of corrosion, degradation, and decay (see cover picture). Not a happy thought with which to start a chapter. But by understanding degradation we can, to a degree, control it. This chapter describes ways in which materials degrade or corrode, the underlying mechanisms, and what can be done to defeat them. Durability is a key material attribute, one central to the safety and economy of products. It is one of the more difﬁcult attributes to characterise, quantify, and use for selection for the following reasons:
It is a function of both the material and the environment in which it operates. There are many mechanisms, some general, some peculiar to particular materials and environments. Material combinations (as in galvanic corrosion) and conﬁguration (as in crevice corrosion) play a role.
Figure 14.1 shows some of the considerations. The central players are materials and environments. But the fact that a given material is resistant to a given environment is not enough e there’s more. First, there is the industrial sector in which the material is to be used: some are limited to lightweight materials, some to non-ﬂammable materials, some to
Petroleum Chemical engineering Mechanical engineering Construction Energy conversion Marine and offshore Food processing Domestic Bio-engineering
Material selection Cathodic protection Corrosion inhibitors
Coating and plating Polymer Metal Ceramic Inspection Regular replacement
Galvanic attack Acid attack Organic solution Sulphurisation Pitting attack Intergranular attack Stress corrosion Crevice corrosion Oxidation
Figure 14.1 Factors affecting durability.
Avoid heterogeneity Avoid galvanic couples Avoid differential aeration Avoid crevices Free water drainage Welding beats fasteners Avoid surface deposits Minimize flow turbulence Inspection, maintenance
14.2 Oxidation, ﬂammability, and photo-degradation
bio-compatible materials. In some applications a certain amount of corrosion can be tolerated (construction, shipping); in others the slightest attack is unacceptable (bio-medical equipment, for instance). Second, there are many mechanisms of attack, some general, some appearing only under special conditions. Third, there are protection methods, some generally applicable (like painting), some speciﬁc to particular combinations of material and environment (such as inhibitors). And ﬁnally there are issues of design, often speciﬁc to a given industry. Thus there are preferred material choices for use in a given environment and industrial context e those that, through experience, best meet both the primary constraint of resisting attack and the secondary constraints of stiffness, strength, cost, compatibility, and the like. We return to these in Section 14.7. Because many different properties are involved here, the exploration of the science and engineering is split into two: ﬁrst covering oxidation, and then corrosion by liquids.
Oxidation, ﬂammability, and photo-degradation
The most stable state of most elements is as an oxide. The earth’s crust is almost entirely made of simple or complex oxides: silicates like granite, aluminates like basalt, carbonates like limestone. The striking exceptions are the carbon and hydrogen that exist in deposits of hydrocarbons (coal, oil, and gas). Techniques of thermo-chemistry, electro-chemistry, cracking, and synthesis allow these to be reﬁned into the materials we use in engineering, but these are not, in general, oxides. From the moment materials are made they start to re-oxidise, some extremely slowly, others more quickly; and the hotter they are, the faster it happens. For safe high-temperature design we need to understand rates of oxidation. Deﬁnition and measurement Oxidation rates of metals are measured in the way sketched in Figure 14.2: a thin sheet of the material (to give a lot of surface) is held at temperature T and the gain or loss in weight, Dw, is measured. If the oxide adheres to the material, the sample gains weight with time t in a way that is either linear (Dw f t) or parabolic (Dw f t1/2); if instead the oxide is volatile, the sample loses weight linearly with time (eDw f t). Polymers, too, oxidise, but in a more spectacular way. That brings us to ﬂammability.
Platinum wire suspension Furnace at temperature T
Weight gain or loss Δw
Linear weight gain
Parabolic weight gain Time t Linear weight loss
Figure 14.2 Measuring oxidation rates: linear weight gain, parabolic gain, and linear loss.
382 Chapter 14 Durability: oxidation, corrosion, degradation Flammability Ceramics and glasses do not burn. Metals, if dispersed as a ﬁne powder, are potentially combustible, but in bulk form ﬂammability is rarely an issue, even for magnesium. Most polymers, on the other hand, are inherently ﬂammable, although to differing degrees: some burn spontaneously if ignited; others are self-extinguishing, burning only when directly exposed to ﬂame. There are several ways to characterise ﬂammability. The most logical is the limiting oxygen index (LOI): it is the oxygen concentration, in %, required to maintain steady burning. Fresh air has about 21% oxygen in it. A polymer with an oxygen index lower than 21% will burn freely in air; one with an oxygen index that is larger will extinguish itself unless a ﬂame is played onto it e then it burns. Photo-degradation You don’t have to set ﬁre to a polymer for it to oxidise. Polymers and elastomers age when exposed to light (particularly UV) and oxygen, causing loss of strength, stiffness and toughness, discolouration and loss of gloss: PP, ABS, PS, PET, PMMA, PC, nylons and PU all need UV protection. This is provided by additives: antioxidants, light stabilisers, and ﬂuorescent whitening agents. Some of these are so universal that even the ‘standard’ grade of the polymer contains them.
Mechanisms of oxidation The rate of oxidation of most metals in dry air at room temperature is too slow to be an engineering problem; indeed, slight oxidation can be beneﬁcial in protecting metals from corrosion of other sorts. But heat them up and the rate of oxidation increases, bringing problems. The driving force for a metal to oxidise is its free energy of oxidation e the energy released when it reacts with oxygen e but a big driving force does not necessarily mean rapid oxidation. The rate of oxidation is determined by the kinetics (diffusion rate) controlling the oxidation reaction, and that has to do with the nature of the oxide. When any metal (except for gold, platinum, and a few others that are even more expensive) is exposed to air, an ultra-thin surface ﬁlm of oxide forms on it immediately, following the oxidation reaction: x MðmetalÞ þ y OðoxygenÞ ¼ Mx Oy ðoxideÞ þ energy
The ﬁlm now coats the surface, separating the metal beneath from the oxygen. If the reaction is to go further, oxygen must get in or the metal must get out through the ﬁlm. The weight gain shown in Figure 14.2 reveals two different types of behaviour. For some metals the gain, expressed as mass per unit area, Dm, is linear, meaning that the oxidation is progressing at a constant rate: dðDmÞ ¼ constant; giving Dm ¼ kl t dt
where kl (kg/m2.s) is the linear kinetic constant. This is because the oxide ﬁlm is porous or cracks (and, when thick, spalls off) and does not screen the underlying metal. Some metals
14.3 Oxidation mechanisms
behave better than this. The ﬁlm that develops on their surfaces is compact, coherent, and strongly bonded to the metal. For these the mass gain per unit area of surface is parabolic, slowing up with time, and this implies an oxidation rate with the form dðDmÞ 1 f giving Dm2 ¼ kp t dt Dm where kp (kg2/m4.s) is the parabolic kinetic constant.
Example 14.1 Rates of oxidation A metal oxidises at 500 C with a parabolic rate constant kp ¼ 3 1010 kg2/m4.s. What is the mass gain per unit area after 1000 h? Answer. The mass gain is Dm ¼ (kpt)1/2 ¼ 0.033 kg/m2.
In these equations Dm is the mass gain per unit area e that means the mass of the oxygen that has been incorporated into the oxide. The mass of the oxide itself is greater than this because it contains metal atoms (M) as well but they were there to start with. If the formula of the oxide is MO, the mass of oxide per unit area is Am þ Ao mox ¼ Dm Ao where Am is the atomic weight of the metal and Ao is that of oxygen. The thickness x of the oxide is simply x ¼ mox/rox where rox is the oxide density. Using equation (14.3) we ﬁnd x2 ¼
Am þ Ao Ao
kp t r2ox
Example 14.2 Rates of oxidation The oxide of the last example is MgO. The atomic weight of magnesium is 24.3 kg/kmol and that of oxygen is 16 kg/kmol, and the density of MgO is 3550 kg/m3. How thick will the oxide be after 1000 h at 500 C? Answer. The mass m of the oxide is: m ¼ 40:3 Dm ¼ 0:083 kg m2 . 16 Thickness x ¼
mass per unit area ¼ 2:3 105 m ¼ 23 microns density
384 Chapter 14 Durability: oxidation, corrosion, degradation Figure 14.3 shows a coherent, strongly bonded, oxide ﬁlm, thickness x. The reaction creating the oxide MO M þ O ¼ MO goes in two steps. The metal ﬁrst forms an ion, say M2þ, releasing electrons: M ¼ M2þ þ 2e The electrons are then captured by an oxygen atom to give an oxygen ion:
O + 2e-
Oxide MO grows at surface
O + 2e-
O þ 2e ¼ O2
Oxide MO grows at interface
Figure 14.3 Oxidation mechanisms: (a) growth by metal ion diffusion and electron conduction, (b) growth by diffusion of oxygen ions and holes.
The problem is that the ﬁrst of these reactions occurs at the metal side of the oxide ﬁlm, whereas the oxygen reaction is on the other side. Either the metal ions and the electrons must diffuse out to meet the oxygen, or the oxygen ions and electron ‘holes’ (described in Chapter 15) must diffuse in to ﬁnd the metal. If the ﬁlm is an electrical insulator, as many oxides are, electrons are stuck, so it is the oxygen that must diffuse in. The concentration gradient of oxygen is that in the surrounding gas Co divided by the ﬁlm thickness, x. Using Fick’s law (Chapter 13), the rate of growth of the ﬁlm is proportional to the ﬂux of atoms diffusing through the ﬁlm, giving dx Co Qd Co fD z Do exp (14.5) dt x RT x where D is the diffusion coefﬁcient and Do and Qd are the pre-exponential constant and the activation energy for oxygen diffusion. Integrating gives Qd x2 f Do exp Co t RT This has the same form as equation (14.4) with
Qd kp f Do Co exp RT
14.4 Resistance to oxidation 385 This explains why the growth is parabolic and why oxidation rates rise so steeply with rising temperature e it’s the exponential temperature dependence. The most protective ﬁlms are those that are both electrical insulators and have low diffusion coefﬁcients, and this means ﬁlms that have high melting points. This is why the Al2O3 oxide ﬁlm on aluminium, the Cr2O3 ﬁlm on stainless steel and chrome plate, and the SiO2 ﬁlm on high-silicon cast iron are so protective. Example 14.3 Rates of oxidation The activation energy for oxygen diffusion in MgO is 370 kJ/mol. If the test in Example 14.2 had been carried out at the temperature T1 ¼ 450 C rather than at To ¼ 500 C, how thick would the oxide be after 1000 h? The gas constant R ¼ 8.314 103 kJ/mol.K.
Answer. The thickness scales with temperature as: xf exp
, so the thickness
x1 after 1000 h at 450 C is less than that, xo, at 500 C by the factor 1=2 1=2 x1 Q 1 1 1 1 ¼ exp d ¼ exp 4:45 104 ¼ 0:137 xo R T1 To 723 773
Thus the thickness after the test at 450 C is 3.1 microns.
Resistance to oxidation
Elements for heaters, furnace components, power generation, and chemical engineering plants all require materials that can be used in air at high temperatures. If you want the ultimate in high temperature and long life, it has to be platinum. If you want something more affordable, it must be an alloy. Oxides, of course, are stable in air at high temperature e they are already oxidised. One way to provide high-temperature protection is to coat metals like cast irons, steels, or nickel alloys with an oxide coating. Stoves are protected by enamelling (a glass coating, largely SiO2); turbine blades are coated with plasma-sprayed thermal barrier coatings (TBCs) based on the oxide zirconia, ZrO2 (see Chapter 13, Section 13.6). But coatings of this sort are expensive, and, if damaged, they cease to protect. There is another way to give oxidation resistance to metals, and it is one that repairs itself if damaged. The oxides of chromium (Cr2O3), aluminium (Al2O3), titanium (TiO2), and silicon (SiO2) have high melting points, so the diffusion of either the metal or oxygen through them is slow, and as they are electrical insulators electrons cannot move through them either, so the rate constant kp is very small. The result: the oxide stops growing when it is a few molecules thick. These oxides adhere well and are very protective; it is they that make these otherwise-reactive metals so passive. The ﬁlms can be artiﬁcially thickened by anodising e an electro-chemical process for increasing their thickness and thus their protective power.
386 Chapter 14 Durability: oxidation, corrosion, degradation Anodised ﬁlms accept a wide range of coloured dyes, giving them a decorative as well as a protective function. If enough chromium, aluminium, or silicon can be dissolved in a metal like iron or nickel e ‘enough’ means 18e20% e a similar protective oxide grows on the alloy. And if the oxide is damaged, more chromium, aluminium, or silicon immediately oxidises, repairing the damage. Stainless steels (typical composition Fee18% Cre8% Ni), widely used for high-temperature equipment, and nichromes (nickel with 10e30% chromium), used for heating elements, get their oxidation resistance in this way; so too do the aluminium bronzes (copper with 10% aluminium), and high-silicon cast irons (iron with 16e18% silicon). To see just how important this way of suppressing oxidation has become, look back for a moment at Figure 13.20. It is the table guiding material choice at low and high temperature. All the metals above the 400 C mark rely on alloy methods for their protection.
Corrosion: acids, alkalis, water, and organic solvents
Table B1 in Appendix B lists some of the liquids that products encounter and where they are found. The same environments appear in the other tables of Appendix B. Aqueous solutions, acids, and alkalis Even when pure, water causes corrosion if oxygen is available. The rusting of steel in fresh water alone has enormous economic and reliability penalties. Add dissolved ions (like NaCl) and the corrosion rate increases dramatically. Strong acids like H2SO4 (sulphuric acid), HNO3 (nitric acid), and HCl (hydrochloric acid) are widely used in the chemical industry. So too are strong alkalis like NaOH (caustic soda). Household products contain some of these in dilute form, but in the home it is organic acids like vinegar (acetic acid) and milder alkalis like washing soda (sodium carbonate) that create problems. Dunk a metal into an acid and you can expect trouble. The sulphates, nitrates, chlorides and acetates of most metals are more stable than the metal itself. The question is not whether the metal will be attacked, but how fast. As with oxidation, this depends on the nature of the corrosion products and on any surface coating the metal may have. The oxide ﬁlm on aluminium, titanium, and chromium protects them from some acids provided the oxide itself is not damaged. Alkalis, too, attack some metals. Zinc, tin, lead and aluminium react with NaOH, for instance, to give zincates, stannates, plumbates and aluminates, as anyone who has heated washing soda in an aluminium pan will have discovered. Ways of combating corrosion by water, acids and alkalis are described in Section 14.7. Corrosion, however, can sometimes be put to aesthetic purpose: the turquoise patina of copper roofs and the rich browns of bronze statues are created by corrosion. Oils and organic solvents Oily liquids are everywhere. We depend on them as fuels and lubricants for cooking, for removing stains, as face cream, as nail varnish, and much more e any material in service will encounter them. Metals, ceramics, and glasses are largely immune to them but not all polymers can tolerate organic liquids without problems. The identiﬁcation of solvents that are incompatible with a given polymer is largely based on experience, trial and error, and intuition guided by such rules as ‘like dissolves like’, meaning that non-polar solvents like benzene (C6H6) or carbon tetrachloride (CCl4) tend to attack non-polar polymers
14.6 Drilling down: mechanisms of corrosion
like polypropylene or polyethylene, while polar solvents such as acetone (CH3COCH3) tend to attack polar polymers like PMMA and nylon.
Drilling down: mechanisms of corrosion
Ions in solution and pH a hydroxyl ion, OH:
Pure water, H2O, dissociates a little to give a hydrogen ion, Hþ, and H2 O4Hþ þ OH
The product of the concentrations of the two ions is constant. This is known as the ‘law of mass action’: þ H $ OH ¼ constant (14.8) where the square brackets mean ‘molar concentration’, the number of moles of an ion per litre of water.
Example 14.4 Molar concentrations Sea water contains 35 g of salt, NaCl, per litre. What is the molar concentration of Cl ions in sea water? Answer. One molecule of NaCl, when dissolved, creates one Cl ion, so the molecular concentration of Cl is the same as that of NaCl. The atomic weight of sodium is 22.99 kg/kmol and that of chlorine is 35.45 kg/kmol, so the molecular weight of NaCl is 58.44 kg/kmol. A 1 mol solution of NaCl therefore contains 58.44 g/litre of solution. Thus the molar concentration of salt (and thus also of Cl ions) in sea water is M¼
35 ¼ 0:599 mol=litre. 58:44
In pure water there are equal numbers of the two types of ion, [Hþ] ¼ [OH], and the measured value of the constant in the law of mass action is 1014. Thus the molar concentration of both ion types is 107; one H2O molecule in 107 is ionised. The pH of the ionised water is deﬁned as the negative of the log of the hydrogen ion concentration: (14.9) pH ¼ log10 Hþ so the pH of pure water is 7. Acids dissociate in water to give Hþ ions. Sulphuric acid, for instance, dissociates as: H2 SO4 42Hþ þ SO2 4
388 Chapter 14 Durability: oxidation, corrosion, degradation This pushes up the concentration of [Hþ] and, because of equation (14.8), it pulls down the concentration of [OH]. Weak acids have a pH of 4e6; strong ones a pH down to 0. Alkalis do the opposite. Sodium hydroxide, for example, dissociates when dissolved in water, to give OH ions: NaOH4Naþ þ OH
Weak alkalis have a pH of 8e10, strong ones a pH up to 13 (Figure 14.4). H+
Figure 14.4 The scales of pH and pOH. Corrosion by acids and alkalis is an electro-chemical reaction. One half of this is the dissociation reaction of a metal M into a metal ion, Mzþ, releasing electrons e: M/Mzþ þ ze where z, an integer of value 1, 2, or 3, is the valency of the metal (introduced in Chapter 4). Acidic environments, with high [Hþ] (and thus low pH) stimulate this reaction; thus a metal such as copper, in sulphuric acid solution, reacts rapidly: ) Cu/Cu2þ þ 2e þ (14.12) Cu2þ þ SO2 4 þ 2H þ 2e /CuSO4 þ H2 H2 SO4 42Hþ þ SO2 4
14.6 Drilling down: mechanisms of corrosion
Some metals are resistant to attack by some acids because the reaction product, here CuSO4, forms a protective surface layer; lead (Pb)-lined containers are used to process sulphuric acid because lead sulphate is protective. Alkalis, too, cause corrosion via an electro-chemical reaction. Zinc, for instance, is attacked by caustic soda via the steps ) Zn/Zn2þ þ 2e (14.13) Zn2þ þ 2Naþ þ 2OH þ 2e /Na2 ZnO2 þ H2 2NaOH42Naþ þ 2OH Fresh and impure water Corrosion, as we have just seen, is the degradation of a metal by an electro-chemical reaction with its environment. Figure 14.5 illustrates in more detail the idea of an electro-chemical reaction. If a metal is placed in a conducting solution like salt water, it dissociates into ions, releasing electrons (as the iron is shown doing in the ﬁgure) via the anodic reaction: Fe/Fe2þ þ 2e
e- e e- ee- e ee-
Figure 14.5 Ionisation in solution.
The electrons accumulate on the iron giving it a negative charge that grows until the electrostatic attraction starts to pull the Fe2þ ions back onto the metal surface, stiﬂing further dissociation. At this point the iron has a potential (relative to a standard, the hydrogen standard) of 0.44 V. Each metal has its own characteristic potential (called the standard reduction potential), shown on the left of Figure 14.6.
390 Chapter 14 Durability: oxidation, corrosion, degradation Standard reduction potentials (Eo)
Galvanic series in sea-water
1 H2O + 2 O2 + 2e
Hg + 2e2+
Wet corrosion not possible
Gold Graphite Titanium Silver Stainless steel (passive)
Cu + 2e-
2H + 2e-
Pb Sn Ni
Nickel based alloys Cupro-nickel
Wet corrosion usual
Fe + 2e3+ Cr + 3e-
Mn + 2e-
Mg + 2e2+
Na + eLi
Lead Stainless steel (active) Lead-tin solder Steel and iron
Figure 14.6 Standard reduction potentials of metals (left) and galvanic series in sea water (right) for engineering alloys.
If two metals are connected together in a cell, like the iron and copper samples in Figure 14.7, a potential difference equal to the difference in their reduction potentials appears between them. The reduction potential of iron, 0.44, differs from that of copper, þ0.34, by 0.78 V, so if no current ﬂows in the connection the voltmeter will register this difference. If a current is now allowed, electrons ﬂow from the iron (the anode) to the copper (the cathode); the iron recommences to ionise (that is, it corrodes), following the anodic reaction of equation (14.14) and, if the solution were one containing copper sulphate, copper ions, Cu2þ, plate out onto the copper following the cathodic reaction: Cu2þ þ 2e /Cu
14.6 Drilling down: mechanisms of corrosion
Figure 14.7 A bi-metal corrosion cell. The corrosion potential is the potential to which the metal falls relative to a hydrogen standard.
Reduction potentials tell you which metal will corrode if you make a bi-metal cell like that of Figure 14.7. Electroplating, you might say, is ‘un-corrosion’, and that is a helpful analogy. If you want to reverse the corrosion path, returning ions to the surface they came from, applying a potential of opposite sign and larger than the corrosion potential will do it. A corrosion cell is a kind of battery. Simple batteries have electrodes separated by an electrolyte. Choosing electrode materials with a big difference in their standard reduction potentials, Eo, is a start, because this difference is the open-circuit voltage of the battery if the electrolyte contains a standard (meaning 1 molar) solution of metal ions, and the metals are pure. If the solution is non-standard the reduction potential changes in a way described by the Nernst equation. The reduction potential E of a metal when the molar concentration is M ¼ Cion instead of M ¼ 1 is E ¼ Eo þ
0:059 log10 ðCion Þ z
where z is the valence of the ion.
Example 14.5 Using the Nernst equation A zinc electrode is put in an electrolyte that is a solution of 2 g of zinc (as Zn2þ ions) in a litre of water. What is its corrected reduction potential at 25 C? The atomic weight of zinc is 65.4 kg/kmol. Answer. The molar concentration of Zn ions is Cion ¼
2 ¼ 0:031 M 65:4
392 Chapter 14 Durability: oxidation, corrosion, degradation The zinc ions have a valence z ¼ 2 and a standard reduction potential Eo of 0.76 (from Figure 14.6). Thus the corrected reduction potential is E ¼ 0:76 þ
0:059 log10 ð0:031Þ ¼ 0:76 0:045 ¼ 0:805 V 2
There are other non-standard inﬂuences that are not so easily ﬁxed. Engineering metals are almost all alloys. Some, like aluminium, titanium and stainless steel, form protective surface layers, making them passive (more corrosion resistant). But in some solutions the passive layer breaks down and the behaviour becomes ‘active’, corroding more quickly. This has led engineers to formulate a more practical, empirical ordering called a galvanic series. They rank engineering alloys by their propensity to corrode in common environments such as sea water when joined to another metal (Figure 14.6, right side). The ranking is such that any metal will become the anode (and corrode) if joined to any metal above it in the list, and it will become the cathode (and be protected) if joined to one below, when immersed in sea water. If you make a mild steel tank with copper rivets and ﬁll it with sea water, the steel will corrode. But if instead you made the tank out of aluminium with mild steel rivets, it is the aluminium that corrodes. The corrosion is most intense just around the rivet, where you least want it to happen. The rate at which corrosion or electro-plating takes place is determined by the corrosion current, I (amps), according to Faraday’s equation. It describes the mass of metal corroded away (or electro-plated), m (in kg), as a function of time t (in seconds): ItM (14.17) zF Here M is the atomic mass of the metal, z (as before) is the valence of its ions, and F is Faraday’s constant ¼ 96,500 Coulombs (the units of electrical charge, with the same units as the quantity It). m¼
Example 14.6 Using Faraday’s equation What product of current density (A/m2) and time are needed to plate a 10 micron thick layer of nickel onto an object? The density of nickel is 8910 kg/m3, its atomic weight is M ¼ 58.7 kg/kmol, and nickel ions have a valence of z ¼ 2. Answer. A 10 micron layer is equivalent to a volume of nickel per unit area of 105 m3/m2. This corresponds to a mass of nickel per unit area of mA ¼ 0.089 kg. Inverting Faraday’s equation, expressed per unit area (subscript A), gives IA t ¼
mA z F M
14.6 Drilling down: mechanisms of corrosion
where IA is the current density and t is the time. Inserting values for the parameters gives IA t ¼ 293 A:s ðor CoulombsÞ per m2 .
Thus, for example, the plating requires 0.1 A/m2 for 2930 s (49 min), or 1 A/m2 for 293 s (4.9 min).
Suppose now that the liquid is not a copper sulphate solution but just water (Figure 14.8). Water dissolves oxygen, so unless it is previously degassed and protected from air, there is oxygen in solution. The iron and the copper still dissociate until their reduction potential difference is established but now, if the current is allowed to ﬂow, there is no reservoir of copper ions to plate out. The iron still corrodes but the cathodic reaction changes; it is now the hydrolysis reaction: H2 O þ O þ 2e 42OH
Figure 14.8 A bi-metal cell containing pure water in which oxygen can dissolve. While oxygen can reach the copper, the corrosion reaction continues, creating Fe2þ ions at the anode and OH ions at the cathode. They react to form insoluble Fe(OH)2, which ultimately oxidises further to Fe2O3$H2O, which is what we call rust. Thus connecting dissimilar metals in either pure water or water with dissolved salts is a bad thing to do: corrosion cells appear that eat up the metal with the lower (more negative) reduction potential. Worse news is to come: it is not necessary to have two metals e both anodic and cathodic reactions can take place on the same surface. Figure 14.9 shows how this happens. Here an iron sample is immersed in water with access to air. The part of the sample nearest the water surface has an easy supply of oxygen; that further away does not. On the remoter part the
394 Chapter 14 Durability: oxidation, corrosion, degradation
Figure 14.9 Corrosion cells created by differential access to oxygen. ionisation reaction of equation (14.14) takes place, corroding the iron and releasing electrons that ﬂow through the metal to the near-surface part where oxygen is plentiful, where they enable the hydrolysis reaction of equation (14.18). The hydrolysis reaction has a reduction potential of þ0.4 V e it is shown on Figure 14.6 e and the difference between this and that of iron, 0.44 V, drives the corrosion. If the sample could be cut in two along the broken line in Figure 14.9 and a tiny voltmeter inserted, it would register the difference: 0.84 V. Differential oxidation corrosion is one of the most common and most difﬁcult forms of corrosion to prevent: where there is water and a region with access to oxygen and one that is starved of it, a cell is set up. Only metals above the hydrolysis reaction potential of þ0.4 V in Figure 14.6 are immune. Selective corrosion Wet corrosion can be uniform but it can also be selective, and this can lead to failure much more rapidly than the uniform rate would suggest. Stress and corrosion acting together (‘stressecorrosion’ and ‘corrosion fatigue’) frequently lead to localised attack, as do local changes in microstructure such as those at a welded joint (Figure 14.10). Brieﬂy, the localised mechanisms are these.
Material Cracking Fague cracking Creep cracking
Stress Applied stress Internal stress Fit-up stress Strain rate
Composion Heat treatment Microstructure Surface state
Corrosion Corrosion cracking Intergranular cracking
Environment Chemical nature Temperature Electrode potenal Time
Figure 14.10 Stress and environment interact to give stress corrosion cracking (SCC).
14.6 Drilling down: mechanisms of corrosion
Intergranular corrosion occurs because grain boundaries have chemical properties that differ from those of the grain; the lower packing density at the boundary gives these atoms higher energy. Grain boundaries can also be electro-chemically different due to the presence of precipitates on the boundaries that do not form within the bulk of the grains. As an example, stainless steels derive their corrosion resistance from the chromium they contain, giving a protective surface layer of Cr2O3. It takes about 18% Cr to give full protection; less than 10% and protection may fail. Incorrect heat treatment, or heating close to a weld, can cause particles of the carbide Cr23C6 to form on grain boundaries, draining the surrounding metal of chromium and leaving it vulnerable to attack (Figure 14.11).
Cr23C6 carbide precipitates
Electro-chemical aack here Zone denuded of chromium
Austenic stainless steel, 18% chromium
Figure 14.11 Grain boundary precipitates causing intergranular corrosion. Stress corrosion cracking (SCC) is accelerated corrosion, localised at cracks in loaded components. As we saw in Chapter 8, fracture becomes possible when the energy released by the growth of a crack exceeds the energy required to make the two new surfaces plus that absorbed in the plastic zone at the crack tip. A corrosive environment provides a new source of energy e the chemical energy released when the material corrodes. Crack advance exposes new, unprotected surfaces and it is also at the crack tip that the elastic strain energy is highest, so the corrosive reaction is most intense there. The result is that cracks grow under a stress intensity Kscc that can be far below K1c. Figure 14.12 shows a beam loaded in bending while immersed in a corrosive environment. The bending moment M creates a tensile stress in the top face, which is further concentrated by any scratch or groove in the surface. Material at the tip is now doubly vulnerable, a victim of both its chemical and its elastic energy. A crack tunnels downward, branching as it goes, until the beam fails. In this example, stress derives from external loading, in bending (so you know it’s there); more insidious are any internal (residual) stresses left by working or welding, because it is harder to know they are there or how large they are e but they have just the same effect. Speciﬁc examples of SCC are brass in an atmosphere containing ammonia, mild steel in caustic soda, and some aluminium and titanium alloys in salt water.
396 Chapter 14 Durability: oxidation, corrosion, degradation Corrosive medium Stress concentraon
Figure 14.12 Stress corrosion cracking.
Pitting corrosion is preferential attack that occurs at breaks in the natural oxide ﬁlm on metals or at precipitated compounds in certain alloys. Galvanic attack at the microstructural level may appear in alloys with a multi-phase microstructure, with mixed grains of different compositions or phases. The adjacent grains will, in general, lie at slightly different points on the reduction potential scale. If immersed in a conducting solution, thousands of tiny corrosion cells appear, causing the phase that lies lower in reduction potential to be eaten away. Corrosion fatigue refers to the accelerated rate at which fatigue cracks grow in a corrosive environment. The endurance limit of some steels in salt water is reduced by a factor as large as four. The rate of fatigue crack growth, too, increases to a level that is larger than the sum of the rates of corrosion and of fatigue, acting in isolation. Polymers, too, can be embrittled by certain environments: examples are polycarbonate in alkalis, PMMA (Plexiglas) in acetone, and some nylons and polyesters in acids. Again, the stress intensity driving the crack may come from working loads or from internal stresses left by moulding. To avoid the second, components made of materials that are sensitive to SCC are heat-treated to remove internal stress before going into service.
In ﬁghting corrosion, there are four broad strategies (Figure 14.13), discussed below:
·· · ·
Judicious design, meaning informed choice of material, shape, and conﬁguration. Protective coatings, either passive (meaning that the coating simply excludes the corrosive medium) or active (meaning that the coating protects even when incomplete). Corrosion inhibitors, chemicals added to the corrosive medium that retard the rate of the corrosion reaction. Monitoring, with protective maintenance or regular replacement.
14.7 Fighting corrosion
Material(s) choice Shape, configuration
Passive coatings Active coatings
Corrosion control Inhibitors
Anodic inhibitors Cathodic inhibitors
Preventive maintenance Regular replacement
Figure 14.13 Strategies for controlling corrosion. Design: material choice Materials differ greatly in their vulnerability to attack by corrosive media, some surviving unscathed while others, in the same environment, are severely attacked. There are no simple rules or indices for predicting susceptibility. The best that can be done is a ranking, based on experience. Table B2 of Appendix B lists the corrosion resistance of common engineering materials to 23 commonly encountered ﬂuids, on a four-point scale ranging from A (excellent resistance to attack; life: tens of years) to D (unacceptably poor resistance; life: days or weeks). Tables like these (or their computer-based equivalent1) allow screening to eliminate materials that might present severe problems. But, as explained in Section 14.1, there is more to it than that. The best choice of material depends not just on the environment in which it must operate, but e for economic reasons e on the application: it may be cheaper to live with some corrosion (providing regular replacement) than to use expensive materials with better intrinsic resistance. And there is the potential for protection of vulnerable materials by coatings, by inhibitors, or by electro-chemical means. Experience in balancing these inﬂuences has led to a set of ‘preferred’ materials for use in any given environment. Table B3 of Appendix B lists these for the same environments that appear in Table B2. Example 14.7 Use Tables B1 and B2 of Appendix B to identify materials that you might use for pipework to handle 10% sodium hydroxide. Consider material combinations as well as single materials. Answer. Table B1, Appendix B, identiﬁes stainless steels, copper alloys and titanium alloys as A-rated in NaOH. So, too, are polyethylene and polypropylene, so they could be used to line a simple steel pipe. Table B2, Appendix B, lists stainless steel, nickel alloys and magnesium alloys as commonly used to contain NaOH. 1
Sources are listed under Further Reading.
398 Chapter 14 Durability: oxidation, corrosion, degradation Design: material choice for implants in the human body The human body is at its best for only about 50 years. From there on it’s downhill, with an increasing chance that bits (arteries, bones, teeth, lenses) will need replacing. That’s where materials come in. What is required of a material that will be implanted in the human body? There are two over-riding considerations, and corrosion is a factor in both:
Bio-compatibility, that is, not exhibiting any toxicity to the surrounding biological system; Durability e the body does not take kindly to repeat replacement of its parts.
Not many materials meet these requirements well. The most successful are listed in the table of Preferred materials and coatings for given environments e body ﬂuids, Table B3 of Appendix B. Let’s take a closer look at them, starting with metals. The human body is not a friendly place for metals. Many body ﬂuids are oxygenated saline electrolytes with a pH around 7.4 and a temperature of 98.6 F (37 C) e perfect conditions for corrosion, particularly as chloride solutions are among the most corrosive to metals. Variations in alloy compositions, heat treatment, cold work and surface ﬁnish create local differences in electro-chemical potential, providing the conditions for galvanic cells to form. Electrolytic activity implies dissolution of one component of the cell and the release of metal ions from it into the body e unacceptable in an implant that may be in place for years. To overcome these electro-chemical problems, implants are pre-passivated using an acid bath or an anodising process to thicken the protective oxide ﬁlm (titanium alloys) or electropolishing (stainless steel and cobalt alloys). In addition, load-bearing implants must meet constraints on strength, strength-to-weight ratio, and fatigue life. Implants involved in joints with sliding surfaces must meet restrictions for wear and fretting resistance to minimise the dispersion of damaging wear debris into the surrounding tissue. Those that work well appear in Table B3. Polymers do better on corrosion issues, less well on strength. Almost all polymers are good insulators so electro-chemical problems disappear. Some polymers e particularly the polyoleﬁns (PE, PP) and the ﬂuoropolymers (PTFE, for example) e are chemically very stable, with zero solubility in body ﬂuids. Many standard grades of these have additions of UV stabilisers, ﬁre retardants, and plasticisers, which leach out and would poison the surrounding tissue, so only the pure, unadulterated polymer is acceptable. Silicones and polyurethanes are the polymers of choice for replacement of soft tissue (facial and breast implants), ultra-high molecular weight polyethylene (UHMW-PE) for sliding surfaces with minimal friction and wear (hip and knee replacements), and acrylic (PMMA) for optical clarity (lens replacements). Bio-ceramics are bio-compatible variants of standard engineering ceramics (bio-alumina and bio-zirconia, for instance); the “bio” preﬁx signiﬁes that they are made with special attention to purity and sterility. Like all ceramics, they have high compressive strength but are less strong in tension or bending because of their low fracture toughness. Their properties are more like those of bone than the other materials just described, so it is as bone replacement that they are most used. Over the recent past, three classes of bio-ceramic have emerged:
Bio-inert ceramics: bio-alumina and bio-zirconia are totally inert, with superb corrosion resistance and good wear properties when used as sliding surfaces.
14.7 Fighting corrosion
Bio-active ceramics bond directly with living bone. This property, called osteo-conduction, works by stimulating the growth of bone-like material through chemical reaction of the ceramic surface with surrounding body ﬂuid. Bio-resorbable ceramics: hydroxyapatite and calcium phosphate resemble bone in their chemistry. They are bio-active but, unlike the other two classes, they break down slowly in body ﬂuids; the chemicals released in the breakdown are processed via the normal metabolic pathways of the body. Bio-coral, derived from natural corals, is one such material. It is now used as a bone-graft substitute that is well tolerated by the body and becomes partially ossiﬁed when the calciﬁed skeleton is resorbed.
Design: shape and conﬁguration Here are the “dos and don’ts”. Allow for uniform attack Nothing lasts forever. Some corrosion can be tolerated, provided it is uniform, simply by allowing in the initial design for the loss of section over life. Avoid ﬂuid trapping (Figure 14.14) Simple design changes permit drainage and minimise the trapping of water and potentially corrosive dirt.
Trapped water Crevice corrosion No trapped water
Figure 14.14 Design changes to prevent trapped ﬂuids reduce the rates of corrosion.
Suppress galvanic attack (Figure 14.15) Two different metals, connected electrically and immersed in water with almost anything dissolved in it, create a corrosion cell like that of Figures 14.7 or 14.8. The metal that lies lower on the scale of reduction potential is the one that is attacked. The rate of attack can be large and localised at or near the contact. Attaching an aluminium body shell to a steel auto chassis risks the same fate, as incautious car-makers have found. Even the weld metal, or the adjacent heat-affected zone, of a weld can differ from the parent plate in reduction potential enough to set up a cell. The answer is to avoid bi-metal couples if water is around or, when this is impossible, to insulate them electrically from each other and reduce the exposed area of the nobler metal to minimise the rate of the cathodic reaction.
400 Chapter 14 Durability: oxidation, corrosion, degradation Galvanic attack
Insulating bush, washers and gasket
Figure 14.15 Design changes to avoid or minimise galvanic attack. Avoid crevices (Figure 14.16) Crevices trap moisture and create the conditions for differential aeration attack. The ﬁgure shows riveted lap joints (the rivet, of course, is made from the same metal as the plate). The water/air surface has free access to oxygen, but the water between the plates does not. The result is corrosion of the joint surface, just where it is least wanted. The answer is to join by welding or soldering, or to put sealant in the joint before riveting. This is not just a joint problem e differential aeration is very hard to avoid. It is the reason why the legs of jetties and piers rust just below the water line, and why some edges of the tank shown in the picture at the start of this chapter are more severely rusted than others.
Adhesive, solder or sealant
Figure 14.16 Design changes to avoid crevice corrosion. Consider cathodic protection (Figure 14.17) If attaching a metal to one lower in reduction potential causes the lower one to corrode, it follows that the upper one is protected. So connecting buried steel pipework to zinc plates sets up a cell that eats the zinc but spares the pipes. The expensive bronze propellers of large ships carry no surface protection (the conditions are too violent for it to stay in place). Copper and bronze lie above steel in the reduction potential table and electrical isolation is impossible. Bronze connected to steel in salt water is a recipe
14.7 Fighting corrosion
for disaster. The solution is to shift the disaster elsewhere by attaching zinc plates to the hull around the propeller shaft. The zinc, in both examples, acts as a sacriﬁcial anode protecting both the bronze and the steel. The term ‘sacriﬁcial’ is accurate e the zinc is consumed e so the protection only lasts as long as the zinc, requiring that it be replaced regularly. Galvanised steel sheet uses the same mechanism (Figure 14.17b), and note that if the coating is scratched, the exposed steel remains protected e but once the Zn has gone, the sheet will rust rapidly.
Wet soil 2+ Zn
2+ Zn 4OH-
Figure 14.17 (a) Protection of steel pipes by a zinc sacriﬁcial anode. (b) Galvanised steel sheet. Beware of stress-corrosion and corrosion fatigue Stresses arising from design loads can be calculated; residual stresses from cold work or from thermal contraction in welds are not so easy to predict. Their interaction with a corrosive environment can be dangerous, giving localised SCC, or adding to cyclic loads to give corrosion fatigue. Internal stresses cannot exceed the yield strength of the material (if they did the material would yield), so, as a rule of thumb, select materials that have as low a yield strength (or hardness) as is consistent with the other constraints of the design. Coatings Metals, as we have said, are reactive. Only gold and a couple of other metals are more stable as metals than as oxides. Coatings allow reactive metals e and particularly steels (the backbone of mechanical engineering) e to be used in environments in which, uncoated, they would corrode rapidly. They work in more than one way. Passive coatings separate the material from the corrosive environment. Some, like chrome, nickel, or gold plate, are inherently corrosion resistant. Polymeric coatings e paints and powder coats e provide an electrically-insulating skin that stiﬂes electro-chemical reactions by blocking the passage of electrons. Ceramic and glass coatings rely on the extreme chemical stability of oxides, carbides, and nitrides to encase the metal in a refractory shell. Passive coatings only work if they are perfect (and perfection, in this world, is unusual); if scratched, cracked, or detached, corrosion starts. Active coatings work even when damaged. Some are metals that lie low on the reduction potential scale of Figure 14.6, e.g. zinc on galvanised steel. Polymeric coatings can be made to
402 Chapter 14 Durability: oxidation, corrosion, degradation work in this way by dispersing zinc powder in them. Others contain corrosion inhibitors (described later) that leach into the corrosive medium, weakening its potency. Cement coatings inhibit attack by providing an alkaline environment. Self-generated coatings rely on alloying, almost always with chromium, aluminium, or silicon, in sufﬁcient concentrations that a ﬁlm of Cr2O3, Al2O3, or SiO2 forms spontaneously on the metal surface. Stainless steels, aluminium bronzes, and silicon iron rely on protection of this sort. When scratched, the ﬁlm immediately re-grows, providing on-going protection. With this background, glance at Table B4 of Appendix B. It lists coatings, all of which you will have encountered even if you didn’t recognise them at the time. Modern engineering is totally dependent on them. They are applied in a number of ways, some illustrated in Figure 14.18. Metallic coatings rely on the intrinsic stability of the coat (gold), on its ability to form a selfgenerated, protective, oxide (chromium, aluminium, chromides, and aluminides) or on its ability to provide cathodic protection (zinc, cadmium). Other platings look good but do not protect as well. A plating of copper sets up a cell that works in the opposite direction e attacking the iron at a scratch rather than the copper. Chromium plating looks as if it should protect since Cr is below Fe in the table, but the chromium protects itself so well with its oxide ﬁlm that it becomes passive and no cell is set up. Polymeric coatings rely either on a solvent that, after application, evaporates (acrylic, alkyds), or on a polymerisation reaction triggered by oxygen (linseed oil-based paints), or by an added catalyst (epoxies). Painting with solvent-based paints was, until recently, the most widely used method, but the evaporating solvent is generally toxic; it is a volatile organic compound (VOC) and, for health reasons, their use is discouraged. Water-based paints overcome the problem but do not yet produce quite as good a paint ﬁlm. Polymer powder coating works by ﬂame-spraying the polymer, or by dipping the component when hot into a ﬂuidised bed of polymer powder, causing a thick ﬁlm of polymer to melt onto the surface. While intact, paint ﬁlms and polymer powder coats work well, but as soon as the coating is damaged the protection ceases unless the underlying metal has a sub-coat of something e like zinc e that protects it. Ceramic and glass (enamel) coatings have to be applied hot, sufﬁciently so to sinter the particles of ceramic or to melt the glass onto the surface of the metal. Only cement coatings are applied cold. Example 14.8 A steel component is nickel-plated. Would you expect the nickel to act as a passive or an active barrier to aqueous corrosion? Why? Answer. Nickel lies above steel in the reduction potential chart of Figure 14.6. It is more noble than steel, and will become the cathode in the corrosion cell. That means it acts only as a passive barrier e the steel will corrode at holes or cracks in the nickel coating.
14.7 Fighting corrosion
Molten zinc bath Workpiece Insulation
(d) Oxyacetylene gas
M+ Deposited metal
1. Spray coat Polymer powder reservoir Burning gas
2. Fuse and bond Coated panel
Furnace at 600 - 900 C Conveyor
Sprayed coating Substrate
Figure 14.18 Ways of applying coatings. (a) Paint spraying. (b) Hot dip galvanising. (c) Electroplating. (d) Metal ﬂame spraying. (e) Polymer powder spraying. (f) Enamelling.
404 Chapter 14 Durability: oxidation, corrosion, degradation Corrosion inhibitors Corrosion inhibitors are chemicals that, when dissolved or dispersed in a corrosive medium, reduce (‘inhibit’) the rate of attack. Some work (like indigestion tablets) by modifying the pH or by coating the part with a gooey ﬁlm. Inhibitors suppress either the anodic or the cathodic step of the corrosion reaction (Section 14.6). The choice of inhibitor depends both on the environment and on the material to be protected. Table B5, Appendix B, lists the more common ones, and the metals and environments for which they work best. Many have bewildering polysyllabic names and are unpleasant in other ways. The things that are useful to know (and the ‘buts’) are itemised here. PTFE ((CF2-CF2)n) is used as a wide-spectrum inhibitor in hydrocarbon fuels, solvents, and lubricants, most commonly in engine oil. It works by forming a protective layer over component surfaces, shielding them from full contact with the medium, reducing corrosion rates by up to 90%. But you must put enough PTFE in e too little is worse than none. Calcium bicarbonate (Ca(HCO3)2) raises the pH and thus inhibits acidic attack. But it makes the water hard, causing calcium deposits (limescale). Thiourea (C(NH2)2S) works by raising the activation energy of the corrosion reaction, thus decreasing the corrosion rates. Small additions can reduce the corrosion rate in hydrochloric acid by as much as 97%. But thiourea is potentially carcinogenic, limiting its use to systems that do not involve human contact. Arsenic (III) oxide (As2O3) is an anodic inhibitor. Even at low concentrations (0.5%) it can provide some protection. It is, of course, toxic. Polyphosphates are polymers containing phosphate (ePO4) groups, found in living organisms (DNA contains polyphosphates). They inhibit corrosion of most metals in water. Polyphosphates are non-toxic, so can be used in drinking water. Chromates inhibit corrosion of metals in non-acidic environments. They work by forming an adsorbed layer of chromate ions, passivating the surface e that is, rendering it inactive. Chromates, like so many inhibitors, are toxic, limiting their use. Monitoring: design for inspection, maintenance, and replacement If you can’t see it and reach it, you can’t ﬁx it. Design for durability ensures that parts liable to corrosion are easy to inspect regularly, clean, and, if necessary, replace. Picking up signs of corrosion early minimises the risk and cost of downtime and repair, or complete failure e like mending a hole in the roof. For safety-critical components the best strategy is replacement at intervals that are too short for corrosion to have caused any serious damage.
Summary and conclusions
Corrosion is like slow incurable cancer: it will kill you unless something else (like wear) kills you ﬁrst. Almost as much money must have been invested in corrosion research as in research on cancer, such is its damaging effect on the economy. This research has revealed what goes on at an atomic scale when materials react with oxygen, acids, alkalis, aerated water, aqueous solutions (including those in the human body), and organic solvents. In oxidation of metals, the metal ionises, releasing electrons; the electrons combine with oxygen molecules to give oxygen ions, which in turn combine with metal ions to form the oxide. As the oxide ﬁlm grows, ions and electrons must diffuse through it to enable further growth; its resistance to this diffusion, and its ability to adhere to the metal surface, determine how protective it is. Polymers oxidise through the action of heat or radiation, including UV light, but can be protected by doping them with additives.
14.9 Further reading and software 405 In corrosion, the electro-chemical reactions occur in the corrosive ﬂuid rather than in the solid. A metal ionises when placed in water, and the extent of ionisation determines its reduction potential. Those with the lowest (most negative) reduction potential are the most vulnerable to attack, and will corrode spontaneously even in pure water if oxygen is present. If a metal with a low reduction potential is in electrical contact with one of higher potential, the ﬁrst corrodes and the second is protected e this is exploited in cathodic protection, using one sacriﬁcial metal to protect another. In designing materials to resist corrosion we rely on the ability of a few of them e chromium, aluminium, silicon, and titanium e to form a protective oxide ﬁlm that adheres strongly to the surface. By using these as alloying elements, other metals can be given the same protection. Alternatively, metals can be protected by coating their surfaces with a corrosion-resistant ﬁlm of polymer or ceramic. And best practice in design can minimise corrosion risks by attention to detail, such as avoiding trapping liquids in crevices and isolating dissimilar metals electrically at joints.
Further reading and software
Bradford, S. A. (1993). Corrosion control. New York, USA: Van Nostrand Reinhold. ISBN: 0-442-01088-5. (A readable text emphasizing practical ways of preventing or dealing with corrosion.) CES EduPack. (2018). Granta design. Cambridge, UK. www.grantadesign.com/education. (A materials information and selection resource that contains data for the behavior of materials in corrosive environments.) DeZurik Materials Selection Guide. http://www.dezurik.com/. (Dezurik MSG allows the selection of materials to operate in a given environment.) Fontana, M. G. (2005). Corrosion engineering (3rd ed.). New York, USA: McGraw Hill. ISBN: 0-07-021463-8. (A text focusing on the practicalities of corrosion engineering rather than the science, with numerous examples and data.) Ford, F. P., & Andresen, P. L. (1997). Design for corrosion resistance. In: Materials selection and design (ASM Handbook, Vol. 20), 545e72. ASM International, Metals Park. Ohio, USA. ISBN: 0-97170-386-6. (A guide to design for corrosion resistance, emphasizing fundamentals, by two experts in the ﬁeld.) McCafferty, E. (2010). Introduction to corrosion science. Verlag: Springer. ISBN: 978-1-4419-0454-6. (A good starting point for readers that do not have backgrounds in electrochemistry.) National Physical Laboratory. (2000). Stress corrosion cracking. http://www.npl.co.uk/upload/pdf/ stress.pdf. (A concise summary of stress corrosion cracking and how to deal with it.) ProFlow Dynamics Chemical Resistance Selector. (2008). (A free online database for ﬁnding a material suitable for use in speciﬁed environments.) http://www.proﬂowdynamics.com/viewcorrosion.aspx. Schweitzer, P. A. (1995). Corrosion resistance tables (Vols. 1e3) (4th ed.). New York, USA: Marcel Dekker. (The ultimate compilation of corrosion data in numerous environments. Not bed-time reading.) Schweitzer, P. A. (1998). Encyclopedia of corrosion technology. New York, USA: Marcel Dekker. ISBN: 0-8247-0137-2. (A curious compilation, organized alphabetically, that mixes deﬁnitions and terminology with tables of data.) Tretheway, K. R., & Chamberlain, J. (1995). Corrosion for science and engineering (2nd ed.). Harlow, UK: Longman Scientiﬁc and Technical. ISBN: 0-582-238692. (An unusually readable introduction to corrosion science, ﬁlled with little bench-top experiments to illustrate principles.)
406 Chapter 14 Durability: oxidation, corrosion, degradation Waterman, N. A., & Ashby, M. F. (1991). Elsevier materials selector (3 Vols.). Oxford, UK: Elsevier. ISBN: 1-85-166-605-2 and, in the CRC edition. ISBN 0-8493-7790-0. (A three-volume compilation of materials data for design, with extensive tables and guidelines for the oxidation and corrosion characteristics of metals and polymers.)
Many metallic structures are partly or wholly buried in soil. How is the corrosive potential of a soil estimated? Use Table B1 of Appendix B to ﬁnd out.
A soil is described as ‘peaty’. What does this mean in terms of pH? The soil has an electrical resistivity of 2 108 mU cm. Would you expect it to be particularly corrosive? Use Table B1 of Appendix B to ﬁnd out.
Where, in daily life, might you encounter acetone? Where might you encounter formaldehyde? Use Table B1 of Appendix B to ﬁnd out.
Where, in daily life, might you ﬁnd ethanol? Use Table B1 of Appendix B to ﬁnd out.
You want to etch your partner’s initials into an elegant glass bowl. That needs hydroﬂuoric (HF) acid. What plastic would you choose to contain the HF during the etching? Use Table B2 of Appendix B to ﬁnd out.
You need a ﬂexible tube to connect a tank of diesel fuel to a burner. Use Table B2 of Appendix B to ﬁnd a suitable plastic.
A 600 litre (200 gallon) tank for storing rain water is made of aluminium. It is intended to for use in the garden, partly buried in top soil. The tank was extensively tested and found to survive without noticeable corrosion. The soil in which it was buried was clay, and thus alkaline. When marketed, customers complained of corrosion problems. On investigation it was found that the soil in the affected regions was peat, and strongly acidic. Could this have been anticipated? Use Table B2 of Appendix B to ﬁnd out.
A wholesale supplier offers nail-varnish remover at a cut-down price if you bring your own container to take it away. You decide on a thermoplastic rather than glass container to avoid breakage. Which thermoplastics would you not choose to contain acetone? Use Table B2 of Appendix B to ﬁnd out.
A brain surgeon consults you. She has the brain of a recently-deceased person and wishes to preserve it in formaldehyde for later analysis. Would an acrylic (Plexiglas) container tolerate formaldehyde? What about polycarbonate? Use Table B2 of Appendix B to ﬁnd out.
Body ﬂuids are corrosive. Why? See Table B1 of Appendix B for basic information. Materials for implants and body-part replacements must meet unusually restrictive constraints since any corrosion releases potentially toxic chemicals into the body. Most choice is based on past experience. Use Table B3 of Appendix B, Preferred materials and coatings for given environments, to identify three polymers that are routinely used for implants.
Buildings near coastlines are exposed to salt as sea-water and wind-carried spray. What are the preferred metals to minimise corrosive attack on the cladding of buildings exposed to marine environments? Use Table B3 of Appendix B to ﬁnd out.
The wire frames in your fridge or dish-washer are coated to protect them from water and food-related ﬂuids by hot-dipping: plunging the frame when hot into a ﬂuidised bed of polymer powder, which melts and sticks to the frame. What’s the polymer likely to be? Use Table B4 of Appendix B, Coatings to enhance durability, to ﬁnd out.
The drive-train of a car or truck is exposed to fuels and oils. Even these are corrosive to metals. What are the most-used corrosion inhibitors to protect metals from these environments? Use Table B5 of Appendix B, Corrosion inhibitors, to ﬁnd out.
You rent a furnished apartment and discover, from the labels on the curtains, that those in the bedroom are made of a material with an LOI ﬂammability rating of 17 and that those in the kitchen are made of a material with an LOI of 20. Would you be happy with these ratings?
A sample of a metal, heated in air, gains mass Dm by oxidising at a rate that declines with time t in a parabolic way, meaning that Dm2 ¼ kp t where kp is a constant. Why does the rate fall off in this way? What does it imply about the nature and utility of the oxide?
A 10 mm square sheet of a metal, exposed on both front and back surfaces, gains mass by 4.2 mg when heated for 20 h in air at 300 C. If the kinetics of oxidation are linear, what is the linear rate constant kl for this metal at 300 C?
A 10 mm square sheet of a metal, exposed on both front and back surfaces, gains mass by 3.6 mg when heated for 10 h in air at 700 C. If the kinetics of oxidation are parabolic, what is the parabolic rate constant kp for this metal at 700 C?
408 Chapter 14 Durability: oxidation, corrosion, degradation Exercise E14.18
Copper oxidises in air at 1000 C with parabolic kinetics, forming a surface ﬁlm of Cu2O. The parabolic rate constant at this temperature, kp, is 2.1 106 kg2/m4 s. What is the mass gain per unit area of the copper surface after 1 h? How thick will the oxide be after this time? (The atomic weight of copper is 63.5 kg/kmol, that of oxygen is 16 kg/kmol, and the density of Cu2O is 6000 kg/m3.)
The oxidation kinetics of titanium to TiO2 are limited by oxygen diffusion, with an activation energy Qd of 275 kJ/mol. If the oxide ﬁlm grows to a thickness of 0.08 microns after 1 h at 800 C, how thick a ﬁlm would you expect if it had been grown at 1000 C for 30 min?
Household vinegar has a pH of 2.8. What is the molar concentration of [Hþ] ions?
A solution of NaOH (caustic soda) has a pH of 10. What is the molar concentration of [OH] ions?
A solution of copper sulphate, CuSO4, contains 100 g of CuSO4 per litre of water. The atomic weight (in kg/kmol) of copper is 63.5, that of sulphur is 32.1, and that of oxygen is 16.0. What is the molecular concentration of copper ions, Cu2þ, in the solution?
What is meant by the standard reduction potential? Copper and platinum electrodes are immersed in a bath of dilute copper sulphate. What potential difference would you expect to measure between them? If they are connected so that a current can ﬂow, which one will corrode?
A study of slowly propagating cracks in high-strength steel plates under constant stress in moist air revealed that the crack growth rate increased with temperature as follows: Growth rate (mm s1) Temperature ( C)
Show, using an appropriate plot, that for these conditions crack propagation is a thermally activated process, and determine the activation energy. It is believed that diffusion of one of the following elements is the ratecontrolling mechanism. Decide which of these elements is likely to be involved.
Diffusing element in a iron
Activation energy for diffusion (kJ/mol)
Hydrogen Nitrogen Carbon Iron
38 72 84 285
A polymer coating is required to protect components of a microchip processing unit from attack by HF. Use Tables B2 and B3 of Appendix B to identify possible choices.
Metal pipework on an oil rig must carry hydrochloric acid solution to acidify the well. Use Tables B2, B3, and B5 of Appendix B to explore ways of providing and protecting the pipe.
A food processing plant uses dilute acetic acid for pickling onions. The acid is piped to and from holding tanks. Use Tables B2 and B3 of Appendix B to select a suitable material for the pipes and tanks, given that, to have sufﬁcient strength and toughness to tolerate external abuse, they must be made of a metal.
An automaker is concerned about the consequences of the introduction of bio-methanol, CH3OH, or bio-ethanol, C2H5OH, into auto fuels. A signiﬁcant concern is the corrosion of aluminium components, particularly the engine block, by methanol or ethanol. What steps could be taken to avoid this? Use Tables B2 and B5 of Appendix B.
The automaker of Exercise E14.28 is also concerned that spillage of methanol or ethanol bio-fuel might damage the polyester/glass ﬁbre sheet moulding compound bodywork of some models. Is the concern justiﬁed?
The waste stream of a fertiliser plant includes dilute sulphuric acid. The dilute acid is stored in surface tanks some distance from the plant. It is suggested that the ducting to carry the acid to the tanks could, most economically, be made of wood. Is this a totally crazy suggestion?
Using the Nernst equation (equation (14.16) of the text). A copper electrode is put in an electrolyte that is a solution of 3 g of copper as Cu2þ ions in a litre of water. What is its corrected reduction potential at 25 C? The atomic weight of copper is 63.5 kg/kmol.
Using the Faraday equation (equation (14.17) of the text). What current and time are needed to plate a 1 mm thick layer of copper onto an object with a surface area of 0.1 m2? The density of copper is 8940 kg/m3, its atomic weight is M ¼ 63.5 kg/kmol, and copper ions have a valence of z ¼ 2.
410 Chapter 14 Durability: oxidation, corrosion, degradation Exercise E14.33
Mild sheet steel guttering is copper-plated to protect it from corroding. The guttering acts as a drain for sea water. If the coating is damaged, exposing the steel, will the guttering corrode in a damaging way? If instead the guttering is zinc-plated, will it be better or less well protected? Use the galvanic series in sea water (Figure 14.6 of the text) to ﬁnd out.
The diagram shows a proposed design for an outdoor water tank. What aspects of the design might cause concern for corrosion?
Mild steel tank
Electrical materials: conductors, insulators, and dielectrics
Conductors (left) and insulators (right). Images courtesy of the Copper Development Association.
Chapter contents 15.1 15.2 15.3 15.4 15.5 15.6 15.7 15.8
Introduction and synopsis Conductors, insulators, and dielectrics Charts for electrical properties Drilling down: the origins and manipulation of electrical properties Design: using the electrical properties of materials Summary and conclusions Further reading Exercises
Copyright Ó 2019 Elsevier Ltd. All rights reserved. https://doi.org/10.1016/B978-0-08-102376-1.00015-9
412 413 420 422 434 440 441 441
412 Chapter 15 Electrical materials: conductors, insulators, and dielectrics
Introduction and synopsis
York Minster, constructed between 1220 and 1400, is one of the great cathedrals of Europe. Many ﬁne sermons have been preached from its pulpit, but when, in 1984, the Archbishop of York expressed his disbelief in the Virgin Birth, the Minster was struck by lightning and severely damaged. Some put this down to the wrath of God, but the reality is simpler e the cathedral was inadequately grounded (earthed). There is a message here: even when you are designing cathedrals, electrical properties matter. This chapter is about the simplest of these: properties relating to conduction, insulation, and dielectric behaviour. Electrical conduction (as in lightning conductors) and insulation (as in electric plug casings) are familiar properties. Superconductivity, semiconduction, and dielectric behaviour may be less so. Superconductivity is the special characteristic of some materials to lose all resistance at very low temperatures so that a current ﬂows without loss. Semiconductors, the materials of transistors and silicon chips, fall somewhere between conductor and insulator, as the name suggests. A dielectric is an insulator. It is usual to use the word ‘insulator’ when referring to its inability to conduct electricity and to use ‘dielectric’ when referring to its behaviour in an electric ﬁeld. Three properties are of importance here. The ﬁrst, the dielectric constant (or relative permittivity), describes the way a material acquires a dipole moment (it polarises) in an electric ﬁeld. The second, the dielectric loss factor, measures the energy dissipated when radio-frequency waves pass through a material, with the energy appearing as heat (the principle of microwave cooking). The third is the dielectric breakdown potential, and this takes us back to York Minster. Lightning is a form of dielectric breakdown, which can be just as damaging on a small scale e in a piece of electrical equipment, for example e as on a large one. There are many different kinds of electrical behaviour, all of them useful. Figure 15.1 gives an overview, with examples of materials and applications. This chapter introduces electrical properties and their physical origins, and gives examples of design for electrical performance. Electrical materials Al, Cu, Ag
(Electrical plugs and switches)
Nb, Nb3Sn, YBCO
(Magnetic resonance imaging)
(Ultrasonic oscillator ink-jet print-heads)
Barium titanate Pure Si, Ge, InSb (Temperature sensing)
(IR sensors thermal imaging)
Doped Si, Ge (Semi-conductor devices)
PZT (Diesel injectors)
Figure 15.1 The hierarchy of electrical behaviour, with examples of materials and applications. Their nature and origins are described in this chapter.
15.2 Conductors, insulators, and dielectrics 413
Conductors, insulators, and dielectrics
Resistivity and conductivity The electrical resistance R (units: ohms1, symbol U) of a rod of material is the potential drop V (Volts2) across it, divided by the current i (A, or amps3) passing through it, as in Figure 15.2. This relationship is Ohm’s law: R¼
L Area A
Potential difference V
Resistance R = V/i Resistivity A R L
Figure 15.2 Measuring electrical resistivity. Resistance also determines the power P dissipated when a current passes through a conductor (measured in Watts4): P ¼ i2 R 1
George Simon Ohm (1789e1854), dropped out of his studies at the University of Erlangen, preferring billiards to mathematics, but later became absorbed in the theory of electricity and magnetism. Alessandro Guiseppe Antonio Anastasio Volta (1745e1827), Italian physicist, inventor of the battery, or as it was then known, the Voltaic Pile. His face used to appear on the 10,000 lire note. André Marie Ampère (1775e1836), French mathematician and physicist, largely self-taught and said to have mastered all known mathematics by the age of 14. His life was not a happy one: his father was guillotined during the French revolution, and he was miserably married and had difﬁcult children e yet he remained extensively productive up to his death, contributing to the theories of electricity, light, magnetism, and chemistry (he discovered ﬂuorine). James Watt (1763e1819), instrument maker and inventor of the steam engine (the idea came to him whilst ‘walking on a ﬁne Sabbath afternoon’), which he doggedly developed. Unlike so many of the footnoted characters of this book, Watt, in his ﬁnal years, was healthy, happy, and famous.
414 Chapter 15 Electrical materials: conductors, insulators, and dielectrics The material property that determines resistance is the electrical resistivity, re. It is related to the resistance by re ¼
A R L
where A is the section and L the length of a test rod of material e think of it as the resistance between opposing faces of a unit cube of the material. Its units in the metric system are U.m, but it is commonly reported in units of mU.cm. It has an immense range, from a little more than 108 in units of U.m for good conductors (equivalent to 1 mU.cm, which is why these units are still used) to more than 1016 U.m (1024 mU.cm) for the best insulators. The electrical conductivity ke is simply the reciprocal of the resistivity. Its units are siemens per metre (S/m or (U.m)1). Example 15.1 Electrical current and power A potential difference of 0.05 V is applied across a nickel wire 100 mm long and 0.2 mm in diameter. What current ﬂows in the wire? How much power is dissipated in the wire? The resistivity re of nickel is 9.5 mU.cm. Answer. The current is given by Ohm’s law, V ¼ iR , where V is the potential difference, i is the current, and R is the resistance. Converting the resistivity from mU.cm to U.m by multiplying by 108 gives re ¼ 9.5 108 U.m, so the resistance R of the wire is R¼
re L 0:1 ¼ 9:5 108 ¼ 0:3U 2 A pð1 104 Þ
The current in the wire is i ¼ V=R ¼ 0:05=0:3 ¼ 0:165 amps
The power dissipated in the wire is P ¼ i2 R ¼ 8.33 103 Watts.
Temperature-dependence of resistivity The resistivity re of metals increases with temperature because thermal vibrations scatter electrons. Incandescent lamps (now rare) depend on this; as the ﬁlament heats, its resistance rises, and this stabilises the temperature at a value that does not cause burn-out. The resistivity of semiconductors, by contrast, decreases as temperature increases, because thermal energy allows more carriers to cross the band gap, entering the conduction band (explained later). Some materials, though, behave in a more dramatic way. Superconducting materials suddenly lose all resistance at a critical temperature, Tc, above 0K. Below Tc, the current in a superconducting material ﬂows without any resistive loss; above Tc, superconductivity is suppressed. An applied magnetic ﬁeld H lowers the temperature at which superconduction starts, and a ﬁeld greater than the zero-Kelvin critical ﬁeld Hc,o suppresses it completely.
15.2 Conductors, insulators, and dielectrics 415 Any electrical current induces a magnetic ﬁeld. Thus the existence of a critical ﬁeld implies an upper-limiting current density that can by carried by the superconductor before its own ﬁeld quenches the superconduction. The critical temperatures and ﬁelds of superconducting materials are plotted in Figure 15.3. Many pure metals become superconducting, though only at very low temperatures, and all have low critical ﬁelds, too low to be of much practical use. The intermetallic compounds Nb3Sn, NbTi, Nb3Ge, and Nb3Al have higher critical temperatures and ﬁelds e high enough to be practical for MRI scanners and superconducting energy storage. In 1986 a third class of superconductor was discovered with critical temperatures and ﬁelds that were higher still. They are (surprisingly) ceramics, exhibiting high resistivity at room temperature yet superconducting at temperatures as high as 130K. This is signiﬁcant because it is above the boiling point of liquid nitrogen, a cheap and widely available refrigerant, making superconducting devices practical and economic. The most widely used at present is the oxide ceramic YBa2Cu3O7 (‘YBCO’), used in high-ﬁeld magnets, magnetic resonance imaging and mag-lev trains.
Superconducting transition temperature Tc (K)
Critical temperature and field
Boiling point of liquid nitrogen
(La,Sr)2CuO4 Nb3Ge Niobium
Zinc Cadmium Zirconium
RbCs2C60 Nb3Sn PbMo6S8
Boiling point of liquid helium Tantalum
Thallium Aluminium Gallium
Indium Rhodium Molybdenum Osmium Ruthenium Titanium
Pure metals Intermetallics
Critical superconduction magnetic field Hc,o (T)
Figure 15.3 The critical ﬁelds and temperatures for metallic and ceramic superconductors. Note the boiling points of liquid nitrogen and helium.
Dielectric properties An electric ﬁeld, E, is a region of space in which charged objects experience a force. The electric ﬁeld strength between two oppositely charged plates separated by a distance t and with a potential difference V between them is V t and is independent of position except near the edge of the plates. E¼
416 Chapter 15 Electrical materials: conductors, insulators, and dielectrics Two conducting plates separated by a dielectric make a capacitor (Figure 15.4). Capacitors (or condensers) store charge. The charge Q (coulombs5) is directly proportional to the voltage difference between the plates, V (Volts): Q ¼ CV
where C (farads6) is the capacitance. The capacitance of a parallel plate capacitor of area A and spacing t, separated by empty space (or by air) is C ¼ εo
where εo is the permittivity of free space (8.85 1012 F/m, where F is farads). If the empty space is replaced by a dielectric, the dielectric polarises and the capacitance increases. The ﬁeld created by the polarisation opposes the ﬁeld E, reducing the voltage difference V needed to support the charge. Thus the capacitance of the condenser is increased to the new value C¼ε
where ε is the permittivity of the dielectric with the same units as εo . It is usual to cite not this but the relative permittivity or dielectric constant, εr : εr ¼
Cwith dielectric ε ¼ εo Cno dielectric
Area A Charge Q
Capacitance C = Q/V
Dielectric constant C (with dielectric) εr = C (no dielectric)
Potential difference V
Figure 15.4 Dielectric constant and dielectric breakdown. 5
Charles Augustin Coulomb (1736e1806), military physicist, laid the foundations of both the mathematical description of electrostatic forces and the laws of friction. Despite his appointment as Intendant des Eaux et Fontaines de Paris, he made no known contributions to hydrodynamics. Michael Faraday (1791e1867), brilliant experimentalist both in physics and chemistry, discoverer of electromagnetic induction and inspiring lecturer at the Royal Institution, London.
15.2 Conductors, insulators, and dielectrics 417 making the capacitance C ¼ εr εo
Being a ratio, εr is dimensionless. Its value for empty space, and for practical purposes for most gases, is 1. Most dielectrics have values between 2 and 20, though low-density foams approach the value 1 because they are largely air. Ferroelectrics are special: they have values of εr as high as 20,000. We return to ferroelectrics later in this chapter. Example 15.2 Capacitance (a) A capacitor has a plate area of A ¼ 0.1 m2 separated by an air gap of t ¼ 100 mm. What is its capacitance? (b) The air gap is replaced by a dielectric of thickness t ¼ 1 mm with a dielectric constant εr ¼ 20. What is its capacitance now? Answer. (a) The capacitance is C1 ¼ εo
(b) The capacitance is C2 ¼ εr εo
¼ 8:851012 A t
0:1 ¼ 8:85 109 F ¼ 8:85 pF 100106
¼ 208:85 1012
0:1 ¼ 1:77 105 F ¼ 17:7 mF 106
Capacitance is one way to measure the dielectric constant of a material (Figure 15.4). The charge stored in the capacitor is measured by integrating the current that ﬂows into it as the potential difference V is increased. The ratio Q/V is the capacitance. The dielectric constant εr is calculated from equation (15.8). Small capacitors, with capacitances measured in micro-farads (mF) or pico-farads (pF), are used in resistor-capacitor (R-C) circuits to tune oscillations and give controlled time delays. The time constant for charging or discharging a capacitor is s ¼ RC
where R is the resistance of the circuit. When charged, the energy stored in a capacitor is 1 1 Ec ¼ QV ¼ CV 2 2 2
‘Super-capacitors’, with capacitances measured in farads, store enough energy to power a hybrid car. The charge density, D (units coulombs/m2), on the surface of a dielectric in a ﬁeld E is D ¼ εr εo E
where E is the electric ﬁeld (voltage across the dielectric divided by its thickness). The breakdown ﬁeld or dielectric strength of a dielectric, Eb (units: V/m or more usually MV/m), is the electrical ﬁeld gradient at which an insulator breaks down and a damaging
418 Chapter 15 Electrical materials: conductors, insulators, and dielectrics surge of current ﬂows through it. It is measured by increasing, at a uniform rate, a 60-Hz alternating potential applied across the faces of a plate of the material in a conﬁguration like that of Figure 15.4 until breakdown occurs, typically at a potential gradient between 1 and 100 MV/m. The maximum charge density that a dielectric can carry is thus when the ﬁeld is just below its breakdown ﬁeld: Dmax ¼ εr εo Eb
1 CV 2 1 ¼ εr εo E2b 2 At 2
and the maximum energy density is
Example 15.3 Energy in a capacitor A supercapacitor is required to be able to store an energy of Ec ¼ 1 kJ when a potential difference V ¼ 100 V is applied to its plates. The dielectric constant of the dielectric is εr ¼ 10,000 and its breakdown potential is Eb ¼ 20 MV/m. What is the minimum dielectric thickness needed to avoid breakdown, and hence what is the minimum area of plate required? Eb , requiring that the dielectric have a thickness 1 t 5 mm. The energy stored in a capacitor is Ec ¼ CV 2 , so a capacitance of 2 21000 C¼ ¼ 0:2 F is needed. To achieve this with a dielectric of thickness t 5 mm ð100Þ2 and dielectric constant 10,000 requires an area Answer. Breakdown occurs if
Ct ¼ 11:3 m2 . εr εo
The loss tangent and the loss factor take a little more explanation. We shall see in Section 15.4 that polarisation involves the small displacement of charge (either of electrons or of ions) or of molecules that carry a dipole moment when an electric ﬁeld is applied. An oscillating ﬁeld drives the charge between two alternative conﬁgurations. This charge-motion is like an electric current that e if there were no losses e would be 90 degrees out of phase with the voltage. In real dielectrics, this current dissipates energy just as a current in a resistor does, giving it a small phase shift, d, between the voltage and current (Figure 15.5). The loss tangent, tan d, or dissipation factor, Df, is the tangent of the loss angle. The power factor, Pf, is the sine of the loss angle. When d is small, as it is for the materials of interest here, all three are essentially equivalent: tan d z sin d z Pf z Df
15.2 Conductors, insulators, and dielectrics 419
Voltage V and current i
Oscillating charge +-Q
Dielectric loss tangent: hf tan δ voltage
π/2 - δ
Figure 15.5 Dielectric loss. More useful, for our purposes, is the loss factor L, which is the loss tangent times the dielectric constant: L ¼ εr tan d
It measures the energy dissipated by a dielectric when in an oscillating ﬁeld. If you want to select materials to minimise or maximise dielectric loss, then the measure you want is L. When a dielectric material is placed in a cyclic electric ﬁeld of amplitude E and frequency f, power P is dissipated, and the ﬁeld is correspondingly attenuated. The power dissipated per unit volume, in W/m3, is P z f E2 ε tan d ¼ f E2 εo εr tan d
This power appears as heat and is generated uniformly (if the ﬁeld is uniform) through the volume of the material. Thus the higher the frequency and ﬁeld strength, and the greater the loss factor εr tan d, the greater the heating and energy loss. Dielectric loss is the basis of microwave cooking and is exploited in materials processing e the radio-frequency welding of polymers is an example. Example 15.4 Dielectric loss (a) An oscillating voltage with an amplitude of 100 V at a frequency f ¼ 60 Hz appears across a nylon insulator of thickness x ¼ 1 mm. Nylon has a dielectric loss factor L z 0.1. How much power is dissipated per unit volume in the nylon? Assuming no heat loss, how fast will the temperature of the nylon rise? (Nylon has a volumetric speciﬁc heat Cp ¼ 3 106 J/m3.K). (b) If the frequency was, instead, f ¼ 1 GHz, what is the heating rate?
420 Chapter 15 Electrical materials: conductors, insulators, and dielectrics Answer. (a) The amplitude of the ﬁeld is E ¼ Vx ¼ 105 V/m. The power dissipated is P ¼ f E2 εo L ¼ 0:53 W m3
The rate of temperature rise is dT P ¼ ¼ 1:8 107 C=s dt Cp
(b) If the frequency is raised to f ¼ 1 GHz, the heating rate becomes
dT ¼ 3 C s dt
All dielectrics change shape in an electric ﬁeld, a consequence of the small shift in charge that allows them to polarise; the effect is called electrostriction. Electrostriction is a one-sided relationship in that an electric ﬁeld causes deformation, but deformation does not produce an electric ﬁeld. Piezoelectric materials, by contrast, display a two-sided relationship between polarisation and deformation: a ﬁeld induces deformation, and deformation induces charge differences between its surfaces, thus creating a ﬁeld. The piezoelectric coefﬁcient is the strain per unit of electric ﬁeld, and although it is very small, it is a true linear effect, and this makes it useful e when you want to position or move a probe with nano-scale precision, it is just what you need. Pyroelectric materials contain molecules with permanent dipole moments that in a single crystal are aligned, giving the crystal a permanent polarisation. When the temperature is changed, the polarisation changes, creating surface charges, or if the surfaces are connected electrically, a pyroelectric current e the principle of intruder-detection systems and of thermal imaging. Ferroelectric materials, too, have a natural dipole moment; they are polarised to start with, and the individual polarised molecules line up so that their dipole moments are parallel. Their special feature is that the direction of polarisation can be changed by applying an electric ﬁeld, and the change causes a change of shape. Applications of all of these are described in Section 15.5.
Charts for electrical properties
All materials have an electrical resistivity, and all dielectrics have a dielectric constant and loss factor. Property charts for these allow comparison between a large and varied population. Thermal conductivity and electrical resistivity Figure 15.6 shows the thermal conductivity l and the electrical conductivity ke . The ﬁrst has a range of 105, the second a range of 1028; no other material property has such a wide range. For metals, thermal and electrical conduction
15.3 Charts for electrical properties 421 are linked because both depend on free electrons, giving the obvious correlation between the two at the upper right of the chart, ke z 105 l
(l in W/m.K, ke in S/m), a relationship known as the WiedemanneFranz law. Electrical resistivity ρe (μΩ.cm) 1027
Thermal and Electrical conductivities
Thermal conductivity (W/m.K)
Copper Aluminium Zinc Iron Lead Titanium Terfenol-D Gadolinium
Si-Ge Hard ferrites
Pb-Te Mn-As Sb-Te
Bismuth Nylons titanate
Metals Semiconductors Piezo-electrics Thermo-electrics Ferrites Ceramics, Glass Polymers
Gold Gallium phosphide
-12 10-15 PVC10 ABS
1 Silicon carbide
Lead lanthanum zirconium titanate Lithium tantalate
Electrical conductivity κe (S/m)
Figure 15.6 Chart of thermal conductivity, l against electrical conductivity,ke ; the electrical resistivity re is the reciprocal of the conductivity and is shown across the top. Dielectric constant, dielectric breakdown, and limiting electric energy density The chart of Figure 15.7 gives an overview of dielectric behaviour. Molecules containing polar groups, such as nylon, polyurethane, and ionic-bonded ceramics, react strongly to an electric ﬁeld and polarise, giving them high dielectric constants. Those with purely covalent or Van der Waals bonding do not polarise easily and have low values. The dielectric strengths differ too e polymers have higher values than ceramics or glasses. The contours show values of the upper limiting energy density 12 εr εo E2b , where εo is the permittivity of vacuum, 8.85 1012 F/m (equation (15.14)). Ferroelectric ceramics stand out due to their high dielectric constants.
422 Chapter 15 Electrical materials: conductors, insulators, and dielectrics Capacitor energy density 100
Energy density Lead lanthanum zirconium titanate
Natural materials 0.001
Polyvinylidene fluoride (PVDF)
Dielectric strength (MV/m)
Figure 15.7 The dielectric properties of materials.
Drilling down: the origins and manipulation of electrical properties
Electrical conductivity Solids are made up of atoms containing electrons that carry a charge ee and a nucleus containing protons, each with a positive charge þe. An electric ﬁeld, E (volts/m), exerts a force E.e on a particle carrying a charge e. If the charge-carriers can move, the force E.e causes them to ﬂow through the material e that is, it conducts. Metals are electronconductors, meaning that the charge-carriers are the electrons. In ionic solids (which are composed of negatively and positively charged ions like Naþ and Cle), the diffusive motion of ions allows ionic conduction, but this is only possible at temperatures at which diffusion is rapid. Many materials have no mobile electrons, and at room temperature they are too cold to be ionic conductors. The charged particles they contain still feel a force in an electric ﬁeld that displaces the charges slightly, but they are unable to move more than a tiny fraction of the atom spacing. These are insulators; the small displacement of charge gives them dielectric properties. Chapter 4, Section 4.5 explained the way electrons of an atom occupy discrete energy states or orbits, arranged in shells (designated 1, 2, 3, etc. from innermost to outermost); each shell is made up of sub-shells (designated s, p, d, and f), each of which contains 1, 3, 5, or 7 orbits respectively. The electrons ﬁll the shells with the lowest energy, two electrons of opposite spin
15.4 Drilling down: the origins and manipulation of electrical properties 423 in each orbit; the Pauli7 exclusion principle prohibits an energy state with more than two. When n atoms (a large number) are brought together to form a solid, the inner electrons remain the property of the atom on which they started, but the outer ones interact. Each atom now sits in the ﬁeld created by the charges of its neighbours. This has the effect of decreasing slightly the energy levels of electrons spinning in a direction favoured by the ﬁeld of its neighbours and raising that of those with spins in the opposite direction, splitting each energy level. Thus the discrete levels of an isolated atom broaden in the solid into bands of very closely spaced levels. The number of electrons per atom depends only on the atomic number; they ﬁll the bands from the bottom, starting from the lowest, until all are on board, so to speak. The topmost ﬁlled energy level at 0K is called the Fermi8 energy (more on this later). Above 0K, thermal energy allows electrons to occupy higher levels with a certain probability; the Fermi level is then deﬁned as the energy level having the probability that it is exactly half ﬁlled with electrons. Levels of lower energy than the Fermi level tend to be entirely ﬁlled with electrons, whereas energy levels higher than the Fermi tend to be empty. If two materials with different Fermi levels are placed in contact, electrons ﬂow from the material with the higher Fermi level into the one with the lower Fermi level, creating a charge difference between them. The electric ﬁeld associated with this charge difference raises the lower Fermi level and lowers the higher Fermi level until the two are equal. An electron at the Fermi level still has an energy that is lower than it would have if it were isolated in vacuum far from the atoms. This energy difference is called, for historical reasons, the work function, because it is the work that is required to remove an electron from the Fermi level to inﬁnity. If you want to create an electron beam, it can be done by heating the metal until some of its electrons have enough energy to exceed the work function, then accelerating them away with a ﬁeld gradient. Whether the material is a conductor or an insulator depends on how full the bands are and whether they overlap. In Figure 15.8, the central column describes an isolated atom, and the outer ones illustrate the possibilities created by bringing atoms together into an array, with the energies spread into energy bands. Conductors like copper, shown on the left, have an unﬁlled outer band; there are many very closely spaced levels just above the last full one, and when accelerated by a ﬁeld, electrons can use these levels to move freely through the material. In insulators, shown on the right, the outermost band with electrons in it is full, and the nearest empty band is separated from it in energy by a wide band gap. Semiconductors, too, have a band gap, but it is narrower e narrow enough that thermal energy can pop a few electrons into the empty band, where they conduct. Deliberate doping (adding trace levels of other elements) creates new levels in the band gap, reducing the energy barrier to entering the empty states and thus allowing more carriers to become mobile. 7
Wolfgang Joseph Pauli (1900e1958), quantum theorist, conceiver of the neutrino and Nobel Prize winner. He was not, however, a happy man, requiring psychotherapy, which he received from none other than the great psychoanalyst Karl Jung. Enrico Fermi (1901e1954), devisor of the statistical laws known as Fermi statistics governing the behaviour of electrons in solids. He was one of the leaders of the team of physicists on the Manhattan Project for the development of the atomic bomb.
424 Chapter 15 Electrical materials: conductors, insulators, and dielectrics Energy Empty
Partly filled band
Figure 15.8 Conductors (left) have a partly ﬁlled outer band. Insulators (right) have a ﬁlled outer band, separated from the nearest unﬁlled band by a band gap. Electrical resistance If a ﬁeld E exerts a force E.e on an electron, why does it not accelerate forever, giving a current that continuously increases with time? This is not what happens; instead, switching on a ﬁeld causes a current that almost immediately reaches a steady value. Referring back to equations (15.1) and (15.3), the current density i /A is proportional to the ﬁeld E, i E ¼ ¼ ke E A re
where re is the resistivity and ke , its reciprocal, is the electrical conductivity. Broadly speaking, the picture is this. Conduction electrons are free to move through the solid. Their thermal energy kT (k ¼ Boltzmann’s constant, T ¼ absolute temperature) causes them to move like gas atoms in all directions. In doing this they collide with scattering centres, bouncing off in a new direction. Impurity or solute atoms are particularly effective scattering centres (which is why alloys always have a higher resistivity than those of pure metals), but electrons are scattered also by imperfections such as dislocations and by the thermal vibration of the atoms themselves. When there is no ﬁeld, there is no net transfer of charge in any direction even though all the conduction electrons are moving freely. A ﬁeld causes a drift velocity vd ¼ me E on the electrons, where me is the electron mobility, and it is this that gives the current (Figure 15.9). The drift velocity is small compared with the thermal velocity; it is like a breeze in air e the thermal motion of the air molecules is far greater than the ‘drift’ that we feel as the breeze. The greater the number of scattering centres, the shorter the mean-free path, lmfp, of the electrons between collisions, and the slower, on average, they move. Just as with thermal conductivity, the electrical conductivity depends on a mean-free path, on the density of carriers (the number nv of mobile electrons per unit volume), and the charge they carry. Thus the current density, i/A, is given by i ¼ nv e nd ¼ nv e me E A
15.4 Drilling down: the origins and manipulation of electrical properties 425
Field E = V/d
Electron path Scattering points
Figure 15.9 An electron, accelerated by the ﬁeld E, is scattered by imperfections that create a resistance to its motion.
Comparing this with equation (15.19) gives the conductivity: ke ¼ nv e me
Thus the conductivity is proportional to the density of free electrons and to the drift velocity, and this is directly proportional to the mean-free path. The purer and more perfect the conductor, the higher the conductivity and the lower its reciprocal, the resistivity. Example 15.5 Electron mobility The resistivity of pure copper is re ¼ 2.32 mU.cm. Each copper atom provides one free electron. The atomic volume of copper is 1.18 1029 m3. What is the electron mobility in copper? Answer. If each atom contributes one electron, the electron concentration in copper is nv ¼
1 ¼ 8:47 1028 per m3 Atomic volume
The resistivity re is related to this by 1 1 ¼ , where e ¼ 1.6 1019 coulombs is the charge on an electron. re ¼ ke nv e m e Converting the resistivity from mU.cm to U.m by multiplying by 108 gives the electron mobility in copper as me ¼
1 ¼ 0:0032 m2 V:s nv e re
426 Chapter 15 Electrical materials: conductors, insulators, and dielectrics Metals are strengthened (Chapter 7) by solid-solution hardening, work hardening, or precipitation hardening. All of these change the resistivity too. Figure 15.10 shows how the strength and resistivity of copper and aluminium are changed by alloying and deformation. Adding solute to either metal increases its strength, but the solute atoms also act as scattering centres, increasing the electrical resistivity as well. Dislocations add strength (by what we called work hardening), and they too scatter electrons a little, though much less than solutes do. Precipitates offer the greatest gain in strength; their effect on resistivity varies, depending on their size and spacing compared to the electron mean-free path and on the amount of residual solute left in the lattice. Precipitation hardening (with low residual solute) and work hardening are therefore the best ways to strengthen conductors. The two ﬁgures show that commercial conductor alloys have much greater strength and only slightly greater resistivity than those of the pure metals.
Copper alloys Copper-nickel, hard drawn
t So lu
g ni n rde e ha
Brasses, bronzes, soft
30 Pure, soft aluminium
Pure, soft copper
Al-Mg, soft (5083 H0)
r Wo rd ha
Al-Mg, wrought (5083 H343)
Wrought (1050 H9)
k en ing
Yield strength (MPa)
Hard drawn copper
Work hardening Pr ec ipi tat e
Yield strength (MPa)
Brass, bronze, hard drawn
Al-Zn-Mg-Cu (7075 T6) Al-Cu-Mg (2024 T861) Al-Si-Mg-Mn (6082 T6)
Work hardening ec ipi tat eh ard eni ng
Electrical resistivity (µohm.cm)
Electrical resistivity (µohm.cm)
Figure 15.10 Strengthening mechanisms increase resistivity. Work hardening and precipitation do so less than solute hardening, as seen here in copper and aluminium alloys. The resistivity of metals increases with temperature because thermal vibrations (phonons) scatter electrons. Resistance decreases as temperature falls, which is why very high-powered electromagnets are pre-cooled in liquid nitrogen. As absolute zero is approached, most metals retain some resistivity, but as discussed earlier, a few suddenly lose all resistance and become superconducting between 0 and 10K. The resistivity of semiconductors, by contrast, decreases as temperature increases for reasons explained next. Semiconductors Semiconductors are based on elements in which four valence electrons ﬁll the valence band, with an energy gap separating them from the next available level (in the conduction band). They get their name from their electrical conductivities, 104 to 10þ4 (S/m),
15.4 Drilling down: the origins and manipulation of electrical properties 427 much smaller than those of metals but still much larger than those of insulators. At 0K, pure semiconductors are perfect insulators because there are no electrons in their conduction band. The band gap, however, is narrow, allowing thermal energy to excite electrons from the valence to the conduction band at temperatures above 0K and leaving holes behind in the valence band. The electrons in the conduction band are mobile and move in an electric ﬁeld, carrying current. The holes in the valence band are also mobile (in reality it is the electrons in the valence band that move cooperatively, allowing the hole to change position), and this charge movement also carries current. Thus the conductivity of a semiconductor has an extra term ke ¼ nv e me þ nh e mh
where nh is the number of holes per unit volume and mh is the hole mobility. In pure semiconductors, each electron promoted to the conduction band leaves a hole in the valence bend, so ne ¼ nh, the conductivity becomes ke ¼ nv e ðme þ mh Þ
and the semiconduction is said to be intrinsic (a fundamental property of the pure material). The number of charge carriers can be controlled in another way, by doping with controlled, small additions of elements that have a different valence than that of the semiconductor itself. This creates free electrons and holes that simply depend on the concentration of dopant, and the semiconducting behaviour is said to be extrinsic (a characteristic of the doping rather than of the base material). Example 15.6 Intrinsic semiconduction The electron mobility me in silicon at 300K is 0.14 m2/V.s, and that of holes mh is 0.04 m2/V.s. The carrier density is 1.5 1016/m3 for both. What is the intrinsic conductivity of silicon at 300K? Answer. The conductivity is (0.14 þ 0.04) ¼ 4.3 104 S/m
ke ¼ nv e (me þ mh) ¼ 1.5 1016 1.6 1019
Dielectric behaviour In the absence of an electric ﬁeld, the electrons and protons in most dielectrics are symmetrically distributed and the material carries no net charge or dipole moment. In the presence of a ﬁeld, the positively charged particles are pushed in the direction of the ﬁeld, and negatively charged particles are pushed in the opposite direction. The effect is easiest to see in ionic crystals, since here neighbouring ions carry opposite charges, as on the left of Figure 15.11. Switch on the ﬁeld and the positive ions (charge þq) are pulled in the ﬁeld direction, the negative ones (charge q) in the reverse, until the restoring force of the
428 Chapter 15 Electrical materials: conductors, insulators, and dielectrics inter-atomic bonds just balances the force due to the ﬁeld at a displacement of Dx, as on the right of the ﬁgure. Two charges q separated by a distance Dx create a dipole with dipole moment, d, given by d ¼ q Dx
Figure 15.11 An ionic crystal (a) in zero applied ﬁeld, and (b) when a ﬁeld V=x is applied. The electric ﬁeld displaces charge, causing the material to acquire a dipole moment. The polarisation of the material, P, is the volume-average of all the dipole moments it contains: P d (15.24) P¼ volume Even in materials that are not ionic, like silicon, a ﬁeld produces a dipole moment because the nucleus of each atom is displaced a tiny distance in the direction of the ﬁeld, and its surrounding electrons are displaced in the opposite direction (Figure 4.22). The resulting dipole moment depends on the magnitude of the displacement and the number of charges per unit volume, and it is this that determines the dielectric constant. The bigger the shift, the bigger the dielectric constant. Thus compounds with ionic bonds, and polymers that contain polar groups like eOH and eNH (nylon, for example), have larger dielectric constants than those that do not. Dielectric loss Think now of polarisation in an alternating electric ﬁeld. When the upper plate of Figure 15.11(b) is negative, the displacements are in the direction shown in the ﬁgure. When its polarity is reversed, the negative ions are displaced upwards and the positive ions downwards; in an oscillating ﬁeld, the ions oscillate. If their oscillations were exactly in phase with the ﬁeld, no energy would be lost, but this is never exactly true, and often the phase shift is considerable. Materials with high dielectric loss usually contain awkwardly shaped molecules that themselves have a dipole moment e the water molecule is an example (look back at
15.4 Drilling down: the origins and manipulation of electrical properties 429 Figure 4.24). These respond to the oscillating ﬁeld by rotating, but because of their shape they interfere with each other (you could think of it as molecular friction), and this dissipates energy that appears as heat e which is how microwave heating works. As equation (15.17) showed, the energy that is dissipated depends on the frequency of the electric ﬁeld. Generally speaking, the higher the frequency, the greater the power dissipated, but there are peaks at certain frequencies that are characteristic of the material structure. Example 15.7 Polarisation in an electric ﬁeld An ionic crystal with a rock-salt structure (see ﬁgure) is made up of equal numbers of positive and negative ions each carrying or lacking the charge carried by a single electron. The lattice parameter of the crystal is 0.45 nm. An electric ﬁeld displaces the ions relative to each other by 1% of the lattice parameter. What is the resulting polarisation? Answer. The dipole moment due to one pair of ions is d ¼ q Dx ¼ 1:6 1019 0:0045 109 ¼ 0:72 1030 C:m
The volume of the unit cell is V ¼ (0.45 109)3 ¼ 9.1 1029 m3, and each cell contains four pairs of ions. Thus the polarisation is P¼
4d ¼ 0:032 C m2 V
Negative ions Positive ions
Dielectric breakdown In metals, as we have seen, even the smallest ﬁeld causes electrons to ﬂow. In insulators, they can’t because of the band gap. But if at some weak spot, one electron is torn free from its parent atom, the force E.e exerted by the ﬁeld E accelerates it and thus gives it kinetic energy; it continues to accelerate until it collides with another atom. A sufﬁciently
430 Chapter 15 Electrical materials: conductors, insulators, and dielectrics large ﬁeld can give the electron so much kinetic energy that in the collision it kicks one or more new electrons out of the atom it hits, creating electron-hole pairs, and they in turn are accelerated and gain energy. The result, sketched in Figure 15.12, is a cascade e an avalanche of charge. It can be sufﬁciently violent that the associated heating damages the material permanently. It can also be harnessed e avalanche-effect transistors use the effect to provide rapid switching of large currents.
Figure 15.12 Breakdown involves a cascade of electrons like a lightning strike. The critical ﬁeld strength to make this happen, called the breakdown potential, is hard to calculate; it is that at which the ﬁrst electron breaks free at the weak spot, a defect in the material such as a tiny crack, void, or inclusion that locally concentrates the ﬁeld. The necessary ﬁelds are large, typically 1e15 MV/m. That sounds like a lot, but such ﬁelds are found in two very different circumstances: when the voltage V is very high, or the distance x is very small. In power transmission, the voltages are sufﬁciently high e 400,000 volts or so e that breakdown can occur at the insulators that support the line, whereas in microcircuits and thin-ﬁlm devices, the distances between components are quite small: a 1 V difference across a distance of 1 micron gives a ﬁeld of 1 MV/m. Piezoelectric materials The word ‘Quartz’ on the face of your watch carries the assurance that its time-steps are set by the oscillations of a piezoelectric quartz crystal. Piezoelectric behaviour is found in crystals in which the ions are not symmetrically distributed (the crystal structure lacks a centre of symmetry), so that each molecule carries a permanent dipole moment (Figure 15.13(a)). If you cut a little cube from such a material, with faces parallel to crystal planes, the faces would carry charge. This charge attracts ions and charged particles from the atmosphere just as a television screen does, giving an invisible surface layer that neutralises the charge.
15.4 Drilling down: the origins and manipulation of electrical properties 431
Figure 15.13 (a) A piezoelectric material has a non-symmetrically distributed charge, giving it a natural dipole moment. (b) When deformed, the dipole moment changes and the surfaces become charged. (c) The inverse is also true; a ﬁeld induces a change of shape, the basis of piezoelectric actuation. If you now squeeze the crystal, its ions move relative to each other, the dipole moment changes, and the charge on the surface changes too (Figure 15.13(b)). Given time, the newly appeared charge would attract neutralising ions, but this does not happen immediately, giving a potential difference. This provides the basis of operation of electric microphones and pick-ups. The potential difference between the faces can be large e large enough to generate a spark across a narrow gap e and this is the way that gas lighters work. A strain, then, induces an electric ﬁeld in a piezoelectric material. The inverse is also true: a ﬁeld induces a strain. The ﬁeld pulls the positive ions and pushes the negative ones, changing their spacing and so changing the shape of the crystal (Figure 15.13(c)). If a small strain produces a large ﬁeld, then a large ﬁeld will produce only a very small strain. But the strain is a linear function of ﬁeld, allowing extremely precise, if small, displacements used for positioning and actuation at the sub-micron scale. Piezoelectric materials respond to a change in electric ﬁeld faster than most materials respond to a stimulus of this or any other kind. Put them in a megahertz ﬁeld and they respond with microsecond precision. That opens up many applications, some described later in this chapter. In particular, it opens up the world of ultrasonics e sound waves with frequencies starting at the upper limit of the human ear, 20 kHz, on up to 20,000 kHz and above. Pyroelectric materials The Greek philosopher Theophrastus9 noted that certain stones, when warmed or cooled, acquired the ability to pick up straw and dry leaves. It was not until the 20th century that this pyroelectric behaviour e polarisation caused by change of temperature e was understood and exploited. Some materials have a permanent dipole moment because their positive and negative ions balance electrically but are slightly out of line with each other. If a thin disk of one of these is cut so that its faces are parallel to the plane in which the misalignment happens, the disc has a spontaneous dipole moment Ps of its own. The unit cells of pyroelectric materials are like this. 9
Theophrastus (372e287 BC), successor to Aristotle, a teacher of science and author of a ten-volume History of Plants, which remained the most important contribution to botanical science for the following 1200 years.
432 Chapter 15 Electrical materials: conductors, insulators, and dielectrics The net dipole moment exists in the absence of an applied electric ﬁeld and is equivalent to a layer of bound charge on each ﬂat surface (Figure 15.14(a)). Nearby free charges such as electrons or ions are attracted to the surfaces, neutralising the charge. Imagine that conductive electrodes are then attached to the surfaces and connected through an ammeter. If the temperature of the sample is constant, then so is Ps, and no current ﬂows through the circuit. An increase in temperature, however, causes expansion and disorder among the dipoles, changing the net dipole moment and the polarisation. Redistribution of free charges to compensate for the change in bound charge results in a current ﬂow e the pyroelectric current e in the circuit (Figure 15.14(b)). Cooling rather than heating reverses the sign of the current. The pyroelectric current only ﬂows while the temperature is changing; it’s the way that intruder alarms, automatic doors, and safety lights are activated.
+ + (b)
+ + (a)
+ + + + + + dT =0 dt
dT >0 dt
Figure 15.14 Pyroelectric behaviour. In an open circuit, the free charges remain on the electrodes, which has its uses too, described in the next section. Pyroelectric materials include minerals such as tourmaline (the one Theophrastus found), ceramics such as barium titanate, polymers such as polyvinylidene ﬂuoride, and even biological materials, such as collagen. Ferroelectric materials Ferroelectrics are a special case of piezoelectric behaviour. They, too, do not have a symmetric structure but have the special ability to switch asymmetry. Barium titanate (BaTiO3), shown schematically in Figure 15.15, is one of these. Below a critical temperature, the Curie10 temperature (about 120 C for barium titanate), the titanium atom, instead of sitting at the centre of the unit cell, is displaced e either up or down, as in (a) and (b), or to one of the four other equivalent positions round the central position. Above the 10
Pierre Curie (1859e1906), French physicist, discoverer of the piezoelectric effect and of magnetic transformations; and husband of the yet more famous Marie Curie. He was killed in a street accident in Paris, a city with dangerous trafﬁc even in 1906.
15.4 Drilling down: the origins and manipulation of electrical properties 433 Curie temperature, the asymmetry disappears and with it the dipole moment, as in (c). In ferroelectrics, these dipoles spontaneously align so that large volumes of the material are polarised even when there is no applied ﬁeld. O-
(a) Polarized up Equivalent dipole
(b) Polarized down
(c) Unpolarized No dipole
Figure 15.15 Ferroelectric materials have a permanent dipole moment that can switch; here the Tiþ
ion can ﬂip from the upper to the lower position. Above the Curie temperature, the asymmetry disappears.
In the absence of an external ﬁeld, a ferroelectric divides itself up into domains e regions in which all the dipoles are aligned in one direction e separated by domain walls at which the direction of polarisation changes (Figure 15.16). The domains orient themselves so that the dipole moment of each domain more or less cancels that of its neighbours. If a ﬁeld is applied, the domain walls move so that those polarised parallel to the ﬁeld grow and those polarised across or against it shrink, until the entire sample is polarised (or ‘poled’) in just one direction.
No applied field No net polarisation
Applied electric field E and polarisation P
Domain of dipoles
Figure 15.16 Ferroelectric domains arrange themselves so that their dipole moments cancel. In an electric ﬁeld E they align, giving the crystal a net dipole moment, which can be large. Figure 15.17 shows how the polarisation P changes as the ﬁeld E is increased: P increases, reaching a maximum at the saturation polarisation Ps. If the ﬁeld is now removed, a large part of the polarisation remains (the remanent polarisation), which is only removed by reversing the ﬁeld to the value eEc, the coercive ﬁeld. The ﬁgure shows a complete cycle through full reverse polarisation, ending up again with full forward poling. The little inserts show the domain structures at points around the cycle.
434 Chapter 15 Electrical materials: conductors, insulators, and dielectrics Polarization P Remanent polarization Saturation polarization
Coercive field Ec Coercive field - Ec
Electric field E
Figure 15.17 A ferroelectric hysteresis curve. Ferroelectric materials have enormous dielectric constants. Those of normal materials with symmetric charge distributions lie in the range 2e20. Those for ferroelectrics can be as high as 20,000. It is this that allows their use for making super-capacitors that can store 1000 times more energy than conventional capacitors. Such is their energy density that super-capacitors now compete with batteries in kinetic-energy recovery systems for vehicles.
Design: using the electrical properties of materials
Transmitting electrical power The objective in power transmission is to minimise electrical loss, PL (equations (15.2) and (15.3), combined): PL ¼ i2 R ¼ i2 re
L i2 L ¼ A ke A
The best choice, for a given cross-section A and length L, is a material with the largest electrical conductivity ke ; if the line is buried or supported along its entire length, the only other constraint is that of material cost. The chart of Figure 15.6 shows that of the materials plotted on it, silver (price z $500/kg) has the highest conductivity. Copper and aluminium come next and are more affordable (price of copper z $5/kg, that of aluminium z$2/kg), and it is these two materials that are most used for power transmission. If instead the line is above ground and supported by widely spaced pylons, strength and density become important: high strength to support self-weight and wind loads; low density to minimise self-weight. Here we have a conﬂict: the materials with the highest conductivities have low strength; those with high strength do not conduct very well. Aluminium and copper conductors used in overhead cables, as shown in Figure 15.10, are work or precipitation hardened to give strength with minimum loss of conductivity. An alternative is a hybrid cable in which two materials are combined, the ﬁrst to give conductivity, the second to give strength. One such is sketched in Figure 15.18. The core is pure, high-conductivity copper or aluminium; it is wrapped in a cage of high-strength carbon-steel wires. With a 50e50 mix, the hybrid, when averaged, has roughly half the strength of the steel and twice the resistivity of the copper per unit length of cable.
15.5 Design: using the electrical properties of materials
Polymer outer casing
Figure 15.18 A hybrid copperesteel cable. Electric energy storage The energy density of a capacitor with a single dielectric layer (Figure 15.19) increases with the square of the ﬁeld E: Energy density ¼
1 εr εo E2 2
where εr is the relative permittivity (dielectric constant) and εo the permittivity of vacuum (8.854 1012 F/m). An upper limit for E is the dielectric strength, Eb , setting an upper limit for energy density: Maximum energy density ¼
1 εr εo E2b 2
Figure 15.19 A capacitor. This upper limit is plotted in Figure 15.7, which illustrates the enormous gains that ferroelectric ceramics offer. Lead zirconium titanate (PZT) has the highest value and is used for high performance capacitors, but barium titanate is the more usual selection because it is cheaper, easier to process, and lead-free. Electrical insulation with thermal conduction: keeping microchips cool As microchips shrink in scale and clock-speeds rise, overheating becomes a problem. The chips in today’s PCs reach 85 C, requiring forced air cooling. Multi-chip modules (MCMs) pack over 100 chips onto a single substrate, and there the problem is more severe. Heating is kept under control by attaching the chip to a heat sink (Figure 15.20), taking care that they are in good thermal contact. The heat sink now becomes a critical component, limiting further development of the electronics.
436 Chapter 15 Electrical materials: conductors, insulators, and dielectrics Substrate
Chips Heat sink Cooling fins
Figure 15.20 A heat sink. It must conduct heat but not electricity. To drain heat away from the chip as fast as possible, the heat sink must have the highest possible thermal conductivity, l. Metals like copper and aluminium have high l, but they are good electrical conductors, and this is bad because it allows electrical coupling and stray capacitance between chip and heat sink, slowing the information transfer rate (remember the time delay in a circuit is s ¼ RC). To prevent this, the heat sink must be an excellent electrical insulator. Figure 15.6 is the chart with the properties we want: thermal conductivity l and electrical resistivity, re. The materials at the top left have high thermal conductivity and very high resistivity e they are electrical insulators. The best choice of materials for the heat sink, then, is aluminium nitride, AlN, alumina, Al2O3, or silicon nitride, Si3N4. It is these that are used for such heat sinks. Using dielectric loss: microwave heating When you cook chicken in a microwave oven, you are using dielectric loss. Looking back at equation (15.17) we see that the dielectric loss, and thus heating, is proportional to the loss factor L ¼ εr tan d. Chickens have a high loss factor, as do all foods that contain water. There are other ways to cook them, but this one has the advantage that it is quick because microwaves absorb throughout the section, giving uniform heating. Microwave heating is not just useful in the kitchen; it is also widely used for industrial heating. Microwave heating has engineering applications too: the curing of adhesives, polymer moulding, ceramic sintering, and the drying of wood. As equation (15.17) implies, the higher the frequency f of the electric ﬁeld, the greater the heating, so it is common, in the industrial application of microwaves, to use gigahertz frequencies (0.3e3 GHz). Using dielectric loss: stealth technology Radar, developed during the Second World War, played a major role in protecting Britain from air attack. It works by transmitting bursts of radio-frequency radiation that are reﬂected back by objects in their path. The signal processing computes the distance and speed of the object being tracked from the time it takes for the reﬂection to arrive back. The metal body of an aircraft is an excellent radar reﬂector, and its curved shape causes it to reﬂect in all directions e just what is needed for safe air-trafﬁc control. But if your aim is to avoid detection, reﬂection is the last thing you want. Stealth technology combines three tricks to minimise it.
A shape made up of ﬂat planes that reﬂect the radar signal away from the detector unless it lies exactly normal to the surface.
15.5 Design: using the electrical properties of materials
Non-metallic structural materials e usually composites e that are semi-transparent to microwaves. Surface coatings of radar-absorbing materials (called RAMs) that absorb microwaves rather than reﬂecting them. A RAM with a large loss factor εr tan d e a ferroelectric, for example e attenuates the incoming wave, diminishing the reﬂected signal.
Avoiding dielectric loss: materials for radomes The function of a radome is to shield a microwave antenna from wind and weather while having as little effect as possible on the signal it sends and receives (Figure 15.21). When trying to detect incoming signals that are weak to begin with, even a small attenuation of the signal as it passes through the radome decreases the sensitivity of the system. Yet the radome must withstand structural loads, loads caused by pressure difference between the inside and outside of the dome, and e in the case of supersonic ﬂight e high temperatures. So the problem here is the opposite of that for stealth coatings; it is how to design materials that do not attenuate electromagnetic waves. The answer is to seek those with exceptionally low values of εr tan d. And since the radome carries structural loads, they should also be strong. Radome
Figure 15.21 A radome. Dielectric loss in the shell must be minimised. Most polymers have low loss factor, but they are not very strong. Reinforcing them with glass ﬁbres, creating GFRPs, combines low loss with good strength. When, additionally, high temperatures are involved, the ceramics e silica (SiO2), alumina (Al2O3) and silicon nitride (Si3N4) e are all employed. Piezoelectric accelerometers generate a force:
Piezoelectric accelerometers rely on the inertia of a mass m to F ¼ ma
when subjected to an acceleration or a deceleration a. If this force is applied to the end of a beam to which a thin layer of piezoelectric material is bonded, the piezoelectric layer is stretched or compressed (Figure 15.22). The resulting charge that appears on the piezoelectric can be detected, and if necessary used to trigger a response if the acceleration or deceleration exceeds a critical value. For this, a material with a high piezoelectric charge coefﬁcient, such as lead zirconium titanate or barium titanate, is desirable. PZT has the highest value for this coefﬁcient.
438 Chapter 15 Electrical materials: conductors, insulators, and dielectrics Encapsulation Piezo layer Silicon Beam Mass
Figure 15.22 A simple piezoelectric accelerometer or energy-harvesting device. Energy harvesting Small portable electronic devices operate with low electrical drain, but their batteries still need to be charged. Mechanical energy from vibration or cyclic movement is present almost everywhere. The conﬁguration shown in Figure 15.22 also allows electrical power to be harvested from mechanical vibration. Here the conversion efﬁciency of mechanical to electrical energy is the dominant consideration, requiring materials with a high electro-mechanical coupling constant. Once again, PZT is the best choice, with lithium niobate as a non-toxic alternative. Piezoelectric actuation: ink-jet printers If you want to convert digital code to hard-copy, inkjet printing is the cheapest way to do it. Early printers used thermal (‘bubble-jet’) technology in which a tiny heating wire boils a minute volume of ink in the print-head, creating a vapor bubble. The pressure-pulse this creates ejects a droplet of ink. The bubble collapses as the wire cools, sucking more ink from a reservoir into the print-head to replace that of the droplet. The technology is simple but it gives little control of the droplet size or shape. The alternative is the piezo print-head, one unit of which is sketched in Figure 15.23. An electric ﬁeld applied to the disk of piezoelectric material transmits a kick to the vibration plate, creating a pressure pulse that spits a droplet of ink from the nozzle. On relaxation, more ink is drawn in to replace it. Like bubble-jet printers, piezo print-heads have 300 to 600 nozzles. The great advantage of piezo technology is the control of the shape and duration of the pulse delivered by the piezo disk. The droplets of ink are signiﬁcantly smaller, and the control of droplet size gives greater resolution and colour gradation.
Vibration plate Direction of actuation Piezo disk with electrodes
Figure 15.23 A piezo print-head.
15.5 Design: using the electrical properties of materials
Pyroelectric thermal imaging Night vision, the location of survivors in disaster areas, the ﬁlming of wildlife e all these make use of thermal imaging. A typical set-up is sketched in Figure 15.24. A lens, made of a material transparent to infrared (IR), such as germanium, focuses the IR radiation from an object on the left to form an image on the pyroelectric disk on the right. The focused IR rays warm points on the disk to different degrees, depending on the temperature and emissivity of the points on the object from which they came, and the change of temperature changes the polarisation. The image creates a pattern of charge on the surface of the disk that can be ‘read’ with an electron beam.
Lens transparent to infra-red Paths of IR rays
Object emitting IR radiation
Thermal image on disk causes local polarization Slotted disk to limit thermal diffusion from pixel to pixel
Figure 15.24 Thermal imaging. Energy harvesting from waste heat The Seebeck11 effect, discovered in 1821, describes the appearance of an electrical potential when two materials are joined and placed in a thermal gradient. In a thermoelectric material, free electrons or holes transport both charge and heat. To a ﬁrst approximation, the electrons and holes behave like a gas of charged particles. If a normal (uncharged) gas is placed in a box within a temperature gradient, the gas molecules at the hot end move faster than those at the cold one. The faster hot molecules diffuse further than the cold ones, leading to a net build-up of molecules at the cold end. The density-gradient drives the molecules to diffuse back towards the hot end so that at steady-state, the two effects exactly compensate and there is no net ﬂow. 11
Thomas Johann Seebeck, 1770e1831, was a Baltic (now Estonian) physicist who studied medicine but succumbed to a fascination with physics. He discovered and quantiﬁed the Seebeck effect, worked with Johann von Goethe, the writer and statesman, on the Theory of Colours, and dabbled with experiments on early photography.
440 Chapter 15 Electrical materials: conductors, insulators, and dielectrics Electrons and holes behave in a similar way. Because they carry charge, the temperature gradient creates a charge gradient between the hot and cold ends of the material; the charge gradient tends to push the charges back to the hot end. If the free charges are positive (the material is p-type), positive charge builds up at the cold face, which acquires a positive potential. If instead they are negative (n-type material) the cold face acquires a negative potential. These can then be connected up to give small-scale thermoelectric generators (Figure 15.25). Heat source
Figure 15.25 Schematic multicouple thermoelectric generator. The Seebeck coefﬁcient S (mV/ C) is a measure of the change in voltage, DV, induced across a thermoelectric material by a thermal gradient, DT. For small temperature changes, the Seebeck coefﬁcient is given by S¼
Thermoelectric performance at temperature T is captured by the ﬁgure of merit, zT: S2 k e T l To provide power, a thermoelectric material must have a high Seebeck coefﬁcient S, a high electrical conductivity ke to reduce resistive losses, and a low thermal conductivity l to maintain a steep temperature gradient between the hot and cold side of the generator e a combination not easily achieved. They appear on the lower right of Figure 15.6, coloured purple; many of them involve the comparatively rare elements antimony and tellurium. Thermoelectric generation is used in space-probes, drawing heat from a radio-active source. The conversion efﬁciency, however, is low, and this has limited the use of thermoelectrics for energy harvesting on earth. Despite this, the automobile industry expresses interest in using them. A third of the energy used by a car is lost as waste heat. Some of this can be converted back to useful electrical energy using thermoelectric generators attached to the exhaust manifold. zT ¼
Summary and conclusions
All materials contain charged particles: electrons, protons, ions, charged molecules, and the like. An electric ﬁeld E exerts a force qE on a charge q, pushing it in the direction of the ﬁeld if q is positive and in the opposite direction if q is negative. If the particles can move freely, as electrons can in metals, an electric current ﬂows through the material, which we refer to as conduction. Special types of conduction are also found e superconductivity at very low temperatures, and semiconduction in the materials of electronics such as silicon and germanium. If, instead, the particles cannot move freely, as is the case in insulators, they are still displaced slightly by the ﬁeld, leading to dielectric polarisation.
Materials that polarise easily have a high dielectric constant. If used as the insulating ﬁlm of a capacitor, the polarisation screens the electrodes from each other, increasing the capacitance. The slight displacement of charge has other consequences. One of these is electrostriction e the charge movement causes the material to change shape slightly. If the material is made up of ions and these are arranged in a way that lacks a centre of symmetry, a further effect appears, that of piezoelectric response. The lack of symmetry means that each molecule carries a dipole moment, and within a single crystal these are aligned. An electric ﬁeld causes a change of shape, and a change of shape changes the molecular dipole moment, thus inducing a change in polarisation and generating a ﬁeld. A change of temperature, too, changes the molecular dipole moment, so materials that are piezoelectric are also pyroelectric. A few materials have a further property, that of molecular asymmetry that can switch direction because ions can occupy one of several equivalent sites in the crystal. These materials are ferroelectric; the molecular dipoles spontaneously align to form polarised domains. In the relaxed state, the domains take up orientations such that the ﬁeld of one is cancelled by those of its neighbours, but when ‘poled’ by placing it in an electric ﬁeld, the domains align, giving a large net polarisation that is retained when the ﬁeld is removed. All of these effects have practical utility, examples of which are described in this chapter.
Braithwaite, N., & Weaver, G. (1990). Electronic materials. Oxford, UK: The Open University and Butterworth Heinemann. ISBN: 0-408-02840-8. (One of the excellent Open University texts that form part of their Materials program.) Callister, W. D., & Rethwisch, D. G. (2011). Materials science and engineering: An introduction (8th ed.). New York, USA: John Wiley. ISBN: 978-0-470-50586-1. (A well-established and comprehensive introduction to the science of materials.) Elfrink, R., Kamel, T. M., Goedbloed, M., Matova, S., Hohlfeld, D., van Andel, Y., et al. (2009). Vibration energy harvesting with aluminum nitride-based piezoelectric devices. Journal of Micromechanics and Microengineering, 19(9). (An analysis of the potential for piezo-electric energy harvesting.) Jiles, D. (2001). Introduction to the electronic properties of materials (2nd ed.). Cheltenham, UK: Nelson Thornes. ISBN: 0-7487-6042-3. (The author develops the electronic properties of materials, relating them to thermal and optical as well as electrical behaviour.) Solymar, L., & Walsh, D. (2004). Electrical properties of materials (7th ed.). Oxford, UK: Oxford University Press. ISBN: 0-19-926793-6. (A mature introduction to electrical materials.)
Why do metals conduct electricity? Why do insulators not conduct electricity, at least when cold?
A potential difference of 4 V is applied across a tungsten wire 200 mm long and 0.1 mm in diameter. What current ﬂows in the wire? How much power is dissipated in the wire? The electrical conductivity ke of tungsten is 1.8 107 S/m.
442 Chapter 15 Electrical materials: conductors, insulators, and dielectrics Exercise E15.3
A gold interconnect 1 mm long and with a rectangular cross-section of 10 mm 1 mm has a potential difference of 1 mV between its ends. What is the current in the interconnect? What is the current density (amps/m2) in the interconnect? How much power is dissipated in it? The resistivity re of gold is 2.5 108 U.m.
The gold interconnect of the previous question (length 1 mm and rectangular cross-section of 10 mm 1 mm with a potential difference of 1 mV across its length) carries power for 10 s. If no heat is lost by conduction, radiation, or convection, how hot will the interconnect get? The resistivity re of gold is 2.5 108 U.m, its speciﬁc heat Cp is 130 J/kg.K, and its density is 19,300 kg/m3.
A 0.5-mm diameter wire must carry a current i ¼10 amps. The system containing the wire will overheat if the power dissipation, P ¼ i2 R, exceeds 5 W/m. The table lists the resistivities re of four possible candidates for the wire. Which ones meet the design requirement? Material
re , mU.cm
Aluminium Copper Nickel Tungsten
2.7 1.8 9.6 5.7
Which metallic superconductors have a critical temperature above the boiling point of helium? Which ceramic superconductors have a critical temperature above the boiling point of liquid nitrogen?
Superconducting materials remain superconducting if they are held below their critical temperature Tc and the magnetic ﬁeld in which they sit remains below the critical ﬁeld Hc . The critical ﬁeld decreases with increasing temperature T as Hc ¼ Hc;o 1 ðT=Tc Þ2 where Hc;o is the critical ﬁeld at 0K. A superconducting magnet design envisages a superconducting coil cooled in liquid nitrogen, generating a magnetic ﬁeld of 30 T. Is it practical to use YBCO (YBa2Cu3O7) as the superconductor? The critical temperature Tc of YBCO is 93K and its zeroKelvin critical ﬁeld Hc;o is 140 T. Liquid nitrogen boils at 77K.
What is a dielectric? What is meant by polarisation? Deﬁne the dielectric constant. Why do some dielectrics absorb microwave radiation more than others?
It is much easier to measure the electrical conductivity of a material than to measure its thermal conductivity. Use the WiedemanneFranz law to ﬁnd the thermal conductivities of: (a) an alloy that has an electrical resistivity re of 28 mU.cm. (b) tungsten of the kind used for lamp ﬁlaments that has an electrical conductivity ke of 1.8 107 S/m.
The metal zinc has free electron concentration per unit volume, nv , of 1.3 1029/m3 and an electron mobility me of 8 104 m2/V.s. The charge carried by an electron, e, is 1.6 1019 coulomb. Based on this information, what is the electrical conductivity of zinc? Handbooks list the measured resistivity of zinc as 5.9 mU.cm. Is this consistent with your calculation? (Watch the units.)
The resistivity of pure silver is re ¼ 1.59 mU.cm. Each silver atom provides one free electron. The atomic volume of silver is 1.71 1029 m3. What is the electron mobility in silver?
Estimate the drift velocity of free electrons when a potential difference of 3 V is applied between the ends of a copper wire 100 mm long. The electron mobility in copper is me ¼ 0.0032 m2/V.s.
The resistivity of brass with 60 atom% copper and 40 atom% of zinc is re ¼ 6.8 mU.cm. Each copper atom contributes one free electron. Each zinc atom contributes two. The atomic volumes of copper and zinc are almost the same (assume them to be equal) and the electron concentration in copper is nv ¼ 8.45 1028/m3. What is the electron mobility me in brass? How does it compare with that of pure copper (me ¼ 0.0032 m2/V.s)?
Graphene is a semiconductor with remarkable electrical properties. It is reported that the free-electron mobility me in graphene is 1.5 m2/V.s and that the effective free electron concentration per unit volume, nv , is 5 1025/m3. If these values are accepted, what would you expect the resistivity of graphene to be?
A power line is to carry 5 kA at 11 kV using pylons 400 m apart. The dip d, in a wire of weight ml per unitlength strung between pylons L apart at a tension T is given by d ¼ L2 ml 8T. The maximum tensile stress allowed is 0.8 of the yield stress, sy . If the maximum allowable dip is 6 m, which of the materials in the table could be used? Material
Yield stress, sy MPa
Density, r kg/m3
Aluminium Copper Steel
125 120 380
2700 8900 7800
444 Chapter 15 Electrical materials: conductors, insulators, and dielectrics Exercise E15.16
A material is required for a transmission line that gives the lowest full-life cost over a 20-year period. The total cost is the sum of the material cost and the cost of the power dissipated in heat. The cost of electricity CE is 6 103 $/MJ. Material prices are listed in the table below. Derive an expression for the total cost per meter of cable in terms of the crosssectional area A (which is a free parameter), the material and electrical costs, and the material parameters. Show that the minimum cost occurs when the two contributions to the cost are equal. Hence derive a performance index for the material and decide on the best materials in the table.
Electrical resistivity re , Um
Density r, kg/m3
Price Cm , $/kg
Aluminium Copper Steel
1.7 108 1.5 108 55 108
2700 8900 7800
1.6 5.2 0.5
In the discussion of power transmission, a 50e50 mix of copper and steel strands was suggested for the cables. Using the values in the table for resistivity and strength, calculate the effective values for the cable, assuming a rule of mixtures for both strength and resistivity. Plot this on copies of the sy re chart for copper alloys of Figure 15.10 to explore its performance.
Strength, sy (MPa)
Resistivity, re (mU cm)
High strength steel, cold drawn High conductivity copper, cold drawn
Roughly 50% of all cork that is harvested in Portugal ends up as cork dust, a worthless by-product. As a materials expert, you are approached by an entrepreneur who has the idea of making useful products out of cork dust by compacting it and heating it, using microwave heating. The loss factor L ¼ εr tan d of cork is 0.21. The entrepreneur reckons he needs a power density P of at least 2 kW/m3 for the process to work. If the maximum ﬁeld E is limited to 102 V/m, what frequency f of microwaves will be needed?
Derive the expression (equation (15.14)) Max energy density ¼
1 εr εo E2b 2
for the maximum limiting electrical energy density that can be stored in a capacitor with plate area A separated by a dielectric of thickness t. Here εr is the dielectric constant of the dielectric, εo is the permittivity of free space, and Eb is the ﬁeld at which the dielectric breaks down.
You are asked to suggest a dielectric material for a capacitor with the highest possible energy density. What material would you suggest? Use Figure 15.7 to ﬁnd out.
The electron mobility me in undoped germanium at 300K is 0.36 m2/V.s and that of holes mh is 0.19 m2/V.s. The carrier density nv is 2.3 1019/m3. What is the conductivity of germanium at 300K? What is its resistivity?
The atomic volume of silicon is 2.0 1029 m3 and the free electron density nv at 300K is 1.5 1016/m3. What fraction of silicon atoms have provided a conduction electron?
You are asked to design a heat-sensing switch to turn the lights off in the garage when no one is moving around in it. What principle would you base it on? What materials would you choose for the sensor?
This page intentionally left blank
Magnet materials in action. The audio-frequency transformer on the left has a soft magnetic core. The DC motor on the right has a hard (permanent) magnetic stator and a soft magnetic rotor.
Chapter contents 16.1 16.2 16.3 16.4 16.5 16.6 16.7 16.8
Introduction and synopsis Magnetic properties: deﬁnition and measurement The big picture: charts for magnetic properties Drilling down: the physics and manipulation of magnetic properties Materials selection for magnetic design Summary and conclusions Further reading Exercises
447 448 455 458 462 470 470 471
Introduction and synopsis
Migrating birds, some think, navigate using the earth’s magnetic ﬁeld. This may be debatable, but what is beyond question is that sailors, for centuries, have navigated in this way, using a natural magnet, lodestone, to track it. Lodestone is a mineral, magnetite (Fe3O4), that sometimes occurs naturally in a magnetised state. Today we know lodestone is a ferri-magnetic ceramic, or ferrite, examples of which can be found in every radio, TV set, tablet, and microwave oven. Ferro-magnetic materials, by contrast, are metals, typiﬁed by iron but including Copyright Ó 2019 Elsevier Ltd. All rights reserved. https://doi.org/10.1016/B978-0-08-102376-1.00016-0
448 Chapter 16 Magnetic materials also nickel, cobalt, and alloys of all three. When placed in a magnetic ﬁeld, these materials become magnetised, a phenomenon called magnetic induction; on removal of the ﬁeld, some (the ‘soft’ magnets) lose their magnetisation, while others (the ‘hard’ magnets) retain it. Magnetic ﬁelds are created by moving electric charge e electric currents in electro-magnets, electron spin in the atoms of magnetic materials. This chapter is about magnetic materials: how they are characterised, where their properties come from, and how they are selected and used. It starts with deﬁnitions of magnetic properties and the way they are measured. As in other chapters, charts display them well, separating the materials that are good for one sort of application from those that are good for others. The chapter continues by drilling down to the origins of magnetic behaviour and concludes with a discussion of applications and the materials that best ﬁll them. There are many different kinds of magnetic behaviour. Figure 16.1 gives an overview, with examples of materials and their applications. Magnetic materials
(High requency filters)
(Magnetic stripe cards)
Figure 16.1 Magnetic behaviours, materials, and applications.
Magnetic properties: deﬁnition and measurement
Magnetic ﬁelds in vacuum First, some deﬁnitions. When a current i passes through a long, empty coil of n turns and length L as in Figure 16.2, a magnetic ﬁeld is generated. The magnitude of the ﬁeld, H, is given by Ampère’s law as H¼
and thus has units of amps/metre (A/m). The ﬁeld has both magnitude and direction e it is a vector ﬁeld.
16.2 Magnetic properties: deﬁnition and measurement
Flux lines of field H
n turns Length L
Figure 16.2 A solenoid creates a magnetic ﬁeld, H. Magnetic ﬁelds exert forces on a wire carrying an electric current. A current i ﬂowing in a single loop of area S generates a dipole moment m where m ¼ iS
with units A.m2, and it too is a vector with a direction normal to the loop S (Figure 16.3). If the loop is placed at right angles to the ﬁeld H it feels a torque T (units: newton metre, or N.m) of T ¼ mo mH
where mo is called the permeability of vacuum, mo ¼ 4p 107 henry/metre (H/m). To link these we deﬁne a second measure of the magnetic ﬁeld, one that relates directly to the torque it exerts on a unit magnetic moment. It is called the magnetic induction or ﬂux density, B, and for vacuum or non-magnetic materials it is B ¼ mo H
Field H Current i Moment m
Moment m Torque T
Figure 16.3 Magnetic moment and moment-ﬁeld interaction.
450 Chapter 16 Magnetic materials Its units are tesla, T, so a tesla1 is 1 HA/m2. A magnetic induction B of 1 T exerts a torque of 1 N.m on a unit dipole at right angles to the ﬁeld H. Magnetic ﬁelds in materials If the space inside the coil of Figure 16.2 is ﬁlled with a material, as in Figure 16.4, the induction within it changes. This is because its atoms respond to the ﬁeld by forming and aligning little magnetic dipoles in ways that are explained in Section 16.4. The material acquires a macroscopic dipole moment or magnetisation, M (its units are A/m, like H). The induction becomes B ¼ mo ðH þ MÞ
Flux lines of inductance B
Figure 16.4 A magnetic material exposed to a ﬁeld H becomes magnetised. The simplicity of this equation is misleading, since it suggests that M and H are independent; but in reality M is the response of the material to H, so the two are coupled. If the material of the core is ferro-magnetic, the response is a very strong one, and it is non-linear, as we shall see in a moment. It is usual to rewrite equation (16.5) in the form B ¼ mR mo H where mR is called the relative permeability, and like the relative permittivity (the dielectric constant) of Chapter 15, it is dimensionless. The magnetisation, M, is thus M ¼ ðmR 1Þ H ¼ cH
where c is the magnetic susceptibility. Neither mR nor c are constants e they depend not only on the material but also on the magnitude of the ﬁeld, H, for the reason just given. 1
Nikola Tesla (1856e1943), Serbian-American inventor, discoverer of rotating magnetic ﬁelds, the basis of most alternating current machinery, inventor of the Tesla coil and of a rudimentary ﬂying machine (never built).
16.2 Magnetic properties: deﬁnition and measurement
The magnetic pressure Pmag (force per unit area) exerted by an electromagnet on a section of core material is Pmag ¼
1 1 B2 mo H 2 ¼ 2 2 mo
provided that the core does not saturate. Iron has a high saturation magnetisation Hs of about 1.8 106 A/m, so the maximum pressure exerted by an electro-magnet with an iron core is 2 1 4p 107 1:8 106 ¼ 2:9 106 N m2 ¼ 2 MPa 2 The energy density stored in a magnetic ﬁeld per unit volume, U/V, has the same form as the magnetic pressure: Pmag ¼
U 1 B2 1 ¼ ¼ mo H 2 J m3 V 2 mo 2
Example 16.1 Magnetic ﬂux density (a) A coil of length L ¼ 3 cm and with n ¼ 100 turns carries a current i ¼ 0.2 A. What is the magnetic ﬂux density B inside the coil? (b) A core of siliconeiron with a relative permeability mR ¼ 10,000 is placed inside the coil. By how much does this raise the magnetic ﬂux density? Answer.
ni 100 0:2 ¼ ¼ 666:7 A m. The magnetic ﬂux density is 2 L 3 10 4 B ¼ m o H ¼ 8.38 10 T.
(a) The ﬁeld is H ¼
(b) The siliconeiron core raises the magnetic ﬂux density to B ¼ mR mo H ¼ 8.38 T.
Example 16.2 Magnetic ﬂux density A cylindrical coil with a length L ¼ 10 mm with n ¼ 50 turns carries a current i ¼ 0.01 A. What is the ﬁeld and ﬂux density in the magnet? A ferrite core with a susceptibility c ¼ 950 is placed in the coil. What is the ﬂux density and what is the magnetisation of the ferrite? Answer. The electro-magnet produces a ﬁeld H¼
ni 50 0:01 ¼ ¼ 50 A=m L 0:01
The ﬂux density is Bo ¼ mo H ¼ 4p 107 50 ¼ 6:3 105 T
452 Chapter 16 Magnetic materials The relative permeability of the ferrite is mR ¼ c þ 1 ¼ 951. When it is inserted into the core the induction increases to B ¼ mR mo H ¼ 951 4p 107 50 ¼ 0:06 T
The magnetisation is M¼
B 0:06 H ¼ 50 ¼ 4:8 104 A=m mo 4p 107
(This is well below the saturation magnetisation of ferrites, see below.)
Example 16.3 Magnetic energy density An electro-magnet generates a ﬁeld of H ¼ 10,000 A/m. What is the magnetic energy density? Answer. The magnetic energy density is U 1 1 ¼ m H2 ¼ 4p107 108 ¼ 62:8 J m3 V 2 o 2
Ferro-magnetic and ferri-magnetic materials Nearly all materials respond to a magnetic ﬁeld by becoming magnetised, but most are paramagnetic with a response so faint that it is of no practical use. A few, however, contain atoms that have large dipole moments and the ability to spontaneously magnetise e to align their dipoles in parallel e as electric dipoles do in ferro-electric materials. These are called ferro-magnetic and ferri-magnetic materials (the second are called ferrites for short), and it is these that are of real practical use. Magnetisation decreases with increasing temperature. Just as with ferro-electrics, there is a temperature, the Curie temperature Tc, above which it disappears, as in Figure 16.5. Its value for the materials we shall meet here is well above room temperature (typically 300e1000 C), but making magnets for use at really high temperatures is a problem. Saturation magnetisation, Ms (A/m)
Ms at 0 K
Curie temperature Tc 0
Temperature, T (K)
Figure 16.5 Saturation magnetisation decreases with increasing temperature.
16.2 Magnetic properties: deﬁnition and measurement
Measuring magnetic properties The magnetic behaviour of a material is characterised by its MH curve (Figure 16.6). If an increasing ﬁeld H is applied to a previously demagnetised sample, starting at A on the ﬁgure, its magnetisation increases, slowly at ﬁrst and then faster, following the broken line, until it ﬁnally tails off to a maximum, the saturation magnetisation Ms at point B. If the ﬁeld is now reduced, M does not retrace its original path; some magnetisation is retained when H reaches zero at point C. The residual magnetisation is called the remanent magnetisation or remanence, Mr, and is usually only a little less than Ms. To decrease M further, we must increase the ﬁeld in the opposite direction until M ﬁnally passes through zero at point D when the ﬁeld is Hc, the coercive ﬁeld, a measure of the resistance to demagnetisation. Beyond point D the magnetisation M starts to increase in the opposite direction, eventually reaching saturation again at point E. If the ﬁeld is now decreased again, M follows the curve through F and G back to full forward magnetic saturation again at B to form a closed MH circuit, or hysteresis loop. Magnetisation, M Remanent magnetisation, Mr
G Coercive field, –Hc
Coercive field, Hc
Magnetic field, H
Saturation magnetisation, Ms
Saturation magnetisation, –Ms
Figure 16.6 A magnetic hysteresis curve. Magnetic materials are characterised by the size and shape of their hysteresis loops. The initial segment AB is called the initial magnetisation curve, and its average slope (or sometimes its steepest slope) is the magnetic susceptibility, c. The other key properties e the saturation magnetisation Ms, the remanence Mr, and the coercive ﬁeld Hc e have already been deﬁned. Each full cycle of the hysteresis loop dissipates an energy per unit volume equal to the area of the loop multiplied by mo, the permeability of vacuum. This energy appears as heat; it is like magnetic friction. Many texts plot the curve of inductance B against H, rather than the MH curve. Equation (16.5) says that B is proportional to (M þ H). Since the value of M (for any magnetic materials worthy of the name) is very much larger than the H applied to it, B z moM and the BeH curve of a ferro-magnetic material looks very like its MH curve (it’s just that the M axis has been scaled by mo).
454 Chapter 16 Magnetic materials There are several ways to measure the hysteresis curve, one of which is sketched in Figure 16.7. Here the material forms the core of what is in effect a transformer. The oscillating current through the primary coil creates a ﬁeld H that induces magnetisation M in the material of the core, driving it round its hysteresis loop. The secondary coil picks up the inductance, from which the instantaneous state of the magnetisation can be calculated, mapping out the loop. Magnetic material
Integrator, giving magnetisation, M
input giving field, H
M Hysteresis loop
Figure 16.7 Measuring the hysteresis curve. Magnetic materials differ greatly in the shape and area of their hysteresis loop, the greatest difference being that between soft magnets, which have thin loops, and hard magnets, which have fat ones, as sketched in Figure 16.8. In fact, the differences are much greater than this ﬁgure suggests: the coercive ﬁeld Hc (which determines the width of the loop) of hard magnetic materials like alnico is greater by a factor of about 105 than that of soft magnetic materials like siliconeiron.
Mr Slope χ
Field, H Hc
Figure 16.8 Magnetisation hysteresis loops: (a) a thin, square loop typical of soft magnets, (b) a fat loop typical of hard magnets.
16.3 The big picture: charts for magnetic properties 455
The big picture: charts for magnetic properties
The remanenceecoercive ﬁeld chart The differences between families of soft and hard magnetic materials are brought out by the chart in Figure 16.9. The axes are remanent magnetisation Mr and coercive ﬁeld Hc. The saturation magnetisation Ms, more relevant for soft magnets, is only slightly larger than Mr, so an MseHc chart looks almost the same as this one. There are 12 distinct families of magnetic materials, each enclosed in a coloured envelope. The members of each family, shown as smaller ellipses, have unhelpful tradenames (such as ‘H Ferrite YBM-1A’) so they are not individually labelled. Soft magnets require high Ms and low Hc; they are the ones on the left, with the best near the top. Hard magnets must hold their magnetism, requiring a high Hc, and to be powerful they need a large Mr; they are the ones on the right, with the best again at the top. Coercive field and magnetisation Fe-Co Permendur alloys
Metglas amorphous alloys
10 6 1 Silicon iron
Permalloys and MuMetal
10 5 Soft (cubic) ferrites 0.01
Remanent induction, BT (T)
Remanent magnetisation, Mr (A/m)
Hard (hexagonal) ferrites 1
Coercive field, Hc (A/m)
Figure 16.9 Remanent magnetisation and coercive ﬁeld. Soft magnetic materials lie on the left, hard magnetic materials on the right. The orange and blue envelopes enclose electrically conducting materials, the green ones enclose insulators. In many applications the electrical resistivity is also important because of eddy-current losses, which will be described later. Changing magnetic ﬁelds induce eddy currents in conductors but not in insulators. The orange and blue envelopes on the chart enclose metallic ferro-magnetic materials, which are good electrical conductors. The green ones describe ferrites, which are electrical insulators.
456 Chapter 16 Magnetic materials Example 16.4 Selecting materials for permanent magnets A material is required for a powerful permanent magnet that must be as small as possible and be resistant to demagnetisation by stray ﬁelds. Use the chart of Figure 16.9 to identify your choice. Answer. The requirement that the magnet be small and powerful requires a high remanent magnetisation, Mr. The need to resist demagnetisation implies a high coercive ﬁeld, Hc. The choice, read from the chart, is the neodymium-based family of hard magnetic materials. (These are the magnets-of-choice for hybrid and electric car motors and for wind turbine generators.) These, however, are expensive, because they contain a rare earth element Nd. The Alnico family, based on aluminium, nickel, and cobalt (hence the name) are cheaper.
The saturation magnetisationesusceptibility chart This is the chart for selecting soft magnetic materials (Figure 16.10). It shows the saturation magnetisation, Ms e the ultimate degree to which a material can concentrate magnetic ﬂux e plotted against its susceptibility, c, which measures the ease with which it can be magnetised. Many texts use, instead, the saturation inductance Bs and maximum relative permeability, mR. They are shown on the other axes of the chart. As in the ﬁrst chart, materials that are electrical conductors are enclosed in orange and blue envelopes; those that are insulators have green ones. Relative permeability, μ R 10 4
Saturation magnetisation and Permeability
Saturation magnetisation, Ms (A/m)
Fe-Co Permendur Metglas alloys amorphous alloys
Low carbon steel
Nickel-iron Permalloys and MuMetal
Soft (cubic) ferrites
Saturation induction, Bs (Tesla)
Figure 16.10 Saturation magnetisation, susceptibility, and relative permeability for soft magnetic materials. The orange and blue envelopes enclose electrically conducting materials, the green ones enclose insulators.
16.3 The big picture: charts for magnetic properties 457 The coercive ﬁeldeCurie temperature chart Two things can disrupt ferro-magnetic behaviour: temperature and demagnetising ﬁelds. The ferro-magnetic response disappears above the Curie temperature, which, as the chart of Figure 16.11 shows, is as low as 100 C for some materials and as high as 1000 C for others. Remanent magnetisation is cancelled or reversed by ﬁelds exceeding the coercive ﬁeld, a risk when permanent magnets must operate in environments with stray ﬁelds. The chart is useful for selecting magnetic materials for use at elevated temperatures e such as actuators in control equipment of engines, for instance. As before, the colours distinguish conducting ferro-magnetic metals from insulating ferrites. Curie temperature (°C) 0
Coercive field and Curie temperature Co-Sm alloys
Coercive field, Hc (A/m)
Hard (hexagonal) ferrites
Soft (cubic) ferrites
Fe-Co Permendur alloys
1 Nickel-iron permalloys and MuMetal
Metglas amorphous alloys
Curie temperature (K)
Figure 16.11 Coercive ﬁeld and Curie temperature. The orange and blue envelopes enclose electrically conducting materials, the green ones enclose insulators.
Example 16.5 Selecting materials for high temperatures and high ﬁelds A permanent magnet is needed for an aerospace application. In use the magnet may be exposed to demagnetising ﬁelds as high as 3 105 A/m (0.38 T) and temperatures of 600 C. What material would you recommend for the magnet? Answer. The coercive ﬁeld must exceed the limit of 3 105 A/m. Figure 16.11 shows that this rules out Alnicos and most hard ferrites. The Curie temperature must comfortably exceed the operating temperature of 600 C. The ﬁgure shows that neodymiumeboron and hard ferrites cannot meet this requirement. This leaves the cobaltesamarium group of hard magnets, which meet both requirements.
458 Chapter 16 Magnetic materials
Drilling down: the physics and manipulation of magnetic properties
The classical picture of an atom is that of a nucleus around which swing electrons, as in Figure 16.12. Moving charge implies an electric current, and an electric current ﬂowing in a loop creates a magnetic moment, as in Figure 16.3. Thus each orbiting electron creates a magnetic dipole. That is not all. Each electron has an additional moment of its own: its spin moment. A proper explanation of this requires quantum mechanics, but a way of envisaging its origin is to think of an electron not as a point charge but as slightly spread out and spinning on its own axis, again creating a rotating charge and a dipole moment e and this turns out to be large. The total moment of the atom is the sum of the whole lot. m No net moment
m m (b)
Moment of 1 Bohr magneton
m m (c)
No net moment
Figure 16.12 Orbital and electron spins create a magnetic dipole. Even numbers of electrons ﬁlling energy levels in pairs have moments that cancel, as in (a) and (c). An unpaired electron gives the atom a permanent magnetic moment, as in (b). A simple atom like helium has two electrons per orbit, and they conﬁgure themselves such that the moment of one exactly cancels the moment of the other, leaving no net moment e as in Figure 16.12(a), which shows helium, or in Figure 16.12(c). But now think of an atom with three electrons as in Figure 16.12(b). The moments of two may cancel, but there remains the third, leaving the atom with a net moment represented by the red arrow at the right. Thus atoms with electron moments that cancel are non-magnetic; those with electron moments that don’t cancel carry a magnetic dipole. Simplifying a little, one unpaired electron gives a magnetic moment of 9.27 1024 A.m2, called a Bohr2 magneton; two unpaired electrons give two Bohr magnetons, three gives three, and so on. 2
Niels Henrik David Bohr (1885e1962), Danish theoretical physicist, elucidator of the structure of the atom, contributor to the Manhattan Project, and campaigner for peace.
16.4 Drilling down: the physics and manipulation of magnetic properties 459 Think now of the magnetic atoms assembled into a crystal. In most materials the atomic moments interact so weakly that thermal energy is enough to randomise their directions, as in Figure 16.13(a) and the structure as a whole has no magnetic moment; these materials are paramagnetic. In a few materials, though, something quite different happens. The ﬁelds of neighbouring atoms interact such that their energy is reduced if their magnetic moments line up. This drop in energy is called the exchange energy, and it is strong enough that it beats the randomising effect of thermal energy so long as the temperature is not too high. The shape of the Curie curve of Figure 16.5 showed how thermal energy overwhelms the exchange energy as the Curie temperature is approached. They may line up anti-parallel, head to tail, so to speak, as in Figure 16.13(b), and we still have no net magnetic moment; such materials are called anti-ferro-magnets. But in a few elements, notably iron, cobalt and nickel, exactly the opposite happens: the moments spontaneously align so that e if all are parallel e the structure has a net moment that is the sum of those of all the atoms it contains (Figure 16.13(c)). These materials are ferro-magnetic. Iron has three unpaired electrons per atom, cobalt has two, and nickel just one, so the net moment if all the spins are aligned (the saturation magnetisation Ms) is greatest for iron, less for cobalt, and still less for nickel.
Figure 16.13 Types of magnetic behaviour. Compounds give a fourth possibility. The materials we have referred to as ferrites are oxides; one class of them has the formula MFe2O4 where M is also a magnetic atom, such as cobalt, Co. Both the Fe and the Co atoms have dipoles but they differ in strength. They line up in the anti-parallel conﬁguration, but because the moments differ, the cancellation is incomplete, leaving a net moment M; these are ferri-magnets, or ferrites for short (Figure 16.13(d)). The partial cancellation and the smaller number of magnetic atoms per unit volume mean they have lower saturation magnetisation than, say, iron. But as they are oxides they have other advantages, notably that they are electrical insulators.
460 Chapter 16 Magnetic materials Domains If atomic moments line up, shouldn’t every piece of iron, nickel or cobalt be a permanent magnet? Although they are magnetic materials they do not necessarily have a magnetic moment. Why not? A uniformly magnetised rod creates a magnetic ﬁeld, H, like that of a solenoid. The ﬁeld has an energy Z 1 U ¼ mo H 2 dV (16.9) 2 V where the integral is carried out over the volume V within which the ﬁeld exists. Working out this integral is not simple, but we don’t need to do it. All we need to note is that the smaller is H, and the smaller the volume V that it invades, the smaller is the energy. If the structure can arrange its moments to minimise its overall H or get rid of it entirely (remembering that the exchange energy wants neighbouring atom moments to stay parallel) it will try to do so. Figure 16.14 illustrates how this can be done. The material splits up into domains within which the atomic moments are parallel, but with a switch of direction between mating domains to minimise the external ﬁeld. The domains meet at domain walls, regions a few atoms thick in which the moments swing from the orientation of one domain to that of the other. Splitting into parallel domains of opposite magnetisation, as at Figure 16.14(b) and (c), reduces the ﬁeld substantially; adding end regions magnetised perpendicular to both as at (d) kills it almost completely. The result is that most magnetic materials, unless manipulated in some way, adopt a domain structure with minimal external ﬁeld e which is the same as saying that, while magnetic, they are not magnets. Flux lines of external field, B Flux lines
(b) Domain walls
Direction of magnetisation
Figure 16.14 Domains cancel the external ﬁeld while retaining magnetisation of the material itself.
16.4 Drilling down: the physics and manipulation of magnetic properties 461 How can they be magnetised? Figure 16.15, left, shows the starting domain wall structure. When placed in a magnetic ﬁeld, created, say, with a solenoid, the domains already aligned with the ﬁeld have lower energy than those aligned against it. The domain wall separating them feels a force, the Lorentz3 force, pushing it in a direction to make the favourably oriented domains grow at the expense of the others. As they grow, the magnetisation of the material increases, moving up the MH curve, ﬁnally saturating at Ms when the whole sample is one domain, oriented parallel to the ﬁeld, as in the right of Figure 16.15. Domain wall
Applied magnetic field H
No applied field
Domain of dipoles
Figure 16.15 An applied ﬁeld causes domain boundaries to move. At saturation the sample has become a single domain, as on the right. Domain walls move easily in soft magnetic materials. Hard magnetic materials are alloyed to prevent their motion.
The saturation magnetisation, then, is just the sum of all the atomic moments contained in a unit volume of material when they are all aligned in the same direction. If the magnetic dipole per atom is nm mB (where nm is the number of unpaired electrons per atom, and mB is the magnetic moment of a Bohr magneton) then the saturation magnetisation is Ms ¼
nm mB U
where U is the atomic volume. Iron has the highest Ms because its atoms have the most unpaired electrons and they are packed close together. Anything that reduces either one reduces the saturation magnetisation. Nickel and cobalt have lower saturation because their atomic moments are less; alloys of iron tend to be lower because the non-magnetic alloying atoms dilute the magnetic iron. Ferrites, which are oxides, have much lower saturation, both because of dilution by oxygen and because of the partial cancellation of atomic moments sketched in Figure 16.13(d). There are, nonetheless, good reasons for alloying even if it dilutes the dipoles. A good permanent magnet retains its magnetisation even when placed in a reverse ﬁeld. That’s achieved by pinning the domain walls to stop them from moving. Impurities, precipitates, and porosity all interact with domain walls, tending to pin them in place. They act as obstacles to dislocation motion too (Chapter 6), so magnetically hard materials are mechanically hard as well. 3
Hendrik Antoon Lorentz (1853e1928), Dutch mathematical physicist, friend and collaborator with Raleigh and Einstein, originator of key concepts in optics, electricity, relativity, and hydraulics (he modelled and predicted the movement of water caused by the building of the Zuyderzee).
462 Chapter 16 Magnetic materials And there are subtler barriers to domain wall motion. One is magnetic anisotropy, arising because certain directions of magnetisation in the crystal are more favourable than others. Another relates to the shape and size of the sample itself: small, single-domain magnetic particles are particularly resistant to having their magnetism reversed, which is why they can be used for information storage. The performance of a hard magnet is measured by its energy product, roughly proportional to the product BrHc, the axes of Figure 16.9. The higher the energy product, the more difﬁcult it is to demagnetise it. Example 16.6 Unpaired electron density Nickel has a saturation magnetisation of Ms ¼ 5.2 105 A/m. Its atomic volume is U ¼ 1.09 1029 m3. What is the effective number of unpaired electrons nm in its conduction band? nm mB . The value of the U 24 2 Bohr magneton is mB ¼ 9.27 10 A.m . The resulting value of nm is nm ¼ 0.61. Answer. The saturation magnetisation is given by Ms ¼
Example 16.7 Calculating saturation magnetisation Iron has a density r of 7870 kg/m3 and an atomic weight Awt of 55.85 kg/kmol. The net magnetic moment of an iron atom, in Bohr magnetons per atom, is nm ¼ 2.2. What is the saturation magnetisation Ms of iron? Answer. The number of atoms per unit volume in iron is n¼
1 NA r ¼ ¼ 8:49 1028 m3 U Awt
(here NA is Avogadro’s number, 6.022 1026 atoms/kmol). The saturation magnetisation Ms is the net magnetic moment per atom nm mB times the number of atoms per unit volume, n: Ms ¼ n nm mB
where mB ¼ 9.27 1024 A.m2 is the magnetic moment of one Bohr magneton. Thus the saturation magnetisation of iron is Ms ¼ 8:49 1028 2:2 9:27 1024 ¼ 1:73 106 A=m
Materials selection for magnetic design
Selection of materials for their magnetic properties follows the same process of translating design requirements followed by screening and ranking. In this case, however, the ﬁrst
16.5 Materials selection for magnetic design
screening step e ‘must be magnetic’ e immediately isolates the special set of materials shown in the property charts of this chapter. The key selection issues are then:
whether a soft or hard magnetic response is required; whether a fat or a thin MH hysteresis loop is wanted; what frequency of alternating ﬁeld the material must carry; whether the material must operate above room temperature in a large external ﬁeld.
Soft magnetic devices Electromagnets, transformers, electron lenses, and the like have magnetic cores that must magnetise easily when the ﬁeld switches on, be capable of creating a high ﬂux density, yet lose their magnetism when the ﬁeld is switched off. They do this by using soft, low Hc, magnetic materials, shown on the left of the chart of Figure 16.8. Soft magnetic materials are used to ‘conduct’ and focus magnetic ﬂux (Figure 16.16). A current-carrying coil induces a magnetic ﬁeld in the core. The ﬁeld, instead of spreading in the way shown in Figure 16.4, is trapped in the extended ferro-magnetic circuit. The higher the susceptibility c, the greater is the magnetisation and ﬂux density induced by a given current loop, up to a limit set by its saturation magnetisation Ms. The magnetic circuit conducts the ﬂux from one coil to another, or from a coil to an air gap where it is further enhanced by reducing the section of the core. The ﬁeld in the gap may be used, for example, to actuate or to focus an electron beam. Thus the ﬁrst requirement of a good soft magnet is a high c and a high Ms. These are the two properties plotted in Figure 16.10. Permendur (FeeCoeV alloys) and Metglas amorphous alloys are particularly good, but being expensive they are used only in small devices. Siliconeiron (Fe 1e4% Si) is much cheaper and easier to make in large sections; it is the staple material for large transformers. Soft magnetic core
Soft magnetic core
Flux intensified by geometry of core
Figure 16.16 Soft magnets ‘conduct’ magnetic ﬂux and concentrate it if the cross-section of the magnet is reduced.
464 Chapter 16 Magnetic materials Most soft magnets are used in AC devices, and then energy loss, proportional to the area of the hysteresis loop, becomes a consideration. Energy loss is of two types: the hysteresis loss already mentioned, proportional to switching frequency f, and eddy current losses caused by the currents induced in the core itself by the AC ﬁeld, proportional to f 2. In cores of transformers operating at low frequencies (meaning f up to 100 Hz or so) the hysteresis loss dominates, so for these we seek high Ms and a thin loop with a small area. Eddy current losses are present but are suppressed when necessary by laminating: making the core from a stack of thin sheets interleaved with thin insulating layers that interrupt the eddy currents. At audio frequencies (f < 50 kHz) losses of both types become greater because they occur on every cycle and now there are more of them, requiring an even narrower loop and thinner laminates; here the more expensive permalloys and Permendurs are used. At higher frequencies still (f in the MHz range) eddy current loss, rising with f2, becomes very large and the only way to stop it is to use magnetic materials that are electrical insulators. The best choice is ferrites, shown in green envelopes on all three charts, even though they have a lower Ms. Above this (f > 100 MHz) only the most exotic ceramic magnets will work. Table 16.1 lists the choices, guided by the charts.
Table 16.1 Materials for soft magnetic applications Application